Peak™ Universal Bond and Peak™ SE
Description:
Peak Universal Bond is a bottle or single syringe delivered bonding resin.
It can be used with self-etch or with total etch. It is 7.5% filled with an ethyl
alcohol solvent carrier and will cure with most high intensity lights including
LEDs. Peak Universal Bond contains 0.2% chlorhexidine which may ensure
long term bond strengths.
Peak SE Primer is a self-etching dentin bonding resin which is comprised ofan etchant and primer in a syringe delivery system.
Ultra-Etch™ is a syringe-delivered, 35% phosphoric acid etch and rinse gel.
Inclusion of the chlorhexidine additive has not shown to correlate with areduction in secondary decay in patients. Clinical studies to evaluate theeffects of chlorhexidine on oral bacterial or caries have not been performed.
Indications for Use:Use for virtually all etching and bonding needs in restorative dentistry forpatients of all ages.
Peak Universal Bond bonds to the following materials:• Dentin and Enamel• Porcelain, zirconia• Metal• Composite

Direct Bonding Technique and Porcelain/
Zirconia Repair
1. Preparea. Dentin/Enamel: Isolate, clean and remove
caries ensuring all non-mineral dentin is removed (Seek/Sable Seekis recommended for this). For abrasion/abfraction Class V preps,
roughen with a diamond bur.
b. Composite: Remove weakened areas of existing composite. Roughen
surface with diamond bur.
c. Metal: Microabrade surface.
d. Zirconia: Clean surface and remove weakened zirconia with a diamondbur.
e. Porcelain: Roughen and remove weakened porcelain with diamondbur. Clean fractured porcelain area for 5 seconds with Ultra-Etch.
Rinse and dry.
2. Etcha. Self-Etch Technique – dentin/enamel, composite and metal
i. Rinse preparation and leave damp.
ii. OPTIONAL – Apply Consepsis™ (where available) with Black Mini™
Brush Tip to preparation with a scrubbing motion and lightly air

dry leaving surface damp.
iii. Apply Peak SE with Black Mini Brush Tip to the tooth preparationfor 20 seconds using continuous agitation on dentin. Do not scrub
the enamel.
iv. Thin/dry for 3 seconds using the air/water syringe or by placing
the high volume suction directly over the preparation.
v. Proceed to “Bond” step below.
b. Total Etch Technique – dentin/enamel, composite and metal
i. Verify the color and consistency of the product flow before
applying by expressing a small amount onto a mixing pad or
gauze. Discard any clear liquid that is expressed.
ii. Apply Ultra-Etch with the Blue Micro™ Tip to all surfaces of the
tooth preparation for 20 seconds.
iii. Rinse thoroughly for 5 seconds.
iv. Lightly dry using the air/water syringe or by placing the highvolume suction directly over the preparation. Leave the surface
slightly damp.
v. OPTIONAL – Apply Consepsis (where available) with Black Mini
Brush Tip to preparation with a scrubbing motion and lightly air
dry leaving surface damp.
vi. Proceed to “Bond” step below.
c. Porcelain Etch – CAUTION – use proper isolation such as an acidneutralizing barrier (EtchArrest™) when using hydrofluoric acid (HF)
(Ultradent™ Porcelain Etch). Do not allow hydrofluoric acid to touchgingiva or dentin.
i. Apply hydrofluoric acid to fractured area for 90 seconds.
ii. Suction acid from surface THEN thoroughly rinse and dry.
iii. Apply Ultra-Etch for 5 seconds to remove porcelain salts anddebris formed by HF etching. Rinse and dry.
iv. Apply puddle coat of silane for 60 seconds.
v. Dry thoroughly. DO NOT RINSE.
vi. Proceed to “Bond” step below.
d. Zirconia – DO NOT ETCH OR USE SILANE
i. Air-abrade fractured surface of prosthesis, rinse and dry.
ii. Apply zirconia primer to fractured area following manufacturer’s
instructions.
iii. Proceed to “Bond” step below.
3. Bonda. Bottle Delivery
i. Dispense 1-3 drops of Peak™ Universal Bond into the “B” side ofthe disposable dappen dish.
ii. Using the Micro Applicator Brush, apply a puddle coat of Peak
Universal Bond to the preparation and gently agitate for 10
seconds.
iii. Thin/dry for 10 seconds using ¼ to ½ air pressure. Preparation
should appear shiny.
iv. Light cure for 10 seconds (20 seconds for lights with
output<600mW/cm2).
v. Restore with flowable or packable composite as per
manufacturer’s instructions.
b. Syringe Delivery
i. Apply a puddle coat of Peak Universal Bond with Inspiral™ Brush
Tip - gently agitate for 10 seconds.
ii. Thin/dry 10 seconds using ¼ to ½ air pressure. Preparation
should appear shiny.
iii. Light cure for 10 seconds (20 seconds for lights with output<600mW/cm2).
iv. Restore with flowable or packable composite as per
manufacturer’s instructions.

Pre-Bind Face Trim

Directions for Use:NOTE: Initial use of Peak SE requires
activation of the two components
separated in the JetMix™ syringe.
1. Peak SE is stable for 120 days after activation.
2. Write the expiration date on the flat area ofthe plunger stem before activation.
3. DO NOT REMOVE LUER LOCK CAP PRIORTO MIXING
4. Quickly and forcefully press “dated” plunger
into middle barrel.
5. Verify that plunger is flush with middle
barrel.

EN

2

Indirect Bonding Technique - Indirect Crowns, In-lays, Onlays,
Zirconia
1. Prepare
a. Remove temporary, clean preparation, rinse, and dry (Consepsis Scrub
with a STARbrush™ to clean, disinfect, and remove residual cement).
b. Verify prosthetic fit.
c. Prepare inside surface of prosthesis.
i. Metal based:
1. Microabrade (sandblast) inside surface of prosthesis.
2. Rinse and dry surface.
ii. Ceramic/porcelain:
1. Apply hydrofluoric acid (HF) (Ultradent Porcelain Etch) to insidesurface of prosthesis for 90 seconds, rinse and dry.
2. Apply Ultra-Etch for 5 seconds to remove porcelain salts anddebris formed by HF etching. Rinse and dry.
3. Apply silane (Ultradent™ Silane) to inside surface of prosthesis for
1 minute, dry and set prosthesis aside. Do not rinse.
iii. Zirconia: DO NOT ETCH OR USE SILANE
1. Air abrade internal surface of prosthesis, rinse and dry.
2. Apply a zirconia primer as per manufacturer instructions.
2. Etch - Prepare tooth surface
a. Self-Etch Technique – dentin/enamel, composite and metal
i. Rinse preparation and leave damp.
ii. OPTIONAL – Apply Consepsis (where available) with Black Mini
Brush Tip to preparation with a scrubbing motion and lightly air
dry leaving surface damp.
iii. Apply Peak™ SE with Black Mini™ Brush Tip - 20 seconds to toothpreparation using continuous agitation on dentin. Do not scrub
the enamel.
iv. Thin/dry for 3 seconds using the air/water syringe or by placing
the high volume suction directly over the preparation.
v. Proceed to “Bond” step below
b. Total Etch Technique – dentin/enamel, composite and metal
i. Apply Ultra-Etch with the Blue Micro Tip to all surfaces of the toothpreparation for 20 seconds.
ii. Rinse thoroughly for 5 seconds.
iii. Lightly dry using the air/water syringe or by placing the highvolume suction directly over the preparation. Leave the surface
slightly damp.
iv. OPTIONAL – Apply Consepsis (where available) with Black Mini
Brush Tip to preparation with a scrubbing motion and lightly air
dry leaving surface damp.
v. Proceed to “Bond” step below.
c. Porcelain Etch – CAUTION – use proper isolation such as an acidneutralizing barrier (EtchArrest) when using hydrofluoric acid (HF)
(Ultradent Porcelain Etch). Do not allow hydrofluoride acid to touchgingiva or dentin.
i. Apply hydrofluoric acid to fractured area for 90 seconds.
ii. Suction acid from surface THEN thoroughly rinse and dry.
iii. Apply Ultra-Etch for 5 seconds to remove porcelain salts and debris
formed by HF etching. Rinse and dry.
iv. Apply puddle coat of silane for 60 seconds.
v. Dry thoroughly. DO NOT RINSE.
vi. Proceed to “Bond” step below.
d. Zirconia – DO NOT ETCH OR USE SILANE
i. Air-abrade internal surface of prosthesis, rinse and dry.
ii. Apply zirconia primer to fractured area following manufacturer’s
instructions.
iii. Proceed to “Bond” step below.
3. Bonda. Bottle Deliveryi.

Dispense 1-3 drops of Peak Universal Bond into the “B” side of thedisposable dappen dish.
ii. Using the Micro Applicator Brush, apply a puddle coat of Peak
Universal Bond to the preparation and gently agitate for 10
seconds.
iii. Thin/dry for 10 seconds using full air pressure. Preparation should
appear shiny.
iv. Light cure for 10 seconds (20 seconds for lights with
output<600mtW/cm2).
b. Syringe Delivery
i. Apply a puddle coat of Peak Universal Bond with Inspiral Brush Tip- gently agitate for 10 seconds.
ii. Thin/dry 10 seconds using full air pressure. Preparation should
appear shiny.
iii. Light cure for 10 seconds (20 seconds for lights with output <600
mW/cm2).
4. Cementa. Apply light cure cement for translucent veneers or dual cure resin
cement to other prostheses and follow manufacturer’s instructions
for use.
NOTE: Immediate Dentin Sealing requires Direct Technique steps 2A
and 3 above. Apply glycerin over Peak Universal Bond and light cure
10 seconds. Rinse Glycerin. Make final impression. Re-apply glycerin topreparation as separating medium prior to cementing the temporary
in place.
Repair of Composite / Metal / Zirconia / Porcelain
1. Composite: Remove weakened areas of existing composite. Roughen
surface with diamond bur.
a. Total-Etch Techniquei. Apply Ultra-Etch with the Blue Micro Tip to all surfaces of toothpreparation for 20 seconds.
ii. Rinse thoroughly for 5 seconds and leave damp.
2. Metal: Microabrade surface
a. Total-Etch Techniquei. Apply Ultra-Etch with the Blue Micro Tip to all surfaces of toothpreparation for 20 seconds.
ii. Rinse thoroughly for 5 seconds and leave damp.
3. Zirconia: Clean surface; remove weakened zirconia with diamond bur.
DO NOT ETCH OR USE SILANE.
a. Air-abrade internal surface of prothesis.
b. Apply zirconia primer to fractured area following manufacturer’s
instructions.
4. Porcelain: Roughen and remove weakened porcelain with diamondbur. Clean fractured porcelain area for 15 seconds with Ultra-Etch. Rinseand dry.
CAUTION - use proper isolation such as an acid neutralizing barrier(EtchArrest) when using hydrofluoric acid (HF) (Ultradent™ Porcelain Etch).
Do not allow hydrofluoric acid to touch gingiva or dentin.
a. Apply hydrofluoric acid to fractured area for 90 seconds.
b. Suction acid from surface then thoroughly rinse and dry surface.
c. Apply Ultra-Etch for 5 seconds to remove porcelain salts and debris
formed by HF etching. Rinse and dry.
d. Apply puddle coat of silane for 1 minute.
e. Dry thoroughly. DO NOT RINSE.
5. Bonda. Bottle Delivery
i. Dispense 1-3 drops of Peak Universal Bond into the “B” side of thedisposable dappen dish.
ii. Using the Micro Applicator Brush, apply a puddle coat of Peak
Universal Bond and gently agitate for 10 seconds.
iii. Thin/dry for 10 seconds using 1/4 to 1/2 air pressure. Preparation

should appear shiny.
iv. Light cure for 10 seconds (20 seconds for lights with output<600mW/cm2).
b. Syringe Delivery
i. Apply a puddle coat of of Peak Universal Bond with Inspiral Brush
Tip - gently agitate for 10 seconds.
ii. Thin/dry for 10 seconds using 1/4 to 1/2 air pressure.
iii. Preparation should appear shiny.
iv. Light cure for 10 seconds (20 seconds for lights with output<600mw/cm2).
6. Restore with flowable and/or packable composite as per manufacturer’s
instructions.

iii. Thoroughly remove excess Peak Universal Bond using the TriAway
Adapter and the 22ga Endo-Eze Tip.
iv. Air dry post space and preparation for 10 seconds using full airpressure to thin/dry with TriAway Adapter and 22ga Endo-Eze Tip
to evaporate any remaining solvent from the bottom up.
v. Light cure down the post space for 20 seconds (40 seconds forlights with output of <600mW/cm2). Use paper point or previously
fitted post to verify post space is not blocked.

Post Cementation and Core Build-up
1. Remove cap from the PermaFlo™ DC syringe.
2. Place a mixing tip onto the dual barrel syringe lining up the two ports.
Twist clockwise until locked in place.
Post and Core
3. Attach the flexible Intraoral Tip™ to the mixing tip for delivery directly into
the canal from the dual barrel syringe.
1. Preparea. Drill post hole using a rubber stop and appropriate size UniCore™ Drill. 4. Express a small amount before placing in the post space.
b. Thoroughly rinse the post space for 10 seconds using the TriAway
5. Insert the tip into the post space to full depth.
Adaptor and a 22ga Endo-Eze™ Tip. Dry with TriAway Adaptor and 22ga 6. Using even pressure deliver PermaFlo DC starting apically and moving
Endo-Eze Tip from the bottom of the preparation up.
coronally.
c. Verify post (UniCore Post) fit and cut to desired length using a high
7. Insert the (UniCore™ Post) slowly, displacing the excess cement.
8. Place curing light directly above the post and light cure 20 seconds; 40
speed diamond disc. NOTE: Carbide and operative burs may frayseconds for lights with output <600mW/cm2).
the fibers.
9. Continue building layers of PermaFlo™ DC around post as needed. NOTE:
2. EtchLight cure for 5 seconds between layers to gel and form core. Do a final
a. Self-Etch Technique
cure on core for 40 seconds.
i. Rinse canal space and leave damp.
Do not remove mixing tip until next use. Disinfect syringe and mixing tip.
ii. Attach a blue 22ga Deliver-Eze™ Brush Tip to Peak SE syringe.
iii. Apply to the post space and coronal preparation for 20 seconds
using an agitating action.
Precautions and warnings:
iv. Blow out excess with TriAway Adaptor and 22ga Endo-Eze Tip from 1. Carefully read and understand all instructions before using Peakthe bottom of the space, upward. Thin/dry for 3 seconds using the
Universal Bond.
air/water syringe or by placing the high volume suction directly
2. For professional use only.
over the preparation.
3. Re-cap immediately following use to avoid polymerization.
v. Proceed to “Bond” step below.
4. Always verify material flow of syringe materials prior to applying
b. Total-Etch Technique:intraorally. If resistance is met, replace tip and re-check.
i. Attach a blue 22ga Endo-Eze Tip to the Ultra-Etch syringe.
5. Keep caps on the bottle until use.
ii. Start apically and fill post space coronally. Apply to coronal
6. Clinician and patient should wear UV protective eyewear when curing
preparation. Etch for 20 seconds.
resin materials.
iii. Suction off excess etchant.
7. If not used daily, refrigerate product.
iv. Using the TriAway Adaptor and 22ga Endo-Eze Tip, rinse thoroughly 8. Bring refrigerated products to room temperature before using.
and lightly air dry, leaving the post space slightly damp.
9. To optimize bond strengths use oil-free and moisture-free air.
v. Proceed to “Bond” step below.
10. Redirect overhead light to prevent premature polymerization of all resin
3. Bondbased materials.
a. Bottle Delivery
11. Resins can be sensitizing. Avoid repeated contact of uncured dental
i. Dispense 1-3 drops of Peak Universal Bond into the “B” side of theresin with skin. Do not use on patients with a known sensitivity todisposable dappen dish.
acrylates or other resins. If allergic reaction, dermatitis or rash develops,
ii. Using the Nano-Brush™ or the NaviTip FX, apply Peak Universal
consult a physician.
Bond to the post space and gently agitate the full length of the
12. Dispose of tips, empty syringes and bottles properly.
canal and tooth preparation for 10 seconds.
13. Keep out of reach of children.
iii. Thoroughly remove excess using the TriAway Adaptor and the 22ga 14. Do not use after expiration date noted on containers.
Endo-Eze Tip.
15. Re-cap, disinfect and wipe syringe with an intermediate leveliv. Air dry post space and preparation for 10 seconds using full air
disinfectant between uses. If disposable syringe cover is used, remove
pressure to thin/dry with TriAway Adapter and 22ga Endo-Eze Tip
tip, re-cap, and discard syringe cover.
to evaporate any remaining solvent from the bottom up.
16. Tips are disposable. To avoid cross-contamination, do not re-use tips.
v. Light cure down the post space for 20 seconds (40 seconds for
17. Keep products out of direct heat/sunlight.
lights with output <600mW/cm2).
18. Isolate strong chemicals to area of treatment.
vi. Use paper point or previously fitted post to verify post space is
not blocked.
NOTE: For SDS and additional information about using Peakb. Syringe Delivery
Universal Bond, Peak SE, and other related products, please go
i. Attach a 30ga NaviTip FX to the Peak Universal Bond syringe.
to www.ultradent.com
ii. Place 1-2 drops into post space and onto preparation, andthen agitate full length of the canal, including the entire toothpreparation, for 10 seconds.

3

DE

Peak™ Universal Bond und Peak™ SE

Beschreibung:Peak Universal Bond ist ein in der Flasche oder einer einzelnen Spritze gelieferter
Dental-Bonding-Kunststoff. Es kann gemäß der Self-Etch- oder Total-Etch-Technik
angewendet werden. Es ist zu 7,5 Gew.-% gefüllt, mit Äthylalkohol als Lösungsmittel
und härtet durch die meisten hochintensiven Leuchten einschließlich LEDs aus. Peak
Universal Bond enthält 0,2 % Chlorhexidin zur langfristigen Erhaltung der Bondkraft.
Peak SE Primer ist ein selbstätzendes Bondingpräparat, das aus einem Ätzmittel
und einem Primer besteht und in einer Spritze geliefert wird.
Ultra-Etch™ ist ein Ätzmittel mit 35 % Phosphorsäure in einer Spritze, für die „Etch& Rinse“-Technik.
Bei Verwendung des Zusatzes Chlorhexidin ist die Korrelation zur Reduzierung von
Sekundärkaries bei Patienten nicht nachgewiesen. Es wurden auch keine klinischenStudien zur Wirkung von Chlorhexidin auf orale Bakterien oder Karies durchgeführt.
Hinweise zum Gebrauch:
Zur Anwendungen in den Bereichen der restaurativen Zahnmedizin, bei denenÄtzmittel und Dentalkunststoffe bei Patienten jedes Alters verwendet werden.
Peak Universal Bond haftet zu den folgenden Materialien:• Dentin und Emaille• Keramik, Zirkon• Metall• Kompositzement
Gebrauchsanweisung:
HINWEIS: Bei der ersten Verwendung von PeakTM
SE ist es notwendig, die zwei in der JetMix
Spritze getrennt aufbewahrten Komponenten
zu aktivieren.
1. Peak SE ist nach der Aktivierung 120 Tageverwendbar.
2. Schreiben Sie vor der Aktivierung das
Verfallsdatum auf den flachen Bereich desSpritzenstempels.
3. ENTFERNEN SIE DIE LUER-LOCK-KAPPE NICHT VOR
DEM MISCHEN.
4. Drücken Sie den „datierten“ Spritzenstempel
schnell und kraftvoll in den mittleren Zylinder.
5. Prüfen Sie, ob der Stempel mit dem mittleren
Zylinder bündig abschließt.

4

Direkt–Bonding-Technik und Keramik-/
Zirkondioxidreparatur
1. Vorbereitunga. Dentin/Zahnschmelz: Isolieren Sie, reinigen Sie und entfernen Sie Karies.
Stellen Sie sicher, dass das gesamte demineralisierte Dentin entfernt wurde(hierzu wird Seek/Sable Seek empfohlen). Bei Abrasions-/AbfraktionsPräparationen der Kavitätenklasse V rauen Sie mit einem Diamantschleifer auf.
b. Komposit: Entfernen Sie brüchige Bereiche an vorhandenen Kompositen.
Rauen Sie die Oberfläche mit einem Diamantschleifer auf.
c. Metall: Bereiten Sie die Oberfläche durch Microabrasion vor.
d. Zirkondioxid: Reinigen Sie die Oberfläche und entfernen Sie brüchiges
Zirkondioxid mit einem Diamantschleifer.
e. Keramik: Mit einem Diamantschleifer aufrauen und brüchige Keramik
entfernen. Den Bereich der frakturierten Keramik für 5 Sekunden mit UltraEtch reinigen. Spülen und trocknen.
2. Ätzena. Self-Etch Technik – Dentin/Zahnschmelz, Komposit und Metall
i. Spülen Sie die Präparation und lassen Sie sie feucht.
ii. OPTIONAL: Tragen Sie Consepsis™ (wo verfügbar) mit einem Black
Mini™ Brush Tip mit einer bürstenden Bewegung auf die Präparation
auf und lufttrocknen Sie leicht, wobei die Oberfläche noch feucht
bleiben sollte.

iii. Tragen Sie Peak SE mit einem Black Mini Brush Tip 20 Sekunden lang
auf die Präparation auf, und massieren Sie es währenddessen in das
Dentin ein. Auf dem Zahnschmelz nur applizieren, nicht einmassieren.
iv. Verblasen/trocknen Sie 3 Sekunden lang mit dem Luftbläser, oderindem Sie die Absaugung direkt über die Präparation halten.
v. Fahren Sie mit dem Schritt „Bonding“ unten fort.
b. Total-Etch-Technik – Dentin / Zahnschmelz, Komposit und Metall
i. Farbe und Konsistenz des Produktflusses sicherstellen, indem Sie einekleine Menge auf einen Mischblock oder auf Gaze auspressen. Eventuellausgepresste klare Flüssigkeit verwerfen.
ii. Tragen Sie Ultra-Etch mit einem Blue Micro™ Tip auf alle Oberflächen
der Zahnpräparation 20 Sekunden lang auf.
iii. Spülen Sie 5 Sekunden lang gründlich.
iv. Trocknen Sie leicht mit dem Luftbläser, oder indem Sie die Absaugung
direkt über die Präparation halten. Lassen Sie die Oberfläche leicht
feucht.
v. OPTIONAL: Tragen Sie Consepsis (wo verfügbar) mit einem Black Mini
Brush Tip mit einer bürstenden Bewegung auf die Präparation auf undlufttrocknen Sie leicht, wobei die Oberfläche noch feucht bleiben sollte.
vi. Fahren Sie mit dem Schritt „Bonding“ unten fort.
c. Keramik-Ätzung: VORSICHT - Verwenden Sie eine gute Isolierung, wie zum
Beispiel eine säureneutralisierende Barriere (EtchArrest™), wenn Sie FlussSäure (HF) verwenden (Ultradent™ Porcelain Etch). Lassen Sie die Fluss-Säurenicht auf Gingiva oder Dentin gelangen.
i. Lassen Sie die Fluss-Säure auf den frakturierten Bereich 90 Sekundenlang einwirken.
ii. Saugen Sie ERST die Säure von der Oberfläche ab und spülen undtrocknen Sie dann gründlich.
iii. Lassen Sie Ultra-Etch 5 Sekunden lang einwirken, um Keramiksalze undAblagerungen der HF-Ätzung zu entfernen. Spülen und trocknen.
iv. Bringen Sie eine satte Schicht Silane auf und lassen Sie diese 60
Sekunden einwirken.
v. Gründlich trockenblasen. NICHT SPÜLEN.
vi. Fahren Sie mit dem Schritt „Bonding“ unten fort.
d. Zirkondioxid - NICHT ÄTZEN, KEIN SILAN VERWENDEN
i. Strahlen Sie die Bruchfläche des prothetischen Teils ab, spülen undtrocknen Sie dann.
ii. Tragen Sie Primer für Zirkondioxid auf den frakturierten Bereich auf,
indem Sie den Herstelleranweisungen folgen.
iii. Fahren Sie mit dem Schritt „Bonding“ unten fort.
3.Bondinga. Anwendung aus der Flasche
i. Geben Sie 1-3 Tropfen Peak™ Universal Bond auf die „B“-Seite eines
Einweg-Dappenbehälters.
ii. Verwenden Sie einen Micro Applicator Brush, um eine satte Schicht
Peak™ Universal Bond auf die Präparation aufzubringen und bewegen
Sie die Schicht 10 Sekunden lang leicht.
iii. Verblasen/trocknen Sie 10 Sekunden lang mit ¼ bis ½ Luftdruck. Die
Präparation sollte glänzen.
iv. Lichthärten Sie 10 Sekunden (20 Sekunden bei Leuchten mit einer
Leistung von <600 mW / cm2).
v. Restaurieren Sie mit fließfähigem oder plastischem Komposit, gemäß
Herstelleranweisung.
b. Anwendung aus der Spritze
i. Verwenden Sie einen Inspiral™ Brush Tip, um eine satte Schicht Peak™
Universal Bond aufzubringen und bewegen Sie die Schicht 10 Sekundenlang leicht.
ii. Verblasen/trocknen Sie 10 Sekunden lang mit ¼ bis ½ Luftdruck.
iii. Lichthärten Sie 10 Sekunden (20 Sekunden bei Leuchten mit einer
Leistung von <600 mW / cm2).
iv. Restaurieren Sie mit fließfähigem oder plastischem Komposit, gemäß
Herstelleranweisung.
Indirekt-Bonding-Techniken - Indirekte Kronen, Inlays, Onlays,
Zirkondioxid

1.Vorbereitunga. Entfernen Sie das Provisorium, reinigen und trocknen Sie die Präparation(Consepsis Scrub mit einer STARbrush™ zur Reinigung, Desinfektion und
Entfernung von Zementrückständen).
b. Stellen Sie den korrekten Sitz der Restauration sicher.
c. Bereiten Sie die Restaurations-Innenfläche vor.
i. Metallbasis:
1. Strahlen Sie die Restaurations-Innenfläche ab.
2. Oberfläche spülen und trocknen.
ii. Keramik/Porzellan:
1. Fluss-Säure (HF) (Ultradent Porcelain Etch) 90 Sekunden auf die
Restaurations-Innenfläche einwirken lassen, spülen und trocknen.
2. Lassen Sie Ultra-Etch 5 Sekunden lang einwirken, um Keramiksalze undAblagerungen der HF-Ätzung zu entfernen. Spülen und trocknen.
3. Silan (Ultradent™ Silane) 1 Minute auf die Restaurations-Innenfläche
einwirken lassen, trockenblasen und Restauration beiseite legen.
NICHT SPÜLEN.
iii. Zirkondioxid: NICHT ÄTZEN, KEIN SILAN VERWENDEN
1. Strahlen Sie die innere Oberfläche der Restauration ab, spülen undtrocknen Sie anschließend.
2. Bringen Sie einen Zirkondioxidprimer gemäß Herstelleranweisungen auf.
2.Ätzen - Vorbereitung der Zahnoberfläche
a. Self-Etch-Technik – Dentin/Zahnschmelz, Komposit und Metall
i. Spülen Sie die Präparation und lassen Sie sie feucht.
ii. OPTIONAL: Tragen Sie Consepsis (wo verfügbar) mit einem Black Mini
Brush Tip mit einer bürstenden Bewegung auf die Präparation auf undlufttrocknen Sie leicht, wobei die Oberfläche noch feucht bleiben sollte.
iii. Tragen Sie Peak™ SE mit einem Black Mini™ Brush Tip 20 Sekunden lang
auf die Präparation auf, und massieren Sie es währenddessen in das
Dentin ein. Auf den Zahnschmelz nur applizieren, nicht einmassieren.
iv. Verblasen/trocknen Sie 3 Sekunden lang mit dem Luftbläser, oder indem
Sie die Absaugung direkt über die Präparation halten.
v. Fahren Sie mit dem Schritt „Bonding“ unten fort.
b. Total-Etch-Technik – Dentin/Zahnschmelz, Komposit und Metall
i. Tragen Sie Ultra-Etch mit dem Blue Micro Tip auf alle Oberflächen derZahnpräparation 20 Sekunden lang auf.
ii. Spülen Sie 5 Sekunden lang gründlich.
iii. Trocknen Sie leicht mit dem Luftbläser, oder indem Sie die Absaugung
direkt über die Präparation halten. Lassen Sie die Oberfläche leicht
feucht.
iv. OPTIONAL: Tragen Sie Consepsis (wo verfügbar) mit einem Black Mini
Brush Tip mit einer bürstenden Bewegung auf die Präparation auf undlufttrocknen Sie leicht, wobei die Oberfläche noch feucht bleiben sollte.
v. Fahren Sie mit dem Schritt „Bonding“ unten fort.
c. Keramik-Ätzung: VORSICHT - Verwenden Sie eine gute Isolierung, wie zum
Beispiel eine säureneutralisierende Barriere (EtchArrest), wenn Sie FlussSäure (HF) verwenden (Ultradent Porcelain Etch). Lassen Sie die Fluss-Säurenicht auf Gingiva oder Dentin gelangen.
i. Lassen Sie die Fluss-Säure auf den frakturierten Bereich 90 Sekundenlang einwirken.
ii. Saugen Sie ERST die Säure von der Oberfläche ab und spülen undtrocknen Sie anschließend gründlich.
iii. Lassen Sie Ultra-Etch 5 Sekunden lang einwirken, um Keramiksalze undAblagerungen der HF-Ätzung zu entfernen. Spülen und trocknen.
iv. Bringen Sie eine satte Schicht Silan auf und lassen Sie diese 60
Sekunden einwirken.
v. Gründlich trockenblasen. NICHT SPÜLEN.
vi. Fahren Sie mit dem Schritt „Bonding“ unten fort.
d. Zirkondioxid - NICHT ÄTZEN, KEIN SILAN VERWENDEN
i. Strahlen Sie die innere Oberfläche der Restauration, spülen und trocknen
Sie dann.
ii. Bringen Sie einen Zirkondioxidprimer gemäß Herstelleranweisungen auf.
iii. Fahren Sie mit dem Schritt „Bonding“ unten fort.
3.Bondinga. Anwendung aus der Flasche
i. Geben Sie 1-3 Tropfen Peak Universal Bond auf die „B“-Seite eines
Einweg-Dappenbehälters.
ii. Verwenden Sie einen Micro Applicator Brush, um eine satte Schicht Peak

Universal Bond auf die Präparation aufzubringen und bewegen Sie sie
10 Sekunden lang leicht.
iii. Verblasen/trocknen Sie 10 Sekunden lang mit vollem Luftdruck. Die
Präparation sollte glänzend aussehen.
iv. Lichthärten Sie 10 Sekunden (20 Sekunden bei Leuchten mit einer
Leistung von <600 mW / cm²).
b. Anwendung aus der Spritze
i. Verwenden Sie einen Inspiral™ Brush Tip, um eine satte Schicht Peak™
Universal Bond aufzubringen und bewegen Sie die Schicht 10 Sekundenlang leicht.
ii. Verblasen/trocknen Sie 10 Sekunden lang mit vollem Luftdruck. Die
Präparation sollte glänzen.
iii. Lichthärten Sie 10 Sekunden (20 Sekunden bei Leuchten mit einer
Leistung von <600 mW / cm2).
4.Zementa. Verwenden Sie lichthärtenden Zement für durchscheinende Verblendschalenoder dualhärtenden Kunststoff-Zement für andere Restaurationen und folgen
Sie den Herstelleranweisungen.
NOTE: Für sofortige Dentinversiegelung die Schritte 2A und 3 der direkten
Technik oben anwenden. Glyzerin über Peak Universal Bond aufbringen und
10 Sekunden lichthärten. Glyzerin abspülen. Definitiven Abdruck erstellen.
Glyzerin wieder als Trennmedium auf die Präparation aufbringen, bevor Sie
das Provisorium einzementieren.
Reparatur von Komposit / Metall / Zirkondioxid / Keramik
1. Komposit: Entfernen Sie brüchige Bereiche des bestehenden Komposits.
Rauen Sie die Oberfläche mit einem Diamantschleifer auf.
a. Total-Etch Techniki. Tragen Sie Ultra-Etch mit dem Blue Micro Tip auf alle Oberflächen derZahnpräparation 20 Sekunden lang auf.
ii. Spülen Sie 5 Sekunden lang gründlich und lassen Sie die Fläche feucht.
2. Metall: Mikroabradieren Sie die Oberfläche
a. Total-Etch Techniki. Tragen Sie Ultra-Etch mit dem Blue Micro Tip auf alle Oberflächen derZahnpräparation 20 Sekunden lang auf.
ii. Spülen Sie 5 Sekunden lang gründlich und lassen Sie die Fläche feucht.
3. Zirkondioxid: Reinigen Sie die Oberfläche; entfernen Sie brüchiges
Zirkondioxid mit einem Diamantschleifer. NICHT ÄTZEN, KEIN SILAN
VERWENDEN.
a. Strahlen Sie die innere Oberfläche des prothetischen Teils ab.
b. Tragen Sie Primer für Zirkondioxid auf den Bruchbereich auf, indem Sie den
Herstelleranweisungen folgen.
4. Keramik: Mit einem Diamantschleifer aufrauen und brüchige Keramik
entfernen. Den Bereich der gebrochenen Keramik für 15 Sekunden mit
Ultra-Etch reinigen. Spülen und trocknen.
VORSICHT - Verwenden Sie eine gute Isolierung, wie zum Beispiel einesäureneutralisierende Barriere (EtchArrest), wenn Sie Fluss-Säure (HF)
verwenden (Ultradent Porcelain Etch). Lassen Sie die Fluss-Säure nicht auf
Gingiva oder Dentin gelangen.
a. Lassen Sie die Fluss-Säure auf die gebrochene Fläche 90 Sekunden langeinwirken.
b. Saugen Sie die Säure von der Oberfläche ab und spülen und trocknen Sieanschließend gründlich.
c. Lassen Sie Ultra-Etch 5 Sekunden lang einwirken, um Keramiksalze undAblagerungen der HF-Ätzung zu entfernen. Spülen und trocknen.
d. Bringen Sie eine satte Schicht Silan auf und lassen Sie diese 1 Minuteeinwirken.
e. Gründlich trockenblasen. NICHT SPÜLEN.
5. Bondinga. Anwendung aus der Flasche
i. Geben Sie 1-3 Tropfen Peak™ Universal Bond auf die „B“-Seite eines
Einweg-Dappenbehälters.
ii. Verwenden Sie einen Micro Applicator Brush, um eine satte Schicht
Peak™ Universal Bond aufzubringen und bewegen Sie die Schicht 10
Sekunden lang leicht.
iii. Verblasen/trocknen Sie 10 Sekunden lang mit ¼ bis ½ Luftdruck. Die
Präparation sollte glänzen.
iv. Lichthärten Sie 10 Sekunden (20 Sekunden bei Leuchten mit einer
Leistung von <600 mW / cm2).

5

6

b. Anwendung aus der Spritze
i. Verwenden Sie einen Inspiral™ Brush Tip, um eine satte Schicht Peak™
Universal Bond aufzubringen und bewegen Sie die Schicht 10 Sekundenlang leicht.
ii. Verblasen/trocknen Sie 10 Sekunden lang mit ¼ bis ½ Luftdruck.
iii. Die Präparation sollte glänzen.
iv. Lichthärten Sie 10 Sekunden (20 Sekunden bei Leuchten mit einer
Leistung von <600 mW / cm2).
6. Restaurieren Sie mit fließfähigem und/oder plastischem Komposit gemäß
Herstelleranweisung.
Wurzelstift und Stumpfaufbau
1.Vorbereitunga. Bohren Sie das Loch für einen Wurzelstift, indem Sie einen UniCore™ Bohrer
der richtigen Größe mit Gummistop einsetzen.
b. Spülen Sie das Bohrloch für 10 Sekunden mit dem TriAway-Adapter undeinem 22ga Endo-Eze™ Tip. Trocknen Sie mit dem TriAway Adapter und einem
22ga Endo-Eze Tip vom Boden der Präparation nach oben.
c. Kontrollieren Sie den Sitz des Stifts (UniCore Post) und kürzen Sie ihn auf die
gewünschte Länge mit einer Diamantscheibe ein. HINWEIS: Hartmetall- undDiamantschleifer können die Fasern ausfransen.
2.Ätzena. Self-Etch Techniki. Spülen Sie den Kanal und lassen Sie ihn feucht.
ii. Setzen Sie einen blauen 22ga Deliver-Eze™ Brush Tip auf die Peak
SE-Spritze.
iii. Bringen Sie es in das Bohrloch ein und auf die koronale Präparation auf,
während 20 Sekunden, mit einer einmassierenden Bewegung.
iv. Blasen Sie Überschuss mit dem TriAway-Adapter und einem 22ga EndoEze Tip vom Boden der Präparation nach oben aus. Verblasen/trocknen
Sie 3 Sekunden lang mit dem Luftbläser, oder indem Sie die Absaugung
direkt über die Präparation halten.
v. Fahren Sie mit dem Schritt „Bonding“ unten fort.
b. Total-Etch Technik:
i. Setzen Sie einen blauen 22ga Endo-Eze Tip auf die Ultra-Etch-Spritze.
ii. Beginnen Sie apikal und füllen Sie das Stiftloch bis koronal. Bringen Sie
es auch auf die koronale Präparation auf. Ätzen Sie 20 Sekunden.
iii. Saugen Sie überschüssiges Ätzmittel ab.
iv. Spülen und lufttrocknen Sie das Bohrloch leicht mit dem Triway-Adapter
und einem 22ga Endo-Eze™ Tip, und lassen Sie das Bohrloch leicht
feucht.
v. Fahren Sie mit dem Schritt „Bonding“ unten fort.
3.Bondinga. Anwendung aus der Flasche
i. Geben Sie 1-3 Tropfen Peak Universal Bond auf die „B“-Seite eines
Einweg-Dappenbehälters.
ii. Bringen Sie Peak Universal Bond mittels eines Nano-Brush™ odereines NaviTip FX in das Stiftloch ein und bewegen Sie es sanft in derGesamtlänge des Kanals und der Zahnpräparation für 10 Sekunden.
iii. Entfernen Sie überschüssiges Material gründlich mit dem TriAwayAdapter und einem 22ga Endo-Eze Tip.
iv. Verblasen/trocknen Sie die äußere Präparation 10 Sekunden lang mit ¼
bis ½ Luftdruck. Die Präparation sollte glänzend aussehen.
v. Lichthärten Sie für 20 Sekunden in das Stiftloch (40 Sekunden bei
Leuchten mit einer Leistung von <600 mW / cm²).
vi. Benutzen Sie Papierspitzen oder den vorher eingepassten Stift, um
sicherzugehen, dass der Kanal nicht blockiert ist.
b. Anwendung aus der Spritze
i. Setzen Sie einen 30ga NaviTip FX auf die Peak™ Universal Bond Spritze auf.
ii. Tropfen Sie 1-2 Tropfen in das Stiftloch und auf die Präparation undbewegen Sie die Flüssigkeit 10 Sekunden lang in der gesamten Länge
des Kanals und auf der Zahnpräparation.
iii. Entfernen Sie überschüssiges Peak™ Universal Bond gründlich mit dem
TriAway-Adapter und dem 22ga Endo-Eze Tip.
iv. Lufttrocknen/verblasen Sie im Stiftloch und auf der Präparation bei
vollem Luftdruck mit dem TriAway-Adapter und dem 22ga Endo-Eze
Tip, um das gesamte verbliebene Lösungsmittel von unten herauf zu
verdunsten.
v. Lichthärten Sie für 20 Sekunden in das Stiftloch (40 Sekunden bei

Leuchten mit einer Leistung von <600 mW / cm2). Benutzen Sie
Papierspitzen oder den vorher eingepassten Stift, um sicherzugehen,dass der Kanal nicht blockiert ist.
Stiftbefestigung und Stumpfaufbau
1. Entfernen Sie die Kappe der PermaFlo™ DC Spritze.
2. Stecken Sie einen Mixing Tip auf die Doppelkolbenspritze, indem Sie die zweiÖffnungen entsprechend ausrichten. Drehen Sie im Uhrzeigersinn, bis sie
eingerastet sind.
3. Setzen Sie den flexiblen Intraoral Tip™ auf den Mixing Tip, um von der
Doppelkolbenspritze direkt in den Kanal zu applizieren.
4. Pressen Sie eine kleine Menge heraus, bevor Sie in den Bereich des Stifts
gehen.
5. Führen Sie den Tip in das Bohrloch bis ganz ans Ende ein.
6. Pressen Sie PermaFlo DC mit gleichmäßigem Druck von apikal beginnend aus
und bewegen Sie sich Richtung koronal.
7. Führen Sie den Stift (UniCore™ Post) ein und lassen Sie den überschüssigen
Zement entweichen.
8. Lichthärten Sie für 20 Sekunden direkt über dem Stift (40 Sekunden bei
Leuchten mit einer Leistung von <600 mW / cm2).
9. Fahren Sie fort, PermaFlo™ DC-Schichten um den Stift herum aufzubauen,
wie es nötig ist. HINWEIS: Lichthärten Sie für 5 Sekunden zwischen den
Schichten, um den Stumpf zu fixieren und zu formen. Führen Sie eine 40
Sekunden lange Endhärtung des Stumpfaufbaus durch. Entfernen Sie den
Mixing Tip bis zur nächsten Anwendung nicht. Desinfizieren Sie Spritze und
Mixing Tip.
Warnungen und Vorsichtsmaßnahmen:
1. Vor der Anwendung von Peak Universal Bond müssen alle Anweisungensorgfältig gelesen und verstanden werden.
2. Nur zur zahnärztlichen Anwendung.
3. Sofort nach der Benutzung wiederverschließen, um Polymerisation zu
verhindern.
4. Stellen Sie den stets korrekten Fluss der Materialien aus der Spritze sicher,bevor Sie intraoral arbeiten. Wenn Sie Widerstand spüren, ersetzen Sie den
Spritzenansatz und prüfen Sie nochmals.
5. Halten Sie die Flaschen bis zur nächsten Benutzung verschlossen.
6. Zahnarzt und Patient sollten während der Lichthärtung der Kunststoffe
UV-Augenschutz tragen.
7. Falls die Materialien nicht täglich benutzt werden, kühl lagern.
8. Gekühlte Produkte vor der Benutzung auf Raumtemperatur bringen.
9. Für optimale Bondkräfte ölfreie und trockene Luft einsetzen.
10. Operationsleuchte so abblenden, dass eine vorzeitige Polymerisation aller
Kunststoffmaterialien verhindert wird.
11. Dentalkunststoffe können sensibilisieren. Vermeiden Sie wiederholten
Hautkontakt von nicht ausgehärtetem Dentalkunststoff. Nicht bei
Patienten verwenden, bei denen eine Sensibilität auf Acrylate oder andere
Dentalkunststoffe bekannt ist. Falls allergische Reaktionen, Dermatitis oder ein
Hautausschlag auftreten, suchen Sie einen Arzt auf.
12. Entsorgen Sie benutzte Spritzenansätze, leere Spritzen und Flaschensachgerecht.
13. Außerhalb der Reichweite von Kindern aufbewahren.
14. Nicht nach dem auf den Behältern aufgedruckten Verfallsdatum benutzen.
15. Die Spritze wieder verschließen und zwischen den Anwendungen mit einem
Oberflächendesinfektionsmittel abwischen und desinfizieren. Falls eine
Einweg-Spritzenhülle verwendet wird, entfernen Sie den Spritzenansatz, setzen
Sie die Kappe wieder auf und entsorgen Sie die Spritzenhülle.
16. Die Spritzenansätze sind Einwegartikel. Um Kreuzkontaminierung zu
vermeiden, benutzen Sie gebrauchte Ansätze nicht erneut.
17. Die Produkte vor direkter Sonneneinstrahlung und Hitze schützen.
18. Beschränken Sie den Einfluss starker Chemikalien auf den
Behandlungsbereich.
HINWEIS: Materialsicherheitsdatenblätter und zusätzliche
Informationen über den Einsatz von Peak™ Universal Bond, Peak™ SE
und anderen damit zusammenhängenden Produkten finden Sie auf
www.ultradent.com

Peak™ Universal Bond et Peak™ SE
Description:
Peak Universal Bond est une résine adhésive appliquée en flacon ou en
seringue. Il peut être utilisée en technique MR2 avec un mordançage total (nousvous recommandons Ultra-Etch ) ou en technique SAM2 avec un primer, utilisé
Peak SE. Il est chargée à 7,5%, contient un solvent à base d’alcool éthylique et se
photopolymérisera avec la plupart des lampes de haute intensité, y compris leslampes LED. Peak Universal Bond contient de la chlorhexidine à 0,2% qui peut
assurer la pérennité de l’adhésion à long terme.
Le primer Peak SE est une résine d’adhésion à la dentine auto-mordançante qui
est composée d’un acide mordançant et d’un primer dans un système d’application
en seringue.
Ultra-Etch™ est un agent de mordançage à l’acide phosphorique à 35%.
L’inclusion de l’additif chlorhexidine n’a pas montré avoir une corrélation avec une
réduction secondaire des caries chez les patients. Aucuneétude clinique pour l’évaluation des effets de la chlorhexidine sur les bactéries ou
les caries orales n’a été faite.
Indications d’emploi :Utilisez-le pour la quasi-totalité de vos besoins de mordançage et de collage endentisterie restauratrice chez les patients de tout âge.
Peak Universal Bond adhère aux matériaux suivants :• Dentine et émail
• La porcelaine et le zircon• Métal• Composite
Mode d’emploi :NOTE : L’utilisation initiale du Peak SE nécessite
l’activation des deux composants séparés dansla seringue JetMixTM.
1. Peak SE est stable pendant 120 jours après
l’activation.
2. Ecrivez la date limite d’utilisation sur la partie
plate du piston avant l’activation.
3. N’ENLEVEZ PAS LE CAPUCHON LUER LOCK AVANT
LE MELANGE.
4. Appuyez rapidement et avec force sur le piston“daté” dans le cylindre central.
5. Vérifiez que le piston est enfoncé à fond dans lecylindre central.
Adhésion direct et réparation de la porcelaine/ la zircone
1.Préparera. La dentine/l’émail : Isolez, nettoyez et enlevez
la carie pour assurer que toute la dentine
non-minérale est éliminée (Seek/Sable Seek
est recommandé dans ce cas). Pour l’abrasion des préparations de classe V,
fraisez avec une fraise diamantée.
b. Composite : Retirez les zones fragilisées de composite existant. fraisez lasurface avec une fraise diamantée.
c. Métal : abrasez la surface.
d. Zircone : Nettoyez la surface et enlevez la zircone affaiblie avec une fraisediamantée.
e. Porcelaine : Avivez et enlevez la porcelaine affaiblie avec une fraisediamantée. Nettoyez la zone de la porcelaine fracturée pendant 5 secondes
avec l’Ultra-Etch. Rincez et séchez.
2. Mordançagea. Technique d’auto- mordançage – sur la dentine/l’émail, le composite etle métali. Rincez la préparation et laissez-la humide.
ii. OPTIONNEL – Appliquez Consepsis™ (selon la disponibilité) avec

FR

un embout pinceau Black Mini Brush sur la préparation avec un
mouvement de frottement et séchez légèrement à l’air en laissant lasurface humide.
iii. Appliquez Peak SE avec l’embout pinceau sur la préparation de la
dent pendant 20 secondes en frottant continuellement sur la dentine.
n’appliquez pas sur l’émail.
iv. Etalez/séchez pendant 3 secondes à l’aide de la seringue air/eau ou en
plaçant l’aspiration à grand volume directement sur la préparation.
v. Continuez avec l’étape « Adhésion » ci-dessous.
b. Technique de mordançage total – sur la dentine/l’émail, le composite etle métali. Vérifiez la couleur et la consistance de l’écoulement du produit avant del’appliquer en exprimant une petite quantité sur un bloc de mélangeou sur de la gaze. Jetez tout liquide clair qui est exprimé.
ii. Appliquez Ultra-Etch avec l’embout Blue Micro™ sur toutes les surfaces
de la préparation de la dent pendant 20 secondes.
iii. Rincez abondamment pendant 5 secondes.
iv. Etalez/séchez à l’aide de la seringue air/eau ou en plaçant l’aspiration
à grand volume directement sur la préparation. Laissez la surface
légèrement humide.
v. OPTIONNEL – Appliquez Consepsis (selon la disponibilité) avec
un embout pinceau Black Mini Brush sur la préparation avec un
mouvement de frottement et séchez légèrement à l’air en laissant lasurface humide.
vi. Continuez avec l’étape « Adhésion » ci-dessous.
c. Mordançage sur porcelaine – ATTENTION – utilisez l’isolation appropriéetelle qu’une barrière de neutralisation des acides (EtchArrest™) lors del’utilisation d’acide fluorhydrique (Ultradent™ Porcelain Etch). Ne laissez pas
l’acide fluorhydrique toucher la gencive ni la dentine.
i. Appliquez l’acide fluorhydrique sur la zone fracturée pendant 90
secondes.
ii. Aspirez l’acide de la surface PUIS rincez soigneusement et séchez.
iii. Appliquez l’Ultra-Etch pendant 5 secondes pour enlevez les selsde porcelaine et les débris formés par le mordançage à l’acide
flurohydrique. Rincez et séchez.
iv. Appliquer le silane pendant 60 secondes.
v. Séchez soigneusement. NE RINCEZ PAS.
vi. Continuez avec l’étape « Adhésion » ci-dessous.
d. Zircone – NE PAS MORDANCER NI UTILISER DE SILANE
i. Faites une micro abrasion sur la surface fracturée de la prothèse,
rincez et séchez.
ii. Appliquez le primer zircone sur la zone fracturée en suivant les
instructions du fabricant.
iii. Continuez avec l’étape « Adhésion » ci-dessous.
3. Adhésion
a. Application en flacon
i. Déposez 1 à 3 gouttes de Peak™ Universal Bond dans le côté “B” d’ungodet Dappen jetable.
ii. A l’aide du Micro Applicator Brush, appliquez une couche épaisse de
Peak Universal Bond sur la préparation et frottez doucement pendant
10 secondes.
iii. Etalez/séchez pendant 10 secondes en utilisant ¼ à ½ de pression
d’air. La préparation devrait avoir un aspect brillant.
iv. Photopolymérisez pendant 10 secondes (20 secondes pour les lampes
ayant une puissance de sortie <600mW/cm2).
v. Restaurez avec un composite fluide ou condensable selon les
instructions du fabricant.
b. Application par seringue
i. Appliquez une couche épaisse de Peak™ Universal Bond à l’aide del’embout Inspiral™ Brush, frottez doucement pendant 10 secondes.
ii. Etalez/séchez pendant 10 secondes en utilisant ¼ à ½ de pression
d’air. La préparation devrait avoir un aspect brillant.
iii. Photopolymérisez pendant 10 secondes (20 secondes pour les lampes
ayant une puissance de sortie <600mW/cm2).
iv. Restaurez avec un composite fluide ou condensable selon les

7

8

instructions du fabricant.
Technique adhésion indirecte - Couronnes indirectes, inlays, onlays,
Zircone1.Préparera. Retirez les restauration temporaires, nettoyez la préparation, rincez et séchez
(Consepsis Scrub avec une brossette STARbrush™ pour nettoyer, désinfecter,et retirer le ciment résiduel).
b. Vérifiez l’ajustement de la prothèse.
c. Préparez l’intrados de la prothèse.
i. A base de métal:1. Micro-abrasez (sablez) l’intrados de la prothèse.
2. Rincez et séchez la surface.
ii. Céramique/porcelaine:
1. Appliquez l’acide fluorhydrique (Ultradent Porcelain Etch) sur l’intradosde la prothèse pendant 90 secondes, rincez et séchez.
2. Appliquez l’Ultra-Etch pendant 5 secondes pour enlevez les selsde porcelaine et les débris formés par le mordançage à l’acide
fluorhydrique. Rincez et séchez.
3. Appliquez le silane (Ultradent™ Silane) sur l’intrados de la prothèse
pendant 1 minute, séchez et mettez la prothèse de côté. Ne rincez
pas.
iii. Zircone : NE PAS MORDANCER NI UTILISER DE SILANE
1. Abrasez à l’air l’intrados de la prothèse, rincez et séchez.
2. Appliquez le primer Zircone selon les instructions du fabricant.
2.Mordancer - Préparer la surface de la dent
a. Technique d’auto- mordançage – sur la dentine/l’émail, le composite et lemétal
i. Rincez la préparation et laissez-la humide.
ii. OPTIONNEL – Appliquez Consepsis (selon la disponibilité) avec
un embout pinceau Black Mini Brush sur la préparation avec un
mouvement de frottement et séchez légèrement à l’air en laissant lasurface humide.
iii. Appliquez Peak™ SE avec l’embout pinceau Black Mini Brush sur la
préparation de la dent pendant 20 secondes en frottant continuellement
sur la dentine. Ne frottez pas l’émail.
iv. Etalez/séchez pendant 3 secondes à l’aide de la seringue air/eau ou en
plaçant l’aspiration à grand volume directement sur la préparation.
v. Continuez avec l’étape « Adhésion » ci-dessous.
b. Technique de mordançage total – sur la dentine/l’émail, le composite etle métali. Appliquez Ultra-Etch avec l’embout Blue Micro sur toutes les surfaces dela préparation de la dent pendant 20 secondes.
ii. Rincez abondamment pendant 5 secondes.
iii. Séchez légèrement à l’aide de la seringue air/eau ou en plaçantl’aspiration à grand volume directement sur la préparation. Laissez lasurface légèrement humide.
iv. OPTIONNEL – Appliquez Consepsi™ (selon la disponibilité) avec
un embout pinceau Black Mini Brush sur la préparation avec un
mouvement de frottement et séchez légèrement à l’air en laissant lasurface humide.
v. Continuez avec l’étape « Adhésion » ci-dessous.
c. Mordançage sur porcelaine – ATTENTION – utilisez l’isolation appropriée telle
qu’une barrière de neutralisation des acides (EtchArrest) lors de l’utilisationd’acide fluorhydrique (FH) (Ultradent Porcelain Etch). Ne laissez pas l’acide
fluorhydrique toucher la gencive ni la dentine.
i. Appliquez l’acide fluorhydrique sur la zone fracturée pendant 90
secondes.
ii. Aspirez l’acide de la surface PUIS rincez soigneusement et séchez.
iii. Appliquez l’Ultra-Etch pendant 5 secondes pour enlevez les sels deporcelaine et les débris formés par le décapage au FH. Rincez et séchez.
iv. Appliquer le silane pendant 60 secondes.
v. Séchez soigneusement. NE RINCEZ PAS.
vi. Continuez avec l’étape « Adhésion » ci-dessous.
d. Zircone – NE PAS MORDANCER NI UTILISER DE SILANE
i. Abrasez à l’air l’intrados de la prothèse, rincez et séchez.
ii. Appliquez l’apprêt zircone sur la zone fracturée en suivant les
instructions du fabricant.
iii. Continuez avec l’étape « Adhésion » ci-dessous.

3.Adhésion
a. Application en flacon
i. Déposez 1 à 3 gouttes de Peak Universal Bond dans le côté “B” d’ungodet Dappen jetable.
ii. Avec l’applicateur Micro Applicator Brush, appliquez Peak Universal
Bond sur la préparation et agitez doucement pendant 10 secondes.
iii. Etalez/séchez pendant 10 secondes en utilisant toute la pression d’air
disponible. La préparation devrait avoir un aspect brillant.
iv. Photopolymérisez pendant 10 secondes (20 secondes pour les lampes
ayant une puissance de sortie <600mW/cm2).
b. Application par seringue
i. Appliquez une couche épaisse de Peak Universal Bond à l’aide del’embout Inspiral™ Brush, frottez doucement pendant 10 secondes.
ii. Etalez/séchez pendant 10 secondes en utilisant toute la pression d’air
disponible. La préparation devrait avoir un aspect brillant.
iii. Photopolymérisez pendant 10 secondes (20 secondes pour les lampes
ayant une puissance de sortie <600mW/cm2).
4.Cimenta. Appliquez un ciment photopolymérisable pour les facettes translucides ou
un ciment Dual-cure à base de résine sur les autres prothèses et suivez les
instructions du fabricant pour l’utilisation.
NOTE: Le scellement immédiat de la dentine requiert les étapes detechnique directe 2A et 3 ci-dessus. Appliquez de la glycérine sur Peak
Universal Bond et photopolymérisez pendant 10 secondes. Rincez laglycérine. Prenez l’empreinte finale. Appliquez de nouveau de la glycérine
sur la préparation avant de sceller la restauration temporaire en place.
Réparation of Composite / Métal / Zircone / Porcelaine
1. Composite : Retirez les zones fragilisées de composite existant. Avivez lasurface avec une fraise diamantée.
a. Technique Total-Etch
i. Appliquez Ultra-Etch avec Blue Micro Tip sur toutes les surfaces de la
préparation de la dent pendant 20 secondes.
ii. Rincez abondamment pendant 5 secondes et laissez humide.
2. Métal : Micro-abrasez la surface.
a. Technique Total-Etch
i. Appliquez Ultra-Etch avec Blue Micro Tip sur toutes les surfaces de la
préparation de la dent pendant 20 secondes.
ii. Rincez abondamment pendant 5 secondes et laissez humide.
3. Zircone : Nettoyez la surface et enlevez la zircone affaiblie avec une fraisediamantée. NE PAS MORDANDER NI UTILISER DE SILANE.
a. Abrasez à l’air l’intrados de la prothèse, rincez et séchez.
b. Appliquez le primer zircone sur la zone fracturée en suivant les instructions
du fabricant.
4. Porcelaine : Avivez et enlevez la porcelaine affaiblie avec une fraise diamantée.
Nettoyez la zone de la porcelaine fracturée pendant 15 secondes avec l’UltraEtch. Rincez et séchez.
ATTENTION – utilisez l’isolation appropriée telle qu’une barrièrede neutralisation des acides (EtchArrest) lors de l’utilisation d’acide
fluorhydrique (FH) (Ultradent™ Porcelain Etch). Ne laissez pas l’acide
fluorhydrique toucher la gencive ni la dentine.
a. Appliquez l’acide fluorhydrique sur la zone fracturée pendant 90 secondes.
b. Aspirez l’acide de la surface puis rincez soigneusement et séchez la surface.
c. Appliquez l’Ultra-Etch pendant 5 secondes pour enlevez les résidus deporcelaine et les débris formés par le mordançage à l’acide flurohydrique.
Rincez et séchez.
d. Appliquer une couche épaisse de silane pendant 1 secondes.
e. Séchez soigneusement. NE RINCEZ PAS.
5. Adhésion
a. Application par flacon
i. Déposez 1 à 3 gouttes de Peak™ Universal Bond dans le côté “B” d’ungodet Dappen jetable.
ii. A l’aide du Micro Applicator Brush, appliquez une couche épaisse de
Peak™ Universal Bond sur la préparation et frottez doucement pendant
10 secondes.
iii. Etalez/séchez pendant 10 secondes en utilisant ¼ à ½ de pression d’air.
La préparation devrait avoir un aspect brillant.
iv. Photopolymérisez pendant 10 secondes (20 secondes pour les lampes

ayant une puissance de sortie <600mW/cm2).
b. Application par seringue
i. Appliquez une couche épaisse de Peak™ Universal Bond à l’aide del’embout pinceau Inspiral™, frottez doucement pendant 10 secondes.
ii. Etalez/séchez pendant 10 secondes en utilisant ¼ à ½ de pression d’air.
iii. La préparation devrait avoir un aspect brillant.
iv. Photopolymérisez pendant 10 secondes (20 secondes pour les lampes
ayant une puissance de sortie <600mW/cm2).
6. Restaurez avec un composite fluide et/ou condensable selon les instructions
du fabricant.
Tenon radiculaire coulé
1. Préparera. Forez à l’aide d’une butée en caoutchouc et d’un foret UniCore™ de tailleappropriée.
b. Rincez soigneusement la preparation canalaire pendant 10 secondes enutilisant un adaptateur TriAway et un embout EndoEze™ de 22ga. Séchez
avec l’adaptateur TriAway et l’embout Endo-Eze 22ga depuis le fond de la
préparation en remontant vers le haut.
c. Vérifiez l’ajustement du tenon (tenon Unicore) et coupez-le à la longueur
souhaitée à l’aide d’un disque diamanté à haute vitesse. NOTE: Les fraises au
carbure et opératoires peuvent faire effilocher les fibres.
2. Mordançagea. Technique d’auto-mordançagei. Rincez le logement de tenon et laissez-le humide.
ii. Fixez un embout pinceau bleu Deliver-Eze™ 22 ga sur la seringue
Peak SE.
iii. Appliquez le primer dans la preparation canalaire et sur la préparation
coronaire pendant 20 secondes avec un mouvement de va-et-vient.
iv. Séchez l’excès avec l’adaptateur TriAway et l’embout Endo-Eze 22ga
depuis le fond en remontant vers le haut. Etalez/séchez pendant 3
secondes à l’aide de la seringue air/eau ou en plaçant l’aspiration à
grand volume directement sur la préparation.
v. Continuez avec l’étape « Adhésion ci-dessous.
b. Technique de mordançage total:
i. Fixez un embout bleu Endo-Eze 22 ga sur la seringue Ultra-Etch.
ii. Commencez à l’apex et remplissez la preparation canalaire en faisantdes cercles. Appliquez sur la préparation coronaire. Mordancez pendant
20 secondes.
iii. Aspirez l’excédent de mordançage.
iv. A l’aide de l’adapteur TriAway et de l’embout EndoEze™ de 22ga, rincez
soigneusement et séchez légèrement à l’air, en laissant la preparation
canalaire légèrement humide.
v. Continuez avec l’étape « Adhésion » ci-dessous.
3. Adhésion
a. Application en flacon
i. Déposez 1 à 3 gouttes de Peak Universal Bond dans le côté “B” d’ungodet Dappen jetable.
ii. A l’aide de la Nano-Brush™ ou du FX NaviTip, appliquez Peak Universal
Bond dans la preparation canalaire et agitez doucement sur toute lalongueur du canal et de la préparation de la dent pendant 10 secondes.
iii. Retirez soigneusement tout excès à l’aide de l’ adaptateur TriAway et del’embout EndoEze™ de 22ga.
iv. Séchez l’espace canalaireet la préparation à l’air pendant 10 secondes
en utilisant toute la pression de l’air pour diluer/sécher à l’aide del’adaptateur TriAway etde l’embout Endo-Eze 22ga pour évaporer tout
solvant à l’extrémité du logement de tenon.
v. Photopolymérisez dans la preparation canalaire pendant 20 secondes(40 secondes pour les lampes ayant une puissance de sortie <600mW/
cm2).
vi. Utilisez une pointe de papier ou un tenon ajusté préalablement pourvérifier la preparation canalaire est libre tout obstacle.
b. Application par seringue
i. Fixez un embout NaviTip FX 30ga à la seringue Peak™ Universal Bond.
ii. Mettez 1 à 2 gouttes dans le logement du tenon et sur la préparation,
puis agiter toute la longueur du canal, y compris l’entière préparationde la dent, pendant 10 secondes.
iii. Retirez soigneusement tout excès de Peak™ Universal Bond à l’aide del’adaptateur TriAway et de l’embout EndoEze™ 22ga.

iv. Séchez le logement et la préparation à l’air pendant 10 secondes
en utilisant toute la pression de l’air pour diluer/sécher à l’aide del’adaptateur TriAway etde l’embout Endo-Eze 22ga pour évaporer tout
solvant à l’extrémité du logement de tenon.
v. Photopolymérisez dans le logement du tenon pendant 20 secondes (40secondes pour les lampes ayant une puissance de sortie <600mW/cm2).
Utilisez une pointe de papier ou un tenon ajusté préalablement pourvérifier que l’espace du tenon n’est pas bloqué.
Scellement du tenon reconstruction de moignon
1. Retirez le capuchon de la seringue PermaFlo™ DC.
2. Mettez un embout mélangeur sur la seringue double en alignant avec lesdeux sorties. Tournez dans le sens des aiguilles d’une montre jusqu’ auverrouillage.
3. Fixez l’embout flexible Intraoral™ sur l’embout mélangeur pour une application
directe dans le canal depuis la seringue double.
4. Délivrez une petite quantité avant de l’appliquer dans la preparation canalaire.
5. Insérez l’embout dans la preparation canalaire sur toute la longueur.
6. En utilisant une pression régulière appliquez le PermaFlo DC en commençant
à l’apex puis en faisant des cercles.
7. Insérez le tenon UniCore™ lentement, en déplaçant l’excédent de ciment.
8. Placez la lampe à polymériser directement au-dessus du tenon etphotopolymérisez pendant 20 secondes (40 secondes pour les lampes ayant
une puissance de sortie <600mW/cm2).
9. Superposez des couches de PermaFlo™ DC autour du tenon selon les besoins.
NOTE : Photopolymérisez pendant 5 secondes entre chaque couche deproduit pour former le moignon. Faites une dernière photopolymérisationde 40 secondes sur le tenon. Ne retirez pas l’embout mélangeur jusqu’à
l’utilisation suivante. Désinfectez la seringue et l’embout mélangeur.
Précautions et avertissements :1. Lisez et comprenez toutes les instructions avant d’utiliser le Peak Universal
Bond.
2. Destiné à un usage professionnel uniquement.
3. Rebouchez immédiatement après utilisation pour éviter une polymérisation.
4. Vérifiez toujours l’écoulement du matériau sortant de la seringue avant del’appliquer en bouche. En cas de résistance, remplacez l’embout et revérifiez.
5. Gardez les bouchons sur le flacon jusqu’à utilisation.
6. Le clinicien et le patient doivent porter des lunettes de protection contre lesUV pendant la polymérisation des résines.
7. S’il n’est utilisé quotidiennement, réfrigérez le produit.
8. Portez les produits réfrigérés à la température ambiante avant de les utiliser.
9. Pour optimiser les forces d’adhésion, utilisez de l’air sans huile et sec.
10. Evitez la lumière du scialytique pour éviter une polymérisation prématuréedes matériaux à base de résine.
11. Les résines peuvent provoquer une sensibilisation. Evitez un contact répété
entre la peau et la résine dentaire non polymérisée. Ne pas utiliser sur despatients ayant une sensibilité connue aux acrylates et autres résines. Si uneréaction allergique, une dermatite ou une éruption cutanée se développe,
consultez un médecin.
12. Jetez les embouts usagés, les seringues et les flacons vides de façon
appropriée.
13. Tenir hors de portée des enfants.
14. Ne pas utiliser après la date de péremption notée sur les récipients.
15. Rebouchez, désinfectez et essuyez les seringues avec un désinfectant deniveau intermédiaire entre chaque utilisation. Si un protège-seringue jetable
est utilisé, retirez l’embout, rebouchez et jetez le protège-seringue.
16. Les embouts sont jetables. Pour éviter la contamination croisée, ne réutilisez
pas les embouts.
17. Gardez ces produits à l’écart de la chaleur/de la lumière directe du soleil.
18. Isolez les produits chimiques forts sur la zone de traitement.
NOTE : Pour la FDS et des renseignements supplémentaires surl’utilisation du Peak Universal Bond, du Peak SE et autres produits
connexes, veuillez visiter www.ultradent.com
9

NL

Peak™ Universal Bond en Peak™ SE

Beschrijving:
Peak Universal Bond is een hechthars die vanuit een fles of één spuit wordt
afgegeven. Het kan met een zelfetsend middel of met een totaal etsmiddel
worden gebruikt. Het is 7,5% gevuld met een ethylalcoholdrager en hardt
uit met alle hoogwaardige uithardingslampen inclusief LED’s. Peak Universal
Bond bevat 0,2% chloorhexidine, dat voor een langdurige hechtsterkte kan
zorgen.
Peak SE Primer is een zelfetsende dentinehechthars bestaande uit een
etsmiddel en een primer die in een spuitsysteem worden geleverd.
Ultra-Etch™ is een in een spuit geleverde ets- en spoelgel bestaande uit 35%
fosforzuur.
De toevoeging van chloorhexidine heeft geen aantoonbare correlatie met
een verlaging van secundaire cariës bij patiënten. Er zijn geen klinische
onderzoeken verricht naar de gevolgen van chloorhexidine op mondbacteriën
of cariës.
Indicaties voor gebruik:
Geschikt voor vrijwel alle ets- en bondingtechnieken in de restauratieve
tandheelkunde voor alle leeftijden.
Peak Universal Bond hect zich aan de volgende materialen:• Dentine en tandglazuur• Porselein, zirkoniumoxide• Metaal• Composiet
Gebruiksaanwijzing:
NB: Voordat Peak SE kan worden gebruikt, moeten de twee
gescheiden componenten in de JetMixTM-spuit worden geactiveerd.
1. Peak SE is 120 dagen na activering stabiel.
2. Noteer vóór activering de uiterste
gebruiksdatum op het platte gedeelte van deplunjersteel.
3. VERWIJDER DE LUER LOCK-DOP NIET VÓÓRHET MENGEN
4. Druk de “gedateerde” plunjer snel en stevig inde middelste patroon.
5. Controleer of de plunjer op één lijn ligt met demiddelste patroon.
Directe bondingtechniek en reparatie vanporselein/zirkoniumoxide
1.Preparerena. Dentine/tandglazuur: Isoleer, reinig en
verwijder cariës en zorg dat alle niet-minerale
dentine is verwijderd (Seek/Sable Seek
wordt daarvoor aangeraden). Voor abrasie-/abfractiepreparaties van klasse V moeten
oppervlakken met een diamantfrees worden
opgeruwd.
b. Composiet: Verwijder de verzwakte delen van
het bestaande composiet. Ruw het oppervlak
op met een diamantfrees.
c. Metaal: Pas microabrasie toe op het oppervlak.
d. Zirkoniumoxide: Reinig het oppervlak en verwijder het verzwakte
zirkoniumoxide met een diamantfrees.
e. Porselein: Ruw het oppervlak op en verwijder het verzwakte porselien
met een diamantfrees. Reinig het porseleingedeelte met de fractuur
gedurende 5 seconden met Ultra-Etch. Spoel en droog.
2. Etsena. Zelfetsende techniek – dentine/tandglazuur, composiet en metaal
i. Spoel de preparatie en laat deze vochtig.
ii. OPTIE - Breng Consepsis™ (indien beschikbaar) met de Black Mini™
10

Brush Tip aan op de preparatie met een wrijvende beweging en
droog deze lichtjes met lucht zodat de preparatie iets vochtig
blijft.
iii. Breng Peak SE met de Black Mini Brush Tip gedurende 20 seconden
aan op de tandpreparatie en wrijf het rond op het dentine. Wrijf het
tandglazuur niet.
iv. Verdun/droog het gedurende 3 seconden met een lucht-/waterspuitof een krachtige afzuiging direct over de preparatie.
v. Ga door met de stap “Bonding” (zie hieronder).
b. Totale etstechniek – dentine/tandglazuur, composiet en metaal
i. Controleer vóór gebruik de kleur en consistentie van deproductstroom door een kleine hoeveelheid op een mengplaatje
of gaasje uit te drukken. Gooi alle uitgedrukte, transparantevloeistof weg.
ii. Breng Ultra-Etch met de Blue Micro™ Tip gedurende 20 seconden
aan op alle oppervlakken van de tandpreparatie.
iii. Spoel grondig gedurende 5 seconden.
iv. Verdun/droog het met een lucht-/waterspuit of een krachtige
afzuiging direct over de preparatie. Laat het oppervlak licht vochtig.
v. OPTIE - Breng Consepsis (indien beschikbaar) met de Black Mini
Brush Tip aan op de preparatie met een wrijvende beweging en
droog deze lichtjes met lucht zodat de preparatie iets vochtig blijft.
vi. Ga door met de stap “Bonding” (zie hieronder).
c. Porseleinets – VOORZICHTIG – Gebruik een goede isolatie zoals een
zuurneutraliserende barrière (EtchArrest™) als u fluorwaterstofzuur (HF)
(Ultradent™ Porcelain Etch) gebruikt. Voorkom dat het fluorwaterstofzuur
de gingiva of het dentine raakt.
i. Breng gedurende 90 seconden fluorwaterstofzuur aan op plaats
met de fractuur.
ii. Zuig het zuur van het oppervlak en spoel en droog het oppervlak
DAN grondig.
iii. Breng Ultra-Etch gedurende 5 seconden aan om de porseleinzouten
en het vuil van het HF-etsen te verwijderen. Spoel en droog.
iv. Breng een druppelvormige laag silaan aan gedurende 60 seconden.
v. Droog grondig. NIET SPOELEN.
vi. Ga door met de stap “Bonding” (zie hieronder).
d. Zirkoniumoxide – NIET ETSEN EN GEEN SILAAN GEBRUIKEN
i. Slijp het gebroken oppervlak van de prothese met lucht, spoel endroog.
ii. Breng zirkoniumoxideprimer aan op de plaats met de fractuur
volgens de aanwijzingen van de fabrikant.
iii. Ga door met de stap “Bonding” (zie hieronder).
3.Bondinga. Afgifte vanuit de fles
i. Breng 1-3 druppels Peak™ Universal Bond aan op de “B”-kant van
het wegwerpdappenglaasje.
ii. Breng met de Micro Applicator Brush een druppelvormige laag
Peak™ Universal Bond aan op de preparatie en agiteer dit voorzichtig
gedurende 10 seconden.
iii. Droog/verdun het gedurende 10 seconden met ¼ tot ½ luchtdruk.
De preparatie moet er glanzend uitzien.
iv. Hard het gedurende 10 seconden uit (20 seconden voor
uithardingslampen met een vermogen < 600 mW/cm2).
v. Restaureer met vloeibaar en/of stopbaar (‘packable’) composiet
volgens de aanwijzingen van de fabrikant.
b. Afgifte vanuit de spuiti. Breng een druppelvormige laag Peak™ Universal Bond aan met
de Inspiral™ Brush Tip en agiteer dit voorzichtig gedurende 10
seconden.
ii. Droog/verdun dit gedurende 10 seconden met ¼ tot ½ luchtdruk.
De preparatie moet er glanzend uitzien.
iii. Hard het gedurende 10 seconden uit (20 seconden voor
uithardingslampen met een vermogen < 600 mW/cm2).
iv. Restaureer met vloeibaar en/of stopbaar (‘packable’) composiet
volgens de aanwijzingen van de fabrikant.

Indirecte hechttechniek - indirecte kronen, inlays, onlays,
zirkoniumoxide
1.Preparerena. Verwijder de tijdelijke prothese, reinig de preparatie, spoel en droog(Consepsis Scrub met een STARbrush™ om deze te reinigen en tedesinfecteren en cementresten te verwijderen).
b. Controleer de pasvorm van de prothese.
c. Prepareer de binnenkant van de prothese.
i. Metaalbasis:
1. Pas microabrasie (zandstralen) toe op het oppervlak van deprothese.
2. Spoel en droog het oppervlak.
ii. Keramiek/porselein:
1. Breng gedurende 90 seconden fluorwaterstofzuur (HF) (Ultradent
Porcelain Etch) aan op het binnenoppervlak van de prothese en
spoel en droog deze dan.
2. Breng Ultra-Etch gedurende 5 seconden aan om de porseleinzouten
en het vuil van het HF-etsen te verwijderen. Spoel en droog.
3. Breng silaan (Ultradent™ Silane) aan op het binnenoppervlak van
de prothese gedurende 1 minuut, droog het en zet de protheseweg. Niet spoelen.
iii. Zirkoniumoxide: NIET ETSEN EN GEEN SILAAN GEBRUIKEN
1. Slijp het binnenoppervlak van de prothese met lucht, spoel en droog.
2. Breng een zirkoniumoxideprimer aan volgens de aanwijzingen vande fabrikant.
2.Etsen - Preparatie van het tandoppervlak
a. Zelfetsende techniek – dentine/tandglazuur, composiet en metaal
i. Spoel de preparatie en laat deze vochtig.
ii. OPTIE - Breng Consepsis (indien beschikbaar) met de Black Mini
Brush Tip aan op de preparatie met een wrijvende beweging en
droog deze lichtjes met lucht zodat de preparatie iets vochtig blijft.
iii. Breng Peak™ SE aan met de Black Mini™ Brush Tip gedurende 20
seconden om de tand te prepareren en wrijf het rond op het dentine.
Wrijf het tandglazuur niet.
iv. Verdun/droog het gedurende 3 seconden met een lucht-/waterspuitof een krachtige afzuiging direct over de preparatie.
v. Ga door met de stap “Bonding” (zie hieronder).
b. Totale etstechniek – dentine/tandglazuur, composiet en metaal
i. Breng Ultra-Etch met de Blue Micro Tip gedurende 20 seconden aan
op alle oppervlakken van de tandpreparatie.
ii. Spoel grondig gedurende 5 seconden.
iii. Verdun/droog het met een lucht-/waterspuit of een krachtige
afzuiging direct over de preparatie. Laat het oppervlak licht vochtig.
iv. OPTIE – Breng Consepsis (indien beschikbaar) met de Black Mini
Brush Tip aan op de preparatie met een wrijvende beweging en
droog deze lichtjes met lucht zodat de preparatie iets vochtig blijft.
v. Ga door met de stap “Bonding” (zie hieronder).
c Porseleinets – VOORZICHTIG – Gebruik een goede isolatie zoals een
zuurneutraliserende barrière (EtchArrest) als u fluorwaterstofzuur (HF)
(Ultradent Porcelain Etch) gebruikt. Voorkom dat het fluorwaterstofzuur
de gingiva of het dentine raakt.
i. Breng gedurende 90 seconden fluorwaterstofzuur aan op plaats
met de fractuur.
ii. Zuig het zuur van het oppervlak en spoel en droog het oppervlak
DAN grondig.
iii. Breng Ultra-Etch gedurende 5 seconden aan om de porseleinzouten
en het vuil van het HF-etsen te verwijderen. Spoel en droog.
iv. Breng een druppelvormige laag silaan aan gedurende 60 seconden.
v. Droog grondig. NIET SPOELEN.
vi. Ga door met de stap “Bonding” (zie hieronder).
d. Zirkoniumoxide – NIET ETSEN EN GEEN SILAAN GEBRUIKEN
i. Slijp het binnenoppervlak van de prothese met lucht, spoel en droog.
ii. Breng zirkoniumoxideprimer aan op de plaats met de fractuur
volgens de aanwijzingen van de fabrikant.
iii. Ga door met de stap “Bonding” (zie hieronder).
3.Bondinga. Afgifte vanuit de fles
i. Breng 1-3 druppels Peak Universal Bond aan op de “B”-kant van het

wegwerpdappenglaasje.
Breng met de Micro Applicator Brush een druppelvormige laag
Peak Universal Bond aan op de preparatie en wrijf dit voorzichtig
gedurende 10 seconden.
iii. Verdun/droog het gedurende 10 seconden met volle luchtdruk. De
preparatie moet er glanzend uitzien.
iv. Hard het gedurende 10 seconden uit (20 seconden voor
uithardingslampen met een vermogen < 600 mW/cm2).
b. Afgifte vanuit de spuiti. Breng een druppelvormige laag Peak™ Universal Bond aan met deInspiral™ Brush Tip en wrijf dit voorzichtig gedurende 10 seconden.
ii. Verdun/droog het gedurende 10 seconden met volle luchtdruk. De
preparatie moet er glanzend uitzien.
iii. Hard het gedurende 10 seconden uit (20 seconden voor
uithardingslampen met een vermogen < 600 mW/cm2).
4.Cementeren
a. Breng lichtuithardend cement aan op translucente veneers of
duaal uithardend harscement op andere prothesen en volg degebruiksaanwijzing van de fabrikant.
NB: Voor een directe afsluiting van het dentine moeten stap 2A en 3 vande Directe techniek worden uitgevoerd (zie hierboven). Breng glycerine
aan op de Peak Universal Bond en hard deze gedurende 10 seconden
uit. Spoel de glycerine eraf. Maak de definitieve afdruk. Breng nogmaals
glycerine aan op de preparatie als scheidingsmiddel, voordat u detijdelijke prothese cementeert.
ii.

Reparatie van composiet/metaal/zirkoniumoxide/porselein
1. Composiet: Verwijder de verzwakte delen van het bestaande composiet.
Ruw het oppervlak op met een diamantfrees.
a. Totale etstechniek
i. Breng gedurende 20 seconden Ultra-Etch met de Blue Micro Tip aan
op alle oppervlakken van de tandpreparatie.
ii. Spoel grondig gedurende 5 seconden en laat het vochtig.
2. Metaal: Pas microabrasie toe op het oppervlak.
a. Totale etstechniek
i. Breng gedurende 20 seconden Ultra-Etch met de Blue Micro Tip aan
op alle oppervlakken van de tandpreparatie.
ii. Spoel grondig gedurende 5 seconden en laat het vochtig.
3. Zirkoniumoxide: Reinig het oppervlak, verwijder het verzwakte
zirkoniumoxide met een diamantfrees. NIET ETSEN EN GEEN SILAANGEBRUIKEN.
a. Slijp het binnenoppervlak van de prothese met lucht
b. Breng zirkoniumoxideprimer aan op de fractuurplaats volgens deaanwijzingen van de fabrikant.
4. Porselein: Ruw het oppervlak op en verwijder het verzwakte porselein met
een diamantfrees. Reinig het porseleingedeelte met de fractuur gedurende
15 seconden met Ultra-Etch. Spoel en droog.
VOORZICHTIG – Gebruik een goede isolatie zoals een zuurneutraliserende
barrière (EtchArrest) als u fluorwaterstofzuur (HF) (Ultradent™ PorcelainEtch) gebruikt. Voorkom dat het fluorwaterstofzuur de gingiva of het
dentine raakt.
a. Breng gedurende 90 seconden fluorwaterstofzuur aan op fractuurplaats.
b. Zuig het zuur van het oppervlak en spoel en droog het oppervlak daarna
grondig.
c. Breng Ultra-Etch gedurende 5 seconden aan om het zout en vuil van het
HF-etsen te verwijderen. Spoel en droog.
d. Breng een druppelvormige laag silaan aan gedurende 1 minuut.
e. Droog grondig. NIET SPOELEN.
5. Bondinga. Afgifte vanuit de fles
i. Breng 1-3 druppels Peak™ Universal Bond aan op de “B”-kant van het
wegwerpdappenglaasje.
ii. Breng met de Micro Applicator Brush een druppelvormige laag
Peak™ Universal Bond aan op de preparatie en agiteer dit voorzichtig
gedurende 10 seconden.
iii. Droog/verdun dit gedurende 10 seconden met 1/4 tot 1/2 luchtdruk.
De preparatie moet er glanzend uitzien.
iv. Hard het gedurende 10 seconden uit (20 seconden voor

11uithardingslampen met een vermogen < 600 mW/cm2).
b. Afgifte vanuit de spuiti. Breng een druppelvormige laag Peak™ Universal Bond aan met deInspiral™ Brush Tip en agiteer dit voorzichtig gedurende 10 seconden.
ii. Droog/verdun dit gedurende 10 seconden met 1/4 tot 1/2 luchtdruk.
iii. De preparatie moet er glanzend uitzien.
iv. Hard het gedurende 10 seconden uit (20 seconden voor
uithardingslampen met een vermogen < 600 mW/cm2).
6. Restaureer met vloeibaar en/of ‘packable’ (condenseerbaar) composiet
volgens de aanwijzingen van de fabrikant.

12

Stift en stomp
1.Preparerena. Boor het stiftgat waarbij u een rubberen stop en de juiste maat UniCore™
Drill gebruikt.
b. Spoel de stiftruimte gedurende 10 seconden met de TriAway Adaptor eneen 22 ga Endo-Eze™ Tip. Droog deze met de TriAway Adaptor en 22 g
Endo-Eze Tip vanaf de onderkant van de preparatie.
c. Controleer of de stift (UniCore Post) goed past en snijd deze af op degewenste lengte met een diamanten schijf met hoog toerental.
NB: Carbide- en operatiefrezen kunnen de vezels uitrafelen.
2.Etsena. Zelfetsende techniek
i. Spoel de kanaalruimte en laat deze vochtig.
ii. Bevestig een blauwe 22 ga Deliver-Eze™ Brush Tip op de Peak SE spuit.
iii. Steek deze in de stiftruimte en tegen de coronale preparatie
gedurende 20 seconden, waarbij u een roerende beweging maakt.
iv. Blaas overtollig etsmiddel met de TriAway Adaptor en 22 g Endo-Eze
Tip eraf, vanaf de onderkant omhoog. Verdun/droog het gedurende 3
seconden met een lucht-/waterspuit of een krachtige afzuiging directover de preparatie.
v. Ga door met de stap “Bonding” (zie hieronder).
b. Totale etstechniek:
i. Bevestig een blauwe 22g Endo-Eze Tip op de Ultra-Etch spuit.
ii. Start apicaal en vul de stiftruimte coronaal. Breng het aan op decoronale preparatie. Ets gedurende 20 seconden.
iii. Zuig het overtollig etsmiddel eraf.
iv. Spoel de preparatie grondig en droog deze lichtjes met lucht met
behulp van de TriAway Adaptor en de 22 ga Endo-Eze Tip, waarbij ude stiftruimte iets vochtig laat.
v. Ga door met de stap “Bonding” (zie hieronder).
3.Bondinga. Afgifte vanuit de fles
i. Breng 1-3 druppels Peak Universal Bond aan op de “B”-kant van het
wegwerpdappenglaasje.
ii. Breng Peak Universal Bond met de Nano-Brush™ of NaviTip FX aan op
de stiftruimte en roer het gedurende 10 seconden voorzichtig over dehele lengte van het kanaal en de preparatie.
iii. Verwijder de overtollige Peak Universal Bond grondig met de TriAway
Adaptor en de 22 ga Endo-Eze Tip.
iv. Droog/verdun het gedurende 10 seconden met ¼ tot ½ luchtdruk.
De preparatie moet er glanzend uitzien.
v. Hard uit vanaf de bovenkant omlaag in de stiftruimte gedurende
20 seconden (40 seconden bij lampen met een vermogen < 600
mW/cm2).
vi. Gebruik een papierstift of eerder geplaatste stift om de controlerenof de stiftruimte niet is geblokkeerd.
b. Afgifte vanuit de spuiti. Bevestig een 30ga NaviTip FX aan de Peak™ Universal Bond-spuit.
ii. Plaats 1-2 druppels in de stiftruimte en op de preparatie, agiteer dezevervolgens gedurende 10 seconden over de gehele lengte van het
kanaal, inclusief de tandpreparatie.
iii. Verwijder het overtollige Peak™ Universal Bond grondig met de
TriAway Adaptor en de 22ga Endo-Eze Tip.
iv. Droog de stiftruimte en preparatie gedurende 10 seconden met lucht
bij volle luchtdruk en verdun/droog met de TriAway Adaptor en de
22ga Endo-Eze Tip om eventueel achtergebleven oplosmiddel vanafde onderkant te verdampen.

Hard uit vanaf de bovenkant omlaag in de stiftruimte gedurende 20
seconden (40 seconden bij lampen met een vermogen < 600 mW/cm2).
Gebruik een papierstift of eerder geplaatste stift om de controleren of destiftruimte niet is geblokkeerd.
Achteraf cementeren en stompopbouw
1. Haal de dop van de PermaFlo™ DC spuit.
2. Plaats een mengtip op de spuit met twee patronen, waarbij u de twee
poorten uitlijnt. Draai de tip rechtsom totdat deze vastklikt.
3. Bevestig de flexibele Intraoral Tip™ op de mengtip zodat u het cement directin het kanaal van de spuit met twee patronen kunt spuiten.
4. Spuit een kleine hoeveelheid eruit voordat u de stift in de ruimte plaatst.
5. Steek de tip helemaal in de stiftruimte.
6. Spuit met gelijkmatige druk PermaFlo DC eruit, eerst apicaal en daarna
coronaal.
7. Steek de stift (UniCore™ Post) er langzaam in, waarbij het overtollig cement
wordt verplaatst.
8. Plaats de uithardingslamp direct bovenop de stift en hard deze gedurende
20 seconden uit (40 seconden bij lampen met een vermogen < 600 mW/
cm2)
9. Ga door met het opbouwen van PermaFlo™ DC-lagen rondom de stift totdat
de gewenste hoogte is bereikt. NB: Hard elke laag gedurende 5 seconden
uit zodat de gel kan uitharden en de stomp zich kan vormen. Hard de
opbouw gedurende 40 seconden definitief uit. Verwijder de mengtip pas bij
het volgende gebruik. Desinfecteer de spuit en mengtip.
Voorzorgsmaatregelen en waarschuwingen:
1. Lees en begrijp alle instructies zorgvuldig voordat u Peak Universal Bondgebruikt.
2. Uitsluitend voor professioneel gebruik.
3. Bevestig de dop na gebruik weer onmiddellijk om polymerisatie tevoorkomen.
4. Controleer altijd de stroming van het materiaal voordat u het intraoraal
gebruikt. Als u weerstand voelt, vervangt u de tip en controleert u opnieuw.
5. Laat de dop op de fles zitten tot het volgende gebruik.
6. Tandarts en patiënt moeten UV-oogbescherming dragen tijdens het
uitharden van harsen.
7. Als het product niet dagelijks wordt gebruikt, moet het in de koelkast
worden bewaard.
8. Laat in de koelkast bewaarde producten op omgevingstemperatuur komen
voordat u deze gebruikt.
9. Gebruik olievrije, vochtvrije lucht om de hechtsterkte te optimaliseren.
10. Verdraai de operatielamp om vroegtijdige polymerisatie van allematerialen op harsbasis te voorkomen.
11. Harsen kunnen tot overgevoeligheid leiden. Voorkom herhaaldelijk
contact tussen de niet-uitgeharde dentale hars en de huid. Niet gebruiken
bij patiënten van wie bekend is dat zij gevoelig zijn voor acrylaten of
andere harsen. Raadpleeg een arts bij een allergische reactie, dermatitisof huiduitslag.
12. Gooi tips, lege spuiten en flessen op de juiste manier weg.
13. Buiten bereik van kinderen houden.
14. Niet gebruiken na de uiterste gebruiksdatum op de verpakking.
15. Breng de dop weer aan en desinfecteer en veeg de spuit af met een
middelmatig desinfectiemiddel voordat u deze weer gebruikt. Als u een
wegwerpspuitdop gebruikt, moet u de tip verwijderen, een andere dop
aanbrengen en de gebruikte spuitdop weggooien.
16. De tips kunnen worden weggegooid. Om kruisbesmetting te voorkomen,
mogen de tips niet opnieuw worden gebruikt.
17. Stel producten niet bloot aan hitte/zonlicht.
18. Breng sterke chemische stoffen alleen aan op de behandelplaats.
NB: Voor de veiligheidsinformatiebladen en nadere informatie
over het gebruik van Peak™ Universal Bond, Peak™ SE en andereverwante producten ga naar www.ultradent.com

Peak™ Universal Bond e Peak™ SE
Descrizione:
Peak Universal Bond è un adesivo dentale su base resinosa confezionato inflacone o siringa singola. Può essere usato con tecnica Self-Etch o Total-Etch.
Contiene riempitivi al 7,5% in una soluzione di alcool etilico come solvente e
polimerizza con la maggior parte delle lampade ad alta intensità, incluse le lampade
LED. Peak Universal Bond contiene lo 0,2% di clorexidina che assicura un’adesionea lungo termine.
Peak SE Primer è una resina adesiva automordenzante per la dentina che è
composta da un mordenzante e un primer ed è confezionato in siringa.
Ultra-Etch™ è un gel al 35% di acido fosforico indicato per la tecnica “etch andrinse” (mordenza e risciacqua) confezionato in siringa.
L’aggiunta dell’additivo alla Clorexidina non ha dimostrato una riduzione delle carie
secondaria nei pazienti. Non sono stati eseguiti studi clinici per valutare gli effettidella Clorexidina sui batteri orali o sulle carie.
Indicazioni:
Può essere utilizzato praticamente per tutte le necessità di adesione e mordenzatura
in odontoiatria restaurativa, per pazienti di tutte le età.
Peak Universal Bond aderisce ai seguenti materiali:• dentina e smalto• porcellana, zirconia• metallo• composito
Istruzioni per l’uso:
NOTA: il primo utilizzo di Peak SE richiedel’attivazione dei due componenti separati nella
siringa JetMix™.
1) Dopo l’attivazione Peak SE è stabile per 120 giorni.
2) Prima dell’attivazione scrivere la data di scadenza
sulla parte piatta dello stantuffo.
3) NON RIMUOVERE IL CAPPUCCIO LUER LOCK PRIMADELLA MISCELAZIONE
4) Premere velocemente e con pressione sullo
stantuffo che riporta la data e spingerlo nella
parte centrale della siringa.
5) Verificare che lo stantuffo sia centrato nel cilindrodella siringa.
Tecnica adesiva diretta e riparazione diporcellana/zirconio
1.Preparazionea) Dentina/Smalto: isolare, pulire e rimuovere lacarie assicurandosi di togliere tutta la dentina
demineralizzata (per questo si consiglia l’uso di
Seek/Sable Seek). Irruvidire le abrasioni/erosioni nelle cavità di Classe V
con una fresa diamantata.
b) Composito: rimuovere le aree indebolite del composito esistente. Irruvidire lasuperficie con una fresa diamantata.
c) Metallo: eseguire la microabrasione della superficie.
d) Zirconio: pulire la superficie e rimuovere lo zirconio indebolito con una fresa
diamantata.
e) Porcellana: irruvidire e rimuovere la porcellana indebolita con una fresa
diamantata. Pulire la zona della porcellana fratturata
applicando per 5 secondi Ultra-Etch. Sciacquare e asciugare.
2. Mordenzaturaa) Tecnica Self-Etch: dentina/smalto, composito e metallo
i. Risciacquare la preparazione e lasciare le superfici lievemente umide.
ii. OPZIONALE – Applicare Consepsis™ (se disponibile) con il puntale
Black Mini™ Brush Tip sulla preparazione e strofinarlo, quindi asciugare
leggermente lasciando la superficie lievemente umida.
iii. Applicare Peak SE con il puntale Black Mini Brush Tip sulla preparazione
dentale per 20 secondi mediante uno strofinamento continuo sulla
dentina. Non strofinare sullo smalto.

IT

iv. Distribuire/asciugare per 3 secondi usando la siringa aria/acquao posizionando l’aspirazione ad alto volume direttamente sulla
preparazione.
v. Passare alla fase di adesione descritta più avanti.
b) Tecnica Total-Etch : dentina/smalto, composito e metallo
i. Controllare il colore e la consistenza del flusso del prodotto primadell’applicazione, estrudendone una piccola quantità su una garza o
un blocchetto di miscelazione. Eliminare l’eventuale liquido trasparenteerogato.
ii. Applicare Ultra-Etch con il puntale Blue Micro™ Tip su tutte le superfici
della preparazione dentale e lasciarlo agire per 20 secondi.
iii. Sciacquare accuratamente per 5 secondi.
iv. Asciugare leggermente usando la siringa aria/acqua o posizionando
l’aspirazione ad alto volume direttamente sulla preparazione. Lasciare lasuperficie lievemente umida.
v. OPZIONALE – Applicare Consepsis (se disponibile) con il puntale
Black Mini Brush Tip sulla preparazione e strofinarlo, quindi asciugare
leggermente lasciando la superficie lievemente umida.
vi. Passare alla fase di adesione descritta più avanti.
c) Mordenzatura della porcellana. ATTENZIONE: ricorrere ad un isolamento
corretto come p.e. una barriera neutralizzante degli acidi (EtchArrest™)
nell’uso dell’acido fluoridrico (HF) (Ultradent™ Porcelain Etch). Evitare chel’acido idrofluoridrico venga a contatto con gengiva o dentina.
i. Applicare l’acido idrofluoridrico sull’area fratturata per 90 secondi.
ii. Aspirare l’acido dalla superficie, QUINDI risciacquare accuratamente
e asciugare.
iii. Applicare Ultra-Etch per 5 secondi per rimuovere i detriti e i sali diporcellana formati dalla mordenzatura con acido idrofluoridrico.
Sciacquare e asciugare.
iv. Applicare uno strato consistente di silano per 60 secondi.
v. Asciugare accuratamente. NON RISCIACQUARE.
vi. Passare alla fase di adesione descritta più avanti.
d) Zirconio - NON MORDENZARE NÉ USARE UN SILANO
i. Irruvidire la superficie fratturata del manufatto protesico medianteabrasione ad aria, risciacquare e asciugare.
ii. Applicare il primer per lo zirconio sull’area fratturata seguendo leistruzioni del produttore.
iii. Passare alla fase di adesione descritta più avanti.
3.Adesionea) Flacone
i. Dispensare 1-3 gocce di Peak™ Universal Bond sul lato “B” del vasetto
dappen monouso.
ii. Con il Micro Applicator Brush, applicare uno strato consistente di
Peak™ Universal Bond sulla preparazione e frizionare delicatamente
per 10 secondi.
iii. Distribuire/asciugare per 10 secondi usando la siringa ad aria conpressione da ¼ a ½. La preparazione deve apparire lucente.
iv. Fotopolimerizzare per 10 secondi (20 secondi per lampade ad intensità
luminosa <600 mW/cm2).
v. Eseguire il restauro con un composito fluido o condensabile seguendo
le istruzioni del produttore.
b) Siringa
i. Applicare uno strato consistente di Peak Universal Bond con il puntale
Inspiral™ Brush e frizionare delicatamente per 10 secondi.
ii. Distribuire/asciugare per 10 secondi usando la siringa ad aria conpressione da ¼ a ½. La preparazione deve apparire lucente.
iii. Fotopolimerizzare per 10 secondi (20 secondi per lampade ad intensità
luminosa <600 mW/cm2).
iv. Eseguire il restauro con un composito fluido o condensabile seguendo
le istruzioni del produttore.
Tecnica adesiva indiretta - Corone, Inlay, Onlay e manufatti in zirconio
1.Preparazionea) Rimuovere il restauro temporaneo, pulire la preparazione, risciacquare e
asciugare (usare Consepsis Scrub con STARbrush™ per pulire, disinfettare e

13

14

rimuovere il cemento residuo).
b) Controllare l’adattamento del manufatto protesico.
c) Preparare la superficie interna del manufatto.
i. Struttura in metallo:
1. Irruvidire la superficie interna del manufatto mediante microabrasione(sabbiare).
2. Sciacquare e asciugare la superficie.
ii. Ceramica/porcellana:
1. Applicare l’acido idrofluoridrico (HF) (Ultradent Porcelain Etch) sulla
superficie interna del manufatto protesico per 90 secondi, risciacquaree asciugare.
2. Applicare Ultra-Etch per 5 secondi per rimuovere i detriti e i sali diporcellana formati dalla mordenzatura con acido idrofluoridrico.
Sciacquare e asciugare.
3. Applicare il silano (Ultradent™ Silane) sulla superficie interna delmanufatto protesico per 1 minuto, asciugare e riporre il manufatto.
Non sciacquare.
iii. Zirconio: NON MORDENZARE NÉ USARE UN SILANO
1. Irruvidire la superficie interna del manufatto mediante abrasione adaria, sciacquare e asciugare.
2. Applicare il primer per lo zirconio seguendo le istruzioni del produttore.
2. Mordenzatura - Preparazione della superficie dentalea) Tecnica Self-Etch: dentina/smalto, composito e metallo
i. Risciacquare la preparazione e lasciare le superfici umide.
ii. OPZIONALE. Applicare Consepsis (se disponibile) con il puntale
Black Mini Brush Tip sulla preparazione, quindi sfregarlo e asciugare
lievemente con un getto d’aria lasciando le superfici umide.
iii. Applicare Peak™ SE con il puntale Black Mini™ Brush Tip per 20 secondi
sulla preparazione dentale, frizionando continuamente sulla dentina.
Non strofinare lo smalto.
iv. Distribuire/asciugare per 3 secondi usando la siringa aria/acquao posizionando l’aspirazione ad alto volume direttamente sulla
preparazione.
v. Passare alla fase di adesione descritta più avanti.
b) Tecnica Total-Etch: dentina/smalto, composito e metallo
i. Applicare Ultra-Etch con il puntale Blue Micro Tip su tutte le superfici
della preparazione dentale e lasciarlo agire per 20 secondi.
ii. Sciacquare accuratamente per 5 secondi.
iii. Asciugare leggermente usando la siringa aria/acqua o posizionando
l’aspirazione ad alto volume direttamente sulla preparazione. Lasciare lasuperficie lievemente umida.
iv. OPZIONALE. Applicare Consepsis (se disponibile) con il puntale
Black Mini Brush Tip sulla preparazione, quindi sfregarlo e asciugare
lievemente con un getto d’aria lasciando le superfici umide.
v. Passare alla fase di adesione descritta più avanti.
c) Mordenzatura della porcellana. ATTENZIONE: ricorrere ad un isolamento
corretto come p.e. una barriera neutralizzante degli acidi (EtchArrest™)
nell’uso dell’acido fluoridrico (HF) (Ultradent Porcelain Etch). Evitare chel’acido idrofluoridrico venga a contatto con gengiva o dentina.
i. Applicare l’acido idrofluoridrico sull’area fratturata per 90 secondi.
ii. Aspirare l’acido dalla superficie, QUINDI risciacquare accuratamente
e asciugare.
iii. Applicare Ultra-Etch per 5 secondi per rimuovere i detriti e i sali diporcellana formati dalla mordenzatura con acido idrofluoridrico.
Sciacquare e asciugare.
iv. Applicare uno strato consistente di silano per 60 secondi.
v. Asciugare accuratamente. NON RISCIACQUARE.
vi. Passare alla fase di adesione descritta più avanti.
d) Zirconio. NON MORDENZARE NÉ USARE UN SILANO
i. Irruvidire la superficie interna del manufatto protesico medianteabrasione ad aria, risciacquare e asciugare.
ii. Applicare il primer per lo zirconio sull’area fratturata seguendo leistruzioni del produttore.
iii. Passare alla fase di adesione descritta più avanti.
3.Adesionea. Flacone
i. Versare 1-3 gocce di Peak Universal Bond sul lato “B” nel vaso dappen
monouso.

ii.

Con il pennellino Micro Applicator Brush, applicare uno strato
consistente di Peak Universal Bond sulla preparazione e frizionarlodelicatamente per 10 secondi.
iii. Distribuire/asciugare per 10 secondi usando la siringa ad aria conpressione massima. La preparazione deve apparire lucente.
iv. Fotopolimerizzare per 10 secondi (20 secondi per lampade ad intensità
luminosa <600mW/cm2).
b. Siringa
i. Applicare uno strato consistente di Peak™ Universal Bond con il puntale
Inspiral™ Brush e frizionare delicatamente per 10 secondi.
ii. Distribuire/asciugare per 10 secondi usando la siringa ad aria conpressione massima. La preparazione deve apparire lucente.
iii. Fotopolimerizzare per 10 secondi (20 secondi per lampade ad intensità
luminosa <600 mW/cm2).
4.Cementazionea) Usare un cemento fotopolimerizzabile per faccette traslucenti o un cemento
duale su base resinosa per altri manufatti protesici, seguendo le istruzioni perl’uso del produttore.
NOTA: la sigillatura immediata della dentina richiede la Tecnica Diretta, passaggi
2A e 3 sopra descritti. Applicare della glicerina sull’adesivo Peak Universal
Bond e fotopolimerizzare per 10 secondi. Risciacquare la glicerina. Prendere
l’impronta finale. Applicare nuovamente la glicerina sulla preparazione comeisolante prima di cementare il restauro provvisorio.
Riparazione di composito/metallo/zirconia/porcellana
1. Composito: rimuovere le aree difettose del composito esistente. Irruvidire lasuperficie con una fresa diamantata.
a) Tecnica Total-Etch
i. Applicare Ultra-Etch con il Blue Micro Tip su tutte le superfici dellapreparazione dentale e lasciarlo agire per 20 secondi.
ii. Risciacquare abbondantemente per 5 secondi e lasciare le superfici
umide.
2. Metallo: eseguire una microabrasione della superficiea) Tecnica Total-Etch
i. Applicare Ultra-Etch con il Blue Micro Tip su tutte le superfici dellapreparazione dentale e lasciarlo agire per 20 secondi.
ii. Risciacquare abbondantemente per 5 secondi e lasciare le superfici
umide.
3. Zirconia: pulire la superficie e rimuovere la zirconia difettosa con una fresa
diamantata. NON MORDENZARE NÉ USARE UN SILANO.
a) Irruvidire la superficie interna del manufatto protesico mediante abrasione
ad aria.
b) Applicare il primer per la zirconia sull’area fratturata seguendo le istruzionidel produttore.
4. Porcellana: irruvidire e rimuovere la porcellana difettosa con una fresa
diamantata. Mordenzare la zona della porcellana fratturata per 15 secondi
con Ultra-Etch. Risciacquare e asciugare.
ATTENZIONE: nell’uso dell’acido idrofluoridrico HF (Ultradent™ Porcelain Etch)
ricorrere ad un isolamento adeguato come p.es. un neutralizzante gli acidi(EtchArrest). Evitare che l’acido idrofluoridrico venga a contatto con la
gengiva o con la dentina.
a) Applicare l’acido idrofluoridrico sull’area fratturata e lasciarlo agire per 90
secondi.
b) Aspirare l’acido dalla superficie, quindi risciacquare accuratamente e
asciugare.
c) Applicare Ultra-Etch per 5 secondi per rimuovere i detriti e i sali di porcellana
formati dalla mordenzatura con acido idrofluoridrico. Risciacquare e
asciugare.
d) Applicare uno strato consistente di silano e lasciarlo agire per 1 minuto.
e) Asciugare accuratamente. NON RISCIACQUARE.
5. Adesionea) Flacone
i. Dispensare 1-3 gocce di Peak™ Universal Bond sul lato “B” del vasetto
dappen monouso.
ii. Con il Micro Applicator Brush, applicare uno strato consistente di Peak
Universal Bond e frizionare delicatamente per 10 secondi.
iii. Distribuire/asciugare per 10 secondi usando la siringa ad aria con

pressione da ¼ a ½. La preparazione deve apparire lucente.
iv. Fotopolimerizzare per 10 secondi (20 secondi per lampade ad intensità
luminosa <600 mW/cm2).
b) Siringa
i. Applicare uno strato consistente di Peak Universal Bond con il puntale
Inspiral™ Brush e frizionare delicatamente per 10 secondi.
ii. Distribuire/asciugare per 10 secondi usando la siringa ad aria conpressione da ¼ a ½.
iii. La preparazione deve apparire lucente.
iv. Fotopolimerizzare per 10 secondi (20 secondi per lampade ad intensità
luminosa <600 mW/cm2).
6. Eseguire il restauro con un composito fluido e/o condensabile seguendo leistruzioni del produttore.
Perno e moncone
1.Preparazionea) Preparare lo spazio per il perno usando una fresa UniCore™ Drill della misuraadatta con un fermo in gomma.
b) Sciacquare abbondantemente lo spazio per il perno per 10 secondi usandol’adattatore TriAway con la cannula 22ga Endo-Eze™ Tip. Asciugare conl’adattatore TriAway con una cannula 22ga Endo-Eze Tip dal basso verso l’altodella preparazione.
c) Verificare l’adattamento del perno (UniCore Post), quindi tagliarlo alla
lunghezza desiderata con un disco diamantato ad alta velocità.
NOTA: le frese in carburo possono sfilacciare le fibre.
2.Mordenzaturaa) Tecnica Self-Etch
i. Risciacquare lo spazio del canale e lasciare le superfici umide.
ii. Inserire una cannula blu 22ga Deliver-Eze™ Brush Tip sulla siringa
Peak SE.
iii. Applicare nello spazio per il perno e sulla preparazione coronale
mediante strofinamento continuo per 20 secondi.
iv. Soffiare l’eccesso usando l’adattatore TriAway con la cannula 22ga EndoEze Tip, dal basso dello spazio verso l’alto. Distribuire/asciugare per 3
secondi usando la siringa aria/acqua o posizionando l’aspirazione ad
alto volume direttamente sulla preparazione.
v. Passare alla fase di adesione descritta più avanti.
b) Tecnica Total-Etch:
i. Inserire una cannula blu 22ga Endo-Eze Tip sulla siringa Ultra-Etch.
ii. Partendo da apicale, riempire lo spazio del perno in direzione coronale.
Applicare sulla preparazione coronale. Mordenzare per 20 secondi.
iii. Aspirare il mordenzante in eccesso.
iv. Usando l’adattatore TriAway con la cannula 22ga Endo-Eze Tip,
sciacquare abbondantemente e asciugare leggermente con aria
lasciando lo spazio per il perno leggermente umido.
v. Passare alla fase di adesione descritta più avanti.
3.Adesionea) Flacone
i. Versare 1-3 gocce di Peak Universal Bond sul lato “B” nel vaso dappen
monouso.
ii. Usando le cannule Nano-Brush™ o NaviTip FX, applicare Peak Universal
Bond nello spazio per il perno e frizionare delicatamente per tutta lalunghezza del canale e sulla preparazione dentale per 10 secondi.
iii. Rimuovere completamente gli eccessi usando l’adattatore TriAway con lacannula 22ga Endo-Eze Tip.
iv. Distribuire/asciugare la preparazione esterna per 10 secondi usando lasiringa ad aria con pressione da ¼ a ½. La preparazione deve apparire
lucente.
v. Fotopolimerizzare tutto lo spazio per il perno per 20 secondi (40 secondi
per le lampade con intensità luminosa <600mW/cm2)
vi. Usare delle punte di carta o perni adattati precedentemente perverificare che lo spazio per il perno non sia ostruito.
b) Siringai. Inserire una cannula NaviTip FX 30 ga sulla siringa Peak Universal Bond.
ii. Applicare 1-2 gocce nello spazio per il perno e sulla preparazione,
quindi frizionare delicatamente per tutta la lunghezza del canale e sulla
preparazione dentale per 10 secondi.
iii. Rimuovere completamente l’eccesso di Peak Universal Bond usandol’adattatore TriAway con la cannula Endo-Eze 22 ga.
iv. Asciugare con aria lo spazio per il perno e la preparazione per 10
secondi usando la siringa ad aria con pressione massima per distribuire/asciugare con l’adattatore TriAway e la cannula Endo-Eze 22 ga inseriti
dal basso verso l’alto, affinchè gli eventuali residui di solvente evaporino.
v. Fotopolimerizzare tutto lo spazio per il perno per 20 secondi (40 secondi
per le lampade con intensità luminosa <600 mW/cm2). Usare delle punte
di carta o perni adattati in precedenza per verificare che lo spazio per ilperno non sia ostruito.
Cementazione del perno e ricostruzione del moncone
1) Rimuovere il cappuccio dalla siringa PermaFlo™ DC.
2) Inserire il puntale di miscelazione sulla siringa doppia allineando le duebocchette. Girare in senso orario per bloccarlo.
3) Collegare il puntale flessibile Intraoral Tip™ al puntale di miscelazione per
facilitare l’erogazione diretta dalla siringa doppia nel canale.
4) Prima di distribuire il cemento nello spazio per il perno estruderne una piccola
quantità.
5) Inserire il puntale nello spazio per il perno fino in fondo.
6) Esercitando una pressione regolare erogare PermaFlo DC partendo da apicale espostandosi verso coronale.
7) Inserire il perno (UniCore™ Post) lentamente, facilitando la fuoriuscita delcemento in eccesso.
8) Posizionare la lampada fotopolimerizzatrice direttamente sopra il perno e
fotopolimerizzare per 20 secondi; 40 secondi per le lampade con intensità
luminosa <600mW/cm2.
9) Proseguire nella stratificazione di PermaFlo™ DC intorno al perno secondo
necessità. NOTA: fotopolimerizzare per 5 secondi i singoli strati per consolidare
il gel e ricostruire il moncone. Infine, polimerizzare il moncone per 40 secondi.
Non rimuovere il puntale di miscelazione fino all’utilizzo successivo. Disinfettare
la siringa e il puntale di miscelazione.
Precauzioni e avvertenze:
1. Leggere attentamente e capire tutte le istruzioni prima di utilizzare Peak
Universal Bond.
2. Esclusivamente ad uso professionale.
3. Richiudere immediatamente dopo l’uso per prevenire la polimerizzazione.
4. Verificare sempre il flusso del materiale nelle siringhe prima di applicarlo
intraoralmente. In presenza di resistenza, sostituire il puntale e riprovare.
5. Tenere i flaconi chiusi fino al momento dell’utilizzo.
6. Gli odontoiatri ed i pazienti devono indossare occhiali di protezione anti-UV
quando si fotopolimerizzano materiali dentali su base resinosa.
7. Se il prodotto non si usa quotidianamente, conservarlo in frigorifero.
8. Portare i prodotti conservati in frigorifero a temperatura ambiente primadell’uso.
9. Per ottimizzare il legame adesivo, usare aria priva di olio e umidità.
10. Allontanare la lampada del riunito per evitare una polimerizzazione precoce ditutti i materiali resinosi.
11. Le resine possono causare sensibilizzazione. Evitare contatti ripetuti dellaresina per uso dentale non polimerizzata con la pelle. Non usare su pazienti
con sensibilità accertata verso acrilati o altre resine. In caso di reazione
allergica, dermatiti o eruzioni cutanee consultare un medico.
12. Smaltire correttamente i puntali, le siringhe e i flaconi vuoti.
13. Tenere fuori dalla portata dei bambini.
14. Non usare dopo la data di scadenza annotata sui contenitori.
15. Richiudere, disinfettare e pulire la siringa con un disinfettante di livellointermedio tra un utilizzo e l’altro. Se si utilizzano cappucci monouso per lasiringa, rimuovere il puntale, richiudere e scartare il cappuccio della siringa.
16. I puntali sono monouso. Per evitare la contaminazione crociata non riutilizzare
i puntali.
17) Tenere i prodotti lontano da luce del sole/fonti di calore dirette.
18) Isolare gli agenti chimici forti dall’area di trattamento.
NOTA: per la scheda dei materiali e per ulteriori informazioni
sull’utilizzo di Peak Universal Bond, Peak SE e altri prodotti correlati
visitare il sito www.ultradent.com
15

ES

Peak™ Universal Bond y Peak™ SE

Descripción:
Peak Universal Bond es un adhesivo resinoso disponible en frasco o en
jeringa. Puede ser utilizado con autograbado o con grabado total. Tiene unvehículo solvente de 7,5% de alcohol etílico y fotopolimerizará con la mayoríade las lámparas de alta intensidad, incluyendo las LEDs. Peak Universal Bond
contiene 0,2% de clorhexidina, que puede asegurar fuerzas de adhesión alargo plazo.
El imprimador Peak SE Primer es una adhesivo resinoso de autograbadopara dentina, compuesto por un imprimador y un grabador en un sistema dedispensado en jeringa.
Ultra-Etch™ es un gel de ácido fosfórico al 35% para grabar, de fácil enjuague,
dispensado en jeringa.
La inclusión del aditivo de clorhexidina no ha demostrado tener correlación
con una reducción de caries secundarias en pacientes. Los estudios clínicospara evaluar los efectos de la clorhexidina en bacterias orales o caries no hansido efectuados.
Indicaciones de uso:
Utilice para prácticamente todas las necesidades de grabado y adhesión enodontología restauradora para pacientes de todas las edades.
Peak Universal Bond se adhiere a los siguientes materiales:• Dentina y esmalte• Porcelana, circonio• Metal• Compuesto
Instrucciones de uso:
NOTA: El primer uso de Peak SE requiere de laactivación de los dos componentes separados
en la jeringa JetMix™.
1. Peak SE permanece estable durante 120 días
después de la activación.
2. Antes de activar, anote la fecha de vencimientoen la zona plana del émbolo.
3. NO SAQUE LA TAPA CON TRABA LUER ANTESDE MEZCLAR.
4. Rápidamente y con fuerza, presione el émbolo“fechado” hacia el interior del émbolo que seencuentra en el medio.
5. Verifique que las pestañas traseras de ambosémbolos estén alineadas entre si.
Técnica de Adhesión Directa y Reparación dePorcelana/Circonia
1.Preparea. Dentina/Esmalte: aísle, limpie y remueva caries
asegurando la remoción de toda la dentina no
mineralizada (para esto se recomienda Sable
Seek). Para preparaciones de abrasiones/abfracciones Clase V, asperice con
una piedra diamantada.
b. Composite: Retire las zonas debilitadas de composite existente. Asperice lasuperficie con una piedra diamantada.
c. Metal: Efectúe una microabrasión de la superficie.
d. Circonia: Limpie la superficie, retire la circonia debilitada con una piedra
diamantada.
e. Porcelana: Asperice y remueva la porcelana debilitada con piedra
diamantada. Limpie la zona de porcelana fracturada por 5 segundos con
Ultra-Etch. Enjuague y seque.
2. Grabea. Técnica de Autograbado – dentina/esmalte, composite y metali. Enjuague la preparación y déjela húmeda.
ii. OPCIONAL – Aplique Consepsis™ (si está disponible) frotándola en la
preparación con la punta Black Mini Brush y seque levemente con airedejando la superficie húmeda.
16

iii.

Aplique Peak SE con la punta Black Mini Brush a la preparación
dentaria por 20 segundos frotando continuamente sobre la dentina.
No frote el esmalte.
iv. Adelgace/seque por 3 segundos usando la jeringa triple o colocando la
succión de alta potencia directamente sobre la preparación.
v. Proceda al paso “Adhiera”, abajo.
b. Técnica de Grabado Total – dentina/esmalte, composite y metal
i. Verifique el color y la consistencia del flujo del producto antes deaplicar, colocando una pequeña cantidad sobre un mezclador o gasa.
Descarte cualquier líquido claro que salga.
ii. Aplique Ultra-Etch con la punta Blue Micro™ en todas las superficies dela preparación por 20 segundos.
iii. Enjuague meticulosamente por 5 segundos.
iv. Seque levemente usando la jeringa triple o colocando la succión dealta potencia directamente sobre la preparación. Deje la preparación
ligeramente húmeda.
v. OPCIONAL – Aplique Consepsis™ (si está disponible) frotándola en la
preparación con la punta Black Mini Brush y seque levemente con airedejando la superficie húmeda.
vi. Proceda al paso “Adhiera”, abajo.
c. Porcelain Etch – PRECAUCIÓN – use aislamiento adecuado como ser
una barrera neutralizadora de ácidos (Etch Arrest™) cuando utilice ácido
fluorhídrico (HF) (Ultradent™ Porcelain Etch). No permita que el ácido
fluorhídrico toque la encía o la dentina.
i. Aplique ácido fluorhídrico a la zona fracturada por 90 segundos.
ii. Aspire el ácido de la superficie, LUEGO enjuague meticulosamente yseque la superficie.
iii. Aplique Ultra-Etch por 5 segundos para remover las sales de porcelanay residuos formados por el grabado con HF. Enjuague y seque.
iv. Aplique una capa generosa de silano por 60 segundos.
v. Seque meticulosamente. NO ENJUAGUE.
vi. Proceda al paso “Adhiera”, abajo.
d. Circonia – NO GRABE NI UTILICE SILANO
i. Efectúe una abrasión por aire de la superficie interna de la prótesis,
enjuague y seque.
ii. Aplique un imprimador de circonia en la zona fracturada siguiendo las
instrucciones del fabricante.
iii. Proceda al paso “Adhiera”, abajo.
3. Adhieraa. Dispensado en Frasco
i. Dispense 1-3 gotas de Peak™ Universal Bond en el lado “B” del vaso
dappen desechable.
ii. Utilizando un micro-aplicador (Micro Applicator Brush), dispense
una capa generosa de Peak Universal Bond en la preparación y frotesuavemente por 10 segundos.
iii. Adelgace/seque por 10 segundos utilizando de ¼ a ½ presión de aire.
La preparación debe verse brillante.
iv. Fotopolimerice por 10 segundos (20 segundos para lámparas con una
potencia <600mW/cm2).
v. Restaure con resina fluida y/o composite de restauración siguiendo las
instrucciones del fabricante.
b. Dispensado en Jeringa
i. Dispense una capa generosa de Peak Universal Bond con la punta
Inspiral™ Brush - frote suavemente por 10 segundos.
ii. Adelgace/seque por 10 segundos utilizando de ¼ a ½ presión de aire.
La preparación debe verse brillante.
iii. Fotopolimerice por 10 segundos (20 segundos para lámparas con una
potencia <600mW/cm2).
iv. Restaure con resina fluida y/o composite de restauración siguiendo las
instrucciones del fabricante.
Técnica de Adhesión Indirecta – Coronas indirectas, Inlays, Onlays,
Circonia
1.Preparea. Remueva el provisional, limpie la preparación, enjuague y seque (utilice
Consepsis Scrub con StarBrush para limpiar, desinfectar y remover elcemento residual).
b. Verifique el calce protético.
c. Prepare la superficie interna de la prótesis.
i. Base metálica:
1. Efectúe una microabrasión o enarene la superficie interna de la
prótesis.
2. Enjuague y seque la superficie.
ii. Cerámica/porcelana:
1. Aplique ácido fluorhídrico (HF) (Ultradent™ Porcelain Etch) a lasuperficie interna de la prótesis por 90 segundos, enjuague y seque.
2. Aplique Ultra-Etch por 5 segundos para remover las sales deporcelana y los residuos formados por el grabado HF. Enjuague yseque.
3. Aplique Silano (Ultradent™ Silane) a la superficie interna de la prótesis
por 1 minuto, seque y coloque la prótesis a un lado. No enjuague.
iii. Circonia: NO GRABE NI UTILICE SILANO
1. Efectúe una abrasión por aire en la superficie interna de la prótesis,
enjuague y seque.
2. Aplique un imprimador de circonia siguiendo las instrucciones delfabricante.
2.Grabe - Prepare la superficie dentaria.
a. Técnica de Autograbado - dentina/esmalte, composite y metali. Enjuague la preparación y déjela húmeda.
ii. OPCIONAL – Aplique Consepsis (si está disponible) en la preparación
frotando con la punta Black Mini Brush y seque levemente con aire,dejando la superficie húmeda.
iii. Aplique Peak SE™ con la punta Black Mini Brush por 20 segundos
frotando continuamente sobre la dentina. No frote el esmalte.
iv. Adelgace/seque por 3 segundos usando la jeringa triple o colocando la
succión de alta potencia directamente sobre la preparación.
v. Proceda al paso “Adhiera”, abajo
b. Técnica de Grabado Total - dentina/esmalte, composite y metal
i. Aplique Ultra-Etch con la punta Blue Micro en todas las superficies de la
preparación por 20 segundos.
ii. Enjuague meticulosamente por 5 segundos.
iii. Seque ligeramente usando la jeringa triple o colocando la succión dealta potencia directamente sobre la preparación. Deje la superficie
ligeramente húmeda.
iv. OPCIONAL – Aplique Consepsis (si está disponible) en la preparación
frotando con la punta Black Mini Brush y seque levemente con aire,dejando la superficie húmeda.
v. Proceda al paso “Adhiera”, abajo
c. Porcelain Etch – PRECAUCIÓN – use aislamiento adecuado como ser
una barrera neutralizadora de ácidos (Etch Arrest™) cuando utilice ácido
fluorhídrico (HF) (Ultradent™ Porcelain Etch). No permita que el ácido
fluorhídrico toque la encía o la dentina.
i. Aplique ácido fluorhídrico a la zona fracturada por 90 segundos.
ii. Aspire el ácido de la superficie, LUEGO enjuague meticulosamente
y seque.
iii. Aplique Ultra-Etch por 5 segundos para remover las sales de porcelana
y los residuos formados por el grabado HF. Enjuague y seque.
iv. Aplique una capa generosa de Silano por 60 segundos.
v. Seque meticulosamente. NO ENJUAGUE.
vi. Proceda al paso “Adhiera”, abajo.
d. Circonia – NO GRABE NI UTILICE SILANO
i. Efectúe una abrasión por aire de la superficie interna de la prótesis.
Enjuague y seque.
ii. Aplique un imprimador de circonia sobre la zona fracturada siguiendolas instrucciones del fabricante.
iii. Proceda al paso “Adhiera”, abajo.
3.Adhieraa. Dispensado en Frasco
i. Dispense 1-3 gotas de Peak™ Universal Bond en el lado “B” del vaso
dappen desechable.
ii. Utilizando un micro-aplicador (Micro Applicator Brush), dispense
una capa generosa de Peak Universal Bond en la preparación y frotesuavemente por 10 segundos.
iii. Adelgace/seque por 10 segundos utilizando presión de aire completa.

La preparación debe verse brillante.
iv. Fotopolimerice por 10 segundos (20 segundos para lámparas con una
potencia <600mW/cm2).
b. Dispensado en Jeringa
i. Dispense una capa generosa de Peak Universal Bond con la punta
Inspiral Brush - frote suavemente por 10 segundos.
ii. Adelgace/seque por 10 segundos utilizando presión de aire completa.
La preparación debe verse brillante.
iii. Fotopolimerice por 10 segundos (20 segundos para lámparas con una
potencia <600mW/cm2).
4.Cementea. Aplique cemento fotopolimerizable para carillas translúcidas o un cemento
resinoso de curado dual en otras prótesis y siga las instrucciones de usodel fabricante.
NOTA: El Sellado Inmediato de Dentina requiere los pasos 2A y 3 de la
Técnica Directa, arriba. Aplique glicerina sobre Peak Universal Bond y
fotopolimerice 10 segundos. Enjuague la glicerina. Tome la impresión
final. Reaplique glicerina a la preparación como medio separador antes decementar el provisional en posición.
Reparación de Composite / Metal / Circonia / Porcelana
1. Composite: Retire las zonas debilitadas de composite existente. Asperice lasuperficie con una piedra diamantada.
a. Técnica de Grabado Total
i. Aplique Ultra-Etch con la punta Blue Micro a todas las superficies de la
preparación por 20 segundos.
ii. Enjuague meticulosamente por 5 segundos y deje húmedo.
2. Metal: Efectúe una microabrasión de la superficie.
a. Técnica de Grabado Total
i. Aplique Ultra-Etch con la punta Blue Micro a todas las superficies de la
preparación por 20 segundos.
ii. Enjuague meticulosamente por 5 segundos y deje húmedo.
3. Circonia: Limpie la superficie; retire la circonia debilitada con una piedra
diamantada. NO GRABE NI USE SILANO.
a. Efectúe una abrasión por aire de la superficie interna de la prótesis.
b. Aplique un imprimador de circonia sobre la zona fracturada siguiendo las
instrucciones del fabricante.
4. Porcelana: Asperice y remueva la porcelana debilitada con una piedra
diamantada. Limpie la zona de porcelana fracturada por 15 segundos con
Ultra-Etch. Enjuague y seque.
PRECAUCIÓN – use aislamiento adecuado como ser una barrera neutralizadorade ácidos (Etch Arrest™) cuando utilice ácido fluorhídrico (HF) (Ultradent™
Porcelain Etch). No permita que el ácido fluorhídrico toque la encía o ladentina.
a. Aplique ácido fluorhídrico a la zona fracturada por 90 segundos.
b. Aspire el ácido de la superficie, LUEGO enjuague meticulosamente y sequela superficiec. Aplique Ultra-Etch por 5 segundos para remover las sales de porcelana yresiduos formados por el grabado HF. Enjuague y seque.
d. Aplique una capa generosa de silano por 1 minuto.
e. Seque meticulosamente. NO ENJUAGUE.
5. Adhieraa. Dispensado en Frasco
i. Dispense 1-3 gotas de Peak Universal Bond en el lado “B” del vaso
dappen desechable.
ii. Utilizando un micro-aplicador (Micro Applicator Brush), dispense una
capa generosa de Peak Universal Bond y frote suavemente por 10
segundos.
iii. Adelgace/seque por 10 segundos utilizando de 1/4 a 1/2 presión deaire. La preparación debe verse brillante.
iv. Fotopolimerice por 10 segundos (20 segundos para lámparas con una
potencia <600mW/cm2).
b. Dispensado en Jeringa
i. Dispense una capa generosa de Peak Universal Bond con la punta
Inspiral Brush - frote suavemente por 10 segundos.
ii. Adelgace/seque por 10 segundos utilizando de 1/4 a 1/2 presiónde aire.

17

iii. La preparación debe verse brillante.
iv. Fotopolimerice por 10 segundos (20 segundos para lámparas con una
potencia <600mW/cm2).
6. Restaure con resina fluida y/o composite de restauración siguiendo las
instrucciones del fabricante.

18

Pernos y Muñones
1. Preparea. Efectúe la perforación para el perno usando un tope de goma y el tamaño
adecuado de Fresa UniCore™.
b. Enjuague a fondo el espacio para perno durante 10 segundos usando el
Adaptador TriAway y una punta Endo-Eze™ 22ga. Seque con el Adaptador
TriAway y una punta Endo-Eze 22ga desde el fondo de la preparación hacia
arriba.
c. Verifique el calce del perno (Perno UniCore) y córtelo a la longitud deseada
usando un disco diamantado de alta velocidad.
NOTA: El carburo y las fresas de operatoria pueden deshilachar las fibras.
2. Grabea. Técnica de Autograbado
i. Enjuague el espacio para perno y deje húmedo.
ii. Coloque una punta Deliver-Eze™ Brush 22ga azul en la jeringa dePeak SE.
iii. Aplique en el espacio para el perno y en la preparación coronaria
movilizándolo en forma constante por 20 segundos.
iv. Sople el exceso hacia el exterior con el Adaptador TriAway y una punta
Endo-Eze 22ga desde el fondo hacia arriba. Adelgace/seque por 3
segundos utilizando la jeringa triple o colocando la succión de altapotencia directamente sobre la preparación.
v. Proceda al paso “Adherir”, abajo.
b. Técnica de Grabado Total:i. Coloque una punta Endo-Eze 22ga azul en la jeringa de Ultra-Etch.
ii. Comience apicalmente y rellene el espacio para perno hacia coronal.
Aplique en la preparación coronaria. Grabe por 20 segundos.
iii. Aspire los excesos de grabador.
iv. Usando el Adaptador TriAway y una punta Endo-Eze 22ga, enjuague
meticulosamente y seque levemente con aire dejando la preparaciónpara perno ligeramente húmeda.
v. Proceda al paso “Adhiera”, abajo.
3. Adhieraa. Dispensado en Frasco
i. Dispense 1-3 gotas de Peak Universal Bond en el lado “B” del vaso
dappen desechable.
ii. Utilizando el Nano-Brush™ o la NaviTip FX, dispense Peak Universal Bonden el espacio para perno y movilícelo suavemente en toda la longituddel conducto y en la preparación dentaria por 10 segundos.
iii. Remueva meticulosamente los excesos usando el Adaptador TriAway yla punta Endo-Eze 22ga.
iv. Utilizando el Adaptador TriAway y la punta Endo-Eze 22ga seque con
aire el espacio para perno y la preparación por 10 segundos con
presión de aire completa para adelgazar/secar y evaporar cualquierremanente de solvente desde el fondo hacia arriba.
v. Fotopolimerice el interior del espacio para perno por 20 segundos (40segundos para lámparas con potencia <600mW/cm2).
vi. Utilice una punta de papel o el perno previamente probado paraverificar que el espacio para perno no se encuentre bloqueado.
b. Dispensado en Jeringa
i. Enrosque una punta NaviTip FX 30ga en la jeringa de Peak Universal
Bond.
ii. Coloque 1-2 gotas en el espacio para perno y sobre la preparación
y luego movilícelo en toda la longitud del conducto, incluyendo la
preparación dentaria completa por 10 segundos.
iii. Remueva meticulosamente los excesos de Peak Universal Bond usando
el Adaptador TriAway y la punta Endo-Eze 22ga.
iv. Utilizando el Adaptador TriAway y la punta Endo-Eze 22ga seque con
aire el espacio para perno y la preparación por 10 segundos con
presión de aire completa para adelgazar/secar y evaporar cualquierremanente de solvente desde el fondo hacia arriba.
v. Fotopolimerice el interior del espacio para perno por 20 segundos (40segundos para lámparas con potencia <600mW/cm2). Use una punta
de papel o el perno previamente probado para verificar que el espacio
para perno no se encuentre bloqueado.
Cementado del Perno y Reconstrucción del Muñón
1. Retire la tapa de la jeringa de PermaFlo™ DC.
2. Coloque una punta mezcladora en la jeringa doble, alineando los dos puertos.
Enrosque en sentido horario hasta trabar en posición.
3. Coloque la flexible punta Intraoral en la punta mezcladora para dispensar
directamente dentro del conducto desde la jeringa doble.
4. Dispense una pequeña cantidad antes de colocar en el espacio para perno.
5. Inserte la punta hasta lo más profundo del espacio para perno.
6. Usando una presión homogénea, dispense PermaFlo DC comenzando
apicalmente y moviéndose hacia coronal.
7. Inserte el perno (Perno UniCore™) lentamente, desplazando los excesos decemento.
8. Coloque la lámpara de polimerización directamente sobre el perno y
fotopolimerice por 20 segundos (40 segundos para lámparas con potencia<600mW/cm2).
9. Continúe construyendo capas de PermaFlo™ DC alrededor del perno según
sea necesario. NOTA: fotopolimerice por 5 segundos entre capas para gelificar
y formar el muñón. Efectúe una polimerización final de 40 segundos sobre
el muñón. No retire la punta mezcladora hasta el próximo uso. Desinfecte lajeringa y la punta mezcladora.
Precauciones y advertencias:
1. Lea cuidadosamente y comprenda todas las instrucciones antes de usar Peak
Universal Bond.
2. Sólo para uso profesional.
3. Vuelva a tapar inmediatamente después del uso para evitar la polimerización.
4. Verifique el flujo del material desde la jeringa antes del uso intraoral. De sentir
resistencia, reemplace la punta y vuelva a controlar.
5. Mantenga el frasco tapado hasta utilizarlo.
6. El clínico y el paciente deben utilizar protección ocular UV cuando se
polimericen materiales de resina.
7. Refrigere el producto si no lo utiliza diariamente.
8. Lleve los productos refrigerados a temperatura ambiente antes de utilizarlos.
9. Para optimizar las fuerzas de adhesión, utilice aire libre de aceite y de
humedad.
10. Redirija la luz operatoria para evitar una polimerización prematura detodos los materiales con base de resina.
11. Las resinas pueden sensibilizar. Evite el contacto repetido de la resina sin
polimerizar con la piel. No utilice en pacientes con sensibilidad conocida
a acrilatos u otras resinas. De surgir una reacción alérgica, dermatitis oerupción, consulte al médico.
12. Descarte adecuadamente las puntas, así como las jeringas y los frascos
vacíos.
13. Mantenga lejos del alcance de los niños.
14. No utilice pasada la fecha de vencimiento anotada en los envases.
15. Vuelva a tapar, desinfecte y limpie las jeringas con un desinfectante denivel intermedio entre usos. Si utiliza una funda descartable para jeringa,
retire la tapa, vuelva a tapar y descarte la funda de la jeringa.
16. Las puntas son desechables. Para evitar la contaminación cruzada, no
reutilice las puntas.
17. Mantenga los productos lejos del calor/luz solar directa.
18. Limite los productos químicos fuertes a la zona de tratamiento.
NOTA: Para ver la FDS e información adicional sobre el uso de Peak
Universal Bond, Peak SE, y otros productos relacionados, por favor
visite www.ultradent.com

Peak™ Universal Bond e Peak™ SE
Descrição:O Peak Universal Bond é uma resina adesiva fornecida em frasco ou seringa
simples. Pode ser utilizada com autocondicionador ou condicionador total. Com
carga a 7,5% com um transportador de álcool etílico como solvente, polimeriza
com a maioria das luzes de alta intensidade, incluindo LEDs. Peak Universal
Bond contém clorexidina 0,2% que poderá assegurar forças de adesão delongo termo.
Peak SE Primer é uma resina adesiva em dentina autocondicionanteconstituída por um condicionador e um primário num sistema de aplicação
com seringa.
A inclusão do aditivo clorexidina não demonstrou nenhuma correlação com
uma redução de desintegração secundária em pacientes. Não foram realizados
estudos clínicos para avaliar os efeitos da clorexidina sobre bactérias orais ou
cáries.
Instruções de utilização:Utilizar para praticamente todas as necessidades de decapagem e colagem emodontologia restauradora para pacientes de todas as idades.
O Peak Universal Bond cola-se aos seguintes materiais:• Dentina e esmalte• Porcelana, zircónia• Metal• Compósito
Instruções de utilização:NOTA: a utilização inicial de Peak SE requer a
ativação de dois componentes separados na
seringa JetMix™.
1) Peak SE permanece estável durante 120 dias
após a ativação.
2) Inscrever a data de validade na área plana dahaste do êmbolo antes da ativação.
3) NÃO REMOVER A TAMPA LUER LOCK ANTES DE
PROCEDER À MISTURA
4) Premir o êmbolo “datado” no cilindro central
rapidamente e com força.
5) Verificar se o êmbolo está nivelado com ocilindro central.
Técnica de adesão direta e reparação deporcelana/zircónia
1.Preparação
a) Dentina/esmalte: isolar, limpar e removera cárie assegurando que toda a dentina
não mineral é removida (recomenda-se Seek/Sable Seek). Para as
preparações de abrasão/abfração de Classe V, desbastar com uma broca
de diamante.
b) Compósito: remover as áreas enfraquecidas de compósito existente.
Desbastar a superfície com uma broca de diamante.
c) Metal: proceder à microabrasão da superfície.
d) Zircónia: limpar a superfície e remover a zircónia enfraquecida com uma
broca de diamante.
e) Porcelana: desbastar e retirar a porcelana enfraquecida com uma broca
de diamante. Limpar a área de porcelana fraturada durante 5 segundos
com Ultra-Etch. Enxaguar e secar.
2.Condicionamentoa) Técnica de autocondicionamento – dentina/esmalte, compósito e metali. Enxaguar a preparação e deixar húmida.
ii. OPCIONAL - Aplicar Consepsis™ (onde disponível) com uma Black
Mini™ Brush Tip na preparação com um movimento de escovagem e
secar ligeiramente com ar deixando a superfície húmida.
iii. Aplicar Peak SE com a Black Mini Brush Tip na preparação do dente
durante 20 segundos utilizando agitação contínua na dentina. NãoPTfriccionar o esmalte.
iv. Alisar/secar durante 3 segundos utilizando uma seringa de ar/água ou aplicando a aspiração de alto volume diretamente sobrea preparação.
v. Continuar com o passo “Adesão” abaixo.
b) Técnica de condicionamento total – dentina/esmalte, compósito e metal
i. Verifique a cor e a consistência do produto escoado antes de aplicar,
depositando uma quantidade pequena em uma placa ou gaze.
Descarte o líquido claro quando esse for exposto.
ii. Aplicar Ultra-Etch com a Blue Micro™ Tip em todas as superfícies dapreparação do dente durante 20 segundos.
iii. Enxaguar abundantemente durante 5 segundos.
iv. Secar ligeiramente utilizando uma seringa de ar/água ou aplicando
a aspiração de alto volume diretamente sobre a preparação. Deixar
a superfície ligeiramente húmida.
v. OPCIONAL - Aplicar Consepsis (onde disponível) com uma Black Mini
Brush Tip na preparação com um movimento de escovagem e secar
ligeiramente com ar deixando a superfície húmida.
vi. Continuar com o passo “Adesão” abaixo.
c) Condicionamento de porcelana – CUIDADO – na utilização de ácido
fluorídrico (HF) (Ultradent™ Porcelain Etch) utilizar um isolamento
adequado, tal como uma barreira neutralizadora de ácido (EtchArrest™).
Não permitir o contacto do ácido fluorídrico com as gengivas e dentina.
i. Aplicar ácido fluorídrico na área fraturada durante 90 segundos.
ii. Aspirar o ácido da superfície, EM SEGUIDA enxaguar
abundantemente e secar.
iii. Aplicar Ultra-Etch durante 5 segundos para remover os sais deporcelana e resíduos formados pelo condicionamento com HF.
Enxaguar e secar.
iv. Aplicar uma camada abundante de silano durante 60 segundos.
v. Secar bem. NÃO ENXAGUAR.
vi. Continuar com o passo “Adesão” abaixo.
d) Zircónia – NÃO CONDICIONAR NEM UTILIZAR SILANO
i. Realizar abrasão com ar da superfície fraturada da prótese,enxaguar e secar.
ii. Aplicar primário de zircónia na área fraturada de acordo com as
instruções do fabricante.
iii. Continuar com o passo “Adesão” abaixo.
3.Adesão
a) Apresentação em frasco
i. Dispense de uma a três gotas do Peak™ Universal Bond no lado “B”
do pote Dappen descartável.
ii. Usando o Micro Applicator Brush, aplique uma camada do Peak™
Universal Bond no preparo e esfregue suavemente por dez
segundos.
iii. Seque por dez segundos usando de ¼ a ½ da pressão de ar. O
preparo deve ter uma aparência brilhante.
iv. Fotopolimerize por dez segundos (ou por vinte segundos com fontes
de luz inferiores a 600mW/cm2).
v. Restaure com resina fluida ou compactável, de acordo com as
instruções do fabricante.
b) Apresentação em seringa
i. Aplique uma camada do Peak™ Universal Bond com a ponta dopincel Inspiral™ e esfregue suavemente por dez segundos.
ii. Seque por dez segundos usando de ¼ a ½ da pressão de ar. O
preparo deve ter uma aparência brilhante.
iii. Fotopolimerize por dez segundos (ou por vinte segundos com fontes
de luz inferiores a 600mW/cm2).
iv. Restaure com resina fluida ou compactável, de acordo com as
instruções do fabricante.
Técnica de adesão indireta – Coroas, inlays, onlays, indiretos dezircónia
1.Preparação
a) Remover o provisório, limpar a preparação, enxaguar e secar (Consepsis

19

20

Scrub com uma StarBrush™ para limpar, desinfetar e remover cimento
residual).
b) Verificar a adaptação da prótese.
c) Preparar a superfície interior da prótese.
i. À base de metal:
1. Realizar a microabrasão (jato de areia) da superfície interior da
prótese.
2. Enxaguar e secar a superfície.
ii. Cerâmica / porcelana:
1. Aplicar ácido fluorídrico (HF) (Ultradent Porcelain Etch) na superfícieinterior da prótese durante 90 segundos, enxaguar e secar.
2. Aplicar Ultra-Etch durante 5 segundos para remover os sais deporcelana e resíduos formados pelo condicionamento com HF.
Enxaguar e secar.
3. Aplicar silano (Ultradent™ Silane) na superfície interior da prótese
durante 1 minuto, secar e colocar a prótese de parte. Não
enxaguar.
iii. Zircónia: NÃO CONDICIONAR NEM UTILIZAR SILANO
1. Realizar abrasão com ar da superfície interna da prótese, enxaguar
e secar.
2. Aplicar um primário de zircónia segundo as instruções dofabricante.
2.Condicionamento - Preparar a superfície do dentea) Técnica de autocondicionamento – dentina/esmalte, compósito e metali. Enxaguar a preparação e deixar húmida.
ii. OPCIONAL - Aplicar Consepsis (onde disponível) com uma Black Mini
Brush Tip na preparação com um movimento de escovagem e secar
ligeiramente com ar deixando a superfície húmida.
iii. Aplicar Peak™ SE com uma Black Mini™ Brush Tip durante 20
segundos na preparação do dente utilizando agitação contínua na
dentina. Não friccionar o esmalte.
iv. Alisar/secar durante 3 segundos utilizando uma seringa de ar/água ou aplicando a aspiração de alto volume diretamente sobre a
preparação.
v. Continuar com o passo “Adesão” abaixo.
b) Técnica de condicionamento total – dentina/esmalte, compósito e metal
i. Aplicar Ultra-Etch com a Blue Micro Tip em todas as superfícies dapreparação do dente durante 20 segundos.
ii. Enxaguar abundantemente durante 5 segundos.
iii. Secar ligeiramente utilizando uma seringa de ar/água ou aplicando
a aspiração de alto volume diretamente sobre a preparação. Deixar asuperfície ligeiramente húmida.
iv. OPCIONAL - Aplicar Consepsis (onde disponível) com uma Black Mini
Brush Tip na preparação com um movimento de escovagem e secar
ligeiramente com ar deixando a superfície húmida.
v. Continuar com o passo “Adesão” abaixo.
c) Condicionamento de porcelana – CUIDADO – na utilização de ácido
fluorídrico (HF) (Ultradent Porcelain Etch) utilizar um isolamento
adequado, tal como uma barreira neutralizadora de ácido (EtchArrest).
Não permitir o contacto do ácido fluorídrico com as gengivas e dentina.
i. Aplicar ácido fluorídrico na área fraturada durante 90 segundos.
ii. Aspirar o ácido da superfície, EM SEGUIDA enxaguar
abundantemente e secar.
iii. Aplicar Ultra-Etch durante 5 segundos para remover os sais deporcelana e resíduos formados pelo condicionamento com HF.
Enxaguar e secar.
iv. Aplicar uma camada abundante de silano durante 60 segundos.
v. Secar bem. NÃO ENXAGUAR.
vi. Continuar com o passo “Adesão” abaixo.
d) Zircónia – NÃO CONDICIONAR NEM UTILIZAR SILANO
i. Realizar abrasão com ar da superfície interna da prótese, enxaguar
e secar.
ii. Aplicar primário de zircónia na área fraturada de acordo com as
instruções do fabricante.
iii. Continuar com o passo “Adesão” abaixo.
3.Adesão
a) Apresentação em frasco
i. Dispensar 1-3 gotas de Peak Universal Bond no lado “B” do pote

Dappen descartável.
Utilizando a escova Micro Applicator Brush, aplicar uma camada
abundante de Peak Universal Bond na preparação e agitar
cuidadosamente durante 10 segundos.
iii. Seque por dez segundos usando a pressão de ar total. O preparo
deve ter uma aparência brilhante.
iv. Fotopolimerizar durante 10 segundos (20 segundos para luzes com
potência <600mW/cm2).
b. Apresentação em seringa
i. Aplique uma camada do Peak™ Universal Bond com a ponta do pincel
Inspiral™ e esfregue suavemente por dez segundos.
ii. Seque por dez segundos usando a pressão de ar total. O preparo
deve ter uma aparência brilhante.
iii. Fotopolimerize por dez segundos (ou por vinte segundos com fontes
de luz inferiores a 600mW/cm2).
4.Cimentação
a) Aplicar cimento fotopolimerizável para facetas translúcidas ou cimento deresina de dupla polimerização em outras próteses e seguir as instruções
de utilização do fabricante.
NOTA: a selagem imediata da dentina requer os passos 2A e 3 acima
da Técnica direta. Aplicar glicerina sobre o Peak Universal Bond e
fotopolimerizar durante 10 segundos. Enxaguar a glicerina. Proceder à
impressão final. Reaplicar glicerina no preparado como um agente deseparação, antes da cimentação do provisório.
ii.

Reparo de resina/metal/zircônia/porcelana
1. Resina: Remova as áreas enfraquecidas da resina existente. Torne asuperfície áspera com uma broca diamantada.
a) Técnica de condicionamento ácido total
i. Aplique o Ultra-Etch com a Blue Micro Tip em todas as superfícies do
preparo do dente por vinte segundos.
ii. Lave bastante por cinco segundos e deixe o preparo úmido.
2. Metal: Faça uma microabrasão na superfíciea) Técnica de condicionamento ácido total
i. Aplique o Ultra-Etch com a Blue Micro Tip em todas as superfícies do
preparo do dente por vinte segundos.
ii. Lave bastante por cinco segundos e deixe o preparo úmido.
3. Zircônia: Limpe a superfície; remova a zircônia enfraquecida com uma
broca diamantada. NÃO FAÇA CONDICIONAMENTO ÁCIDO OU USE SILANO.
a) Execute o jateamento de ar na superfície interna da prótese.
b) Aplique o primer de zircônia na área fraturada seguindo as instruções
do fabricante.
4. Porcelana: Torne a superfície áspera e remova a porcelana enfraquecida
com uma broca diamantada. Limpe a área de fratura da porcelana por
quinze segundos com o Ultra-Etch. Lave e seque.
CUIDADO - use um isolamento adequado como uma barreira
neutralizadora de ácido (EtchArrest) ao usar o ácido fluorídrico (HF)
(Ultradent™ Porcelain Etch). Não deixe o ácido fluorídrico ter contato com agengiva ou com a dentina.
a) Aplique o ácido fluorídrico na área fraturada por noventa segundos.
b) Aspire o ácido da superfície e, em seguida, lave bastante e seque asuperfície.
c) Aplique o Ultra-Etch por cinco segundos para remover os sais da porcelana
e os debris formados pelo condicionamento com ácido fluorídrico. Lavee seque.
d) Aplique uma camada de silano por um minuto.
e) Seque completamente. NÃO LAVE.
5. Adesivoa) Apresentação em frasco
i. Dispense de uma a três gotas do Peak™ Universal Bond no lado “B”
do pote Dappen descartável.
ii. Usando o Micro Applicator Brush , aplique uma camada do Peak™
Universal Bond e esfregue suavemente por dez segundos.
iii. Seque por dez segundos usando de ¼ a ½ da pressão de ar. O
preparo deve ter uma aparência brilhante.
iv. Fotopolimerize por dez segundos (ou por vinte segundos com fontes
de luz inferiores a 600mW/cm2).
b) Apresentação em seringa

i. Aplique uma camada do Peak™ Universal Bond com a ponta do pincel
Inspiral™ e esfregue suavemente por dez segundos.
ii. Seque por dez segundos usando de ¼ a ½ da pressão de ar.
iii. O preparo deve ter uma aparência brilhante.
iv. Fotopolimerize por dez segundos (ou por vinte segundos com fontes
de luz inferiores a 600mW/cm2).
6. Restaure com resina fluida ou compactável, de acordo com as instruções
do fabricante.
Pino e núcleo
1.Preparação
a) Furar o furo para o pino utilizando um batente de borracha e uma broca
UniCore™ de tamanho adequado.
b) Enxaguar abundantemente o espaço do pino durante 10 segundos
utilizando o adaptador TriAway e uma ponta Endo-Eze Tip calibre 22.
Secar com o adaptador TriAway e ponta Endo-Eze Tip calibre 22g a partir
da base da preparação em sentido ascendente.
c) Verificar a adaptação do pino (UniCore Post) e cortar até ao tamanhopretendido utilizando um disco de diamante de alta velocidade.
NOTA: Brocas de carboneto e brocas cirúrgicas podem fragilizar as fibras.
2.Condicionamentoa) Técnica de autocondicionamento:
i. Enxaguar o espaço do canal e deixar húmido.
ii. Aplicar uma ponta Deliver-Eze™ Brush Tip azul calibre 22 na seringa
Peak SE.
iii. Aplicar no espaço do pino e na preparação coronária durante 20
segundos utilizando uma ação de agitação.
iv. Soprar o excesso com o adaptador TriAway e uma ponta Endo-Eze
Tip calibre 22, a partir da base do espaço em sentido ascendente.
Alisar/secar durante 3 segundos utilizando uma seringa de ar/água ou aplicando a aspiração de alto volume diretamente sobre a
preparação.
v. Continuar com o passo “Adesão” abaixo.
b) Técnica de condicionamento total:
i. Aplicar uma ponta Endo-Eze Tip calibre 22 azul na seringa Ultra-Etch.
ii. Começar apicalmente e encher o espaço do pino coronariamente.
Aplicar na preparação coronária. Condicionar durante 20 segundos.
iii. Aspirar o condicionador em excesso.
iv. Utilizando o adaptador TriAway e a ponta Endo-Eze Tip calibre 22
enxaguar abundantemente e secar ligeiramente com ar deixando oespaço do pino ligeiramente húmido.
v. Continuar com o passo “Adesão” abaixo.
3.Adesão
a) Apresentação em frasco
i. Dispensar 1-3 gotas de Peak Universal Bond no lado “B” do pote
Dappen descartável.
ii. Utilizando a Nano-Brush™ ou NaviTip FX, aplicar Peak Universal Bondno espaço do pino e agitar cuidadosamente ao longo de todo ocomprimento do canal e incluindo todo o preparo do dente durante
10 segundos.
iii. Retirar muito bem o excesso utilizando o adaptador TriAway e aponta Endo-Eze Tip calibre 22.
iv. Alisar/secar a preparação exterior durante 10 segundos utilizandopressão de ar ¼ a ½. O preparo deve ter um aspeto brilhante.
v. Fotopolimerizar em sentido descendente ao longo do espaço dopino durante 20 segundos (40 segundos para luzes de potência
<600mW /cm2).
vi. Utilizar uma ponta de papel ou pino previamente adaptado paraverificar se o espaço do pino não está bloqueado.
b) Apresentação em seringa
i. Encaixe uma ponta 30ga NaviTip FX na seringa do Peak Universal
Bond.
ii. Coloque de uma a duas gotas no espaço do pino e no preparo e, em
seguida, esfregue em todo o comprimento do canal, incluindo todo opreparo do dente, por dez segundos.
iii. Remova totalmente o excesso do Peak Universal Bond usando oadaptador TriAway e a ponta 22ga Endo-Eze.
iv. Seque o espaço do pino e o preparo com ar por dez segundosv.

usando a pressão de ar total para secar o adaptador TriAway e aponta 22ga Endo-Eze para evaporar o solvente remanescente debaixo para cima.
Fotopolimerize o espaço do pino por vinte segundos (ou porquarenta segundos com fontes de luz inferiores a 600mW/cm2). Usecones de papel ou pinos ajustados previamente para verificar se oespaço do pino não está bloqueado.

Cimentação do pino e formação do núcleo
1) Retirar a tampa da seringa PermaFlo™ DC.
2) Aplicar uma ponta de mistura na seringa de cilindro duplo alinhando as
duas portas. Rodar no sentido dos ponteiros do relógio até engatar.
3) Aplicar a Intraoral Tip™ flexível na ponta de mistura para a aplicação direta
no canal a partir da seringa de cilindro duplo.
4) Dispensar uma pequena quantidade antes da colocação no espaço do pino.
5) Inserir a ponta no espaço do pino até ao comprimento total.
6) Aplicar PermaFlo DC começando apicalmente e deslocando-se no sentido
coronário utilizando uma pressão uniforme.
7) Inserir o pino (UniCore™ Post) lentamente, deslocando o cimento em
excesso.
8) Colocar a luz de polimerização diretamente acima do pino e fotopolimerizar
durante 20 segundos; 40 segundos para luzes com potência <600mW/
cm2).
9) Continuar a formação de camadas de PermaFlo™ DC à volta do pino
conforme necessário. NOTA: Fotopolimerizar durante 5 segundos
entre camadas para polimerizar o gel e formar o núcleo. Realizar uma
polimerização final no núcleo durante 40 segundos. Não retirar a ponta demistura até à próxima utilização. Desinfetar a seringa e a ponta de mistura.
Precauções e advertências:
1. Ler atentamente e compreender todas as instruções antes da utilização do
Peak Universal Bond.
2. Destina-se apenas à utilização profissional.
3. Colocar novamente a tampa a seguir à utilização para evitar apolimerização.
4. Verificar sempre o fluxo dos materiais da seringa antes da aplicação
intraoral. Em caso de resistência, substituir a ponta e verificar novamente.
5. Manter as tampas no frasco até à utilização.
6. Os médicos e pacientes devem usar proteção ocular UV na polimerização
de materiais de resina.
7. Se não utilizado diariamente, refrigerar o produto.
8. Deixar os produtos refrigerados atingir a temperatura ambiente antes dautilização.
9. Para otimizar a força de adesão utilizar ar isento de óleo e sem humidade.
10. Redirecionar o foco odontológico para evitar a polimerização prematurade todos os materiais à base de resina.
11. As resinas podem ser sensibilizantes. Evitar o contacto repetido de resina
dentária não polimerizada com a pele. Não utilizar em pacientes com
sensibilidade conhecida a acrilatos ou outras resinas. Em caso de reação
alérgica, dermatite ou se surgir erupção cutânea, consultar um médico.
12. Descartar as pontas, seringas vazias e frascos de forma adequada.
13. Manter fora do alcance das crianças.
14. Não utilizar após a data de validade anotada no recipiente.
15. Entre utilizações recolocar a tampa, desinfetar e limpar a seringa com um
desinfetante de nível intermédio. Se for utilizada uma cobertura de seringa
descartável, retirar a ponta, recolocar a tampa e descartar a coberturada seringa.
16. As pontas são descartáveis. Para evitar a contaminação cruzada, nãoreutilizar as pontas.
17. Manter os produtos afastados de calor/luz solar direta.
18. Isolar a área de tratamento contra químicos fortes.
OBSERVAÇÃO: Para obter SDS e informações adicionais sobreo uso do Peak Universal Bond, Peak SE e de outros produtos
relacionados, visite o site www.ultradent.com.visite www.
ultradent.com
21

SV

Peak™ Universal Bond och Peak™ SE

Beskrivning:
Peak Universal Bond är ett bondingharts som levereras i flaska eller i en singelspruta.
Det kan användas med självets eller med totalets. Det är till 7,5 % fyllt med entransportör av etylalkohollösningsmedel och härdas med de flesta högintensiva ljus
inklusive LED-ljus. Peak Universal Bond innehåller 0,2 % klorhexidin som kan garanteralångvarig bondingstyrka.
Peak SE Primer är ett självetsande dentinbondingharts som består av etsningsmedeloch primer i ett sprutinföringssystem.
Ultra-Etch™ är ett etsnings- och sköljningsgel med 35 % fosforsyra som levereras ien spruta.
Inkluderandet av tillsatsämnet klorhexidin har inte visat sig korrelera med en minskning
av sekundär röta hos patienter. Kliniska studier för att evaluera effekterna av klorhexidin
på orala bakterier eller karies har inte utförts.
Användningsindikationer:
Används för praktiskt taget alla etsnings- och bindningsbehov i restaurerande tandvård
för patienter i alla åldrar.
Peak Universal Bond binder till följande material:• Dentin och emalj• Porslin, zirconia• Metall• Komposit
Bruksanvisning:
OBS: Första användning av Peak SE kräver
aktivering av de två komponenterna som äråtskilda i JetMix™-sprutan.
1) Peak SE är stabilt i 120 dagar efter aktivering.
2) Skriv utgångsdatum på den släta ytan i kolvskaftet
före aktiveringen.
3) AVLÄGSNA INTE LUER-LOCK-LOCKET FÖREBLANDNING.
4) Pressa snabbt och kraftfullt den “daterade” kolven in iden mellersta cylindern.
5) Kontrollera att kolven är i jämnhöjd med denmellersta cylindern.

22

Direkt bondingteknik och porslins-/
zirconiareparation
1.Förbereda) Dentin/emalj: Isolera, rengör och avlägsna karies
och kontrollera att allt icke mineralt dentin har
avlägsnats (Seek/Sable Seek rekommenderas för
detta). Gör ytan grövre med en diamantborr för abrasion/abfraktion av klass
V preparat.
b) Komposit: Avlägsna bestående kompositers försvagade områden. Gör ytan
grövre med diamantborr.
c) Metall: Mikroabradera ytan.
d) Zirconia: Rengör ytan och avlägsna försvagad zirconia med en diamantborr.
e) Porslin: Gör ytan grövre och avlägsna försvagat porslin med en diamantborr.
Rengör ett sprucket porslinsområde i 5 sekunder med
Ultra-Etch. Skölj och torka.
2.Etsa) Självetsningsteknik - dentin/emalj, komposit och metall
i. Skölj preparatet och lämna det fuktigt.
ii. VALFRITT - Applicera Consepsis™ (där det är tillgängligt) med Black Mini™
Brush Tip på preparatet med en skrubbande rörelse och lufttorka lätt och
lämna ytan fuktig.
iii. Applicera Peak SE med Black Mini Brush Tip i 20 sekunder på
tandpreparatet under ständig omrörning på dentinet. Skrubba inte
emaljen.
iv. Tunna ut/torka i 3 sekunder genom att använda en luft/vattenspruta eller

genom att placera sug med hög volym direkt ovanför preparatet.
v. Övergå till steget “Bonding” nedan.
b) Totaletsningsteknik - dentin/emalj, komposit och metall
i. Kontrollera färgen och konsistensen på produktflödet före applicering
genom att trycka ut en liten mängd på en blandningsdyna eller gasväv.
Kassera all klar vätska som trycks ut.
ii. Applicera Ultra-Etch med Blue Micro Tip™ på alla tandpreparatets ytor i
20 sekunder.
iii. Skölj grundligt i 5 sekunder.
iv. Torka lätt genom att använda en luft/vattenspruta eller genom att placera
sug med hög volym direkt ovanför preparatet. Lämna ytan något fuktig.
v. VALFRITT - Applicera Consepsis (där det är tillgängligt) med Black Mini
Brush Tip på preparatet med en skrubbande rörelse och lufttorka lätt och
lämna ytan fuktig.
vi. Övergå till steget “Bonding” nedan.
c) Porslinets – VARNING – använd ordentlig isolering såsom en syraneutraliserandebarriär (EtchArrest™) då fluorvätesyra (HF) (Ultradent™ Porcelain Etch) används.
Tillåt inte att fluorvätesyra vidrör gingiva eller dentin.
i. Applicera fluorvätesyra på det spruckna området i 90 sekunder.
ii. Sug syra från ytan, skölj och torka SEDAN ytan noggrant.
iii. Applicera Ultra-Etch i 5 sekunder för att avlägsna porslinssalter och skräp
som bildats genom etsning med HF. Skölj och torka.
iv. Applicera en tjock hinna silan i 60 sekunder.
v. Torka noggrant. SKÖLJ INTE.
vi. Övergå till steget “Bonding” nedan.
d) Zirconia – ANVÄND INTE ETS ELLER SILAN
i. Luftskrubba protesens spruckna yta, skölj och torka.
ii. Applicera zirconia primer på sprucket område enligt tillverkarens
anvisningar.
iii. Övergå till steget “Bonding” nedan.
3.Bondinga) Flaskdispensering
i. Tryck 1-3 droppar Peak™ Universal Bond in i “B”-sidan av en dappen dishför engångsbruk.
ii. Applicera på preparatet en tjockare hinna av Peak™ Universal Bond med
Micro Applicator Brush och rör försiktigt om i 10 sekunder.
iii. Tunna ut/torka i 10 sekunder genom att använda ¼ till ½ lufttryck.
Preparatet bör se glansigt ut.
iv. Ljushärda i 10 sekunder (i 20 sekunder för ljus med en energiutveckling< 600 mW/cm2).
v. Restaurera med flytande eller packbar komposit enligt tillverkarens
anvisningar.
b) Sprutdispensering
i. Applicera en tjockare hinna av Peak™ Universal Bond med Inspiral™ Brush
Tip – rör försiktigt om i 10 sekunder.
ii. Tunna ut/torka i 10 sekunder genom att använda ¼ till ½ lufttryck.
iii. Ljushärda i 10 sekunder (i 20 sekunder för ljus med en energiutveckling< 600 mW/cm2).
iv. Restaurera med flytande eller packbar komposit enligt tillverkarens
anvisningar.
Indirekt bondingteknik – indirekta kronor, inlägg, onlay, zirconia
1.Förbereda) Avlägsna temporära rena preparat, skölj och torka (Consepsis Scrub med en
StarBrush™ för att rengöra, desinficera och avlägsna överbliven cement).
b) Kontrollera att protesen passar.
c) Förbered protesens inre yta.
i. Metallbaserad:(1) Mikroabradera (sandblästra) protesens inre yta.
(2) Skölj och torka ytan.
ii. Keramik/porslin:(1) Applicera fluorvätesyra (HF) (Ultradent™ Porcelain Etch) på protesens inre
yta i 90 sekunder, skölj och torka.
(2) Applicera Ultra-Etch i 5 sekunder för att avlägsna porslinssalter och skräp
som bildats genom etsning med HF. Skölj och torka.

(3) Applicera silan (Ultradent™ Silane) på protesens inre yta i 1 minut, torka
och lägg protesen åt sidan. Skölj inte.
iii. Zirconia: ANVÄND INTE ETS ELLER SILAN(1) Luftskrubba protesens inre yta, skölj och torka.
(2) Applicera zirconia primer enligt tillverkarens anvisningar.
2.Ets - Förbered tandens ytaa) Självetsningsteknik - dentin/emalj, komposit och metall
i. Skölj preparatet och lämna det fuktigt.
ii. VALFRITT - Applicera Consepsis (där det är tillgängligt) med Black Mini™
Brush Tip på preparatet med en skrubbande rörelse och lufttorka lätt och
lämna ytan fuktig.
iii. Applicera Peak™ SE med Black Mini™ Brush Tip - i 20 sekunder på
tandpreparatet under ständig omrörning på dentinet. Skrubba inte emaljen.
iv. Tunna ut/torka i 3 sekunder genom att använda en luft/vattenspruta eller
genom att placera sug med hög volym direkt ovanför preparatet.
v. Övergå till steget “Bonding” nedan.
b) Totaletsningsteknik - dentin/emalj, komposit och metall
i. Applicera Ultra-Etch med Blue Micro Tip på alla tandpreparatets ytor i 20
sekunder.
ii. Skölj grundligt i 5 sekunder.
iii. Torka lätt genom att använda en luft/vattenspruta eller genom att placera
sug med hög volym direkt ovanför preparatet. Lämna ytan något fuktig.
iv. VALFRITT - Applicera Consepsis (där det är tillgängligt) med Black Mini
Brush Tip på preparatet med en skrubbande rörelse och lufttorka lätt och
lämna ytan fuktig.
v. Övergå till steget “Bonding” nedan.
c) Porslinets – VARNING – använd ordentlig isolering såsom en syraneutraliserandebarriär (EtchArrest™) då fluorvätesyra (HF) (Ultradent™ Porcelain Etch) används.
Tillåt inte att fluorvätesyra vidrör gingiva eller dentin.
i. Applicera fluorvätesyra på det spruckna området i 90 sekunder.
ii. Sug syra från ytan, skölj och torka SEDAN ytan noggrant.
iii. Applicera Ultra-Etch i 5 sekunder för att avlägsna porslinssalter och skräp
som bildats genom etsning med HF. Skölj och torka.
iv. Applicera en tjock hinna silan i 60 sekunder.
v. Torka noggrant. SKÖLJ INTE.
vi. Övergå till steget “Bonding” nedan.
d) Zirconia – ANVÄND INTE ETS ELLER SILAN
i. Luftskrubba protesens inre yta, skölj och torka.
ii. Applicera zirconia primer på sprucket område enligt tillverkarens
anvisningar.
iii. Övergå till steget “Bonding” nedan.
3.Bondinga) Flaskdispensering
i. Tryck 1-3 droppar Peak Universal Bond in i “B”- sidan av en dappen dishför engångsbruk.
ii. Applicera på preparatet en tjockare hinna av Peak Universal Bond med Micro
Applicator Brush och rör försiktigt om i 10 sekunder.
iii. Tunna ut/torka i 10 sekunder genom att använda fullt lufttryck. Preparatet
bör se glansigt ut.
iv. Ljushärda i 10 sekunder (i 20 sekunder för ljus med en energiutveckling <600 mW/cm2).
b) Sprutdispensering
i. Applicera en tjockare hinna av Peak™ Universal Bond med Inspiral™ Brush
Tip – rör försiktigt om i 10 sekunder.
ii. Tunna ut/torka i 10 sekunder genom att använda fullt lufttryck. Preparatet
bör se glansigt ut.
iii. Ljushärda i 10 sekunder (i 20 sekunder för ljus med en energiutveckling <600 mW/cm2).
4.Cementa) Applicera ljushärdningscement för genomskinliga fasader eller
dubbelhärdningscement för andra proteser och följ tillverkarens anvisningar.
OBS: Omedelbar dentinförsegling kräver steg 2A och 3 i direkt teknik ovan.
Applicera glycerin över Peak Universal Bond och ljushärda i 10 sekunder. Skölj
glycerinet. Gör det slutliga avtrycket Applicera på nytt glycerin på preparatet som
ett separationsmedium före cementering av det provisoriet på plats.
Reparation av komposit/metall/zirconia/porslin
1. Komposit: Avlägsna bestående kompositers försvagade områden. Gör ytan grövre

med diamantborr.
a) Totaletsningsteknik
i. Applicera Ultra-Etch med Blue Micro Tip på alla tandpreparatets ytor i 20
sekunder.
ii. Skölj grundligt i 5 sekunder och lämna fuktigt.
2. Metall: Mikroabradera ytana) Totaletsningsteknik
i. Applicera Ultra-Etch med Blue Micro Tip på alla tandpreparatets ytor i 20
sekunder.
ii. Skölj grundligt i 5 sekunder och lämna fuktigt.
3. Zirconia: Rengör ytan. Avlägsna försvagad zirconia med en diamantborr. ANVÄND
INTE ETS ELLER SILANa) Luftskrubba protesens inre yta.
b) Applicera zirconia primer på sprucket område enligt tillverkarens anvisningar.
4. Porslin: Gör ytan grövre och avlägsna försvagat porslin med en diamantborr.
Rengör ett sprucket porslinsområde i 15 sekunder med Ultra-Etch. Skölj och torka.
VARNING – använd ordentlig isolering såsom en syraneutraliserande barriär(EtchArrest) då fluorvätesyra (HF) (Ultradent™ Porcelain Etch) används. Tillåt inte att
fluorvätesyra vidrör gingiva eller dentin.
a) Applicera fluorvätesyra på det spruckna området i 90 sekunder.
b) Sug syra från ytan, skölj och torka sedan ytan noggrant.
c) Applicera Ultra-Etch i 5 sekunder för att avlägsna porslinssalter och skräp som
bildats genom etsning med HF. Skölj och torka.
d) Applicera en tjock hinna silan i 1 minut.
e) Torka noggrant. SKÖLJ INTE.
5. Bondinga)Flaskdispensering
i. Tryck 1-3 droppar Peak™ Universal Bond in i “B”-sidan av en dappen dishför engångsbruk.
ii. Applicera på preparatet en tjockare hinna av Peak™ Universal Bond med
Micro Applicator Brush och rör försiktigt om i 10 sekunder.
iii. Tunna ut/torka i 10 sekunder genom att använda ¼ till ½ lufttryck.
Preparatet bör se glansigt ut.
iv. Ljushärda i 10 sekunder (i 20 sekunder för ljus med en energiutveckling <600 mW/cm2).
b) Sprutdispensering
i. Applicera en tjockare hinna av Peak™ Universal Bond med Inspiral™ Brush
Tip – rör försiktigt om i 10 sekunder.
ii. Tunna ut/torka i 10 sekunder genom att använda ¼ till ½ lufttryck.
iii. Preparatet bör se glansigt ut.
iv. Ljushärda i 10 sekunder (i 20 sekunder för ljus med en energiutveckling <600 mW/cm2).
6. Restaurera med flytande och/eller packbar komposit enligt tillverkarens anvisningar.
Reparation av komposit/metall/zirconia/porslin
1. Komposit: Avlägsna bestående kompositers försvagade områden. Gör ytan grövre
med diamantborr.
a) Totaletsningsteknik
i. Applicera Ultra-Etch med Blue Micro Tip på alla tandpreparatets ytor i 20
sekunder.
ii. Skölj grundligt i 5 sekunder och lämna fuktigt.
2. Metall: Mikroabradera ytana) Totaletsningsteknikiii. Applicera Ultra-Etch med Blue Micro Tip på alla tandpreparatets ytor i 20
sekunder.
iv. Skölj grundligt i 5 sekunder och lämna fuktigt.
3. Zirconia: Rengör ytan. Avlägsna försvagad zirconia med en diamantborr. ANVÄND
INTE ETS ELLER SILANa) Luftskrubba protesens inre yta.
b) Applicera zirconia primer på sprucket område enligt tillverkarens anvisningar.
4. Porslin: Gör ytan grövre och avlägsna försvagat porslin med en diamantborr.
Rengör ett sprucket porslinsområde i 15 sekunder med Ultra-Etch. Skölj och torka.
VARNING – använd ordentlig isolering såsom en syraneutraliserande barriär(EtchArrest) då fluorvätesyra (HF) (Ultradent™ Porcelain Etch) används. Tillåt inte att
fluorvätesyra vidrör gingiva eller dentin.
a) Applicera fluorvätesyra på det spruckna området i 90 sekunder.
b) Sug syra från ytan, skölj och torka sedan ytan noggrant.
c) Applicera Ultra-Etch i 5 sekunder för att avlägsna porslinssalter och skräp som23

bildats genom etsning med HF. Skölj och torka.
d) Applicera en tjock hinna silan i 1 minut.
e) Torka noggrant. SKÖLJ INTE.
5. Bondinga) Flaskdispensering
i. Tryck 1-3 droppar Peak™ Universal Bond in i “B”-sidan av en dappen dishför engångsbruk.
ii. Applicera på preparatet en tjockare hinna av Peak™ Universal Bond med
Micro Applicator Brush och rör försiktigt om i 10 sekunder.
iii. Tunna ut/torka i 10 sekunder genom att använda ¼ till ½ lufttryck.
Preparatet bör se glansigt ut.
iv. Ljushärda i 10 sekunder (i 20 sekunder för ljus med en energiutveckling <600 mW/cm2).
b) Sprutdispensering
i. Applicera en tjockare hinna av Peak™ Universal Bond med Inspiral™ Brush
Tip – rör försiktigt om i 10 sekunder.
ii. Tunna ut/torka i 10 sekunder genom att använda ¼ till ½ lufttryck.
iii. Preparatet bör se glansigt ut.
iv. Ljushärda i 10 sekunder (i 20 sekunder för ljus med en energiutveckling <600 mW/cm2).
6. Restaurera med flytande och/eller packbar komposit enligt tillverkarens anvisningar.

24

ii.

Placera 1-2 droppar i stiftutrymmet och på preparatet, rör om i kanalenshela längd inkluderande hela tandpreparatet i 10 sekunder.
iii. Avlägsna ordentligt överflödigt Peak™ Universal Bond genom att använda
TriAway Adaptor och en 22 ga Endo-Eze Tip.
iv. Lufttorka stiftutrymmet och preparatet i 10 sekunder med fullt lufttryck för
att tunna ut/torka med TriAway Adaptor och 22 ga Endo-Eze Tip för att alltåterstående lösningsmedel från botten uppåt ska avdunsta.
v. Ljushärda ner i stiftutrymmet i 20 sekunder (i 40 sekunder för ljus med enenergiutveckling <600mW/cm2). Använd en pappersspets eller ett stift som
tidigare har passats in för att kontrollera att stiftutrymmet inte är blockerat.

Stiftcementering och uppbyggnad av pelare
1) Avlägsna locket från PermaFlo™ DC-sprutan.
2) Placera blandarspetsen på sprutan med två cylindrar genom att passa de tvåportarna i linje Vrid medurs tills den är låst på plats.
3) Fäst den flexibla Intraoral Tip™-spetsen på blandarspetsen för direkt införing ikanalen från sprutan med två cylindrar.
4) Tryck ut en liten mängd före placering i stiftutrymmet.
5) För in spetsen ända ner i stiftutrymmet.
6) Spruta in PermaFlo™ DC genom att använda ett jämnt tryck med början apikalt ochi en rörelse koronalt.
7) För in stiftet (UniCore™ Post) långsamt genom att tränga undan överflödigt cement.
Stift och pelare
8) Placera härdningsljuset rakt ovanför stiftet och ljushärda i 20 sekunder (40
1. Förbered
sekunder för ljus med en energiutveckling < 600 mW/cm2).
a) Borra ett stifthål genom att använda en gummistoppare och en UniCore™ Drill
9) Fortsätt att bygga upp lager av PermaFlo™ DC omkring stiftet enligt behov. OBS:
av rätt storlek.
Ljushärda i 5 sekunder mellan lagren för att göra gelet stelt och bilda en pelare.
b) Skölj stiftutrymmet ordentligt i 10 sekunder genom att använda TriAway Adaptor
Ljushärda en sista gång i 40 sekunder. Avlägsna inte blandningsspetsen förrän den
och en 22ga Endo-Eze™ Tip. Torka med TriAway Adaptor och en 22ga Endo-Eze Tip
ska användas nästa gång. Desinficera sprutan och blandarspetsen.
från preparatets botten uppåt.
c) Kontrollera att stiftet (UniCore Post) passar och skär till önskad längd genom att
Försiktighetsåtgärder och varningar:
använda en diamantskiva med hög hastighet. OBS: Karbidoch operationsborrar
1. Läs noga igenom och förstå alla instruktioner före användning av Peak Universal
kan slita fibrerna.
Bond.
2.Ets
2. Endast för användning av tandläkare.
a) Självetsningsteknik
3. Sätt omedelbart locket åter på för att undvika polymerisering.
i. Skölj kanalutrymmet och lämna det fuktigt.
4. Kontrollera alltid sprutans materialflöde före intraoral applicering. Om det finns
ii. Fäst en blå 22ga Deliver-Eze™ Brush Tip på Peak SE-sprutan.
motstånd ska spetsen bytas ut och flödet kontrolleras på nytt.
iii. Applicera i stiftutrymmet och på det koronala preparatet i 20 sekunder
5. Håll lock på flaskan tills den ska användas.
genom att röra om.
6. Läkaren och patienten ska använda UV-skyddsglasögon vid härdning av
iv. Blås bort överflödigt ets med en TriAway Adaptor och en 22ga Endo-Eze
hartsmaterial.
Tip från botten av utrymmet uppåt. Tunna ut/torka i 3 sekunder genom att
7. Förvara produkten i kylskåp om den inte användas dagligen
använda en luft/vattenspruta eller genom att placera sug med hög volym
8. Låt produkten uppnå rumstemperatur före användning.
direkt ovanför preparatet.
9. För att utveckla optimal bondingstyrka ska oljefri, fuktfri luft användas.
v. Övergå till steget “Bonding” nedan.
10. Rikta bort ljus ovanifrån för att förhindra för tidig polymerisering av allab) Totaletsningsteknik:
hartsbaserade material.
i. Fäst en blå 22ga Endo-Eze Tip på Ultra-Etch-sprutan.
11. Harts kan vara sensibiliserande. Undvik att huden kommer i upprepad kontaktii. Börja apikalt och fyll ut stiftutrymmet koronalt. Applicera på det koronala
med ohärdat dentalt harts. Använd inte på patienter med känd känslighet för
preparatet. Etsa i 20 sekunderakrylater eller andra hartser. Om allergisk reaktion, dermatit eller utslag utvecklasiii. Sug bort överflödigt ets.
bör läkare vidtalas.
iv. Skölj ordentligt och lufttorka lätt genom att använda TriAway Adaptor och en 12. Kasta bort spetsar, tomma sprutor och flaskor på korrekt sätt.
22ga Endo-Eze Tip. Lämna stiftutrymmet något fuktigt.
13. Förvaras utom räckhåll för barn.
v. Övergå till steget “Bonding” nedan.
14. Använd inte efter utgångsdatum som finns angivet på behållarna.
3.Bonding
15. Sätt tillbaka locket, desinficera och torka av sprutan med ett intermediärta) Flaskdispensering
desinficeringsmedel mellan användningarna. Om engångssprutskydd används bör
i. Tryck 1-3 droppar Peak Universal Bond in i “B”-sidan av en dappen dish för
locket sättas tillbaka och sprutskyddet kastas.
engångsbruk.
16. Spetsarna är avsedda för engångsbruk. För att undvika korskontamination ska
ii. Applicera i stiftutrymmet Peak Universal Bond med Nano-Brush™ eller
spetsarna inte återanvändas.
NaviTip FX och rör försiktigt om i kanalens hela längd och tandpreparatet
17. Utsätt inte produkterna för värme/solljus.
i 10 sekunder.
18. Isolera starka kemikalier till behandlingsområdet.
iii. Avlägsna ordentligt överflödigt ämne genom att använda TriAway Adaptor
och en 22ga Endo-Eze Tip.
OBS: För materialsäkerhetsblad och ytterligare information om
iv. Tunna ut/torka yttre preparatet i 10 sekunder genom att använda ¼ till ½
användning av Peak™ Universal Bond, Peak™ SE samt andra relaterade
produkter, se www.ultradent.com
lufttryck. Preparatet bör se glansigt ut.
v. Ljushärda ner i stiftutrymmet i 20 sekunder (40 sekunder för ljus med enenergiutveckling < 600 mW/cm2).
vi. Använd en pappersspets eller ett stift som tidigare har passats in för att
kontrollera att stiftutrymmet inte är blockerat.
b) Sprutdispensering
i. Fäst en 30 ga NaviTip FX på Peak™ Universal Bond-sprutan.

Peak™ Universal Bond og Peak™ SE
Beskrivelse:
Peak Universal Bond er et resinbaseret adhæsiv, der leveres i en flaske elleren enkelt sprøjte. Det kan anvendes med Self etch og Total etch. Det er 7,5 %
fyldt med en bærer af et ethanolopløsningsmiddel, og kan lyspolymeriseres
med de fleste lamper med høj intensitet, heriblandt LED’er. Peak Universal Bond
indeholder 2 % klorhexidin, som kan sikre en langvarig bindingsstyrke.
Peak SE Primer er et selvætsende dentinadhæsiv, som består af et ætsemiddel
og en primer i et sprøjtesystem.
Ultra-Etch™ er en æts-og-skyl gel med 35 % fosforsyre i en sprøjte.
Inkludering af klorhexidin som tilsætningsstof har ikke vist sig at korrelere med
en reduktion i sekundær karies. Der er ikke udført kliniske undersøgelser til at
evaluere effekten af klorhexidin på orale bakterier eller karies.
Indikationer:
Anvendes til stort set alle ætsnings- og bindingsbehov i genoprettende
tandpleje til patienter i alle aldre.
Peak Universal Bond binder til følgende materialer:• Dentin eller emalje• Porcelæn, zirconium• Metal• Komposit
Brugsanvisning:BEMÆRK: Ved den første anvendelse af PeakSE aktiveres de to komponenter, der er delt i
JetMix™ sprøjten.
1) Peak SE er stabilt i 120 dage efter aktiveringen.
2) Skriv udløbsdatoen på den flade del påstempelsystemet inden aktivering.
3) LUERLOCK-HÆTTEN MÅ IKKE TAGES AF INDENBLANDINGSTIDSPUNKTET
4) Tryk hurtigt og kraftigt det daterede stempel ned
i den midterste patron.
5) Kontrollér, at stemplet står lige ud for den
midterste patron.
Direkte adhæsivteknik og reparation af
porcelæn/zirconium
1.Præparationa) Dentin/emalje: Tørlæg, rengør og fjern karies.
Kontroller, at al ikke-mineraliseret dentin er
fjernet (Seek/Sable Seek anbefales). Ved abrasion/abfraktion klasse Vpræparationer gøres overfladen ru med et diamantbor.
b) Kompositmateriale: Fjern de svækkede områder af det eksisterende
kompositmateriale. Gør overfladen ru med et diamantbor.
c) Metal: Mikroabrader overfladen.
d) Zirconium: Rengør overfladen, og fjern det svækkede zirconium med etdiamantbor.
e) Porcelæn: Gør overfladen ru, og fjern det svækkede porcelæn med etdiamantbor. Rengør det frakturerede porcelænsområde i 5 sekunder
med Ultra-Etch. Skyl og tør.
2.Ætsninga) Selvætsende teknik – dentin/emalje, kompositmateriale og metali. Skyl præparationen og efterlad den fugtig.
ii. VALGFRIT - Applicer Consepsis™ (hvis tilgængelig) med Black Mini™
penselspids på præparationen med en skrubbende bevægelse og
lufttørring og efterlad overfladen i fugtig tilstand.
iii. Applicer Peak SE med Black Mini penselspids i 20 sekunder påDApræparationen med konstant omrøring på dentinen. Emaljen må
ikke skrubbes.
iv. Udtynd/tør i 3 sekunder med trefunktionssprøjten eller kraftigt sug
direkte over præparationen.
v. Fortsæt til trinet “Adhæsiv” herunder.
b) Total-ætsende teknik – dentin/emalje, kompositmateriale og metal
i. Kontrollér farven og konsistensen af produktet inden anvendelse
ved at trykke en lille smule ud på en blandeblok eller et stykke gaze.
Bortskaf eventuel klar væske, der trykkes ud.
ii. Applicer Ultra-Etch med Blue Micro™ spids på alle overflader af
præparationen i 20 sekunder.
iii. Skyl grundigt i 5 sekunder.
iv. Tør let i 3 sekunder med trefunktionssprøjten eller kraftigt sug
direkte over præparationen. Efterlad overfladen let fugtig.
v. VALGFRIT - Applicer Consepsis (hvis tilgængelig) med Black Mini
penselspids på præparationen med en skrubbende bevægelse og
lufttørring og efterlad overfladen i fugtig tilstand.
vi. Fortsæt til trinet “Adhæsiv” herunder.
c) Porcelain Etch –FORSIGTIG – der skal anvendes hensigtsmæssig isolation
som fx. en syreneutraliserende barriere (EtchArrest™) ved brug af flussyre(Ultradent™ Porcelain Etch). Flussyre må ikke komme i berøring med
gingiva eller dentin.
i. Applicer flussyre på det frakturerede område i 90 sekunder.
ii. Syren suges væk fra overfladen, som DEREFTER skal grundigt skylles
og tørres.
iii. Applicer Ultra-Etch i 5 sekunder for at fjerne porcelænssalte og
debris, der blev dannet ved flussyreætsningen. Skyl og tør.
iv. Applicer et tykt lag Silane i 60 sekunder.
v. Tør grundigt. DER MÅ IKKE SKYLLES.
vi. Fortsæt til trinet “Adhæsiv” herunder.
d) Zirconium - DER MÅ HVERKEN ÆTSES ELLER ANVENDES SILANE
i. Luft-abrader restaureringens frakturerede overflade, skyl efterog tør.
ii. Applicer zirconiumprimer på det frakturerede område ifølge
producentens vejledninger.
iii. Fortsæt til trinet “Adhæsiv” herunder.
3.Adhæsiv
a) Anvendelse af flaskei. Tryk 1-3 dråber Peak™ Universal Bond ned i “B”-siden på
dappenglasset til engangsbrug.
ii. Brug Micro Applicator Brush til at applicere et tykt lag Peak™
Universal Bond på præparationen og forsigtigt røre rundt i det i
10 sekunder.
iii. Udtynd/tør i 10 sekunder med ¼ til ½ lufttryk. Præparationen skal
have et skinnende udseende.
iv. Lyspolymeriser i 10 sekunder (20 sekunder for lamper med en effektpå < 600 mW/cm2).
v. Restaurer med flydende /eller kondenserbart kompositmateriale
ifølge producentens vejledninger.
b. Anvendelse af sprøjte
i. Applicer et tykt lag Peak Universal Bond med Inspiral™ penselspids –rør forsigtigt rundt i det i 10 sekunder.
ii. Udtynd/tør i 10 sekunder med ¼ til ½ lufttryk. Præparationen skal
have et skinnende udseende.
iii. Lyspolymeriser i 10 sekunder (20 sekunder for lamper med en effektpå < 600 mW/cm2).
iv. Restaurer med flydende /eller kondenserbart kompositmateriale
ifølge producentens vejledninger.
Indirekte adhæsivteknik - indirekte kroner, inlays, onlays, zirconium
1.Præparationa) Den temporære restaurering fjernes, præparationen rengøres, skylles og

25

tørres (Consepsis Scrub med en StarBrush™ til at rengøre, desinficere og
fjerne resterende cement).
b) Kontroller restaureringens tilpasning.
c) Præparer restaureringens indvendige overflade.
i. Metalbaseret:(1) Mikroabrader (sandblæs) restaureringens indvendige overflade.
(2) Skyl og tør overfladen.
ii. Keramik/porcelæn:(1) Applicer flussyre (Ultradent Porcelain Etch) på restaureringens
indvendige overflade i 90 sekunder. Skyl og tør.
(2) ApplicerUltra-Etch i 5 sekunder for at fjerne porcelænssalte og
debris, der blev dannet ved flussyreætsningen. Skyl og tør.
(3) Applicer silan (Ultradent™ Silan) på restaureringens indvendige
overflade i et minut. Tør efter, og sæt restaureringen til side. Den
må ikke skylles.
iii. Zirconium: DER MÅ HVERKEN ÆTSES ELLER ANVENDES SILAN(1) Luft-abrader restaureringens indvendige overflade, skyl og tør.
(2) Applicer en zirconiumprimer ifølge producentens anvisninger.
2.Ætsning - Præparer tandoverfladena) Selvætsende teknik – dentin/emalje, kompositmateriale og metali. Skyl præparationen og efterlad den fugtig.
ii. VALGFRIT - Applicer Consepsis (hvis tilgængelig) med Black Mini
penselspids på præparationen med en skrubbende bevægelse og
lufttørring og efterlad overfladen i fugtig tilstand.
iii. Applicer Peak™ SE med Black Mini™penselspids i 20 sekunder påpræparationen med konstant omrøring på dentinen. Emaljen må
ikke skrubbes.
iv. Udtynd/tør i 3 sekunder med trefunktionssprøjten eller kraftigt sug
direkte over præparationen.
v. Fortsæt til trinet “Adhæsiv” herunder.
b) Total-ætsende teknik – dentin/emalje, kompositmateriale og metal
i. Applicer Ultra-Etch med Blue Micro-spids på alle overflader af
præparationen i 20 sekunder.
ii. Skyl grundigt i 5 sekunder.
iii. Tør let med trefunktionssprøjten eller kraftigt sug direkte overpræparationen. Efterlad overfladen let fugtig.
iv. VALGFRIT - Applicer Consepsis (hvis tilgængelig) med Black Mini
penselspids på præparationen med en skrubbende bevægelse og
lufttørring og efterlad overfladen i fugtig tilstand.
v. Fortsæt til trinet “Adhæsiv” herunder.
c) Porcelain Etch –FORSIGTIG – der skal anvendes hensigtsmæssig isolation
som fx. en syreneutraliserende barriere (EtchArrest) ved brug af flussyre(Ultradent Porcelain Etch). Flussyre må ikke komme i berøring med
gingiva eller dentin.
i. Applicer flussyre på det frakturerede område i 90 sekunder.
ii. Syren suges væk fra overfladen, som DEREFTER skal grundigt skylles
og tørres.
iii. Applicer Ultra-Etch i 5 sekunder for at fjerne porcelænssalte og
debris, der blev dannet ved flussyreætsningen. Skyl og tør.
iv. Applicer et tykt lag silan i 60 sekunder.
v. Tør grundigt. DER MÅ IKKE SKYLLES.
vi. Fortsæt til trinet “Adhæsiv” herunder.
d) Zirconium - DER MÅ HVERKEN ÆTSES ELLER ANVENDES SILAN
i. Luft-abrader restaureringens indvendige overflade, skyl og tør.
ii. Applicer zirconiumprimer på det frakturerede område ifølge
producentens vejledninger.
iii. Fortsæt til trinet “Adhæsiv” herunder.
3.Adhæsiv
a) Anvendelse af flaskei. Tryk 1-3 dråber Peak Universal Bond ned i “B”-siden på
dappenglasset til engangsbrug.
ii. Brug Micro Applicator-penslen til at applicere et tykt lag Peak
Universal Bond på præparationen og forsigtigt røre rundt i 10
sekunder.
iii.
Udtynd/tør i 10 sekunder med fuldt lufttryk. Præparationen skal have26

et skinnende udseende.
iv. Lyspolymeriser i 10 sekunder (20 sekunder for lamper med <600
mW/cm2).
b) Anvendelse af sprøjte
i. Applicer et tykt lag Peak™ Universal Bond med Inspiral™ penselspids –rør forsigtigt rundt i 10 sekunder.
ii. Udtynd/tør i 10 sekunder med fuldt lufttryk. Præparationen skal haveet skinnende udseende.
iii. Lyspolymeriser i 10 sekunder (20 sekunder for lamper med en effektpå < 600 mW/cm2).
4.Cementa) Læg lyspolymeriserbar cement på translucente facader eller
dualhærdende resincement på andre restaureringer og følg producentens
vejledninger.
BEMÆRK: Ved immediat dentinforsegling skal trin 2a og 3 i Direkte
teknik ovenfor udføres. Læg et lag glycerin over Peak Universal Bond og
lyspolymeriser i 10 sekunder. Skyl glycerinen af. Tag det endelige aftryk.
Læg et nyt lag glycerin på præparationen som et separationsmiddel inden
cementering af provisoriet.
Reparation af kompositmateriale / metal / zirconium / porcelæn
1. Kompositmateriale: Fjern de svækkede områder af det eksisterende
kompositmateriale. Gør overfladen ru med et diamantbor.
a) Total ætsteknik
i. Applicer Ultra-Etch med Blue Micro Tip på alle overflader af
præparationen i 20 sekunder.
ii. Skyl grundigt i 5 sekunder, og efterlad den præparerede overflade
i fugtig tilstand.
2. Metal: Mikroslib overfladena) Total ætsteknik
i. Applicer Ultra-Etch med Blue Micro Tip på alle overflader af
præparationen i 20 sekunder.
ii. Skyl grundigt i 5 sekunder, og efterlad den præparerede overflade
i fugtig tilstand.
3. Zirconium: Rengør overfladen, og fjern det svækkede zirconium med etdiamantbor. DER MÅ HVERKEN ÆTSES ELLER ANVENDES SILANE.
a) Slib den indvendige overflade af restaureringen med blæseluft.
b) Applicer zirconiumprimer på det frakturerede område ifølge producentens
vejledninger.
4. Porcelæn: Gør overfladen ru og fjern det svækkede porcelæn med etdiamantbor. Rengør det frakturerede porcelænområde i 15 sekunder med
Ultra-Etch. Skyl efter og tør.
FORSIGTIG – der skal anvendes hensigtsmæssig isolering, som fx. en
syreneutraliserende barriere (EtchArrest), når der anvendes flussyre (HF)
(Ultradent™ Porcelain Etch). Flussyre må ikke komme i berøring med
gingiva eller dentin.
a) Applicer flussyre på det frakturerede område i 90 sekunder.
b) Efter et minut skal syren suges væk fra overfladen, som derefter skal
grundigt skylles og tørres.
c) Applicer Ultra-Etch i 5 sekunder for at fjerne porcelænssalte og urenheder,
der blev dannet ved HF-ætsningen. Skyl efter og tør.
d) Applicer et tykt lag Silane i et minut.
e) Tør grundigt. DER MÅ IKKE SKYLLES.
5. Adhæsiv
a) Anvendelse af flaskei. Tryk 1-3 dråber Peak™ Universal Bond ned i “B”-siden på
dappenglasset til engangsbrug.
ii. Brug Micro Applicator Brush til at applicere et tykt lag Peak Universal
Bond på præparationen og forsigtigt røre rundt i det i 10 sekunder.
iii. Udtynd/tør i 10 sekunder med ¼ til ½ lufttryk. Præparationen skal
have et skinnende udseende.
iv. Lyspolymeriser i 10 sekunder (20 sekunder for lamper med en effektpå < 600 mW/cm2).
b) Anvendelse af sprøjte

i.

Applicer et tykt lag Peak Universal Bond med Inspiral™ penselspids –rør forsigtigt rundt i det i 10 sekunder.
ii. Udtynd/tør i 10 sekunder med ¼ til ½ lufttryk.
iii. Præparationen skal have et skinnende udseende.
iv. Lyspolymeriser i 10 sekunder (20 sekunder for lamper med en effektpå < 600 mW/cm2).
6. Restaurer med flydende og/eller kondenserbart kompositmateriale ifølge
producentens vejledninger.

Stiftcementering og opbygning
1) Tag hætten af PermaFlo™ DC-sprøjten.
2) Sæt en blandespids på dobbeltsprøjten, og sæt de to åbninger ud forhinanden. Drej i urets retning, indtil den er låst på plads.
3) Sæt den fleksible Intraoral Tip™ fast på blandespidsen for at pressematerialet direkte ind i kanalen fra dobbeltsprøjten.
4) Tryk en lille smule ud, inden stiften placeres i hullet.
5) Indsæt spidsen i stifthullet i den fulde dybde.
Stift og opbygning
6) Pres PermaFlo DC ud med jævnt tryk, idet der startes apikalt og bevæges
1. Præparation
i koronal retning.
a) Udbor et stifthul ved brug af en gummistopper og et UniCore™ bor i7) Indsæt stiften (UniCore™) langsomt, idet den overskydende cement
hensigtsmæssig størrelse.
fortrænges.
b) Skyl stifthullet grundigt i 10 sekunder med TriAway-adapteren og en 22 ga 8) Anbring polymeriseringslampen direkte over stiften og lyspolymeriser i 8
Endo-Eze™ spids. Tør efter med TriAway Adaptor og 22 ga Endo-Eze spids
sekunder, (40 sekunder for lys med udgang <600mW/cm2).
fra bunden af præparationen og opefter.
9) Fortsæt med at bygge PermaFlo™ DC lagvist op rundt om stiften efter
behov. BEMÆRK: Lyspolymeriser i 5 sekunder mellem hvert lag for atc) Kontroller stiftens (UniCore Post) tilpasning, og skær den til den ønskede
polymerisere det til gelkonsistens og forme opbygningen. Foretag enlængde med en diamantskive ved høj hastighed.
endelig lyspolymerisering af opbygningen i 40 sekunder.
2.Ætsning
Blandespidsen må ikke tages af før næste anvendelse. Desinficér sprøjte oga) Selvætsende teknik
blandespids.
i. Skyl kanalen og efterlad den fugtig.
™
ii. Sæt en blå 22 ga Deliver-Eze penselspids fast på Peak SE-sprøjten.
iii. Applicer det i stiftrummet og på den koronale præparation i 20
Forholdsregler og advarsler:
sekunder med en let rystende bevægelse.
1. Læs alle vejledninger nøje inden anvendelse af Peak Universal Bond.
iv. Blæs overskydende materiale ud med TriAway adapteren og en 22 ga 2. Må kun anvendes af tandlægepersonale.
Endo-Eze spids fra bunden og opefter. Udtynd/tør i 3 sekunder med 3. Sæt hætten på igen umiddelbart efter anvendelse for at undgå
trefunktionssprøjten eller kraftigt sug direkte over præparationen.
polymerisering.
v. Fortsæt til trinet “Adhæsiv” herunder.
4. Kontroller altid sprøjtematerialets flow inden intraoral anvendelse. Hvis derb) Total ætsteknik:
mødes modstand, skal spidsen udskiftes og kontrolleres igen.
i. Sæt en blå 22 G Endo-Eze spids fast på Ultra-Etch-sprøjten.
5. Behold hætterne på flasken indtil anvendelse.
ii. Start apikalt og fyld stiftrummet koronalt. Applicer materialet på den 6. Tandlæger, klinikassistenter og patienter skal bære UV-beskyttelsesbriller
koronale præparation. Æts i 20 sekunder.
ved lyspolymerisering.
iii. Sug overskydende ætsmiddel op.
7. Hvis produktet ikke anvendes dagligt, skal det opbevares i køleskab.
iv. Brug TriAway adapteren og 22 ga Endo-Eze spidsen til at skylle
8. Produkter fra køleskabet skal opnå stuetemperatur inden anvendelse.
grundigt. Tør efter med lidt luft og efterlad stiftrummet lettere fugtigt. 9. Der skal anvendes olie- og fugtfri luft for at opnå den højst mulige
v. Fortsæt til trinet “Adhæsiv” herunder.
adhæsivstyrke.
3.Adhæsiv
10. Vend lamperne i en anden retning for at forhindre præmatura) Anvendelse af flaske
polymerisering af alle kompositmaterialer.
i. Tryk 1-3 dråber Peak Universal Bond ned i “B”-siden på
11. Kompositmaterialer kan være sensibiliserende. Undgå gentagen kontakt
dappenglasset til engangsbrug.
mellem uafbundne dentale kompositmaterialer og hud. Må ikke anvendes
ii. Brug Nano-Brush™ eller NaviTip FX til at applicere Peak Universal
på patienter med kendt sensitivitet overfor acrylater eller andre resiner.
Bond i stiftrummet og anvend en let rystende bevægelse i hele
Hvis der opstår en allergisk reaktion, dermatitis eller eksem, skal der
kanalen og tandpræparationen i 10 sekunder.
søges læge.
iii. Fjern grundigt overskydende materiale ved brug af TriAway
12. Spidser, tomme sprøjter og flasker skal bortskaffes korrekt.
adapteren og 22 ga Endo-Eze-spidsen.
13. Opbevares utilgængeligt for børn.
iv. Udtynd/tør den udvendige præparation i 10 sekunder med ¼ til ½
14. Må ikke anvendes efter udløbsdatoen på beholderne.
lufttryk. Præparationen skal have et skinnende udseende.
15.Sæt hætten på igen, desinficér og tør sprøjten af med et mellemstærkt
v. Lyspolymeriser ned i stifthullet i 20 sekunder (40 sekunder for lys
desinfektionsmiddel mellem hver brug. Hvis der anvendes en hygiejnepose
med output <600mw /cm2).
over sprøjten, fjernes spidsen, hætten sættes på igen, og hygiejneposen
vi. Brug paperpoints eller en tidligere tilpasset stift til at kontrollere, atbortskaffes.
stiftrummet ikke er blokeret.
16. Spidserne er til engangsbrug. Spidserne må ikke genbruges for at undgå
b) Anvendelse af sprøjte
krydskontaminering.
i. Sæt en 30 G NaviTip FX -penselspids fast på sprøjten til Peak
17. Produkterne skal holdes væk fra varme/sollys.
Universal Bond.
18. Isoler stærke kemikalier til behandlingsområdet.
ii. Læg 1-2 dråber i stiftrummet og på præparationen, og rør derefterrundt i kanalens fulde længde, herunder hele tandpræparation, iBEMÆRK: Se www.ultradent.com for sikkerhedsdatablade og
10 sekunder.
yderligere oplysninger om brug af Peak Universal Bond, Peak SE
iii. Fjern overskydende Peak Universal Bond grundigt ved brug af
og andre relaterede produkter.
TriAway-adapteren og 22 G Endo-Eze-spidsen.
iv. Tør stiftrummet og præparationen i 10 sekunder med fuldt lufttryk forat udtynde/tørre med TriAway-adapteren og 22 Endo-Eze-spidens forat få evt. resterende opløsningsmiddel til at fordampe fra bunden op.
v. Lyspolymeriser ned i stifthullet i 20 sekunder (40 sekunder for lys
med output < 600mw /cm2). Brug paperpoints eller en tidligere
tilpasset stift til at kontrollere, at stiftrummet ikke er blokeret.
27

FI

Peak™ Universal Bond ja Peak™ SE

Kuvaus:Peak Universal Bond –sidostusainetta voidaan levittää pullosta tai yhdellä
ruiskulla. Sitä voidaan käyttää itse-etsaavien tai total-etch-valmisteiden kanssa. Se
sisältää kantoaineena 7,5 % etyylialkoholiliuotinta ja sen kovettamiseen voidaan
käyttää useimpia suuren intensiteetin omaavia valokovetuslaitteita, LED-laitteet
mukaan lukien. Peak Universal Bond sisältää 0,2 % klooriheksidiiniä, joka saattaa
tehostaa sidostuksen kestoaikaa.
Peak SE Primer -praimeri on itse-etsaava sidostusresiini, joka koostuu
etsausaineesta ja praimerista syringe-in-syringe-antojärjestelmässä.
Ultra-Etch™ on ruiskulla annosteltava 35 % fosforihappoa sisältävä huuhdeltava
etsausgeeli.
Klooriheksidiinin lisäämisen ei ole todettu korreloivan sekundaarisen karieksen
vähenemisen kanssa. Klooriheksidiinin vaikutuksia suun bakteerikasvustoon tai
kariekseen ei ole selvitetty kliinisillä tutkimuksilla.
Käyttöohje:
Sopii kaikenikäisille potilaille ja lähes kaikkiin korjaavan hammashoidon etsaus- ja
kiinnitystarpeisiin.
Peak Universal Bond -sidosaine kiinnittyy seuraaviin aineisiin:• Hammasluu ja -kiille• Posliini, zirkonia• Metalli• Komposiitti
Käyttöohjeet:
HUOMAUTUS: Peak SE:n käytön aloittaminenedellyttää JetMix™-ruiskussa olevan kahden
toisistaan erillään olevan komponentin
aktivointia.
1) Peak SE pysyy vakaana 120 vuorokauden ajan
aktivoinnin jälkeen.
2) Kirjoita viimeinen käyttöpäivämäärä
männänvarren tasaiselle pinnalle ennen
aktivointia.
3) ÄLÄ POISTA LUER-LOCK-KORKKIA ENNEN
SEKOITTAMISTA.
4) Paina päivämäärällä merkitty mäntä nopeasti janapakasti ruiskun sylinterin keskiosaan.
5) Varmista, että mäntä on keskimmäisen sylinterin
tasalla.

28

Suora sidostustekniikka ja posliinin/
zirkoniumoksidin korjaus
1.Præparationa) Dentiini/kiille: Eristä, puhdista ja poista karies ja varmista, että kaikki
mineralisoitumaton dentiini poistetaan (Seekiä /Sable Seekiä suositellaan
käytettäväksi tähän). Karhenna timanttiporalla luokan V abraasioiden/
abfraktioiden valmistelussa.
b) Yhdistelmämuovi: Poista hampaassa olevan yhdistelmämuovinheikentyneet osat. Karhenna pinta timanttiporalla.
c) Metalli: Mikrohiekkapuhalla pinta.
d) Zirkoniumoksidi: Puhdista pinta ja poista heikentynyt zirkoniumoksidi
timanttiporalla.
e) Posliini: Karhenna ja poista heikentynyt posliini timanttiporalla. Puhdista
rikkoutunut posliini Ultra-Etchillä 5 sekunnin ajan. Huuhtele ja kuivaa.
2.Etsausa) Itse-etsaava tekniikka -dentiini/kiille, yhdistelmämuovi ja metalli
i. Huuhtele valmiste ja jätä kosteaksi.
ii. VALINNAINEN MENETELMÄ - Levitä Consepsista™ (jos sitä on
saatavilla) Black Mini™ -sivellinkärjellä hankaavalla liikkeellä ja
ilmakuivaa kevyesti jättäen valmisteen hieman kosteaksi.

iii. Levitä Peak SE hammasvalmisteeseen Black Mini –sivellinkärjellä 20
sekunnin ajan sekoittaen jatkuvasti dentiinin pintaan. Älä hankaa
kiillettä.
iv. Ohenna ja kuivaa 3 sekunnin ajan ilma/vesiruiskulla tai voimakkaalla
imulla suoraan valmistellun alueen päältä.
v. Jatka jäljempänä kuvattuun sidostusvaiheeseenb) Total-etch-tekniikka - dentiini/kiille, yhdistelmämuovi ja metalli
i. Tarkista tuotteen väri ja koostumus ennen kuin puristat sitä pienen
määrän sekoituslehtiölle tai harsotaitokseen. Hävitä mahdollinen ulos
tullut kirkas neste.
ii. Levitä Ultra-Etch -etsausainetta Blue™ Micro -sivellinkärjellä
hammasvalmisteen kaikille pinnoille ja anna vaikuttaa 20 sekuntia.
iii. Huuhtele perusteellisesti 5 sekunnin ajan.
iv. Ohenna ja kuivaa kevyesti 3 sekunnin ajan ilma/vesiruiskulla tai
voimakkaalla imulla suoraan valmistellun alueen päältä. Jätä pinta
hieman kosteaksi.
v. VALINNAINEN MENETELMÄ - Levitä Consepsista (jos sitä on saatavilla)
Black Mini-sivellinkärjellä hankaavalla liikkeellä ja ilmakuivaa kevyesti
jättäen valmisteen hieman kosteaksi.
vi. Jatka sidostusvaiheeseenc) Posliinin etsaus – VAROITUS – käytä asianmukaista eristystä, kuten happoa
neutraloivaa aidaketta (EtchArrest™) kun käytät fluorivetyhappoa sisältävää
etsausainetta (HF) (Ultradent™ Porcelain Etch). Älä anna fluorivetyhapon
joutua kosketukseen ikenen tai dentiinin kanssa.
i. Levitä fluorivetyhappoa karhennetulle alueelle ja anna vaikuttaa 90
sekuntia.
ii. Ime happo pois pinnalta ja huuhtele SEN JÄLKEEN perusteellisesti
ja kuivaa pinta.
iii. Levitä Ultra Etchiä ja anna vaikuttaa 5 sekunnin ajan
fluorivetyhappoetsauksen aiheuttamien posliinisuolojen ja jätteen
poistamiseksi. Huuhtele ja kuivaa.
iv. Levitä pinnalle silanea lammikoksi 60 sekunnin ajaksi.
v. Kuivaa perusteellisesti. ÄLÄ HUUHTELE.
vi. Jatka jäljempänä kuvattuun sidostusvaiheeseend) Zirkoniumoksidi – ÄLÄ ETSAA TAI KÄYTÄ SILAANIA
i. Hiekkapuhalla proteesin murrettu pinta, huuhtele ja kuivaa.
ii. Levitä zirkoniumoksidipraimeria karhennetulle alueelle valmistajan
ohjeiden mukaisesti.
iii. Jatka jäljempänä kuvattuun sidostusvaiheeseen.
3.Sidostusa) Annostelu pullosta
i. Annostele 1 – 3 tippaa Peak™ Universal Bondia kertakäyttöisen maljan
B-puolelle.
ii. Levitä Micro Applicator Brush –siveltimellä Peak™ Universal Bondia
lammikoksi valmisteen pinnalle ja sekoita kevyesti 10 sekunnin ajan.
iii. Ohenna/kuivaa 10 sekunnin ajan käyttäen ilmasuihkua ¼ – ½
paineella. Valmisteen pitäisi näyttää kiiltävältä.
iv. Valokoveta 10 sekunnin ajan. Jos käytät valokovettimia, joiden teho onalle 600 mW/cm2, pidennä kovetusaika 20 sekuntiin.
v. Restauroi juoksevalla ja/tai pakattavalla yhdistelmämuovillavalmistajan ohjeiden mukaisesti.
b) Annostelu ruiskullai. Levitä Peak™ Universal Bond -sidostusainetta Inspiral™-sivellinkärjelläniin, että muodostuu pieni lammikko ja sekoita varovasti 10 sekunnin
ajan.
ii. Ohenna/kuivaa 10 sekunnin ajan käyttäen ¼ – ½ ilmanpainetta.
iii. Valokoveta 10 sekunnin ajan. Jos käytät valokovettimia, joiden teho onalle 600 mW/cm2, pidennä kovetusaika 20 sekuntiin.
iv. Restauroi juoksevalla ja/tai pakattavalla yhdistelmämuovillavalmistajan ohjeiden mukaisesti.
Epäsuora sidostustekniikka - epäsuorat kruunut, inlayt, onlayt ja
zirkoniumoksidi
1.Valmistelu

a) Puhdista väliaikainen puhdas valmiste, huuhtele ja kuivaa (Käytä
Consepsis™ Scrub -puhdistusainetta ja STARBrush™-harjaa puhdistamiseen,
desinfektioon ja sementin jäämien poistoon).
b) Varmista proteesin sopivuus.
c) Valmistele proteesin sisäpinta.
i. Metallipohjaiset:(1) Mikrohio (hiekkapuhalla) proteesin sisäpinta.
(2) Huuhtele ja kuivaa pinta.
ii. Keraami/posliini:(1) Levitä fluorivetyhappoa (HF)(Ultradent™ Porcelain Etch) proteesin
sisäpinnalle, anna vaikuttaa 90 sekuntia, huuhtele ja kuivaa.
(2) Levitä Ultra Etchiä ja anna vaikuttaa 5 sekunnin ajan
fluorivetyhappoetsauksen aiheuttamien posliinisuolojen ja jätteen
poistamiseksi. Huuhtele ja kuivaa.
(3) Levitä silaania (Ultradent™ Silane) proteesin sisäpinnalle, anna
vaikuttaa yhden minuutin, kuivaa ja aseta proteesi syrjään. Älä
huuhtele.
iii. Zirkoniumoksidi: ÄLÄ ETSAA TAI KÄYTÄ SILAANIA(1) Hiekkapuhalla proteesin sisäpinta, huuhtele ja kuivaa.
(2) Levitä zirkoniumoksidipraimeria valmistajan ohjeiden mukaisesti.
2.Etsaus - Hampaan pinnan valmistelua) Itse-etsaava tekniikka -dentiini/kiille, yhdistelmämuovi ja metalli
i. Huuhtele valmiste ja jätä kosteaksi.
ii. VALINNAINEN MENETELMÄ – Levitä Consepsista™ (jos sitä on saatavilla)
Black Mini™ -sivellinkärjellä hankaavalla liikkeellä ja ilmakuivaa kevyesti
jättäen valmisteen pinta kosteaksi.
iii. Levitä Peak™ SE hammasvalmisteeseen Black Mini™ –sivellinkärjellä
20 sekunnin ajan sekoittaen jatkuvasti dentiinin pintaan. Älä hankaa
kiillettä.
iv. Ohenna ja kuivaa 3 sekunnin ajan ilma/vesiruiskulla tai voimakkaalla
imulla suoraan valmistellun alueen päältä.
v. Jatka jäljempänä kuvattuun sidostusvaiheeseen.
b) Total-etsaustekniikka – dentiini/kiille, yhdistelmämuovi ja metalli
i. Levitä Ultra-Etch -etsausainetta Blue Micro -sivellinkärjellä
hammasvalmisteen kaikille pinnoille ja anna vaikuttaa 20 sekuntia.
ii. Huuhtele perusteellisesti 5 sekunnin ajan.
iii. Ohenna ja kuivaa kevyesti 3 sekunnin ajan ilma/vesiruiskulla tai
voimakkaalla imulla suoraan valmistellun alueen päältä. Jätä pinta
hieman kosteaksi.
iv. VALINNAINEN MENETELMÄ – Levitä Consepsista™ (jos sitä on saatavilla)
Black Mini™ -sivellinkärjellä hankaavalla liikkeellä ja ilmakuivaa kevyesti
jättäen valmisteen pinta kosteaksi.
v. Jatka jäljempänä kuvattuun sidostusvaiheeseen.
c) Posliinin etsaus – VAROITUS – käytä asianmukaista eristystä, kuten happoa
neutraloivaa aidaketta (EtchArrest) kun käytät fluorivetyhappoa sisältävää
etsausainetta (HF) (Ultradent Porcelain Etch). Älä anna fluorivetyhapon
joutua kosketukseen ikenen tai dentiinin kanssa.
i. Levitä fluorivetyhappoa murretulle alueelle ja anna vaikuttaa 90
sekuntia.
ii. Lme happo pois pinnalta ja huuhtele SEN JÄLKEEN perusteellisesti jakuivaa pinta.
iii. Levitä Ultra Etchiä ja anna vaikuttaa 5 sekunnin ajan
fluorivetyhappoetsauksen aiheuttamien posliinisuolojen ja jätteen
poistamiseksi. Huuhtele ja kuivaa.
iv. Levitä pinnalle silanea lammikoksi 60 sekunnin ajaksi.
v. Kuivaa perusteellisesti. ÄLÄ HUUHTELE.
vi. Jatka jäljempänä kuvattuun sidostusvaiheeseen.
d) Zirkoniumoksidi – ÄLÄ ETSAA TAI KÄYTÄ SILAANIA
i. Hiekkapuhalla proteesin sisäpinta, huuhtele ja kuivaa.
ii. Levitä zirkoniumoksidipraimeria karhennetulle alueelle valmistajan
ohjeiden mukaisesti.
iii. Jatka jäljempänä kuvattuun sidostusvaiheeseen.
3.Sidostus
a. Annostelu pullosta
i. Annostele 1-3 tippaa Peak Universal Bondia kertakäyttöisen maljan
B-puolelle.
ii. Levitä Micro Applicator –siveltimellä Peak Universal Bondia lammikoksi
valmisteen pinnalle ja sekoita kevyesti 10 sekunnin ajan.

iii. Ohenna/kuivaa 10 sekunnin ajan käyttäen täyttä ilmanpainetta.
Valmisteen pitäisi näyttää kiiltävältä.
iv. Valokoveta 10 sekunnin ajan. Jos käytät valokovettimia, joiden teho onalle 600 mW/cm2, pidennä kovetusaika 20 sekuntiin.
b) Annostelu ruiskullai. Levitä Peak™ Universal Bond -sidostusainetta Inspiral™-sivellinkärjelläniin, että muodostuu pieni lammikko ja sekoita varovasti 10 sekunnin
ajan.
ii. Ohenna/kuivaa 10 sekunnin ajan käyttäen täyttä ilmanpainetta.
Valmisteen pitäisi näyttää kiiltävältä.
iii. Valokoveta 10 sekunnin ajan. Jos käytät valokovettimia, joiden teho onalle 600 mW/cm2, pidennä kovetusaika 20 sekuntiin.
4.Sementöinti
a) Levitä läpikuultavia laminaatteja varten tarkoitettua valokovetteista
sementtiä tai muille proteeseille tarkoitettua kaksoiskovetteista
resiinisementtiä noudattaen valmistajan ohjeita.
OTE: Dentiinin välitön eristys edellyttää edellä esitetyn suoran tekniikan
vaiheiden 2A ja 3 käyttöä. Levitä glyseriiniä Peak Universal Bond-sidostusaineen päälle ja valokoveta 10 sekuntia. Huuhtele glyseriini pois.
Tee lopullinen jäljennös. Levitä glyseriiniä valmisteen päälle uudestaan
erottavaksi aineeksi ennen väliaikaisvalmisteen sementöintiä paikalleen.
Yhdistelmämuovin/metallin/zirkoniumoksidin/posliinin korjaus
1. Yhdistelmämuovi: Poista yhdistelmämuovin heikentyneet osat. Karhenna
pinta timanttiporalla.
a) Total-Etch -etsaustekniikka
i. Levitä Ultra-Etch -etsausainetta Blue Micro Tip -sivellinkärjellä
hammasvalmisteen kaikille pinnoille ja anna vaikuttaa 20 sekuntia.
ii. Huuhtele perusteellisesti 5 sekunnin ajan ja jätä valmistellut pinnat
kosteiksi.
2. Metalli: Mikrohiekkapuhalla pintaa) Total-Etch -etsaustekniikka
i. Levitä Ultra-Etch -etsausainetta Blue Micro Tip -sivellinkärjellä
hammasvalmisteen kaikille pinnoille ja anna vaikuttaa 20 sekuntia.
ii. Huuhtele perusteellisesti 5 sekunnin ajan ja jätä valmistellut pinnat
kosteiksi.
3. Zirkoniumoksidi: Puhdista pinta ja poista heikentynyt zirkoniumoksidi
timanttiporalla. ÄLÄ ETSAA TAI KÄYTÄ SILAANIA.
a) Hiekkapuhalla proteesin sisäpinta.
b) Levitä zirkoniumoksidipraimeria karhennetulle alueelle valmistajan ohjeiden
mukaisesti.
4. Posliini: Karhenna ja poista heikentynyt posliini timanttiporalla. Puhdista
karhennettu posliini Ultra-Etchillä 15 sekunnin ajan. Huuhtele ja kuivaa.
VAROITUS – käytä asianmukaista eristystä, kuten happoa neutraloivaa
aidaketta (EtchArrest) kun käytät fluorivetyhappoa sisältävää etsausainetta(HF) (Ultradent™ Porcelain Etch). Älä anna fluorivetyhapon joutua
kosketukseen ikenen tai dentiinin kanssa.
a) Levitä fluorivetyhappoa karhennetulle alueelle ja anna vaikuttaa 90 sekuntia.
b) Ime happo pois pinnalta ja huuhtele sen jälkeen perusteellisesti ja kuivaa
pinta.
c) Levitä Ultra Etchiä ja anna vaikuttaa 5 sekunnin ajanhydrofluorihappoetsauksen aiheuttamien posliinisuolojen ja jätteen
poistamiseksi. Huuhtele ja kuivaa.
d) Levitä silanea lammikoksi yhden minuutin ajaksi..
e) Kuivaa perusteellisesti. ÄLÄ HUUHTELE.
5. Sidostusa) Annostelu pullosta
i. Annostele 1 – 3 tippaa Peak™ Universal Bondia kertakäyttöisen maljan
B-puolelle.
ii. Levitä Micro Applicator Brush –siveltimellä Peak™ Universal Bondia
lammikoksi valmisteen pinnalle ja sekoita kevyesti 10 sekunnin ajan.
iii. Ohenna/kuivaa 10 sekunnin ajan käyttäen ¼ – ½ ilmanpainetta.
Valmisteen pitäisi näyttää kiiltävältä.
iv. Valokoveta 10 sekunnin ajan. Jos käytät valokovettimia, joiden teho onalle 600 mW/cm2, pidennä kovetusaika 20 sekuntiin.
b) Annostelu ruiskullai. Levitä Peak™ Universal Bond -sidostusainetta Inspiral™-sivellinkärjellä
29niin, että muodostuu pieni lammikko ja sekoita varovasti 10 sekunnin
ajan.
ii. Ohenna/kuivaa 10 sekunnin ajan käyttäen ¼ – ½ ilmanpainetta.
iii. Valmisteen pitäisi näyttää kiiltävältä.
iv. Valokoveta 10 sekunnin ajan. Jos käytät valokovettimia, joiden teho onalle 600 mW/cm2, pidennä kovetusaika 20 sekuntiin.
6. Restauroi juoksevalla ja/tai pakattavalla yhdistelmämuovilla valmistajan
ohjeiden mukaisesti.

varmistamaan, ettei nastan reikä ole tukkeutunut.

Nastan sementöinti ja ytimen rakentaminen
1. Poista korkki PermaFlo™ DC -ruiskusta.
2. Aseta sekoituskärki kaksisylinteriseen ruiskuun ja kohdista molemmat portit.
Kierrä myötäpäivään, kunnes se kiinnittyy paikalleen.
3. Kiinnitä taipuisa Intraoral Tip™ -kärki sekoituskärkeen, jotta voit annostellasuoraan juurikanavaan kaksoissylinteriruiskusta.
4. Pursota pieni määrä ennen kuin viet kärjen nastan reikään.
5. Vie kärki nastan reikään aivan pohjaan saakka.
Nasta ja ydin
6. Annostele PermaFlo DC tasaisella paineella alkaen apikaalisesti
1. Valmistelu
koronaalisuuntaan.
a) Poraa nastan reikä käyttämällä kumista pysäytintä ja sopivan kokoista
7. Työnnä UniCore™-nasta paikalleen hitaasti siten, että ylimääräinen sementti
UniCore™-poraa.
b) Huuhtele nastan pesä perusteellisesti 10 sekunnin ajan käyttäen TriAwaysyrjäytyy.
™
sovitetta ja 22g:n Endo-Eze -kärkeä. Kuivaa käyttäen TriAway -sovitetta ja
8. Aseta valokovettimen linssi suoraan nastan päälle ja valokoveta 20 sekunnin
22g:n Endo-Eze -kärkeä alkaen valmisteen pohjasta jatkaen ylöspäin.
ajan. Jos käytät valokovettimia, joiden teho on alle 600 mW/cm2, pidennäc) Varmista Uni-Core-nastan sopivuus ja katkaise se sopivan pituiseksi nopeasti
kovetusaika 40 sekuntiin.
pyörivällä timanttikiekolla. HUOMAA: Karbidi- ja leikkausporat saattavat
9. Jatka PermaFlo™ DC -kerrosten rakentamista nastan ympärille tarpeen
mukaan. HUOMAUTUS: Valokoveta 5 sekuntia kerrosten välillä, jotta ydin
aiheuttaa kuitujen rispaantumista.
geeliytyy ja muodostaa ytimen. Valokoveta ydintä lopuksi 40 sekunnin
2.Etsausajan. Älä poista ruiskun sekoituskärkeä ruiskusta, vaan jätä se paikalleena) Itse-etsaava tekniikka:seuraavaa käyttökertaa varten. Desinfioi sekoituskärki ja ruisku.
i. Huuhtele juurikanava ja jätä kosteaksi.
ii. Kiinnitä sininen 22g Deliver-Eze™ -sivellinkärki Peak SE -ruiskuun.
iii. Levitä ainetta nastan reikään ja koronaalivalmisteeseen 20 sekunnin
Varoituksia ja varotoimenpiteitä:
ajaksi koko ajan sekoittaen.
1. Lue kaikki ohjeet huolellisesti ja sisäistä ne ennen Universal Peak Bondin
iv. Puhalla liika aine pois TriAway-sovitteella ja 22g Endo-Eze –kärjellä
käyttöä.
pohjasta alkaen ylöspäin. Ohenna ja kuivaa 3 sekunnin ajan ilma/
2. Vain ammattikäyttöön.
vesiruiskulla tai voimakkaalla imulla suoraan valmistellun alueen
3. Sulje korkki välittömästi käytön jälkeen polymerisaation välttämiseksi.
päältä.
4. Varmista aina materiaalin juoksevuus ennen kuin levität sitä suunsisäisesti.
v. Jatka jäljempänä kuvattuun sidostusvaiheeseen.
Jos virtausvastusta ilmenee, vaihda kärki ja tarkista virtaus uudelleen.
b) Total-Etch -etsaustekniikka:
5. Pidä pullot suljettuina korkeilla käyttöön saakka.
i. Kiinnitä sininen 22g Endo-Eze -kärki Ultra-Etch -ruiskuun.
6. Hammaslääkärin, avustajan ja potilaan pitää käyttää UV-valolta suojaavia
ii. Aloita apikaalisesti ja täytä nastan reikä koronaalitasolle. Levitä
silmiensuojaimia resiinimateriaaleja kovetettaessa.
koronaalivalmisteeseen. Etsaa 20 sekuntia.
7. Jos valmistetta ei käytetä päivittäin, säilytä sitä jääkaapissa.
iii. Poista liika etsausaine imulla.
8. Anna jääkaapissa säilytettyjen tuotteiden lämmitä huoneenlämpöön ennen
iv. Huuhtele perusteellisesti käyttäen TriAway-sovitetta ja 22g Endo-Eze
käyttöä.
-kärkeä, ilmakuivaa kevyesti TriAway–sovitteella ja 22g Endo-Eze
9. Sidoksen lujuuden optimoimiseksi käytä kuivaamiseen öljytöntä ja kuivaa-kärjellä siten, että nastan reikä jää hieman kosteaksi.
ilmaa.
v. Jatka jäljempänä kuvattuun sidostusvaiheeseen.
10. Suuntaa kattovalaistus syrjään kaikkien resiinimateriaalien ennenaikaisen
3.Sidostus
polymerisoitumisen välttämiseksi.
a. Annostelu pullosta
11. Resiinit voivat olla herkistäviä. On vältettävä kovettumattoman resiinin
i. Annostele 1 – 3 tippaa Peak Universal Bondia kertakäyttöisen maljan
toistuvaa ihokosketusta. Älä käytä potilaille, jotka ovat herkistyneet
B-puolelle.
akrylaatille tai muille resiineille. Jos ilmenee allerginen reaktio, ihotulehdus
ii. Levitä Nano-Brush™-sivellintä tai NaviTip FX -kärkeä käyttäen Peaktai ihottuma, ota yhteys lääkäriin.
Universal Bondia nastan reikään ja sekoita kevyesti koko kanavan ja
12. Hävitä kärjet ja tyhjät ruiskut ja pullot asianmukaisesti.
hammasvalmisteen pituudelta 10 sekunnin ajan.
13. Pidä poissa lasten ulottuvilta ja näkyviltä.
iii. Poista liika TriAway-sovitteella ja 22ga Endo-Eze-kärjellä.
14. Ei saa käyttää pakkaukseen merkityn viimeisen käyttöpäivämäärän jälkeen.
iv. Ohenna/kuivaa ulompi valmiste 10 sekunnin ajan käyttäen ilmasuihkua 15. Aseta korkki takaisin, desinfioi ja pyyhi ruisku keskitason desinfektioaineella¼ – ½ paineella. Valmisteen pitäisi näyttää kiiltävältä.
käyttökertojen välillä. Jos käytät ruiskun kertakäyttösuojaa, poista kärki, aseta
v. Valokoveta 20 sekunnin ajan nastan reikää pitkin alaspäin. Jos käytät
korkki takaisin ja hävitä ruiskun suojus.
valokovettimia, joiden teho on alle 600 mW/cm2, pidennä kovetusaika 16. Kärjet ovat käytön jälkeen hävitettäviä. Kärkiä ei saa käyttää uudelleen
40 sekuntiin.
ristikontaminaation välttämiseksi.
vi. Käytä paperikärkeä tai valmiiksi sovitettua nastaa varmistamaan, ettei
17. Suojaa tuote suoralta kuumudelta ja auringonvalolta.
nastan reikä ole tukkeutunut.
18. Käsiteltävän alueen ulkopuoliset alueet pitää suojata väkeviltä kemikaaleiltab) Annostelu ruiskulla
eristämällä.
i. Kiinnitä 30 g:n NaviTip FX -sivellinkärki Peak™ Universal -sidostusainetta
sisältävään ruiskuun.
HUOMAUTUS: Käyttöturvallisuustiedote ja Peak™ Universal
Bond– ja Peak™ SE-valmisteiden käyttöä ja muita niiden
ii. Tiputa 1–2 tippaa nastan reikään ja valmisteelle, sekoita sitten 10
yhteydessä käytettäviä tuotteita koskevia tietoja on saatavana
minuutin ajan koko juurikanavan pituudelta, koko valmisteen alue
verkkosivustoltamme www.ultradent.com
mukaan lukien.
iii. Poista liika Peak™ Universal Bond -sidostusaine perusteellisesti
käyttäen TriAway-sovitetta ja 22 g:n Endo-Eze-kärkeä.
iv. Haihduta kaikki liuotinjäämät pohjasta alkaen kuivaamalla nastan reikä
ja valmiste ilmalla täydellä paineella 10 sekunnin ajan TriAway-sovitetta
ja 22 g:n Endo- Eze -kärkeä käyttämällä.
v. Valokoveta 20 sekunnin ajan nastan reikää pitkin alaspäin. Jos käytät
valokovettimia, joiden teho on alle 600 mW/cm2, pidennä kovetusaika
40 sekuntiin. Käytä paperikärkeä tai valmiiksi sovitettua nastaa
30

Peak™ Universal Bond og Peak™ SE
Beskrivelse:
Peak Universal Bond er et bindingsresin, levert i én flaske eller én enkelt
sprøyte. Det kan brukes med selvetsing
eller totaletsing. Det er fylt 7,5 % med et etylalkohol løsemiddel og vil herde
under de fleste høyintensitetslys,
inkludert LED-er. Peak Universal Bond inneholder 0,2 % klorheksedin, som
kan bidra til langtids bindestyrke.
Peak SE Primer er et selvetsende dentinbindingssystemresin, som består av
et etsemiddel og en primer i et sprøyte-leveringssystem.
Ultra-Etch™ er en sprøytelevert, 35 % fosforsyre etse- og skyllegelé.
Inkludering av klorheksidintilsetningen har vist seg ikke å samsvare med en
reduksjon i sekundær nedbrytning i pasienter. Kliniske studier for å evaluere
virkningen av klorheksidin på orale bakterier eller karies har ikke vært utført.
Indikasjoner for bruk:
Bruk for så og si alle etsing- og festebehov i gjenoppbyggende tannarbeide
for pasienter av alle aldre.
Peak Universal Bond fester til følgende materialer:• Dentin og emalje• Porselen, zirkoniumoksid• Metall• Kompositt
Retningslinjer for bruk:
MERK: Første gangs bruk av Peak SE kreveraktivering av de to komponentene, som er
separerte i JetMix™ sprøyten.
1) Peak™ SE er stabil i 120 dager etter aktivering.
2) Skriv utløpsdatoen på det flate området til
stempelstammen før aktivering.
3) IKKE FJERN LUERLÅSHETTEN FØR BLANDING.
4) Press det “daterte” stempelet hurtig og kraftig
inn i den midterste beholderen.
5) Bekreft at stempelet er i flukt med midterste
beholder.
Direkte bindingsteknikk og porselen/zirkoniumreparasjon
1. Klargjøra) Dentin/emalje: Isoler, rengjør og fjern karies
under påsyn av at alt ikke-mineraldentin
fjernes (Seek/Sable Seek anbefales for dette). For abrasjon/
abfraksjon, klasse V preparasjoner, gjør overflaten ru med etdiamantbor.
b) Kompositt: Fjerne svake deler av eksisterende komposittmateriale.
Gjør overflaten ru med et diamantbor.
c) Metall: Mikroabrader overflaten.
d) Zirkonium: Rengjør overflaten og fjern svekket zirkonium med etdiamantbor.
e) Porselen: Gjør overflaten ru og fjern svakt porselen med etdiamantbor. Rengjør sprukket porselensområde i 5 sekunder med
Ultra-Etch. Skyll og tørk.
2. Etsninga) Selvetsningsteknikk – dentin/emalje, kompositt og metall
i. Skyll preparatet og la være fuktig.
ii. ALTERNATIVT – Påfør Consepsis™ (hvor tilgjengelig) med Black
Mini™ Brush-spiss på preparatet med en skurebevegelse ogNOlufttørk slik at overflaten blir værende fuktig.
iii. Påfør Peak SE med Black Mini /Brush Tip på tannpreparatet i
20 sekunder under stadig omrøring på dentinet. Emaljen må
ikke skures.
iv. Tynn ut/tørk i 3 sekunder ved bruk av luft-/vannsprøyten eller vedå plassere et høyvolumsug direkte over tannpreparatet.
v. Gå videre til “Binding”-trinnet nedenfor.
b) Totaletsningsteknikk – dentin/emalje, kompositt og metalli. Bekreft fargen og konsistensen til produktflyten før bruk vedå trykke ut en liten mengde på en blandeflate eller gasbind.
Avhend klar væske som trykkes ut.
ii. Påfør Ultra-Etch med Blue Micro-spiss på alle overflatene tiltannpreparatet i 20 sekunder.
iii. Skyll grundig i 5 sekunder.
iv. Tørk lett ved bruk av luft-/vannsprøyten eller ved å plassere
høyvolumsuget direkte over tannpreparatet. La overflaten værelett fuktig.
v. ALTERNATIVT – Påfør Consepsis (hvor tilgjengelig) med Black Mini
Brush-spiss på preparatet med en skurebevegelse og lufttørk slik
at overflaten blir værende fuktig.
vi. Gå videre til “Binding”-trinnet nedenfor.
c) Porselenetsning – VÆR VARSOM – bruk skikkelig isolasjon, slik som ensyrenøytraliserende barriere (EtchArrest™), ved bruk av hydrofluorsyre(HF) (Ultradent™-porselensetser). Påse at hydrofluorsyre ikke siver
gjennom og kommer i berøring med gingiva eller dentin.
i. Påfør hydrofluorsyre på det sprukne området i 90 sekunder.
ii. Sug syre fra overflaten, skyll DERETTER godt og tørk.
iii. Påfør Ultra-Etch i 5 sekunder for å fjerne porselensalter og avfall
dannet av HF-etsningen. Skyll og tørk.
iv. Påfør et lag med silan i 60 sekunder.
v. Tørk godt. IKKE SKYLL.
vi. Gå videre til “Binding”-trinnet nedenfor.
d) Zirkonium – IKKE ETS ELLER BRUK SILAN.
i. Luftabrader sprukne overflater på protesen, skyll og tørk.
ii. Påfør zirkoniumoksidet på sprukket området i henhold til
produsentens instruksjoner.
iii. Gå videre til “Binding”-trinnet nedenfor.
3. Bindinga) Bruksanvisning for flaske
i. Dispensere 1-3 dråper Peak™ Universal Bond i b-siden på
engangsblandebrettet.
ii. Påfør en pøl med Peak™ Universal Bond med Micro Applicator
Brush på den preparerte tannen. Rør forsiktig i 10 sekunder.
iii. Tørk/fortynn ut i 10 sekunder ved bruk av ¼ til ½ lufttrykk.
Preparasjonen skal ha et skinnende utseende.
iv. Herd med lys i 10 sekunder (20 sekunder for lys med <600 mW/
cm2).
v. Gjenoppbygg med flytende eller fast kompositt i henhold til
produsentens instruksjoner.
b) Bruksanvisning for sprøyten
i. Lag en pytt av Peak™ Universal Bond med Inspiral™ Brush Tip. Rør
forsiktig i 10 sekunder.
ii. Tørk/fortynn i 10 sekunder ved bruk av ¼ til ½ lufttrykk.
Preparasjonen skal ha et skinnende utseende.
iii. Herd med lys i 10 sekunder (20 sekunder for lys med <600 mW/
cm2).
iv. Gjenoppbygg med flytende eller fast kompositt i henhold til
produsentens instruksjoner.
31

Indirekte bindingsteknikk – Indirekte kroner, innlegg, pålegg,
zirkoniumoksid
1. Klargjøra) Fjern midlertidig, rengjør og tørk preparatet, skyll og tørk (Consepsis
Scrub med en StarBrush™ for å rengjøre og fjern overflødig sement).
b) Bekreft protesetilpasning.
c) Klargjør den indre overflaten av protesen.
i. Metallbasert:(1) Mikroabrader (sandblås) protesens indre overflate.
(2) Skyll og tørk overflaten.
ii. Keramikk/ porselen:(1) Påfør hydrofluorsyre (HF) (Ultradent Porcelain Etch) påprotesens indre overflate i 90 sekunder, skyll og tørk.
(2) Påfør Ultra-Etch i 5 sekunder for å fjerne porselensalter og
avfall dannet av HF-etsningen. Skyll og tørk.
(3) Påfør silan (Ultradent™ Silane) på protesens indre overflate i 1
minutt, tørk og sett protesen til side. Ikke skyll.
iii. Zirkonium: IKKE ETS ELLER BRUK SILAN(1) Luftabrader de indre overflatene på protesen, skyll og tørk.
(2) Påfør en zirkonium-primer i henhold til produsentens
anvisninger.
2. Ets - Klargjør tannoverflatena) Selvetsningsteknikk – dentin/emalje, kompositt og metall
i. Skyll preparatet og la være fuktig.
ii. ALTERNATIVT – Påfør Consepsis (hvor tilgjengelig) med Black Mini
Brush-spiss på preparatet med en skurebevegelse og lufttørk slik
at overflaten blir værende fuktig.
iii. Påfør Peak™ SE med Black Mini™ /Brush Tip – i 20 sekunder for å
klargjøre tannen, under stadig omrøring. Emaljen må ikke skures.
iv. Tynn ut/tørk i 3 sekunder ved bruk av luft-/vannsprøyten eller vedå plassere et høyvolumsug direkte over tannpreparatet.
v. Gå videre til “Binding”-trinnet nedenfor.
b) Totaletsningsteknikk – dentin/emalje, kompositt og metalli. Påfør Ultra-Etch med Blue Micro-spiss på alle overflatene tiltannpreparatet i 20 sekunder.
ii. Skyll grundig i 5 sekunder.
iii. Tørk lett ved bruk av luft-/vannsprøyten eller ved å plassere
høyvolumsuget direkte over tannpreparatet. La overflaten værelett fuktig.
iv. ALTERNATIVT – Påfør Consepsis (hvor tilgjengelig) med Black Mini
Brush-spiss på preparatet med en skurebevegelse og lufttørk slik
at overflaten blir værende fuktig.
v. Gå videre til “Binding”-trinnet nedenfor.
c) Porselenetsning – VÆR VARSOM – bruk skikkelig isolasjon, slik som ensyrenøytraliserende barriere (EtchArrest), ved bruk av hydrofluorsyre(HF) (Ultradent-porselensetser). Påse at hydrofluorsyre ikke kommer iberøring med gingiva eller dentin.
i. Påfør hydrofluorsyre på det sprukne området i 90 sekunder.
ii. Sug syre fra overflaten, skyll DERETTER godt og tørk.
iii. Påfør Ultra-Etch i 5 sekunder for å fjerne porselensalter og avfall
dannet av HF-etsningen. Skyll og tørk.
iv. Påfør et lag med silan i 60 sekunder.
v. Tørk godt. IKKE SKYLL.
vi. Gå videre til “Binding”-trinnet nedenfor.
d) Zirkonium – IKKE ETS ELLER BRUK SILAN.
i. Luftabrader de indre overflatene på protesen, skyll og tørk.
ii. Påfør zirkoniumoksidet på sprukket området i henhold til
produsentens instruksjoner.
iii. Gå videre til “Binding”-trinnet nedenfor.
3. Bindinga) Bruksanvisning for flaskei. Trykk ut 1-3 dråper med Peak Universal Bond på “B”-siden av
engangs-dappenplaten.
ii. Bruk Micro Applicator-børsten, påfør et bunnlag med Peak
32

Universal Bond på preparatet og rør forsiktig i 10 sekunder.
iii. Tørk/fortynn ut i 10 sekunder ved bruk av fullt lufttrykk.
Preparasjonen skal ha et skinnende utseende.
iv. Lysherd i 10 sekunder (20 sekunder for lys med <600 mW/cm2).
b) Bruksanvisning for sprøyten
i. Lag en pytt av Peak™ Universal Bond med Inspiral™ Brush Tip. Rør
forsiktig i 10 sekunder.
ii. Tørk/fortynn ut i 10 sekunder ved bruk av fullt lufttrykk.
Preparasjonen skal ha et skinnende utseende.
iii. Herd med lys i 10 sekunder (20 sekunder for lys med <600 mW/
cm2).
4. Sementa) Påfør lysherdet sement for gjennomsiktige emaljer eller
dobbeltherdende resinsement på protesen og følg produsentens
anvisninger for bruk.
MERK: Direkte dentinforsegling krever Direkte teknikk trinn 2A og
3 ovenfor. Påfør glyserin over Peak Universal Bond og lysherd i 10
sekunder. Skyll av glyserin. Lag endelig avtrykk. Påfør glyserin på
preparatet igjen, som et separasjonsmiddel før midlertid sementering
på plass.
Reparasjon av kompositt/metall/zirkoniumoksid/porselen
1. Kompositt: Fjerne svake deler av eksisterende komposittmateriale. Gjør
overflaten ru med et diamantbor.
a) Totaletsningsteknikk
i. Påfør Ultra-Etch med Blue Micro Tip på alle overflatene på den
klargjorte preparerte tannen i 20 sekunder.
ii. Skyll grundig i 5 sekunder og la den forbli fuktig.
2. Metall: Forbered overflaten med mikroabrasjona) Totaletsningsteknikk
iii. Påfør Ultra-Etch med Blue Micro Tip på alle overflatene på den
klargjorte preparerte tannen i 20 sekunder.
iv. Skyll grundig i 5 sekunder og la den forbli fuktig.
3. Zirkoniumoksid: Rengjør overflaten, fjern svekket zirkoniumoksid med
diamantbor. IKKE ETS ELLER BRUK SILAN.
a) Preparer protesens innvendige overflate med luft-abrasjon.
b) Påfør zirkoniumoksid-grunner på området med frakturer i henhold til
produsentens instruksjoner.
4. Porselen: Gjør overflaten ru og fjern svakt porselen med et diamantbor.
Rengjør sprukket porselensområde i 15 sekunder med Ultra-Etch. Skyllog tørkVÆR VARSOM – bruk skikkelig isolasjon, slik som en syrenøytraliserende
barriere (EtchArrest™), ved bruk av flussyre (HF) (Ultradent™
porselensetser). Påse at flussyren ikke siver gjennom og kommer iberøring med gingiva eller dentin.
a) Påfør flussyre på det området med frakturer i 90 sekunder.
b) Sug syren fra overflaten, skyll deretter godt og tørk overflaten.
c) Påfør Ultra-Etch i 5 sekunder for å fjerne porselensalter og avfall
dannet av HF-etsingen. Skyll og tørkd) Påfør et lag med silan i 1 minutt.
e) Tørk godt. IKKE SKYLL.
5. Bondinga) Bruksanvisning for flaske
i. Dispensere 1-3 dråper Peak™ Universal Bond i b-siden på
engangsblandebrettet.
ii. Påfør en pøl med Peak™ Universal Bond med Micro Applicator
Brush og rør forsiktig i 10 sekunder.
iii. Tørk/fortynn i 10 sekunder ved bruk av ¼ til ½ lufttrykk.
Preparasjonen skal ha et skinnende utseende.
iv. Herd med lys i 10 sekunder (20 sekunder for lys med <600 mW/cm2).
b) Bruksanvisning for sprøyten
i. Lag en pytt av Peak™ Universal Bond med Inspiral™ Brush Tip. Rørforsiktig i 10 sekunder.
ii. Tørk/fortynn i 10 sekunder ved bruk av ¼ til ½ lufttrykk.
iii. Preparasjonen skal ha et skinnende utseende.
iv. Herd med lys i 10 sekunder (20 sekunder for lys med <600 mW/
cm2).
6. Gjenoppbygg med flytende og/eller fast kompositt i henhold til
fabrikantens instruksjoner.
Stift og kjerne
1. Klargjøra) Bor hull til stiften ved bruk av en gummistopper og passende størrelse
UniCore™ Drill.
b) Skyll stiftrommet grundig i 10 sekunder ved bruk av en TriAway
Adaptor og en 22 g Endo-Eze™-spiss. Tørk med TriAway-adapter og 22
g Endo-Eze Tip fra bunnen av preparasjonen og opp.
c) Bekreft stifttilpasningen (UniCore Post) og kutt til ønsket lengde meden høyhastighets diamantskive. MERK: Karbid- og operative bor kan
frynse fibrene.
2. Etsninga) Selvetsningsteknikk
i. Skyll kanalrommet og la være fuktig.
ii. Fest en blå 22 g Deliver-Eze™-børstespiss til Peak SE-sprøyten.
iii. Påfør på stiftområdet og kronepreparasjon i 20 sekunder underomrøring.
iv. Blås ut overflødig materiale med TriAway Adaptor og 22 g
Endo-Eze Tip, fra bunnen av rommet, oppover. Tynn ut/tørk i 3
sekunder ved bruk av luft-/vannsprøyten eller ved å plassere et
høyvolumsug direkte over tannpreparatet.
v. Gå videre til “Binding”-trinnet nedenfor.
b) Selvetsningsteknikk
i. Fest en blå 22 g Endo-Eze Tip til Ultra-Etch-sprøyten.
ii. Start apisk og fyll stiftrommet koronalt. Påfør koronalt preparat.
Ets i 20 sekunderiii. Sug av overflødig etsningsmiddel.
iv. Ved bruk av TriAway Adaptor og 22 g Endo-Eze Tip, skyll grundig
og lufttørk lett til stiftrommet er lett fuktig.
v. Gå videre til “Binding”-trinnet nedenfor.
3. Bindinga) Bruksanvisning for flaskei. Trykk ut 1-3 dråper med Peak Universal Bond på “B”-siden av
engangs-dappenplaten.
ii. Ved bruk av Nano-Brush™ eller NaviTip FX, påfør Peak Universal
Bond på stiftrommet og rør forsiktig i hele kanallengden og
tannpreparatet i 10 sekunder.
iii. Fjern grundig overflødig materiale ved bruk av TriAway Adaptor og
22 g Endo-Eze Tip.
iv. Tynn ut/tørk i 10 sekunder ved bruk av ¼ til ½ lufttrykk. Preparatet
skal se skinnende ut.
v. Lysherd nedover stiftområdet i 20 sekunder (40 sekunders lys med
utgang <600mw /cm2 ).
vi. Bruk papirspiss eller tidligere tilpasset stift for å bekrefte at
stiftrommet ikke er blokkert.
b) Bruksanvisning for sprøyten
i. Fest en 30 gr NaviTip™ FX Brush Tip til Peak Universal Bondsprøyten.
ii. Påfør 1-2 dråper i stiftrommet og på preparasjonen, rør deretterom i hele kanalens lengde, inkludert hele det preparerte området
på tannen, i 10 sekunder.
iii. Fjern grundig alt overflødig Peak Universal Bond ved bruk av
TriAway Adaptor og 22 gr Endo-Eze Tip.
iv. Tørk stiftrommet og det preparerte området på tannen med luft
i 10 sekunder ved bruk av fullt lufttrykk for å fortynne/tørke med
TriAway Adaptor og 22 gr Endo-Eze Tip for å fordampe eventuelt
gjenværende løsemiddel fra bunnen og opp.

v.

Herd med lys inne i stiftrommet i 20 sekunder (40 sekunder for lys
med <600 mW/cm2). Bruk papirspiss eller tidligere tilpasset stiftfor å bekrefte at stiftrommet ikke er blokkert.

Stiftsementering og kjerneoppbygging
1) Fjern hetten fra PermaFlo™ DC-sprøyten.
2) Plasser blandespissen i den doble sprøyten, jamfør de to åpningene.
Skru med klokken inntil de låses på plass.
3) Fest fleksibel Intraoral Tip™ til blandespissen for levering direkte ikanalen fra den doble sprøyten.
4) Trykk ut en liten mengde før plassering i stiftrommet.
5) Før spissen inn i stiftrommet i full dybde.
6) Ved bruk av jevnt trykk leveres PermaFlo DC apisk og i retning kronen.
7) Sett stiften (UniCore™ Post) sakte inn, slik at den fortrenger overflødig
sement.
8) Plasser herdelyst direkte over stiften og lysherd i 20 sekunder – 40
sekunder for lys med utgang <600mW/cm2).
9) Fortsett å bygge opp lag av PermaFlo DC rundt stiften, etter behov.
MERK: Lysherd i 5-4 sekunder mellom lag for å danne gelé og forme en
kjerne. Foreta en endelig herding av kjernen i 40 sekunder. Ikke fjern
blandespissen før neste bruk. Desinfiser sprøyten og blandespissen.
Forholdsregler og advarsler:
1. Forsikre deg om at du nøye har lest og forstått alle instruksjonene før
bruk av Peak Universal Bond.
2. Kun for profesjonell bruk.
3. Sett hetten tilbake på plass direkte etter bruk for å unngå
polymerisering.
4. Bekreft alltid flyt av sprøytematerialer før interoral bruk. I tilfelle
motstand, erstatt spissen og sjekk igjen.
5. La hettene sitte på flasken inntil bruk.
6. Kliniker og pasient må bruke UV-beskyttelsesbriller under herding av
komposittmaterialer.
7. Hvis ikke i daglig bruk, oppbevar produktet i kjøleskap.
8. La nedkjølte produkter nå romtemperatur før bruk.
9. For å optimere bindestyrke, bruk olje- og vannfri luft.
10. Snu vekk overhengende lys for å hindre for tidlig polymerisering av alleresinbaserte materialer.
11. Resiner kan forårsake følsomhet. Unngå gjentatt hudkontakt med
uherdet dentalresin. Ikke bruk på pasienter med en kjent følsomhet
til akrylater eller andre resiner. I tilfelle allergisk reaksjon, utvikling av
dermatitt eller utslett, kontakt lege.
12. Kast brukte spisser, tomme sprøyter og flasker forskriftsmessig.
13. Oppbevares utilgjengelig for barn.
14. Ikke bruk etter utløpsdato som er merket på beholderne.
15. Sett hetten tilbake på plass, desinfiser og tørk av sprøyten med
en mellomnivå desinfiserer mellom bruk. Dersom det brukes
sprøytetrekk som kastes etter bruk, sett hetten tilbake på plass og kast
sprøytetrekket.
16. Spissene er til engangsbruk. For å unngå krysskontaminering, ikke brukspissene mer enn én gang.
17. Hold produktene vekke fra varmekilder og direkte sollys.
18. Isoler bruk av sterke kjemikalier til behandlingsområdet.
MERK: For SDS og tilleggsinformasjon om bruk av Peak
Universal Bond, Peak SE og Peak LC-bindingsresin eller relaterte
produkter, vennligst gå til www.ultradent.com

33

EL

Peak™ Universal Bond και Peak™ SE

Περιγραφή:Το Peak Universal Bond είναι ρητίνη συγκόλλησης που παρέχεται είτε με φιαλίδιο
είτε με μονή σύριγγα. Δύναται να χρησιμοποιηθεί με την αυτοαδροποιούμενη τεχνική
ή με ολική αδροποίηση. Περιέχει ενισχυτικές ουσίες σε ποσοστό 7,5% με έκδοχο
διαλύτη αιθυλικής αλκοόλης και θα πολυμεριστεί με τα περισσότερα φώτα υψηλής
έντασης συμπεριλαμβανομένων και των LED. Το Peak Universal Bond περιέχει 0,2%χλωρεξιδίνη που μπορεί να εξασφαλίσει μακροχρόνια ισχύ συγκόλλησης.
Το primer Peak SE είναι μία συγκολλητική ρητίνη οδοντίνης η οποία περιέχει
αδροποίηση και primer σε σύστημα τοποθέτησης με σύριγγα.
Το Ultra-Etch™ είναι μία συγκολλητική ρητίνη οδοντίνης η οποία περιέχει αδροποίηση
και primer σε σύστημα τοποθέτησης με σύριγγα.
Η προσθήκη χλωρεξιδίνης δεν έχει δείξει να σχετίζεται με την μείωση της δευτερογενής
τερηδόνας σε ασθενείς. Δεν έχουν διεξαχθεί κλινικές μελέτες για την αξιολόγηση τηςχλωρεξιδίνης σε στοματικά βακτηρίδια ή τερηδόνα.
Ενδείξεις για χρήση:Χρησιμοποιείται για σχεδόν όλες σας τις ανάγκες για αδροποίηση και συγκόλληση
στην επανορθωτική οδοντιατρική και για ασθενείς όλων των ηλικιών.
Το Peak Universal Bond συγκολλάται με τα παρακάτω υλικά:• Οδοντίνη και Αδαμαντίνη• Πορσελάνη, ζιρκόνια
• Μέταλλο• Σύνθετη Ρητίνη
Οδηγίες χρήσης:ΣΗΜΕΙΩΣΗ: Η αρχική χρήση του Peak SEαπαιτεί ενεργοποίηση των δύο συστατικών πουδιαχωρίζονται στη σύριγγα JetMix™.
1) Το Peak SE είναι σταθερό για 120 ημέρες μετά τηνενεργοποίηση.
2) Γράψτε την ημερομηνία λήξης στην επίπεδη περιοχή
του εμβόλου πριν από την ενεργοποίηση.
3) ΜΗΝ ΑΦΑΙΡΕΙΤΕ ΤΟ ΠΩΜΑ ΤΗΣ ΑΣΦΑΛΙΣΗΣ LUERΠΡΙΝ ΑΠΟ ΤΗΝ ΑΝΑΜΙΞΗ4) Πατήστε γρήγορα και δυνατά το έμβολο πουφέρει την ημερομηνία μέσα στο μεσαίο τμήμα
του εμβολου.
5) Επαληθεύστε ότι το έμβολο είναι στο ίδιο επίπεδο με
το μεσαίο τμήμα του εμβόλου.

34

Τεχνική άμεσης συγκόλλησης και επισκευή
πορσελάνης / ζιρκόνιας
1.Προετοιμασίαα) Οδοντίνης/Αδαμαντίνης: Απομονώστε, καθαρίστε
και αφαιρέστε την τερηδόνα επιβεβαιώνονταςότι έχει αφαιρεθεί όλη η μη ενασβεστιωμένη οδοντίνη (Συνιστάται το Seek/
Sable Seek γι αυτό). Για αποτριβές σε αποκαταστάσεις Ομάδας V, τραχύνετε
με φρέζα διαμαντιού.
β) Σύνθετη Ρητίνη: Αφαιρέστε τις εξουθενωμένες περιοχές υπάρχουσας σύνθετης
ρητίνης. Τραχύνετε την επιφάνεια με φρέζα διαμαντιού.
γ) Μέταλλο: Εκτελείτε μικροαποτριβή στην επιφάνεια.
δ) Ζιρκόνια: Καθαρίστε την επιφάνεια και αφαιρέστε την εξουθενωμένη ζιρκόνια
με φρέζα διαμαντιού.
ε) Πορσελάνη: Τραχύνετε και αφαιρείτε την εξουθενωμένη πορσελάνη μεφρέζα διαμαντιού. Καθαρίστε την περιοχή σπασμένης πορσελάνης επί 5δευτερόλεπτα με Ultra-Etch. Ξεπλένετε και στεγνώνετε.
2.Αδροποιητικό
α)Αυτοαδροποιούμενη Τεχνική – οδοντίνη/αδαμαντίνη, σύνθετη ρητίνη και μέταλλο
i. Ξεπλένετε την παρασκευή και την αφήνετε υγρή.
ii. ΠΡΟΑΙΡΕΤΙΚΟ – Απλώστε Consepsis™ (όπου διατίθεται) με έτο ρύγχος
Black Mini Brush βουρτσίζοντας την παρασκευή και στεγνώνετε ελαφρά
με αέρα αφήνοντας την επιφάνεια υγρή.
iii. Απλώστε το Peak SE με το ρύγχος Black Mini Brush στην παρασκευή επί 20δευτερόλεπτα τρίβοντας την οδοντίνη. Μην τρίψετε την αδαμαντίνη.
Αραιώστε/στεγνώστε επί 3 δευτερόλεπτα χρησιμοποιώντας τη σύριγγα
αέρα/ νερού ή τοποθετώντας την χειρουργική αναρρόφηση απευθείας
επάνω από την παρασκευή.
v. Συνεχίστε με το βήμα «Συγκόλληση» παρακάτω.
β) Τεχνική ολικής αδροποίησης – οδοντίνη/αδαμαντίνη, σύνθετη ρητίνη και μέταλλο
i. Επιβεβαιώστε το χρώμα και την πυκνότητα ροής του προϊόντος προτού
το εφαρμόσετε, τοποθετώντας μια μικρή ποσότητα σε επίθεμα ανάμιξης ή
γάζα. Πετάξτε όλο το διαυγές υγρό που βγαίνει.
ii. Απλώστε Ultra-Etch με το ρύγχος Blue Micro™ σε όλες τις επιφάνειες τηςπαρασκευής του δοντιού επί 20 δευτερόλεπτα.
iii. Ξεπλένετε καλά επί 5 δευτερόλεπτα.
iv. Στεγνώνετε ελαφρά με τη σύριγγα αέρα/νερού ή τοποθετείτε τηνχειρουργική αναρρόφηση απευθείας επάνω από την παρασκευή. Αφήστε
την επιφάνεια ελαφρώς υγρή.
v. ΠΡΟΑΙΡΕΤΙΚΟ – Απλώστε Consepsis (όπου διατίθεται) με το ρύγχος Black
Mini Brush βουρτσίζοντας την παρασκευή και στεγνώνετε ελαφρά με αέρααφήνοντας την επιφάνεια υγρή.
vi. Συνεχίστε με το βήμα «Συγκόλληση» παρακάτω.
γ) Αδροποίηση πορσελάνης – ΠΡΟΣΟΧΗ – χρησιμοποιήστε κατάλληλη απομόνωση
όπως ένα προϊόν προστασίας/ εξουδετέρωσης οξέων (EtchArrest™) ότανχρησιμοποιείτε υδροφθορικό οξύ (HF) (Αδροποιητικό Πορσελάνης Ultradent™).
Μην αφήνετε το υδροφθορικό οξύ να αγγίξει τα ούλα ή την οδοντίνη.
i. Απλώστε υδροφθορικό οξύ στην περιοχή που χρειάζεται επιδιόρθωση
επί 90 δευτερόλεπτα.
ii. Κάνετε αναρρόφηση του οξέος από την επιφάνεια και ΚΑΤΟΠΙΝ ξεπλένετε
καλά και στεγνώνετε.
iii. Απλώστε Ultra-Etch επί 5 δευτερόλεπτα για να αφαιρεθούν τα άλατα
πορσελάνης και τα υπολείμματα που δημιουργήθηκαν από τηναδροποίηση HF. Ξεπλένετε και στεγνώνετε.
iv. Απλώστε μια παχιά στρώση από σιλάνιο επί 60 δευτερόλεπτα.
v. Στεγνώστε καλά. ΜΗΝ ΞΕΠΛΕΝΕΤΕ.
vi. Συνεχίστε με το βήμα «Συγκόλληση» παρακάτω.
δ) Ζιρκόνια – ΜΗΝ ΑΔΡΟΠΟΙΕΙΤΕ ΚΑΙ ΜΗ ΧΡΗΣΙΜΟΠΟΙΕΙΤΕ ΣΙΛΑΝΙΟ
i. Κάντε αεραποτριβή στην σπασμένη επιφάνεια της προσθετικής εργασίας,την ξεπλένετε και την στεγνώνετε.
ii. Απλώστε primer ζιρκόνιας στη σπασμένη περιοχή τηρώντας τις οδηγίες
του κατασκευαστή.
iii. Συνεχίστε με το βήμα «Συγκόλληση» παρακάτω.
3.Συγκόλλησηα) Παροχή με φιαλίδιο
i. Βάλτε 1-3 σταγόνες από το Peak™ Universal Bond στην πλευρά «Β» τουαναλώσιμου ιγδίου.
ii. Με το Micro Applicator Brush, απλώστε μια παχιά στρώση από
Peak™ Universal Bond στην παρασκευή και το τρίβετε απαλά επί 10δευτερόλεπτα.
iii. Το αραιώνετε/στεγνώνετε επί 10 δευτερόλεπτα με πίεση αέρα ¼ έως ½. Ηπαρασκευή πρέπει να έχει γυαλιστερή εμφάνιση.
iv. Φωτοπολυμερίστε επί 10 δευτερόλεπτα (20 δευτερόλεπτα για συσκευές μεένταση <600mW/cm2).
v. Αποκαταστήστε με λεπτόρρευστη ή σύνθετη ρητίνη, σύμφωνα με τιςοδηγίες του κατασκευαστή.
β) Παροχή με σύριγγα
i. Απλώστε μια παχιά στρώση από Peak™ Universal Bond με το ρύγχος
Inspiral Brush - το τρίβετε απαλά επί 10 δευτερόλεπτα.
ii. Το αραιώνετε/στεγνώνετε επί 10 δευτερόλεπτα με πίεση αέρα ¼ έως ½. Ηπαρασκευή πρέπει να έχει γυαλιστερή εμφάνιση.
iii. Φωτοπολυμερίστε επί 10 δευτερόλεπτα (20 δευτερόλεπτα για φώτα με
παραγωγή <600mW/cm2).
iv. Αποκαταστήστε με λεπτόρρευστη ή σύνθετη ρητίνη, σύμφωνα με τιςοδηγίες του κατασκευαστή.
Τεχνική έμμεσης συγκόλλησης – Έμμεσες στεφάνες, ένθετα, επένθετα,ζιρκόνια1. Προετοιμασία
α) Αφαιρέστε την προσωρινή, καθαρίστε την παρασκευή, ξεπλένετε καιστεγνώνετε (Consepsis Scrub με ένα βουρτσάκι STARbrush™ για να καθαρίσετε,iv.

απολυμάνετε και για να αφαιρέσετε τα υπολείμματα κονίας).
β) Επιβεβαιώστε την εφαρμογή της προσθετικής εργασίας.
γ) Προετοιμάστε την εσωτερική επιφάνεια της προσθετικής εργασίας.
i. Με βάση το μέταλλο:(1) Εκτελέστε μικροαποτριβή (αμμοβολισμό) στην εσωτερική επιφάνεια
προσθετικής εργασίας.
(2) Ξεπλένετε και στεγνώνετε την επιφάνεια.
ii. Κεραμικό/πορσελάνη:(1) Απλώστε υδροφθορικό οξύ (HF) (Αδροποιητικό Πορσελάνης
Ultradent) στην εσωτερική επιφάνεια της προσθετικής εργασίας επί 90δευτερόλεπτα, ξεπλένετε και στεγνώνετε.
(2) Απλώστε Ultra-Etch επί 5 δευτερόλεπτα για να αφαιρεθούν τα άλατα
πορσελάνης και τα υπολείμματα που δημιουργήθηκαν από το HF.
Ξεπλένετε και στεγνώνετε.
(3) Απλώστε σιλάνιο (Σιλάνιο Ultradent™) στην εσωτερική επιφάνεια τηςπροσθετικής εργασίας επί 1 λεπτό, στεγνώστε και αφήστε την προσθετική
εργασία στην άκρη. Μην ξεπλένετε.
iii. Ζιρκόνια: ΜΗΝ ΑΔΡΟΠΟΙΕΙΤΕ ΚΑΙ ΜΗ ΧΡΗΣΙΜΟΠΟΙΕΙΤΕ ΣΙΛΑΝΙΟ(1) Κάντε αεραποτριβή στην εσωτερική πλευρά της προσθετικής εργασίας,ξεπλένετε και στεγνώνετε.
(2) Απλώστε ένα primer ζιρκόνιας, σύμφωνα με τις οδηγίες τουκατασκευαστή.
2.Αδροποιήστε – Προετοιμάστε την επιφάνεια δοντιούα) Αυτοαδροποιούμενη Τεχνική – οδοντίνη/αδαμαντίνη, σύνθετη ρητίνη και μέταλλο
i. Ξεπλένετε την παρασκευή και την αφήνετε υγρή.
ii. ΠΡΟΑΙΡΕΤΙΚΟ – Απλώστε Consepsis (όπου διατίθεται) με το ρύγχος Black
Mini Brush τρίβοντας την παρασκευή και στεγνώστε ελαφρά με αέρααφήνοντας την επιφάνεια υγρή.
iii. Απλώστε το Peak™ SE με το ρύγχος Black Mini Brush στην παρασκευή επί 20δευτερόλεπτα τρίβοντας την οδοντίνη. Μην τρίβετε την αδαμαντίνη.
iv. Αραιώστε /στεγνώστε επί 3 δευτερόλεπτα χρησιμοποιώντας τη σύριγγα
αέρα/ νερού ή τοποθετώντας την χειρουργική αναρρόφηση όγκου
απευθείας επάνω από την παρασκευή.
v. Συνεχίστε με το βήμα «Συγκόλληση» παρακάτω.
β) Τεχνική ολικής αδροποίησης – οδοντίνη /αδαμαντίνη, σύνθετη ρητίνη και μέταλλο
i. Απλώστε Ultra-Etch με το ρύγχος Blue Micro σε όλες τις επιφάνειες τηςπαρασκευής επί 20 δευτερόλεπτα.
ii. Ξεπλένετε καλά επί 5 δευτερόλεπτα.
iii. Στεγνώνετε ελαφρά με τη σύριγγα αέρα /νερού ή τοποθετείτε τηνχειρουργική αναρρόφηση όγκου απευθείας επάνω από την παρασκευή.
Αφήστε την επιφάνεια ελαφρώς υγρή.
iv. ΠΡΟΑΙΡΕΤΙΚΟ – Απλώστε Consepsis (όπου διατίθεται) με το ρύγχος Black
Mini Brush τρίβοντας την παρασκευή και στεγνώστε ελαφρά με αέρααφήνοντας την επιφάνεια υγρή.
v. Συνεχίστε με το βήμα «Συγκόλληση» παρακάτω.
γ) Αδροποίηση πορσελάνης – ΠΡΟΣΟΧΗ – χρησιμοποιήστε κατάλληλη απομόνωση
όπως ένα προϊόν προστασίας/ εξουδετέρωσης οξέων (EtchArrest) ότανχρησιμοποιείτε υδροφθορικό οξύ (HF) (Αδροποιητικό Πορσελάνης Ultradent).
Μην αφήνετε το υδροφθορικό οξύ να αγγίξει τα ούλα ή την οδοντίνη.
i. Απλώστε υδροφθορικό οξύ στη ραγισμένη περιοχή επί 90 δευτερόλεπτα.
ii. Κάνετε αναρρόφηση του οξέος από την επιφάνεια και ΚΑΤΟΠΙΝ ξεπλένετε
καλά και στεγνώνετε.
iii. Απλώστε Ultra-Etch επί 5 δευτερόλεπτα για να αφαιρεθούν τα άλατα
πορσελάνης και τα υπολείμματα που δημιουργήθηκαν από τηναδροποίηση HF. Ξεπλένετε και στεγνώνετε.
iv. Απλώστε μια παχιά στρώση από σιλάνιο επί 60 δευτερόλεπτα.
v. Στεγνώστε καλά. ΜΗΝ ΞΕΠΛΕΝΕΤΕ.
vi. Συνεχίστε με το βήμα «Συγκόλληση» παρακάτω.
δ) Ζιρκόνια – ΜΗΝ ΑΔΡΟΠΟΙΕΙΤΕ ΚΑΙ ΜΗ ΧΡΗΣΙΜΟΠΟΙΕΙΤΕ ΣΙΛΑΝΙΟ
i. Κάντε αεραποτριβή στην εσωτερική πλευρά της προσθετικής εργασίας,ξεπλύντε και στεγνώστε.
ii. Απλώστε primer ζιρκόνιας στη στην περιοχή που χρειάζεται επιδιόρθωση
τηρώντας τις οδηγίες του κατασκευαστή.
iii. Συνεχίστε με το βήμα «Συγκόλληση» παρακάτω.
3.Συγκόλλησηα. Παροχή με φιαλίδιο
i. Βάλτε 1-3 σταγόνες από Peak Universal Bond στην πλευρά «B» τουαναλώσιμου ιγδίου.
ii. Χρησιμοποιώντας το Micro Applicator Brush, απλώστε μια παχιά στρώση

από Peak Universal Bond στην παρασκευή και τρίψτε ελαφρά επί 10δευτερόλεπτα.
iii. Το αραιώνετε/στεγνώνετε επί 10 δευτερόλεπτα με πλήρη πίεση αέρα. Η
παρασκευή πρέπει να έχει γυαλιστερή εμφάνιση.
iv. Φωτοπολυμερίστε επί 10 δευτερόλεπτα (20 δευτερόλεπτα για συσκευές μεένταση<600mW/cm2).
β) Παροχή με σύριγγα
i. Απλώστε μια παχιά στρώση από Peak™ Universal Bond με το ρύγχος Inspiral
Brush - τρίψτε απαλά επί 10 δευτερόλεπτα.
ii. Το αραιώνετε/στεγνώνετε επί 10 δευτερόλεπτα με πλήρη πίεση αέρα. Η
παρασκευή πρέπει να έχει γυαλιστερή εμφάνιση.
iii. Φωτοπολυμερίστε επί 10 δευτερόλεπτα (20 δευτερόλεπτα για συσκευές μεένταση<600 mW/cm2).
4.Κονίαα) Χρησιμοποιήστε φωτοπολυμεριζόμενη κονία για ημιδιαφανής όψεις ή ρητινώδη
κονία διπλού πολυμερισμού για άλλες προσθετικές εργασίες και τηρήστε τιςοδηγίες χρήσης του κατασκευαστή.
ΣΗΜΕΙΩΣΗ: Για την άμεση απόφραξη των οδοντινοσωληναρίων με τη χρήση
συγκολλητικού παράγοντα (Immediate Dentin Sealing), δείτε τα βήματα 2Α και 3της ανωτέρας Άμεσης Τεχνικής. Απλώστε γλυκερίνη επάνω από το Peak Universal
Bond και φωτοπολυμερίστε επί 10 δευτερόλεπτα. Ξεπλένετε τη γλυκερίνη.
Πάρτε το τελικό αποτύπωμα. Απλώστε ξανά γλυκερίνη στην παρασκευή ωςμέσο διαχωρισμού προτού κολλήσετε την προσωρινή προσθετική εργασία στηθέση της με κονία.
Επιδιόρθωση Σύνθετης ρητίνης / Μέταλλου / Ζιρκονίας / Πορσελάνης
1. Σύνθετη Ρητίνη: Αφαιρέστε τις εξασθενισμένες περιοχές υπάρχουσας σύνθετης
ρητίνης. Τραχύνετε την επιφάνεια με φρέζα από διαμάντι.
α) Τεχνική ολικής αδροποίησης
i. Απλώστε το Ultra-Etch με το Blue Micro Tip σε όλες τις επιφάνειες τηςπαρασκευής επί 20 δευτερόλεπτα.
ii. Το ξεπλένετε σχολαστικά επί 5 δευτερόλεπτα και το αφήνετε υγρό.
2. Μέταλλο: Εκτελείτε μικροαποτριβή στην επιφάνεια
α) Τεχνική ολικής αδροποίησης
i. Απλώστε το Ultra-Etch με το Blue Micro Tip σε όλες τις επιφάνειες τηςπαρασκευής επί 20 δευτερόλεπτα
ii. Το ξεπλένετε σχολαστικά επί 5 δευτερόλεπτα και το αφήνετε υγρό.
3. Ζιρκονία: Καθαρίστε την επιφάνεια, αφαιρέστε την εξασθενισμένη ζιρκονία
με φρέζα από διαμάντι. ΜΗΝ ΑΔΡΟΠΟΙΗΣΕΤΕ ΟΥΤΕ ΝΑ ΧΡΗΣΙΜΟΠΟΙΗΣΕΤΕΣΙΛΑΝΙΟ.
α) Κάντε αεραποτριβή στην εσωτερική επιφάνεια της προσθετικής εργασίας.
β) Απλώστε primer ζιρκονίας στην σπασμένη περιοχή ακολουθώντας τις οδηγίες
του κατασκευαστή.
4. Πορσελάνη: Τραχύνετε και αφαιρείτε την εξασθενισμένη πορσελάνη μεφρέζα από διαμάντι. Καθαρίστε την σπασμένη περιοχή πορσελάνης επί 15δευτερόλεπτα με Ultra-Etch. Ξεπλένετε και στεγνώνετε.
ΠΡΟΣΟΧΗ – χρησιμοποιήστε την κατάλληλη απομόνωση όπως ένα προϊόν
προστασίας/ εξουδετέρωσης οξέων (EtchArrest) όταν χρησιμοποιείτε
υδροφθορικό οξύ (HF) (Αδροποιητικό Πορσελάνης της Ultradent™). Μην αφήνετετο υδροφθορικό οξύ να αγγίξει τα ούλα ή την οδοντίνη.
α) Απλώστε υδροφθορικό οξύ στην σπασμένη περιοχή επί 90 δευτερόλεπτα.
β) Κάνετε αναρρόφηση του οξέος από την επιφάνεια και κατόπιν ξεπλένετε
σχολαστικά και στεγνώνετε την επιφάνεια.
γ) Απλώστε Ultra-Etch επί 5 δευτερόλεπτα για να αφαιρέσετε τα άλατα πορσελάνης
και τα υπολείμματα που δημιουργήθηκαν από την αδροποίηση με HF. Ξεπλένετε
και στεγνώνετε.
δ) Απλώστε μια παχιά στρώση από σιλάνιο επί 1 λεπτό.
ε) Στεγνώνετε σχολαστικά. ΜΗΝ ΤΟ ΞΕΠΛΕΝΕΤΕ.
5. Συγκόλλησηα) Παροχή με φιαλίδιο
i. Βάλτε 1-3 σταγόνες από το Peak™ Universal Bond στην πλευρά «Β» τουαναλώσιμου ιγδίου.
ii. Με το Micro Applicator Brush, απλώστε μια παχιά στρώση από Peak™
Universal Bond και το τρίβετε απαλά επί 10 δευτερόλεπτα.
iii. Το αραιώνετε/στεγνώνετε επί 10 δευτερόλεπτα με πίεση αέρα 1/4 to 1/2. Ηπαρασκευή πρέπει να έχει γυαλιστερή εμφάνιση.
iv. Φωτοπολυμερίστε επί 10 δευτερόλεπτα (20 δευτερόλεπτα για συσκευές μεένταση<600mW/cm2).
β) Παροχή με σύριγγα

35

36

i. Απλώστε μια παχιά στρώση από Peak™ Universal Bond με το ρύγχος Inspiralv. Φωτοπολυμερίστε το χώρο του ενδοριζικού άξονα επί 20 δευτερόλεπτα (40Brush - τρίψτε απαλά επί 10 δευτερόλεπτα.
δευτερόλεπτα συσκευές με ένταση <600mW/cm2). Χρησιμοποιήστε κώνοχάρτου ή τον πρώην προσαρμοσμένο άξονα για να βεβαιωθείτε ότι δεν
ii. Το αραιώνετε/στεγνώνετε επί 10 δευτερόλεπτα με πίεση αέρα 1/4 to 1/2.
είναι φραγμένος ο χώρος για τον άξονα.
iii. Η παρασκευή πρέπει να έχει γυαλιστερή εμφάνιση.
iv. Φωτοπολυμερίστε επί 10 δευτερόλεπτα (20 δευτερόλεπτα για συσκευές μεΣυγκόλληση και ανασύσταση του άξονα
ένταση<600mw/cm2).
1) Αφαιρέστε το πώμα από τη σύριγγα PermaFlo™ DC.
6. Αποκαταστήστε με λεπτόρρευστη ή σύνθετη ρητίνη, σύμφωνα με τις οδηγίες του2) Τοποθετήστε ένα ρύγχος ανάμιξης στη διπλή σύριγγα ευθυγραμμίζοντας τις δύοκατασκευαστή.
θύρες. Περιστρέψτε δεξιόστροφα μέχρις ότου κλειδωθεί στη θέση του.
3) Προσαρτήστε το εύκαμπτο Intraoral Tip™ στο ρύγχος ανάμιξης για την τοποθέτηση
Άξονας και Ανασύσταση
στο ριζικό σωλήνα απευθείας από τη διπλή σύριγγα.
1. Προετοιμασία
4) Βγάλτε μια μικρή ποσότητα πριν το τοποθετήσετε στην παρασκευή του άξονα.
α) Δημιουργήστε την παρασκευή για τον ενδοριζικό άξονα χρησιμοποιώντας ένα5) Εισάγετε το ρύγχος στο χώρο για τον άξονα στο πλήρες βάθος του.
πλαστικό στοπ και Τρυπάνι UniCore™ κατάλληλου μεγέθους.
β) Ξεπλένετε καλά την παρασκευή για τον άξονα επί 10 δευτερόλεπτα
6) Με ομοιόμορφη πίεση παρέχετε PermaFlo DC ξεκινώντας ακρορριζικά καιχρησιμοποιώντας τον αντάπτορα TriAway και ένα Ρύγχος 22ga Endo-Eze™.
συνεχίζοντας μυλικά.
Στεγνώστε με τον αντάπτορα TriAway και Ρύγχος 22ga Endo-Eze από το κάτω7) Εισάγετε τον άξονα UniCore™ αργά, εκτοπίζοντας την περίσια κονία.
8) Τοποθετήστε το φως πολυμερισμού απευθείας επάνω από για συσκευές με ένταση
μέρος της παρασκευής προς τα επάνω.
και φωτοπολυμερίστε επί 20 δευτερόλεπτα, (40 δευτερόλεπτα για συσκευές μεγ) Επιβεβαιώστε ότι ταιριάζει το μέγεθος του επιλεγμένου άξονα (UniCore Post) καιένταση <600mW/cm2).
κόψτε στο μήκος που θέλετε χρησιμοποιώντας ένα δίσκο διαμαντιού υψηλής
9) Συνεχίστε κάνοντας ανασύσταση με το PermaFlo™ DC γύρω από τον άξονα
ταχύτητας. ΣΗΜΕΙΩΣΗ: Οι φρέζες από καρβίδιο και οι χειρουργικές φρέζεςόσο χρειάζεται. ΣΗΜΕΙΩΣΗ: Φωτοπολυμερίστε επί 5 δευτερόλεπτα μεταξύ τωνενδέχεται να ξεφτίσουν τις ίνες.
στρώσεων για να σταθεροποιηθούν και να δημιουργήσετε την ανασύσταση.
2.Αδροποίηση
Εφόσον ολοκληρώσετε την ανασύσταση, φωτοπολυμερίστε επί 40 δευτερόλεπτα.
α) Αυτοαδροποιούμενη Τεχνική
Μην αφαιρείτε το ρύγχος ανάμιξης μέχρι την επόμενη χρήση. Απολυμαίνετε τη
i. Ξεπλένετε το παρασκευή για τον άξονα και το αφήνετε υγρό.
™
σύριγγα και το ρύγχος ανάμιξης.
ii. Βιδώστε ένα ρύγχος 22ga Deliver-Eze Brush στην σύριγγα Peak SE.
iii. Τοποθετήστε το σε ολόκληρη την παρασκευή του άξονα μέχρι την μυλική
παρασκευή επί 20 δευτερόλεπτα τριβοντάς το.
Προφυλάξεις και προειδοποιήσεις:
iv. Φυσήξτε τις περίσσειες με τον αντάπτορα TriAway και το ρύγχος 22ga
1. Διαβάστε προσεκτικά και κατανοήστε όλες τις οδηγίες προτού χρησιμοποιήσετε
Endo-Eze από το κάτω μέρος της παρασκευής, προς τα επάνω. Αραιώστε /το Peak Universal Bond.
στεγνώστε επί 3 δευτερόλεπτα χρησιμοποιώντας τη σύριγγα αέρα/νερού
2. Για επαγγελματική χρήση μόνο.
ή τοποθετώντας την χειρουργική αναρρόφηση απευθείας επάνω από την
3. Επανατοποθετήστε αμέσως το πώμα μετά τη χρήση προς αποφυγή πολυμερισμού.
παρασκευή.
4. Επαληθεύστε πάντοτε τη ροή των υλικών σε σύριγγα προτού τα τοποθετήσετε
v. Συνεχίστε με το βήμα «Συγκόλληση» παρακάτω.
ενδοστοματικά. Εάν αισθανθείτε αντίσταση, αντικαταστήστε το ρύγχος καιβ) Τεχνική ολικής αδροποίησης:ελέγξτε εκ νέου.
i. Συνδέστε ένα μπλε ρύγχος 22ga Endo-Eze με τη σύριγγα Ultra-Etch.
5. Κρατήστε το φιαλίδιο με το καπάκι κλειστό μέχρις ότου το χρησιμοποιήσετε.
ii. Ξεκινήστε ακρορριζικά και πληρώστε την παρασκευή για τον άξονα μέχρι
6. Ο ιατρός και ο ασθενής πρέπει να φοράνε προστατευτικά γυαλιά με προστασία
την μυλική παρασκευή. Αδροποιήστε επί 20 δευτερόλεπτα.
έναντι των υπεριωδών ακτίνων όταν φωτοπολυμερίζονται ρητινώδης υλικά.
iii. Αναρροφήστε το περίσσιο αδροποιητικό.
7. Φυλάξτε το προϊόν στο ψυγείο, εάν δεν το χρησιμοποιείτε καθημερινά.
iv. Χρησιμοποιώντας τον αντάπτορα TriAway και ένα ρύγχος 22ga Endo-Eze,
8. Φέρτε τα προϊόντα από το ψυγείο σε θερμοκρασία δωματίου προτού ταξεπλένετε καλά και στεγνώνετε ελαφρά με αέρα, αφήνοντας την παρασκευή
χρησιμοποιήσετε.
για τον άξονα ελαφρώς υγρή.
9. Για την μέγιστη δυνατή δύναμη συγκόλλησης, χρησιμοποιήστε αέρα χωρίς έλαια
v. Συνεχίστε με το βήμα «Συγκόλληση» παρακάτω.
και υγρασία.
3.Συγκόλληση10. Επανακατευθύνετε τον προβολέα της έδρας προς αποφυγή πρώιμου
α. Παροχή με φιαλίδιο
πολυμερισμού όλων των υλικών που έχουν βάση τη ρητίνη.
i. Βάλτε 1-3 σταγόνες από Peak Universal Bond στην πλευρά «B» του
11. Οι ρητίνες ενδέχεται να προκαλέσουν ευαισθησία. Αποφύγετε τηναναλώσιμου ιγδίου.
επαναλαμβανόμενη επαφή της απολυμέριστης ρητίνης με το δέρμα. Μην
ii. Χρησιμοποιώντας το Nano-Brush™ ή το NaviTip FX, απλώστε Peak Universalτο χρησιμοποιείτε σε ασθενείς με γνωστή ευαισθησία σε ακρυλικά ή άλλες
Bond στην παρασκευή του άξονα και τρίψτε απαλά όλα τα τοιχώματα τουρητίνες. Εάν παρουσιαστεί αλλεργική αντίδραση, δερματίτιδα ή εξάνθημα,ριζικού σωλήνα και της παρασκευής επί 10 δευτερόλεπτα.
συμβουλευτείτε ιατρό.
iii. Αφαιρέστε εντελώς τις περίσσειες με τον αντάπτορα TriAway και το Ρύγχος 12. Πετάξτε τα ρύγχη, τις άδειες σύριγγες και τα φιαλίδια με τον κατάλληλο τρόπο.
22ga Endo-Eze.
13. Φυλάξτε το μακριά από τα παιδιά.
iv. Στενώστε την παρασκευή του άξονα με πλήρη αέρα για 10 δευτερόλεπτα
14. Μην το χρησιμοποιείτε αφότου παρέλθει η ημερομηνία λήξης που αναγράφεταιχρησιμοποιώντας τον αντάπτορα TriAway και το ρύγχος 22ga Endo-Eze γιαστα δοχεία.
να εξατμιστεί ο εναπομένον διαλύτης.
15. Επανατοποθετήστε το πώμα, απολυμαίνετε και σκουπίστε τη σύριγγα μεv. Φωτοπολυμερίστε την παρασκευή του άξονα επί 20 δευτερόλεπτα (40ένα απολυμαντικό μεσαίου επιπέδου μεταξύ χρήσεων. Εάν χρησιμοποιηθεί2δευτερόλεπτα για συσκευές με ένταση <600mW/cm ).
αναλώσιμο κάλυμμα σύριγγας, αφαιρέστε το ρύγχος, επανατοποθετήστε τοvi. Χρησιμοποιήστε κώνο χάρτου ή τον άξονα που προσαρμόστηκε πριν για ναπώμα, και πετάξτε το κάλυμμα σύριγγας.
επιβεβαιώσετε ότι δεν είναι φραγμένος ο χώρος για τον άξονα.
16. Τα ρύγχη είναι αναλώσιμα. Προς αποφυγή διασταυρούμενης μόλυνσης, μηνβ) Παροχή με σύριγγα
επαναχρησιμοποιείτε τα ρύγχη.
i. Προσαρμόστε ένα ρύγχος 30ga NaviTip FX στη σύριγγα με το Peak™
17. Φυλάξτε τα προϊόντα μακριά από άμεση θερμότητα /ηλιακό φως.
Universal Bond.
18. Απομονώστε τις ισχυρές χημικές ουσίες στην περιοχή θεραπείας.
ii. Βάλτε 1-2 σταγόνες στο χώρο του ενδοριζικού άξονα και στην παρασκευή,και κατόπιν τρίψτε ολόκληρη την παρασκευή επί 10 δευτερόλεπτα.
ΣΗΜΕΙΩΣΗ: Για το Φύλλο Δεδομένων Ασφαλείας (SDS) και
iii. Αφαιρείτε όλο το περίσσιο Peak™ Universal Bond με το TriAway Adapter καισυμπληρωματικές πληροφορίες σχετικά με τη χρήση του Peak™
το Ρύγχος 22ga Endo-Eze.
Universal Bond, Peak™ SE, και άλλων σχετικών προϊόντων,επισκεφθείτε τη διεύθυνση www.ultradent.com
iv. Στεγνώνετε το χώρο του ενδοριζικού άξονα και την παρασκευή με πλήρη
πίεση αέρα επί 10 δευτερόλεπτα χρησιμοποιώντας το TriAway Adapter καιτο Ρύγχος 22ga Endo-Eze για να εξατμιστεί κάθε εναπομένον διαλύτης απόκάτω προς τα επάνω.

Адгезив Peak™ Universal Bond и праймер Peak™ SEОписание:Peak Universal Bond — это композитный адгезив, поставляемый в одном шприцеили во флаконе. Он может использоваться как с самопротравливанием, так и стотальным протравливанием. Адгезив на 7,5 % состоит из этанолового растворителяи отвердевает под большинством ярких ламп, в том числе светодиодных.
Peak Universal Bond содержит 0,2%-ый хлоргексидин, что может обеспечивать
долгосрочную прочность соединения.
Праймер Peak SE Primer — это самопротравливающий композитный адгезив,обеспечивающий сцепление с дентином. Он состоит из протравливающего
компонента и праймера, которые наносятся с помощью шприца.
Ultra-Etch™ — это протравливающий и промывочный гель, на 35 % состоящий изортофосфорной кислоты, поставляемый в шприце.
Введение добавки хлоргексидина не приводит к снижению вторичного кариесау пациентов. Клинические испытания для оценки влияния хлоргексидина набактериальную среду ротовой полости или кариес не приводились.
Показания к применению
Материалы используются практически для всех видов протравливания и фиксации ввосстановительной стоматологии для пациентов всех возрастов.
Композитный цемент Peak Universal Bond обеспечивает сцепление с указанными
ниже материалами:• Дентин и эмаль
• Керамика, цирконий
• Металл
• Композит
Указания по применению
ПРИМЕЧАНИЕ. При первом использовании
праймера Peak SE необходимо активироватьдва компонента, которые
разделены в шприце JetMix™.
1) Праймер Peak SE остается стабильным в течение
120 дней после активации.
2) Перед активацией запишите дату истечения срока
стабильности препарата на плоской поверхности
штока поршня.
3) НЕ СНИМАЙТЕ ЛЮЭРОВСКИЙ КОЛПАЧОК ДОСМЕШИВАНИЯ
4) Быстро и с силой вдавите поршень (с отмеченной
датой) в средний цилиндр.
5) Убедитесь в том, что поршень вошел в средний
цилиндр.
Техника прямой фиксации и восстановление
керамических или циркониевых коронок
1.Подготовка.
a) Дентин и эмаль. Изолируйте и очистите область, а также удалите кариес так,чтобы на зубах не осталось деминерализованного дентина (рекомендуется
использовать препарат Seek/Sable Seek). При препарировании абразивных/абфракционных дефектов класса V создайте шероховатость с помощью
алмазного бора.
b) Композит. Удалите ослабленные участки композита. Создайте шероховатостьс помощью алмазного бора.
c) Металл. Выполните микроабразивную обработку поверхности.
d) Цирконий. Очистите поверхность и удалите ослабленные участки циркония спомощью алмазного бора.
e) Керамика. Создайте шероховатость и удалите ослабленные участки керамикис помощью алмазного бора. Очищайте треснувший участок керамики 5секунд с помощью препарата Ultra-Etch. Промойте и высушите поверхность.
2.Протравливание.
a) Методика самопротравливания: дентин или эмаль, композит и металл.
i. Промойте подготовленную область и оставьте ее влажной.
ii. НЕ ОБЯЗАТЕЛЬНО К ВЫПОЛНЕНИЮ: с помощью насадки Black Mini™
Brush Tip чистящими движениями нанесите препарат Consepsis™
(при наличии) на препарированную область и слегка высушите зуб спомощью воздуха, так чтобы поверхность осталась влажной.
iii. С помощью насадки Black Mini Brush Tip нанесите праймер Peak SE на

RUпрепарированную область на 20 секунд, постоянно размазывая егобыстрыми движениями по дентину. Не поцарапайте эмаль.
iv. Распределяйте по поверхности и сушите препарат в течение трехсекунд с помощью пистолета с водой или воздухом либо интенсивного
отсоса, размещенного непосредственно над препарируемой областью.
v. Переходите к этапу «Фиксация».
b) Методика тотального протравливания: дентин или эмаль, композит и металл.
i. Перед аппликацией проверьте цвет и консистенцию материала,выдавив небольшое количество на бумагу для замешивания илимарлю. Если выдавится прозрачная жидкость, уберите ее.
ii. С помощью насадки Blue Micro™ Tip нанесите гель Ultra-Etch на всеповерхности препарируемого зуба на 20 секунд.
iii. Тщательно промойте зуб в течение 5 секунд.
iv. Слегка подсушите зубы с помощью пистолета с водой или воздухом
либо интенсивного отсоса, размещенного непосредственно надпрепарируемой областью. Оставьте поверхность немного влажной.
v. НЕ ОБЯЗАТЕЛЬНО К ВЫПОЛНЕНИЮ: с помощью насадки Black Mini
Brush Tip чистящими движениями нанесите препарат Consepsis (приналичии) на препарированную область и слегка высушите зуб спомощью воздуха, так чтобы поверхность осталась влажной.
vi. Переходите к этапу «Фиксация».
c) Средство для протравки керамики – ОСТОРОЖНО! Фтористоводородную
кислоту (Ultradent™ Porcelain Etch) разрешено использовать только снадлежащей изоляцией, например, с нейтрализующим кислоту барьером
(EtchArrest™). Не допускайте контакта фтористоводородной кислоты сдеснами и дентином.
i. Нанесите фтористоводородную кислоту на треснувшую область на
90 секунд.
ii. Удалите кислоту с поверхности с помощью отсоса, а ЗАТЕМ промойте ивысушите область.
iii. Нанесите Ultra-Etch на 5 секунд, чтобы удалить с керамики соли ипосторонние частицы от фтористоводородной протравки. Промойте ивысушите поверхность.
iv. Нанесите силан на 60 секунд.
v. Тщательно высушите. НЕ ПРОМЫВАЙТЕ ОБЛАСТЬ.
vi. Переходите к этапу «Фиксация».
d) ЗАПРЕЩАЕТСЯ ПРОТРАВЛИВАТЬ ЦИРКОНИЙ И НАНОСИТЬ НА НЕГО СИЛАН.
i. С помощью воздуха выполните абразивную обработку поврежденной
поверхности протеза, промойте и высушите обработанную область.
ii. Нанесите праймер для циркония на треснутую область в соответствии синструкциями производителя.
iii. Переходите к этапу «Фиксация».
3.Фиксация.
a) Флакон
i. Выдавите 1–3 капли адгезива Peak™ Universal Bond на сторону «B»одноразового стеклянного стаканчика.
ii. Используя микрощеточку-аппликатор Micro Applicator Brush, нанесите
адгезив Peak™ Universal Bond на препарированную область и осторожно
размазывайте его в течение 10 секунд.
iii. Размазывайте и сушите в течение 10 секунд с помощью воздуха поддавлением ¼- ½. Отпрепарированная область должна блестеть.
iv. Выполните отверждение светом в течение 10 секунд (20 секунд дляламп мощностью менее 600 мВт/см2).
v. Выполните восстановление с помощью жидкотекучего или пакуемого
композита в соответствии с инструкциями производителя.
b) Шприц
i. C помощью насадки Inspiral™ Brush Tip нанесите адгезив Peak Universal
Bond и осторожно размазывайте его в течение 10 секунд.
ii. Размазывайте и сушите в течение 10 секунд с помощью воздуха поддавлением ¼-½. Отпрепарированная область должна блестеть.
iii. Выполните отверждение светом в течение 10 секунд (20 секунд дляламп мощностью менее 600 мВт/см2).
iv. Выполните восстановление с помощью жидкотекучего или пакуемого
композита в соответствии с инструкциями производителя.
Методика непрямой фиксации — коронки, изготовленные непрямым
способом, вкладки, накладки и цирконий
1.Подготовка.
a) Снимите временную коронку, очистите, промойте и высушите
препарируемую область (используйте средство Consepsis Scrub с насадкой

37

38

STARbrush™ для чистки, дезинфекции и удаления оставшегося цемента).
b) Проверьте, правильно ли сидит протез.
c) Подготовьте внутреннюю поверхность протеза.
i. Металл.
(1) Выполните микроабразивную или пескоструйную обработку
внутренней поверхности протеза.
(2) Промойте и высушите поверхность.
ii. Керамика.
(1) Нанесите фтористоводородную кислоту (Ultradent Porcelain Etch) навнутреннюю поверхность протеза на 90 секунд, после чего промойтеи высушите ее.
(2) Нанесите Ultra-Etch на 5 секунд, чтобы удалить с керамики соли ипосторонние частицы от фтористоводородной протравки. Промойте ивысушите поверхность.
(3) Нанесите силан (Ultradent™ Silane) на внутреннюю поверхность
протеза на 1 минуту, после чего высушите протез и отложите протез.
Не промывайте.
iii. Цирконий. ЗАПРЕЩАЕТСЯ ПРОТРАВЛИВАТЬ ЦИРКОНИЙ И НАНОСИТЬНА НЕГО СИЛАН.
(1) С помощью воздуха выполните абразивную обработку внутренней
поверхности протеза, промойте и высушите обработанную область.
(2) Нанесите праймер для циркония в соответствии с инструкциями
производителя.
2.Протравливание: подготовка поверхности зуба.
a) Методика самопротравливания: дентин или эмаль, композит и металл.
i. Промойте подготовленную область и оставьте ее влажной.
ii. НЕ ОБЯЗАТЕЛЬНО К ВЫПОЛНЕНИЮ: с помощью насадки Black Mini Brush
Tip чистящими движениями нанесите препарат Consepsis (при наличии)на препарированную область и слегка высушите зуб с помощью воздуха,так чтобы поверхность осталась влажной.
iii. С помощью насадки Black Mini™ Brush Tip нанесите праймер Peak™ SEна подготовленную область на 20 секунд, постоянно размазывая егобыстрыми движениями по дентину. Не поцарапайте эмаль.
iv. Распределяйте по поверхности и сушите препарат в течение трех секундс помощью пистолета с водой или воздухом либо интенсивного отсоса,размещенного непосредственно над препарируемой областью.
v. Переходите к этапу «Фиксация».
b) Методика тотального протравливания: дентин или эмаль, композит и металл.
i. С помощью насадки Blue Micro Tip нанесите гель Ultra-Etch на всеповерхности препарируемого зуба на 20 секунд.
ii. Тщательно промойте зуб в течение 5 секунд.
iii. Слегка подсушите зубы с помощью пистолета с водой или воздухом
либо интенсивного отсоса, размещенного непосредственно надпрепарируемой областью. Оставьте поверхность немного влажной.
iv. НЕ ОБЯЗАТЕЛЬНО К ВЫПОЛНЕНИЮ: с помощью насадки Black Mini Brush
Tip чистящими движениями нанесите препарат Consepsis (при наличии)на препарированную область и слегка высушите зуб с помощью
воздуха, так чтобы поверхность осталась влажной.
v. Переходите к этапу «Фиксация».
c) Средство для протравки керамики – ОСТОРОЖНО! Фтористоводородную
кислоту (Ultradent Porcelain Etch) разрешено использовать только снадлежащей изоляцией, например с нейтрализующим кислоту барьером
(EtchArrest). Не допускайте контакта фтористоводородной кислоты с деснамии дентином.
i. Нанесите фтористоводородную кислоту на треснувшую область на 90секунд.
ii. Удалите кислоту с поверхности с помощью отсоса, а ЗАТЕМ промойте ивысушите область.
iii. Нанесите Ultra-Etch на 5 секунд, чтобы удалить с керамики соли ипосторонние частицы от фтористоводородной протравки. Промойте ивысушите поверхность.
iv. Нанесите силан на 60 секунд.
v. Тщательно высушите. НЕ ПРОМЫВАЙТЕ ОБЛАСТЬ.
vi. Переходите к этапу «Фиксация».
d) ЗАПРЕЩАЕТСЯ ПРОТРАВЛИВАТЬ ЦИРКОНИЙ И НАНОСИТЬ НА НЕГО СИЛАН.
i. С помощью воздуха выполните абразивную обработку внутренней
поверхности протеза, промойте и высушите обработанную область.
ii. Нанесите праймер для циркония на треснутую область в соответствии синструкциями производителя.
iii. Переходите к этапу «Фиксация».
3.Фиксация.
a) Флакон
i. Выдавите 1–3 капли адгезива Peak Universal Bond на сторону «B»одноразового стеклянного стаканчика.
Используя микрощеточку-аппликатор, нанесите адгезив Peak Universal
Bond на препарированную область и осторожно размазывайте его втечение 10 секунд.
iii. Размазывайте и сушите препарат в течение 10 секунд с помощью
воздуха под полным давлением. Отпрепарированная область должна
блестеть.
iv. Выполните отверждение светом в течение 10 секунд (20 секунд для лампмощностью менее 600 мВт/см2).
b) Шприц
i. С помощью насадки Inspiral™ Brush Tip нанесите адгезив Peak™ Universal
Bond и осторожно размазывайте его в течение 10 секунд.
ii. Размазывайте и сушите в течение 10 секунд с помощью воздуха подполным давлением. Отпрепарированная область должна блестеть.
iii. Выполните отверждение светом в течение 10 секунд (20 секунд для лампмощностью менее 600 мВт/см2).
4.Цемент.
a) Нанесите светоотверждаемый цемент для прозрачных виниров или цемент
двойного отверждения на протез или следуйте инструкциям производителяпо использованию.
ПРИМЕЧАНИЕ. При немедленной герметизации дентина требуется выполнить
описанные выше действия 2а и 3 для методики прямой фиксации. Нанесите
глицерин на адгезив Peak Universal Bond и выполните отверждение светом втечение 10 секунд. Смойте глицерин. Выполните окончательную доработку
внешнего вида. Перед изготовлением временной коронки повторно нанесите
глицерин на подготовленную область. Он будет выступать в качестве
разделительной среды.
ii.

Ремонт композитных / металлических / циркониевых / керамических
протезов и коронок
1. Композит. Удалите ослабленные участки композита. Создайте шероховатость спомощью алмазного бора.
a) Техника тотального протравливания
i. С помощью насадки Blue Micro Tip нанесите гель Ultra-Etch на всеподготовленные поверхности зубов на 20 секунд.
ii. Тщательно промойте в течение 5 секунд и не просушивайте.
2. Металл. Выполните микроабразивную обработку поверхности.
a) Техника тотального протравливания
i. С помощью насадки Blue Micro Tipto нанесите гель Ultra-Etch на всеподготовленные поверхности зубов на 20 секунд.
ii. Тщательно промойте в течение 5 секунд и не просушивайте.
3. Цирконий. Очистите поверхность. Удалите ослабленные участки цирконияс помощью алмазного бора. ЗАПРЕЩАЕТСЯ ПРОТРАВЛИВАТЬ ЦИРКОНИЙ ИНАНОСИТЬ НА НЕГО СИЛАН.
a) С помощью воздуха выполните абразивную обработку внутренней
поверхности протеза.
b) Нанесите праймер для циркония на треснутую область в соответствии синструкциями производителя.
4. Керамика. Создайте шероховатость и удалите ослабленные участки керамики спомощью алмазного бора. Очищайте треснувший участок керамики 15 секундс помощью геля Ultra-Etch. Промойте и высушите.
ОСТОРОЖНО! Фтористоводородную кислоту (Ultradent™ Porcelain Etch)разрешено использовать только с надлежащей изоляцией, например снейтрализующим кислоту барьером (EtchArrest™). Не допускайте контакта
фтористоводородной кислоты с деснами и дентином.
a) Нанесите фтористоводородную кислоту на треснувшую область на 90 секунд.
b) Отсосите кислоту с поверхности, а затем промойте и высушите поверхность.
c) Нанесите гель Ultra-Etch на 5 секунд, чтобы удалить с керамики соли иобразования от фтористоводородной протравки. Промойте и высушите
поверхность.
d) Нанесите силан на 1 минуту.
e) Тщательно высушите. НЕ ПРОМЫВАЙТЕ.
5. Фиксация
a) Флакон
i. Выдавите 1–3 капли адгезива Peak™ Universal Bond на сторону «B»одноразового стеклянного стаканчика.
ii. Используя микрощеточку-аппликатор Micro Applicator Brush, нанесите
адгезив Peak Universal Bond и осторожно размазывайте его в течение
10 секунд.
iii. Размазывайте и сушите в течение 10 секунд с помощью воздуха поддавлением ¼- ½. Отпрепарированная область должна блестеть.
iv. Выполните отверждение светом в течение 10 секунд (20 секунд для лампмощностью менее 600 мВт/см2).

b) Шприц
i. С помощью насадки Inspiral™ Brush Tip нанесите адгезив Peak Universal
Bond и осторожно размазывайте его в течение 10 секунд.
ii. Размазывайте и сушите в течение 10 секунд с помощью воздуха поддавлением ¼- ½.
iii. Отпрепарированная область должна блестеть.
iv. Выполните отверждение светом в течение 10 секунд (20 секунд для лампмощностью менее 600 мВт/см2).
6. Выполните восстановление с помощью жидкотекучего или пакуемого композитав соответствии с инструкциями производителя.
Штифтовая культевая вкладка
1. Подготовка.
a) Просверлите канал для штифта с помощью резинового стопора и бораUniCore™ Drill соответствующего размера.
b) Тщательно промойте канал для штифта в течение 10 секунд с помощью
переходника TriAway Adaptor и насадки 22ga Endo-Eze™ Tip. Высушите
подготовленную область с помощью переходника TriAway Adaptor и насадки
22ga Endo-Eze Tip, двигаясь снизу вверх.
c) Правильно разместите штифт (UniCore Post) и обрежьте его до нужной длиныс помощью алмазного диска с высокой скоростью вращения. ПРИМЕЧАНИЕ.
Твердосплавные и оперативные боры могут приводить к износу волокон.
2.Протравливание.
a) Методика самопротравливания.
i. Промойте полость канала и оставьте ее влажной.
ii. Наденьте голубую насадку 22ga Deliver-Eze™ Brush Tip на шприц Peak SE.
iii. Быстрыми размазывающими движениями введите препарат в канал дляштифта и на область, подготовленную под коронку, на 20 секунд.
iv. Удалите излишки препарата с помощью переходника TriAway Adaptor
и насадки 22ga Endo-Eze Tip, двигаясь снизу вверх. Распределяйтепо поверхности и сушите препарат в течение трех секунд спомощью пистолета с водой или воздухом либо интенсивного отсоса,размещенного непосредственно над препарируемой областью.
v. Переходите к этапу «Фиксация».
b) Методика тотального протравливания.
i. Наденьте голубую насадку 22ga Deliver-Eze Tip на шприц Ultra-Etch.
ii. Заполните канал для штифта по направлению от корня к коронке
зуба. Нанесите препарат на область, подготовленную под коронку.
Протравливайте ее в течение 20 секунд.
iii. Удалите излишки протравки с помощью отсоса.
iv. С помощью переходника TriAway Adaptor и насадки 22ga Endo-Eze Tipтщательно промойте и слегка высушите зуб с помощью воздуха, такчтобы канал для штифта остался немного влажным.
v. Переходите к этапу «Фиксация».
3.Фиксация.
a. Флакон
i. Выдавите 1–3 капли адгезива Peak Universal Bond на сторону «B»одноразового стеклянного стаканчика.
ii. Используя Nano-Brush™ или NaviTip FX, нанесите адгезив Peak Universal
Bond на подготовленную область и осторожно размазывайте его втечение 10 секунд.
iii. Тщательно удалите излишки адгезива Peak Universal Bond с помощью
переходника TriAway Adaptor и насадки 22ga Endo-Eze Tip.
iv. Распределяйте по внешней поверхности и сушите в течение 10 секундс помощью воздуха под давлением ј–Ѕ. Отпрепарированная область
должна блестеть.
v. Выполните отверждение канала светом в течение 20 секунд (40 секунддля ламп мощностью менее 600 мВт/см2).
vi. С помощью бумажного или заранее подобранного штифта убедитесь втом, что полость канала не закупорена.
b) Шприц
i. Наденьте насадку 30ga NaviTip FX на шприц с адгезивом Peak Universal
Bond.
ii. Капните 1–2 капли адгезива в канал для штифта и на подготовленную
область, а затем размажьте его по всей длине канала, включая всюподготовленную область зуба, в течение 10 секунд.
iii. Тщательно удалите лишний адгезив Peak Universal Bond с помощью
переходника TriAway Adaptor и насадки 22ga Endo-Eze Tip.
iv. Высушите канал для штифта и подготовленную область в течение
10 секунд воздухом под полным давлением, после чего размажьте ивысушите адгезив с помощью переходника TriAway Adaptor и насадки
22ga Endo-Eze Tip, чтобы испарить остатки растворителя. При этомследует двигаться снизу вверх.

v.

Выполните отверждение канала светом в течение 20 секунд (40 секунддля ламп мощностью менее 600 мВт/см2). С помощью бумажного илизаранее подобранного штифта убедитесь в том, что полость канала незакупорена.

Цементирование штифта и формирование вкладки
1) Снимите колпачок со шприца PermaFlo™ DC.
2) Наденьте на шприц с двумя цилиндрами смешивающую насадку, совместив дваотверстия. Поверните ее по часовой стрелке до фиксации.
3) Прикрепите к смешивающей насадке гибкую насадку Intraoral Tip™ для ввода
цемента непосредственно в канал из шприца с двумя цилиндрами.
4) Перед тем как вставлять насадку в канал для штифта выдавите из неенебольшое количество цемента.
5) До упора вставьте насадку в канал для штифта.
6) Равномерными надавливаниями введите цемент PermaFlo DC в канал, двигаясьот корня зуба к коронке.
7) Медленно вставьте штифт (UniCore™ Post), выдавливая из канала излишки
цемента.
8) Разместите лампу непосредственно над штифтом и выполните отверждение
светом в течение 20 секунд (40 секунд для ламп мощностью менее 600 мВт/см2).
9) При необходимости продолжайте формировать слои цемента PermaFlo™ DCвокруг штифта. ПРИМЕЧАНИЕ. Между слоями выполняйте отверждение светомв течение 5 секунд для их загустевания и формирования вкладки. Выполните
окончательное отверждение вкладки в течение 40 секунд. Не снимайте
смешивающую насадку до следующего применения. Продезинфицируйте
шприц и смешивающую насадку.
Меры предосторожности и предупреждения
1. Перед использованием адгезива Peak Universal Bond внимательно прочитайтеи уясните все инструкции.
2. Только для профессионального применения.
3. После использования немедленно надевайте колпачок в целях
предотвращения полимеризации.
4. Перед применением средства в ротовой полости всегда проверяйте, насколько
хорошо оно выдавливается. Если средство выдавливается с трудом, замените
насадку и повторите проверку.
5. Не снимайте колпачки с флаконов до их использования.
6. Медработник и пациент во время отверждения композита должны использовать
средства защиты глаз от УФ-излучения.
7. Если материал не используется ежедневно, храните его в холодильнике.
8. Перед использованием необходимо дать находившимся в холодильнике
материалам нагреться до комнатной температуры.
9. Чтобы повысить надежность фиксации, пользуйтесь сухим безмасляным
воздухом.
10. Перенаправьте верхний свет, чтобы предотвратить преждевременную
полимеризацию всех композитных материалов.
11. Композиты могут повышать чувствительность. Избегайте частых контактов
неотвержденных стоматологических композитов с кожей. Не используйте
препараты для лечения пациентов с повышенной чувствительностью какрилатам и другим композитам. При появлении аллергической реакции,дерматита или сыпи проконсультируйтесь с терапевтом.
12. Утилизируйте наконечник, пустые шприцы и флаконы надлежащим образом.
13. Храните в недоступном для детей месте.
14. Не используйте после истечения срока годности, указанного на упаковке.
15. Между использованиями закрывайте, дезинфицируйте и протирайте
шприц дезинфицирующим средством среднего уровня. При использовании
одноразового защитного чехла для шприца снимите насадку, наденьте нашприц колпачок и выбросьте защитный чехол.
16. Насадки являются одноразовыми. Во избежание перекрестного заражения неиспользуйте насадки повторно.
17. Не подвергайте материалы прямому воздействию высоких температур/солнечного света.
18. Избегайте попадания сильнодействующих химических веществ за пределы
области лечения.
ПРИМЕЧАНИЕ. Данные о безопасности материалов идополнительные сведения по использованию адгезива Peak
Universal Bond, праймера Peak SE и других сопутствующих продуктов
см. на веб-сайте www.ultradent.com.

39

PL

Uniwersalny środek wiążący Peak™ Universal Bond oraz Peak™ SE

Opis:
Uniwersalny system wiążący Peak to to występująca w butelce lub strzykawceżywica wiążąca. Może być używana wraz z samowytrawiaczem lub w technicecałkowitego wytrawiania. Zawiera 7,5% rozpuszczalnika w postaci alkoholu etylowego
i ulega polimeryzacji przy naświetlaniu większością lamp polimeryzacyjnych o dużym
natężeniu światła, w tym lamp typu LED. Uniwersalny system wiążący Peak zawiera 0,2%chlorheksydyny, co może zapewnić długotrwałą wytrzymałość wiązania.
Primer Peak SE to występująca w strzykawce samowytrawiająca żywica wiążąca się zzębiną, która składa się z wytrawiacza i primera.
Ultra-Etch™ to znajdujący się w strzykawce żel składający się z 35% kwasu fosforowego
do wytrawiania i spłukiwania.
Zastosowanie chlorheksydyny nie wykazało korelacji ze zmniejszeniem ryzyka próchnicy
wtórnej u pacjentów. Badania kliniczne mające na celu ocenę wpływu chlorheksydyny naflorę bakteryjną jamy ustnej i na próchnicę nie były prowadzone.
Wskazania:
Do praktycznie wszystkich potrzeb związanych z wytrawianiem i wiązaniem w
stomatologii zachowawczej u pacjentów w każdym wieku.
Peak Universal Bond wiąże się z następującymi
materiałami:• Zębina i szkliwo• Porcelana, tlenek cyrkonu• Metal• Kompozyt
Sposób użycia:
UWAGA: Peak SE zawiera dwa oddzielone od siebie
składniki w strzykawce JetMix™, które muszą zostać
wymieszane (aktywowane) przed pierwszym
użyciem.
1) Peak SE zachowuje stabilność przez okres do 120 dni
po aktywacji.
2) Na tłoczku znajduje się płaska biała powierzchniaumożliwiająca napisanie na niej daty aktywacji.
3) NIE WOLNO ODKRĘCAĆ ZAKRĘTKI LUER LOCKSTRZYKAWKI PRZED WYMIESZANIEM
4) Należy szybko i zdecydowanie wcisnąć cienki tłok znapisaną datą do grubszego, właściwego tłoka.
5) Należy upewnić się, że cienki tłok doszedł do dna
komory właściwego tłoka.

40

Uzupełnienia bezpośrednie i naprawa wypełnień
porcelanowych/z tlenku cyrkonu
1.Przygotowaniea) Zębina/szkliwo: Należy wyizolować, oczyścić i usunąć próchnicę upewniając
się, że zostały usunięte wszystkie niezmineralizowane resztki zębiny (zaleca
się zastosowanie wykrywacza próchnicy i ujść kanalików Seek/Sable Seek).
Ubytki klasy V pochodzenia niepróchnicowego należy opracować wiertłem
diamentowym w celu otrzymania chropowatej powierzchni.
b) Kompozyt: Usunąć osłabione części istniejącego wypełnienia kompozytowego.
Uzyskać chropowatą powierzchnię za pomocą wiertła diamentowego.
c) Metal: Przeprowadzić mikroabrazję.
d) Tlenek cyrkonu: Oczyścić powierzchnię i usunąć osłabione części wypełnienia przyużyciu wiertła diamentowego.
e) Wypełnienie porcelanowe: Uzyskać chropowatą powierzchnię i usunąć osłabioneczęści wypełnienia przy użyciu wiertła diamentowego. Oczyszczać obszar
popękanego wypełnienia przez 5 sekund przy użyciu wytrawiacza Ultra-Etch.
Opłukać i osuszyć.
2.Wytrawianiea) Technika samowytrawiania – zębina/szkliwo, kompozyt i metali. Wypłukać opracowywaną powierzchnię i pozostawić ją wilgotną.
ii. OPCJONALNIE – Na opracowywane miejsce nałożyć pastę Consepsis™ (gdyjest dostępna) przy użyciu końcówki z pędzelkiem Black Mini™ Brush Tip
ruchem naśladującym tarcie i lekko osuszyć tę powierzchnię pozostawiając

ją wilgotną.
iii. Przez 20 sekund nanosić ciągłymi kolistymi ruchami na zębinę
opracowywanego zęba wytrawiacz Peak SE, posługując się do tego celukońcówką z pędzelkiem Black Mini Brush Tip. Nie dotykać szkliwa.
iv. Rozrzedzać/suszyć przez 3 sekundy, stosując strzykawkę wodno-powietrzną
lub umieszczając silne ssącą końcówkę bezpośrednio nad opracowywaną
powierzchnią.
v. Przejść do etapu „Wiązanie”.
b) Technika Total Etch (całkowite wytrawianie) – zębina/szkliwo, kompozyt i metali. Przed zastosowaniem należy potwierdzić kolor i konsystencję produktu,
wyciskając niewielką ilość na podkładkę do mieszania lub gazę. Wyciśnięty
przezroczysty płyn należy wyrzucić.
ii. Posługując się niebieską końcówką Blue Micro™ Tip na 20 sekund nanieść
na wszystkie powierzchnie opracowywanego zęba wytrawiacz Ultra-Etch.
iii. Dokładnie przepłukiwać przez 5 sekund.
iv. Delikatnie suszyć, stosując strzykawkę wodno-powietrzną lub umieszczając
silnie ssącą końcówkę bezpośrednio nad opracowywaną powierzchnią.
Pozostawić powierzchnię odrobinę wilgotną.
v. OPCJONALNIE – Na opracowywane miejsce nałożyć pastę Consepsis (gdyjest dostępna) przy użyciu końcówki z pędzelkiem Black Mini Brush Tip
ruchem naśladującym tarcie i lekko osuszyć tę powierzchnię pozostawiając
ją wilgotną.
vi. Przejść do etapu „Wiązanie”.
c) UWAGA: podczas użycia kwasu fluorowodorowego (wytrawiacza do porcelany
Ultradent™) należy zapewnić właściwą izolację pola zabiegowego dzięki
zobojętnieniu nadmiaru kwasu przy użyciu preparatu EtchArrest™. Nie należy
dopuścić do kontaktu kwasu fluorowodorowego z dziąsłem lub zębiną.
i. Nanieść kwas fluorowodorowy na pęknięty obszar na 90 sekund.
ii. Odessać kwas z powierzchni, a POTEM dokładnie opłukać i osuszyć
powierzchnię.
iii. Nałożyć Ultra-Etch na 5 sekund w celu usunięcia soli porcelany i resztek
powstałych podczas wytrawiania kwasem fluorowodorowym. Opłukać iosuszyć.
iv. Nałożyć warstwę silanu na 60 sekund.
v. Dokładnie osuszyć. NIE SPŁUKIWAĆ.
vi. Przejść do etapu „Wiązanie”.
d) Tlenek cyrkonu – NIE WYTRAWIAĆ I NIE UŻYWAĆ SILANU
i. Pękniętą powierzchnię protezy poddać abrazji powietrznej, wypłukać iosuszyć.
ii. Nałożyć primer do tlenku cyrkonu na popękany obszar, stosując się dozaleceń producenta.
iii. Przejść do etapu „Wiązanie”.
3)Wiązaniea) Użycie środka dostarczanego w butelcei. Upuścić 1-3 krople preparatu Peak™ Universal Bond na stronę „B”
jednorazowego kieliszka na preparaty.
ii. Przy użyciu aplikatora z pędzelkiem Micro Applicator Brush nakładać
warstwę uniwersalnego środka wiążącego Peak™ Universal Bond i delikatnie
przecierać przez 10 sekund.
iii. Rozrzedzać/suszyć przez 10 sekund, stosując powietrze o ciśnieniu
obniżonym do ¼ - ½. Opracowana powierzchnia powinna być błyszcząca.
iv. Utwardzać przez 10 sekund (20 sekund w przypadku lamp o mocy
<600mW/cm2).
v. Uzupełnić kompozytem płynnym lub uszczelniającym zgodnie z instrukcjami
producenta.
b) Użycie środka dostarczanego w strzykawce.
i. Przy użyciu końcówki pędzelka Inspiral™ nakładać warstwę uniwersalnegośrodka wiążącego Peak™ Universal Bond i delikatnie przecierać przez 10
sekund.
ii. Rozrzedzać/suszyć przez 10 sekund, stosując powietrze o ciśnieniu
obniżonym do ¼ - ½. Opracowana powierzchnia powinna być błyszcząca.
iii. Utwardzać przez 10 sekund (20 sekund w przypadku lamp o mocy
<600mW/cm2).
iv. Uzupełnić kompozytem płynnym lub uszczelniającym zgodnie z instrukcjami
producenta.
Pośrednia metoda wiązania – uzupełniania koronowe pośrednie, wkłady inakłady koronowe, tlenek cyrkonu
1) Przygotowaniea) Usunąć fleczer, oczyścić, opłukać i osuszyć opracowywaną powierzchnię (pędzelek
StarBrush™ z pastą Consepsis Scrub do oczyszczania, dezynfekcji i usuwania
resztek cementu).
b) Skontrolować dopasowanie uzupełnienia protetycznego.
c) Przygotować wewnętrzną powierzchnię uzupełnienia protetycznego.
i. Uzupełnienie z podłożem metalowym:(1) Wykonać mikroabrazję (piaskowanie) wewnętrznej powierzchni
uzupełnienia protetycznego.
(2) Opłukać i osuszyć powierzchnię.
ii. Ceramiczne/porcelanowe:(1) Przez 90 sekund wytrawiać wewnętrzną powierzchnię uzupełnienia
protetycznego kwasem fluorowodorowym (Ultradent Porcelain Etch),
opłukać i osuszyć.
(2) Nałożyć Ultra-Etch na 5 sekund w celu usunięcia soli porcelany i resztek
powstałych podczas wytrawiania kwasem fluorowodorowym. Opłukać
i osuszyć.
(3) Na 1 minutę nałożyć silan (Ultradent™ Silane) na wewnętrzną powierzchnię
uzupełnienia protetycznego, osuszyć i odłożyć uzupełnienie na bok. Nie
płukać.
iii. Tlenek cyrkonu: NIE WYTRAWIAĆ I NIE UŻYWAĆ SILANU(1) Należy wypiaskować wewnętrzne powierzchnie protezy a następnie
opłukać je i osuszyć.
(2) Nałożyć primer do tlenku cyrkonu zgodnie z instrukcjami producenta.
2)Wytrawianie – Opracowanie powierzchni zębaa) Technika samowytrawiania – zębina/szkliwo, kompozyt i metali. Wypłukać opracowywaną powierzchnię i pozostawić ją wilgotną.
ii. OPCJONALNIE – Na opracowywane miejsce nałożyć pastę Consepsis (gdyjest dostępna) przy użyciu końcówki z pędzelkiem Black Mini Brush Tip
ruchem naśladującym tarcie i lekko osuszyć tę powierzchnię pozostawiając
ją wilgotną.
iii. Przez 20 sekund nanosić ciągłymi kolistymi ruchami na zębinę
opracowywanego zęba wytrawiacz Peak™ SE, posługując się do tego celukońcówką z pędzelkiem Black Mini™ Brush Tip. Nie dotykać szkliwa.
iv. Rozrzedzać/suszyć przez 3 sekundy, stosując strzykawkę wodno-powietrzną
lub umieszczając silne ssącą końcówkę bezpośrednio nad opracowywaną
powierzchnią.
v. Przejść do etapu „Wiązanie”.
b) Technika Total Etch (całkowite wytrawiania) – zębina/szkliwo, kompozyt i metali. Posługując się niebieską końcówką Blue Micro Tip na 20 sekund nanieść na
wszystkie powierzchnie opracowywanego zęba wytrawiacz Ultra-Etch.
ii. Dokładnie przepłukiwać przez 5 sekund.
iii. Delikatnie suszyć, stosując strzykawkę wodno-powietrzną lub umieszczając
silnie ssącą końcówkę bezpośrednio nad opracowywaną powierzchnią.
Pozostawić powierzchnię odrobinę wilgotną.
iv. OPCJONALNIE – Na opracowywane miejsce nałożyć pastę Consepsis (gdyjest dostępna) przy użyciu końcówki z pędzelkiem Black Mini Brush Tip
ruchem naśladującym tarcie i lekko osuszyć tę powierzchnię pozostawiając
ją wilgotną.
v. Przejść do etapu „Wiązanie”.
c) UWAGA: podczas użycia kwasu fluorowodorowego (wytrawiacza do porcelany
Ultradent) należy zapewnić właściwą izolację pola zabiegowego dzięki
zobojętnieniu nadmiaru kwasu przy użyciu preparatu EtchArrest. Nie należy
dopuścić do kontaktu kwasu fluorowodorowego z dziąsłem lub zębiną.
i. Nanieść kwas fluorowodorowy na pęknięty obszar na 90 sekund. Odessać
kwas z powierzchni, a POTEM dokładnie opłukać i osuszyć powierzchnię.
ii. Nałożyć Ultra-Etch na 5 sekund w celu usunięcia soli porcelany i resztek
powstałych podczas wytrawiania kwasem fluorowodorowym. Opłukać iosuszyć.
iii. Nałożyć warstwę silanu na 60 sekund.
iv. Dokładnie osuszyć. NIE SPŁUKIWAĆ.
v. Przejść do etapu „Wiązanie”.
d) Tlenek cyrkonu – NIE WYTRAWIAĆ I NIE UŻYWAĆ SILANU
i. Należy wypiaskować wewnętrzne powierzchnie uzupełniania protetycznego anastępnie opłukać je i osuszyć.
ii. Nałożyć primer do tlenku cyrkonu na popękany obszar stosując się dozaleceń producenta.
iii. Przejść do etapu „Wiązanie”.
3.Wiązaniea) Użycie środka dostarczanego w butelcei.

Upuścić 1-3 kropli uniwersalnego środka wiążącego Peak™ Universal Bond na
stronę „B” jednorazowego kieliszka na preparaty.
Używając końcówki aplikatora Micro Applicator Brush nakładać kolistymi
ruchami przez 10 sekund warstwę uniwersalnego środka wiążącego Peak™
Universal Bond.
iii. Rozrzedzać/suszyć przez 10 sekund, stosując powietrze o normalnymciśnieniu. Opracowywana powierzchnia powinna błyszczeć.
iv. Utwardzać przez 10 sekund (20 sekund w przypadku lamp o mocy <600
mW/cm2).
b) Użycie środka dostarczanego w strzykawce.
i. Przy użyciu końcówki pędzelka Inspiral™ nakładać warstwę uniwersalnegośrodka wiążącego Peak™ Universal Bond i delikatnie przecierać przez 10
sekund.
ii. Rozrzedzać/suszyć przez 10 sekund, stosując powietrze o normalnymciśnieniu. Opracowana powierzchnia powinna być błyszcząca.
iii. Utwardzać przez 10 sekund (20 sekund w przypadku lamp o mocy <600
mW/cm2).
4. Cementowaniea) Nałożyć światłoutwardzalny cement do licówek lub podwójnie utwardzany cementna bazie żywicy do innych protez i zastosować się do instrukcji producenta.
UWAGA: Zabezpieczanie zębiny natychmiast po oszlifowaniu wymaga
zastosowania kroków 2A i 3 techniki bezpośredniej opisanej powyżej. Na
uniwersalny system wiążący Peak nałożyć glicerynę i utwardzać lampą
polimeryzacyjną przez 10 sekund. Spłukać glicerynę. Wykonać końcowy wycisk.
Ponownie nałożyć glicerynę jako środek oddzielający przed założeniem fleczera.
ii.

Naprawa kompozytu/metalu/tlenku cyrkonu/wypełniania porcelanowego
1. Kompozyt: Usunąć osłabione części istniejącego wypełnienia kompozytowego.
Uzyskać chropowatą powierzchnię przy pomocy wiertła diamentowego.
a) Technika całkowitego wytrawienia
i. Posługując się niebieską końcówką Blue Micro Tip na 20 sekund nanieść na
wszystkie powierzchnie opracowanego zęba wytrawiacz Ultra-Etch.
ii. Dokładnie przepłukiwać przez 5 sekund i pozostawić powierzchnię wilgotną.
2. Metal: Mikroabrazjaa) Technika całkowitego wytrawienia
i. Posługując się niebieską końcówką Blue Micro Tip na 20 sekund nanieść na
wszystkie powierzchnie opracowanego zęba wytrawiacz Ultra-Etch.
ii. Dokładnie przepłukiwać przez 5 sekund i pozostawić powierzchnię wilgotną.
3. Tlenek cyrkonu: Oczyścić powierzchnię; usunąć osłabione części tlenku cyrkonu
przy pomocy wiertła diamentowego. NIE WYTRAWIAĆ I NIE UŻYWAĆ SILANU.
a) Pękniętą powierzchnię protezy poddać abrazji powietrznej.
b) Nałożyć podkład do tlenku cyrkonu na popękany obszar, stosując się do zaleceń
producenta.
4. Wypełnienia porcelanowe: Uzyskać chropowatą powierzchnię i usunąć osłabioneczęści wypełnienia porcelanowego przy pomocy wiertła diamentowego. Czyścić
pękniętą powierzchnię wypełnienia porcelanowego przez 15 sekund przy pomocy
wytrawiacza Ultra-Etch. Wypłukać i osuszyć.
UWAGA - podczas użycia kwasu fluorowodorowego (wytrawiacza do porcelany
Ultradent™) należy zapewnić właściwą izolację pola zabiegowego dzięki zobojętnieniu
nadmiaru kwasu przy użyciu preparatu EtchArrest. Nie należy dopuścić do kontaktu
kwasu fluorowodorowego z dziąsłem lub zębinąa) Nanieść kwas fluorowodorowy na pęknięty obszar na 90 sekund.
b) Odessać kwas z powierzchni, a potem dokładnie opłukać i osuszyć powierzchnię.
c) Nałożyć Ultra-Etch na 5 sekund w celu usunięcia soli porcelany i resztek
powstałych podczas wytrawiania kwasem fluorowodorowym. Wypłukać i osuszyć.
d) Nałożyć warstwę silanu na 1 minutę.
e) Dokładnie osuszyć NIE SPŁUKIWAĆ.
5. Wiązaniea) Użycie środka dostarczanego w butelcei. Upuścić 1-3 krople preparatu Peak™ Universal Bond na stronę „B”
jednorazowego kieliszka na preparaty.
ii. Przy użyciu aplikatora z pędzelkiem Micro Applicator Brush nakładać
warstwę uniwersalnego środka wiążącego Peak™ Universal Bond i delikatnie
przecierać przez 10 sekund.
iii. Rozrzedzać/suszyć przez 10 sekund, stosując powietrze o ciśnieniu
obniżonym do ¼ - ½. Opracowana powierzchnia powinna być błyszcząca.
iv. Utwardzać przez 10 sekund (20 sekund w przypadku lamp o mocy <600mW/
cm2).
b) Użycie środka dostarczanego w strzykawce.
i. Przy użyciu końcówki pędzelka Inspiral™ nakładać warstwę uniwersalnegośrodka wiążącego Peak™ Universal Bond i delikatnie przecierać przez 1041

sekund.
Rozrzedzać/suszyć przez 10 sekund, stosując powietrze o ciśnieniu
obniżonym do ¼ - ½.
iii. Opracowana powierzchnia powinna być błyszcząca.
iv. Utwardzać przez 10 sekund (20 sekund w przypadku lamp o mocy <600mW/
cm2).
6. Uzupełnić kompozytem płynnym i/lub uszczelniającym zgodnie z instrukcjami
producenta.
ii.

Wkłady koronowo-korzeniowe
1)Przygotowaniea) Wywiercić otwór w kanale przy z zastosowaniem odpowiedniego wiertła UniCore™
oraz gumowego stopera.
b) Dokładnie opłukiwać powstałą przestrzeń przez 10 sekund, używając końcówkiEndo-Eze™ nr 22 założonej na adapter TriAway. Przy użyciu tej samej końcówki
osuszyć opracowany kanał przechodząc od dołu do góry.
c) Sprawdzić dopasowanie wkładu (UniCore Post) i przyciąć na żądaną długość przyużyciu wysokoobrotowego krążka diamentowego. UWAGA: Wiertła z węglików
spiekanych i wiertła operacyjne mogą postrzępić włókna wkładu.
2.Wytrawianiea) Technika z użyciem samowytrawiacza
i. Wypłukać powierzchnię kanału i pozostawić ją wilgotną.
ii. Dołączyć niebieską końcówkę aplikacyjną Deliver-Eze™ nr 22 do strzykawki
Peak SE.
iii. Aplikować kolistymi ruchami preparat do opracowanego kanału przez 20
sekund.
iv. Przy użyciu końcówki Endo-Eze nr 22 nałożonej na adapter TriAway usunąć
nadmiar preparatu, zaczynając od dołu i kierując się ku górze. Rozrzedzać/
suszyć przez 3 sekundy, stosując strzykawkę wodno-powietrzną lubumieszczając silnie ssącą końcówkę bezpośrednio nad opracowywaną
powierzchnią.
v. Przejść do etapu „Wiązanie”.
b) Technika całkowitego wytrawiania:
i. Dołączyć niebieską końcówkę aplikacyjną Endo-Eze nr 22 do strzykawki
Ultra-Etch.
ii. Aplikować preparat do opracowanego kanału – zaczynać od dna i napełniać
do krawędzi. Nanieść na przygotowane uzupełnienie koronowe. Wytrawiać
przez 20 sekund.
iii. Odessać nadmiar wytrawiacza.
iv. Przy użyciu końcówki Endo-Eze nr 22 założonej na adapter TriAway dokładnie
spłukać, a następnie lekko osuszyć, pozostawiając powierzchnię nieco
wilgotną.
v. Przejść do etapu „Wiązanie”.
3.Wiązaniea) Użycie środka dostarczanego w butelcei. Upuścić 1-3 kropli uniwersalnego środka wiążącego Peak™ Universal Bondna stronę „B” jednorazowego kieliszka na preparaty.
ii. Dołączyć końcówkę z pędzelkiem Nano-Brush™ lub NaviTip FX, nakładać
kolistymi ruchami uniwersalny środek wiążący Peak Universal Bond w
miejsce na wkład i na opracowaną powierzchnię korony przez 10 sekund.
iii. Przy użyciu końcówki Endo-Eze nr 22 nałożonej na adapter TriAway
dokładnie usunąć nadmiar.
iv. Suszyć/rozrzedzać zewnętrzną opracowaną powierzchnię przez 10 sekund,stosując powietrze o ciśnieniu obniżonym do ¼ - ½. Opracowywana
powierzchnia powinna być błyszcząca.
v. Utwardzać obszar wkładu przez 20 sekund (40 sekund w przypadku lampy
o mocy <600 mW/cm2).
vi. Przy pomocy sączka papierowego lub uprzednio dopasowanego wkładu
skontrolować drożność kanału.
b) Użycie środka dostarczanego w strzykawce.
i. Dołączyć końcówkę NaviTip FX nr 30 do strzykawki uniwersalnego systemuwiążącego Peak™ Universal Bond.
ii. Upuścić 1-2 krople na obszar wkładu i opracowywaną powierzchnię, anastępnie przecierać na całej długości kanału, w tym całą powierzchnię
opracowanego zęba przez 10 sekund.
iii. Dokładnie usunąć nadmiar systemu wiążącego Peak™ Universal Bond przypomocy adaptera TriAway i końcówki Endo-Eze nr 22.
iv. Przy pomocy końcówki Endo-Eze™ nr 22 założonej na adapter TriAway
rozrzedzić /osuszyć powstałą przestrzeń przez 10 sekund, stosując powietrzeo normalnym ciśnieniu, aby osuszyć opracowany kanał przechodząc od
dołu do góry
42v.

Utwardzać obszar wkładu przez 20 sekund (40 sekund w przypadku lamp
o mocy <600mW/cm2). Przy pomocy sączka papierowego lub uprzednio
dopasowanego wkładu skontrolować drożność kanału.

Cementowanie wkładu koronowo-korzeniowego i odbudowa zrębu zęba1. Zdjąć zakrętkę zabezpieczającą ze strzykawki zawierającej PermaFlo™ DC.
2. Dołączyć końcówkę mieszającą, dopasowując ją do obu otworów wylotowych
podwójnej (dwukomorowej) strzykawki. Zabezpieczyć połączenie przekręcając
w prawo.
3. Do końcówki mieszającej dołączyć elastyczną końcówkę Intraoral Tip™ umożliwiającą
podawanie preparatu z podwójnej strzykawki bezpośrednio do kanału.
4. Przed podaniem do kanału wycisnąć niewielką ilość preparatu.
5. Wsunąć końcówkę do przygotowanego kanału, aż do dna.
6. Równomiernym naciskiem aplikować PermaFlo DC, zaczynając od wierzchołka ipostępując ku koronie.
7. Wsunąć powoli wkład (UniCore™ Post) do kanału, wyciskając nadmiar cementu.
8. Utwardzać lampą polimeryzacyjną obszar wkładu przez 20 sekund; 40 sekund w
przypadku lampy o mocy <600 mW/cm2.
9. Nakładać wokół wkładu kolejne warstwy PermaFlo™ DC. UWAGA: W celu zżelowania
masy i umożliwienia uformowania rdzenia należy kolejne warstwy utwardzać lampą
po 5 sekund. Końcowe utwardzanie rdzenia powinno trwać 40 sekund. Nie odłączać
końcówki mieszającej aż do następnego użycia. Strzykawkę zdezynfekować razemz końcówką mieszającą.
Przestrogi i ostrzeżenia:
1. Przed użyciem należy dokładnie przeczytać i zrozumieć wszystkie zalecenia
instrukcji dotyczące uniwersalnego środka wiążącego Peak.
2. Wyłącznie do profesjonalnego użytku.
3. By uniknąć polimeryzacji natychmiast po użyciu należy nałożyć zatyczkę.
4. Przed użyciem w jamie ustnej należy zawsze skontrolować równomierność wypływu
materiałów ze strzykawki przez końcówkę aplikacyjną. W przypadku wystąpienia
oporu należy wymienić końcówkę i ponownie skontrolować wypływ.
5. Zakrętki powinny znajdować się na butelkach, dopóki nie są używane.
6. Podczas utwardzania materiałów na bazie żywicy stomatolog i pacjent powinni
stosować okulary ochronne.
7. Jeśli produkt nie jest używany codziennie, powinno się go przechowywać w
lodówce.
8. Przed użyciem produkty powinny mieć temperaturę pokojową.
9. W celu uzyskania optymalnej siły wiązania należy używać powietrza
niezawierającego cząstek oleju i cząsteczek wody.
10. By nie dopuścić do przedwczesnej polimeryzacji materiałów na bazie żywicy należy
odchylać lampę unitu na bok.
11. Żywice mogą uczulać. Nie dopuszczać do powtarzających się kontaktów
niezwiązanej żywicy preparatów dentystycznych ze skórą. Nie używać u pacjentów
ze stwierdzoną nadwrażliwością na akrylany i inne żywice. W przypadku
wystąpienia reakcji alergicznej, zapalenia skóry lub wysypki, należy skonsultowaćsię z lekarzem.
12. Po użyciu końcówki, puste strzykawki i butelki należy zutylizować zgodnie z
przepisami.
13. Przechowywać w miejscu niedostępnym dla dzieci.
14. Nie stosować po upływie terminu przydatności podanego na pojemnikach.
15. Między kolejnymi zastosowaniami ponownie nałożyć zakrętkę, zdezynfekować
i wytrzeć strzykawkę, stosując środek dezynfekujący o poziomie średnim.
W przypadku stosowania jednorazowej osłonki strzykawki, zdjąć końcówkę,strzykawkę należy zamknąć a jednorazową osłonkę – wyrzucić.
16. Końcówki przeznaczone są do użytku jednorazowego. Nie używać ponowniekońcówek, aby uniknąć przeniesienia zakażenia.
17. Przechowywać z dala od bezpośredniego źródła wysokiej temperatury i światła
słonecznego.
18. Ograniczyć działanie silnych środków chemicznych do opracowywanego obszaru.
UWAGA: Karty charakterystyki substancji (SDS) oraz dodatkowe
informacje dotyczące używania uniwersalnego środka wiążącego Peak™,
Peak™ SE oraz produktów pokrewnych można znaleźć na stronie www.
ultradent.com.

Peak™ Universal Bond ve Peak™ SE
Tanım:
Peak Universal Bond, şişe veya tek bir şırınga ile enjekte edilen bonding
rezindir. Self-etch veya total-etch ile birlikte kullanılabilir.
Etil alkol solvent taşıyıcı içerir ve %7,5 oranında doldurulmuştur. LED’ler de dâhilolmak üzere en yüksek yoğunluktaki ışıklarla
polimerize olur. Peak Universal Bond %0,2 oranında, uzun süreli bağlanma
dayanımı sağlayabilen klorheksidin içerir.
Peak SE Primer, şırınga taşıyıcı sisteminde bir etchant ve primerden oluşan selfetching dentin bonding rezindir.
Ultra-Etch™ , şırınga ile uygulanan %35 fosforik asit etch ve yıkama jelindenoluşur.
Klorheksidin aditifinin eklenmesi hastalarda sekonder çürümede bir azalmayla
korelasyon göstermemiştir. Klorheksidinin oral bakteriler veya çürükler
üzerindeki etkilerini değerlendirmek üzere klinik çalışmalar yapılmamıştır.
Kullanım Endikasyonları:
Her yaştan hasta için restoratif diş hekimliğinde hemen hemen tüm ethcing ve
bonding işlemlerinde kullanılabilir.
Peak Universal Bond aşağıdaki materyallere bağlanır:• Dentin ve Mine
• Porselen, zirkonyum• Metal• Kompozit
Kullanım Talimatları:
NOT: Peak SE’yi ilk kez kullanırken JetMix™
şırıngada ayrı olarak bulunan iki bileşeni
aktive etmeniz gerekir.
1. Peak SE, aktivasyondan sonra 120 gün boyuncastabil kalır.
2. Aktivasyondan önce pistonun baş kısmındaki düz
alana son kullanma tarihini yazın.
3. KARIŞTIRMADAN ÖNCE LUER LOCK KAPAĞI
ÇIKARMAYIN.
4. “Tarih atılmış” pistonu hızlı ve kuvvetli bir şekildeorta hazneye bastırın.
5. Pistonun orta hazneyle aynı hizada olduğundanemin olun.
Direkt Bonding Tekniği ve Porselen/
Zirkonyum Tamiri
1.Preparasyon
a. Dentin/Mine: Bütün non-mineral dentinlerinçıkarıldığından emin olarak çürükleri izole edin, temizleyin ve çıkarın (buişlem için Seek/Sable Seek kullanılması önerilir). Klas V preparatlarınabrazyonu/abfraksiyonunda elmas frez ile pürüzlendirin.
b. Kompozit: Mevcut kompozitin incelmiş alanlarını çıkarın. Yüzeyi elmas frez
ile pürüzlendirin.
c. Metal: Yüzeye mikroabrazyon uygulayın.
d. Zirkonyum: Yüzeyi temizleyin ve incelmiş zirkonyumu elmas frez ile çıkarın.
e. Porselen: İncelmiş porseleni elmas frez ile pürüzlendirin ve çıkarın.
Kırık porselen alanını 5 saniye süreyle Ultra-Etch ile temizleyin. Yıkayıp
kurutun.
2.Etcha. Self-Etch Tekniği – dentin/mine, kompozit ve metali. Preparatı yıkayın ve nemli bırakın.
ii. OPSİYONEL – Preparata Black Mini™ Fırça Uç ile ovma hareketiyle
Consepsis™ (mümkünse) uygulayın ve yüzey hafif nemli kalacakşekilde kurumaya bırakın.

TRiii. Dentin üzerine sürekli karıştırma hareketi yaparak diş preparatınaBlack Mini Fırça Uç ile 20 saniye süreyle Peak SE uygulayın. Mineyi
ovmayın.
iv. Hava/su şırıngası kullanarak veya doğrudan preparatın üzerine
yüksek hacimli vakumlama işlemi yaparak 3 saniye süreyle inceltin/
kurutun.
v. Aşağıdaki “Bond” adımına geçin.
b. Total-Etch Tekniği – dentin/mine, kompozit ve metal
i. Uygulamadan önce, karıştırma pedine veya gazlı beze küçük bir
miktar sıkarak akan ürünün rengini ve kıvamını doğrulayın. Sıkılanşeffaf sıvıyı atın.
ii. Blue Micro™ Uç ile 20 saniye süreyle tüm diş preparatı yüzeylerine
Ultra-Etch uygulayın.
iii. 5 saniye süreyle iyice yıkayın.
iv. Hava/su şırıngası kullanarak veya doğrudan preparatın üzerine
yüksek hacimli vakumlama işlemi yaparak hafifçe kurutun. Yüzeyi
hafif nemli bırakın.
v. OPSİYONEL – Preparata Black Mini Fırça Uç ile ovma hareketiyle
Consepsis (mümkünse) uygulayın ve yüzey hafif nemli kalacakşekilde kurumaya bırakın.
vi. Aşağıdaki “Bond” adımına geçin.
c. Porselen Etch – DİKKAT – hidroflorik asit (HF) kullanırken (Ultradent™
Porselen Etch) asit nötralize edici bariyer (EtchArrest™) gibi uygun bir
izolasyon kullanın. Hidroflorik asitin dişetlerine veya dentine temas
etmesini önleyin.
i. Kırık alanına 90 saniye süreyle hidroflorik asit uygulayın.
ii. Yüzeyden asiti aspire edin, DAHA SONRA iyice yıkayın ve kurutun.
iii. HF etching işleminin oluşturduğu porselen bileşiklerini ve kalıntıları
temizlemek için 5 saniye süreyle Ultra-Etch uygulayın. Yıkayıp
kurutun.
iv. 60 saniye süreyle kalın bir silan tabakası uygulayın.
v. İyice kurulayın. YIKAMAYIN.
vi. Aşağıdaki “Bond” adımına geçin.
d. Zirkonyum – ETCH UYGULAMAYIN VE SİLAN KULLANMAYIN
i. Protezin kırılan yüzeyini hava ile aşındırın, yıkayın ve kurutun.
ii. Üreticinin talimatlarına uyarak kırık alanına zirkonyum primer
uygulayın.
iii. Aşağıdaki “Bond” adımına geçin.
3.Bonda. Şişe Enjeksiyonu
i. Tek kullanımlık likit kabının “B” tarafına 1 – 3 damla Peak™ Universal
Bond uygulayın.
ii. Micro Applicator Brush kullanarak preparata kalın bir Peak™ Universal
Bond tabakası uygulayın ve 10 saniye boyunca hafifçe karıştırın.
iii. ¼ ila ½ hava basıncı kullanarak 10 saniye boyunca inceltin/kurutun.
Preparat parlak görünmelidir.
iv. 10 saniye boyunca ışıkla sertleştirin (çıkış gücü < 600 mW/cm2 olanışıklar için 20 saniye).
v. Üreticinin talimatları doğrultusunda akışkan veya kondanse edilebilir
kompozitle restore edin.
b. Şırınga Enjeksiyonu
i. Inspiral™ Fırça Uç ile kalın bir Peak™ Universal Bond tabakası
uygulayın – 10 saniye boyunca hafifçe karıştırın.
ii. ¼ ila ½ hava basıncı kullanarak 10 saniye boyunca inceltin/kurutun.
Preparat parlak görünmelidir.
iii. 10 saniye boyunca ışıkla sertleştirin (çıkış gücü < 600 mW/cm2 olanışıklar için 20 saniye).
iv. Üreticinin talimatları doğrultusunda akışkan veya kondanse edilebilir
kompozitle restore edin.
İndirekt Bonding Tekniği - İndirekt Kronlar, İnleyler, Onleyler,

43

44

Zirkonyum
1. Preparasyon
a. Geçici protez/kronu çıkarın, preparatı temizleyin, yıkayıp kurutun(temizlemek, dezenfekte etmek ve artık sementi çıkarmak için STARbrush™
özellikli Consepsis™ Fırça kullanın).
b. Protezin yerine oturduğundan emin olun.
c. Protezin iç yüzeyini hazırlayın.
i. Metal bazlı:
1. Protezin iç yüzeyine mikroabrazyon (kumlama) uygulayın.
2. Yüzeyi yıkayıp kurutun.
ii. Seramik/porselen:
1. Protezin iç yüzeyine 90 saniye boyunca hidroflorik asit (HF)
(Ultradent™ Porselen Etch) uygulayın, yıkayıp kurutun.
2. HF etching işleminin oluşturduğu porselen bileşiklerini ve kalıntıları
temizlemek için 5 saniye süreyle Ultra-Etch uygulayın. Yıkayıp
kurutun.
3. Protezin iç yüzeyine 1 dakika boyunca silan (Ultradent™ Silane)
uygulayıp kurutun ve protezi bir kenara koyun. Yıkamayın.
iii. Zirkonyum: ETCH UYGULAMAYIN VE SİLAN KULLANMAYIN
1. Protezin iç yüzeyini hava ile aşındırın ve yıkayıp kurutun.
2. İmalatçının talimatlarına göre zirkonyum primer uygulayın.
2.Etch - Diş yüzeyini hazırlayına. Self-Etch Tekniği – dentin/mine, kompozit ve metali. Preparatı yıkayın ve nemli bırakın.
ii. OPSİYONEL – Preparata Black Mini™ Fırça Uç ile ovma hareketiyle
Consepsis™ (mümkünse) uygulayın ve yüzey hafif nemli kalacakşekilde kurumaya bırakın.
iii. 20 saniye boyunca dentin üzerine sürekli karıştırma hareketi yaparakdiş preparatına Black Mini™ Fırça Uçlu Peak™ SE uygulayın. Mineyi
ovmayın.
iv. Hava/su şırıngası kullanarak veya doğrudan preparatın üzerine yüksek
hacimli vakumlama işlemi yaparak 3 saniye süreyle inceltin/kurutun.
v. Aşağıdaki “Bond” adımına geçin.
b. Total-Etch Tekniği – dentin/mine, kompozit ve metali. Blue Micro™ Uç ile 20 saniye süreyle tüm diş preparatı yüzeylerine
Ultra-Etch uygulayın.
ii. 5 saniye süreyle iyice yıkayın.
iii. Hava/su şırıngası kullanarak veya doğrudan preparatın üzerine
yüksek hacimli vakumlama işlemi yaparak hafifçe kurutun. Yüzeyi hafif
nemli bırakın.
iv. OPSİYONEL – Preparata Black Mini™ Fırça Uç ile ovma hareketiyle
Consepsis™ (mümkünse) uygulayın ve yüzey hafif nemli kalacakşekilde kurumaya bırakın.
v. Aşağıdaki “Bond” adımına geçin.
c. Porselen Etch – DİKKAT – hidroflorik asit (HF) kullanırken (Ultradent™
Porselen Etch) asit nötralize edici bariyer (EtchArrest™) gibi uygun bir
izolasyon kullanın. Hidroflorik asitin dişetlerine veya dentine temas
etmesini önleyin.
i. Kırık alanına 90 saniye süreyle hidroflorik asit uygulayın.
ii. Yüzeyden asiti aspire edin, DAHA SONRA iyice yıkayın ve kurutun.
iii. HF etching işleminin oluşturduğu porselen bileşiklerini ve kalıntıları
temizlemek için 5 saniye süreyle Ultra-Etch uygulayın. Yıkayıp kurutun.
iv. 60 saniye süreyle kalın bir silan tabakası uygulayın.
v. İyice kurulayın. YIKAMAYIN.
vi. Aşağıdaki “Bond” adımına geçin.
d. Zirkonyum – ETCH UYGULAMAYIN VE SİLAN KULLANMAYIN
i. Protezin iç yüzeyini hava ile aşındırın ve yıkayıp kurutun.
ii. Üreticinin talimatlarına uyarak kırık alanına zirkonyum primer
uygulayın.
iii. Aşağıdaki “Bond” adımına geçin.
3.Bonda. Şişe Enjeksiyonu
i. Tek kullanımlık karıştırma kabının “B” yüzünde 1–3 damla Peak
Universal Bond hazırlayın.
ii. Micro Aplikatör Fırça kullanarak preparata kalın bir tabaka halinde

Universal bond uygulayın ve 10 saniye süreyle yavaşça karıştırın.
iii. Tam hava basıncı ile 10 saniye boyunca inceltin/kurutun. Preparat
parlak görünmelidir.
iv. 10 saniye ışıkla polimerize edin (çıkış gücü <600mW/cm2 olan ışıklar
için 20 saniye).
b. Şırınga Enjeksiyonu
i. Inspiral™ Fırça Uç ile kalın bir Peak™ Universal Bond tabakası uygulayın– 10 saniye boyunca hafifçe karıştırın.
ii. Tam hava basıncı ile 10 saniye boyunca inceltin/kurutun. Preparat
parlak görünmelidir.
iii. 10 saniye boyunca ışıkla sertleştirin (çıkış gücü < 600 mW/cm2 olanışıklar için 20 saniye).
4.Sementa. Diğer protezlere uygulanacak translüsent veneerler veya dual curesementler için ışıkla polimerize olan sement uygulayın ve üreticininkullanma talimatlarını takip edin.
NOT: Dentinin hemen örtülmesi için yukarıdaki 2A ve 3 adımlarında
anlatılan Direkt Tekniği uygulanmalıdır. Peak Universal Bond üzerine
gliserin uygulayın ve 10 saniye ışıkla polimerize edin. Gliserini durulayın.
Son impresyonu yapın. Geçici protez/kronu yerine sementlemeden öncepreparata ayırıcı madde olarak tekrar gliserin uygulayın.
Kompozit Onarımı / Metal / Zirkonyum / Porselen
1. Kompozit: Mevcut kompozitin zayıflamış kısımlarını çıkarın. Elmas bur ile
yüzeyi pürüzlendirin.
a. Total-Etch Tekniği
i. Blue Micro Tip ile 20 saniye boyunca tüm diş preparatı yüzeylerine
Ultra-Etch uygulayın.
ii. 5 saniye boyunca iyice yıkayın ve nemli bırakın.
2. Metal: Microabrade yüzey
a. Total-Etch Tekniği
i. Blue Micro Tip ile 20 saniye boyunca tüm diş preparatı yüzeylerine
Ultra-Etch uygulayın.
ii. 5 saniye boyunca iyice yıkayın ve nemli bırakın.
3. Zirkonyum: Yüzeyi temizleyin; zayıflamış zirkonyumu elmas bur ile çıkarın.
ETCH UYGULAMAYIN VE SİLAN KULLANMAYIN.
a. Protezin iç yüzeyini hava ile aşındırın.
b. Kırılan bölgeye üreticinin talimatları doğrultusunda zirkonyum primer
uygulayın.
4. Porselen: Zayıflamış porseleni elmas bur ile pürüzlendirin ve çıkarın. Kırılanporselen alanını 15 saniye boyunca Ultra-Etch ile temizleyin. Yıkayıp kurutun.
DİKKAT - Hidroflorik asit (HF) (Ultradent™ Porcelain Etch) kullanırken asit
nötrleştirici bariyer (EtchArrest) gibi uygun bir izolasyon kullanın. Hidroflorik
asidin gingiva veya dentine temas etmesine izin vermeyin.
a. Kırılan bölgeye 90 saniye boyunca hidroflorik asit uygulayın.
b. Yüzeydeki asidi vakumlayın, daha sonra yüzeyi iyice yıkayın ve kurutun.
c. HF etching işleminin oluşturduğu porselen bileşiklerini ve kalıntıları
temizlemek için 5 saniye boyunca Ultra-Etch uygulayın. Yıkayıp kurutun.
d. 1 dakika boyunca kalın bir silan tabakası uygulayın.
e. İyice kurutun. YIKAMAYIN.
5. Bonda. Şişe Enjeksiyonu
i. Tek kullanımlık likit kabının “B” tarafına 1 – 3 damla Peak™ Universal
Bond uygulayın.
ii. Micro Applicator Brush kullanarak kalın bir Peak™ Universal Bondtabakası uygulayın ve 10 saniye boyunca hafifçe karıştırın.
iii. ¼ ila ½ hava basıncı kullanarak 10 saniye boyunca inceltin/kurutun.
Preparat parlak görünmelidir.
iv. 10 saniye boyunca ışıkla sertleştirin (çıkış gücü < 600 mW/cm2 olanışıklar için 20 saniye).
b. Şırınga Enjeksiyonu
i. Inspiral™ Fırça Uç ile kalın bir Peak™ Universal Bond tabakası uygulayın– 10 saniye boyunca hafifçe karıştırın.
ii. ¼ ila ½ hava basıncı kullanarak 10 saniye boyunca inceltin/kurutun.

iii. Preparat parlak görünmelidir.
iv. 10 saniye boyunca ışıkla sertleştirin (çıkış gücü < 600 mW/cm2 olanışıklar için 20 saniye).
6. Üreticinin talimatları doğrultusunda akışkan ve/veya kondanse edilebilir
kompozitle restore edin.
Post ve Kor
1.Preparasyona. Lastik tampon ve uygun ebatta Unicore™ Drill kullanarak post deliği açın.
b. TriAway Adaptör ve 22 ga Endo-Eze™ Uç kullanarak 10 saniye süreyle postboşluğunu iyice yıkayın. TriAway Adaptör ve 22 ga Endo-Eze Uç kullanarak
preparatı altından üstüne kadar kurutun.
c. Postun (UniCore Post) yerine oturduğundan emin olun ve yüksek hızlı
elmas disk kullanarak istediğiniz uzunlukta kesin. NOT: Karbür ve operatif
frezler fiberleri aşındırabilir.
2.Etcha. Self-Etch Tekniği
i. Kanal boşluğunu yıkayın ve nemli bırakın.
ii. Peak SE şırıngaya mavi 22 ga Deliver-Eze™ Fırça Uç takın.
iii. Karıştırma hareketi ile post boşluğuna ve koronal preparata 20 saniyesüreyle uygulayın.
iv. TriAway Adaptör ve 22 ga Endo-Eze Uç kullanarak boşluktaki
fazlalıkları alttan üste doğru püskürtün. Hava/su şırıngası kullanarak
veya doğrudan preparatın üzerine yüksek hacimli vakumlama işlemi
yaparak 3 saniye süreyle inceltin/kurutun.
v. Aşağıdaki “Bond” adımına geçin.
b. Total-Etch Tekniği:i. Ultra-Etch şırıngaya mavi 22 ga Endo-Eze Uç takın.
ii. Apikalle başlayıp post boşluğunu koronal olarak doldurun. Koronal
preparata uygulayın. 20 saniye süreyle etch uygulayın.
iii. Artık etchantı aspire edin.
iv. TriAway Adaptör ve 22 ga Endo-Eze™ Uç kullanarak iyice yıkayın ve
post boşluğu hafif nemli kalacak şekilde kurumaya bırakın.
v. Aşağıdaki “Bond” adımına geçin.
3.Bonda. Şişe Enjeksiyonu
i. Tek kullanımlık karıştırma kabının “B” yüzünde 1–3 damla Peak
Universal Bond hazırlayın.
ii. Nano-Brush™ veya NaviTip FX kullanarak post boşluğuna Peak
Universal Bond uygulayın ve kanalın ve diş preparatının tamamını 10
saniye yavaşça karıştırın.
iii. TriAway Adaptör ve 22 ga Endo-Eze Ucu kullanarak fazlalıkları
tamamen çıkarın.
iv. ¼ ila ½ hava basıncı kullanarak dış preparatı 10 saniye inceltin/
kurutun. Preparat parlak görünmelidir.
v. 20 saniye süreyle post boşluğunun dibini ışıkla polimerize edin (çıkış
gücü < 600 mW/cm2 olan ışıklar için 40 saniye).
vi. Paper point ya da daha önceden yerleştirilmiş postları kullanarak postboşluğunun kapanmadığından emin olun.
b. Şırınga Enjeksiyonu
i. Peak™ Universal Bond şırıngaya 30 ga NaviTip FX takın.
ii. Post boşluğuna ve preparata 1 – 2 damla damlatın ve 10 saniye
boyunca tüm diş preparatı da dâhil olmak üzere kanalı bütünüylekarıştırın.
iii. TriAway Adaptör ve 22 ga Endo-Eze Uç kullanarak fazla Peak™
Universal Bond’u çıkarın.
iv. Kalan bütün solventleri aşağıdan yukarıya doğru buharlaştırmak
amacıyla tam hava basıncıyla 10 saniye boyunca post boşluğunu ve
preparatı kurumaya bırakarak TriAway Adaptör ve 22 ga Endo-Eze Uçile inceltin/kurutun.
v. 20 saniye boyunca post boşluğunun dibini ışıkla sertleştirin (çıkış
gücü < 600 mW/cm2 olan ışıklar için 40 saniye). Paper point ya dadaha önceden yerleştirilmiş postları kullanarak post boşluğunun
kapanmadığından emin olun.

Post Sementasyon ve Kor Oluşturma
1. PermaFlo™ DC şırınganın kapağını çıkarın.
2. İki portu aynı hizaya getirerek iki hazneli şırıngaya karıştırma ucu takın.
Yerine tam olarak oturana kadar saat yönünde çevirin.
3. Çift hazneli şırıngadan doğrudan kanalın içine enjekte etmek için esnek
Intraoral Tip™ ucu karıştırma ucuna takın.
4. Post boşluğuna uygulamadan önce küçük bir miktar sıkın.
5. Ucu post boşluğunun sonuna kadar sokun.
6. Apikalle başlayıp koronal devam ederek ve eşit baskı uygulayarak PermaFlo™
DC enjekte edin.
7. Fazla sementi alarak postu (Unicore™ Post) yavaşça sokun.
8. Polimerizasyon ışığını doğrudan postun üzerine yerleştirin ve 20 saniye
boyunca ışıkla polimerize edin (çıkış gücü < 600 mW/cm2 olan ışıklar için
40 saniye).
9. Postun etrafında gerektiği kadar PermaFlo™ DC katmanı oluşturmaya devam
edin. NOT: Jel ve kor oluşturmak için katmanlar arasında 5 saniye boyuncaışıkla polimerizasyon uygulayın. Kor üzerinde son bir kez daha 40 saniyelik
bir polimerizasyon yapın.
Bir sonraki kullanıma kadar karıştırma ucunu çıkarmayın. Şırınga ve karıştırma
ucunu dezenfekte edin.
Önlemler ve uyarılar:1. Peak Universal Bond’u kullanmadan önce bütün talimatları dikkatlice
okuyun ve anlayın.
2. Yalnızca profesyonel kullanıma yöneliktir.
3. Polimerizasyonu önlemek için kullandıktan sonra hemen kapağını kapatın.
4. Ağız içine uygulamadan önce şırıngadaki materyalin akıp akmadığını
mutlaka kontrol edin. Dirençle karşılaşırsanız ucu değiştirin ve yeniden
kontrol edin.
5. Şişelerin kapağını yalnızca şişeyi kullanacağınız zaman açın.
6. Rezin materyalleri polimerize edilirken klinisyen ve hasta UV koruyucu
gözlük takmalıdır.
7. Aynı gün içinde kullanmayacaksanız ürünü soğutucuda muhafaza edin.
8. Kullanmadan önce soğutulmuş ürünleri oda sıcaklığına getirin.
9. Bağlanma dayanımını optimize etmek için yağsız ve nemsiz hava kullanın.
10. Bütün rezin bazlı materyallerin erken polimerizasyonunu önlemek için tepeışığını başka yöne çevirin.
11. Rezinler duyarlılık oluşturabilir. Polimerize edilmemiş dental rezinin deriyle
tekrarlanan temasından kaçının. Akrilat veya diğer rezinlere karşı duyarlılığı
olduğu bilinen hastalarda kullanmayın. Alerjik reaksiyon, dermatit veya deri
döküntüsü oluşursa bir hekime danışın.
12. Uçları, boş şırıngaları ve şişeleri uygun biçimde atın.
13. Çocukların ulaşamayacağı yerlerde muhafaza edin.
14. Kapların üzerinde belirtilen son kullanma tarihi geçtikten sonrakullanmayın.
15. Her kullanımdan sonra şırınganın kapağını kapatın, şırıngayı orta düzeyli
bir dezenfektan ile dezenfekte edin ve silin. Tek kullanımlık şırınga kılıfı
kullanırsanız ucu çıkarın, kapağı geri takın ve şırınga kılıfını atın.
16. Uçlar tek kullanımlıktır. Çapraz kontaminasyonu önlemek için uçları tekrar
kullanmayın.
17. Ürünleri doğrudan ısıya/güneş ışığına maruz bırakmayın.
18. Güçlü kimyasalları tedavi bölgesinden uzak tutun.
NOT: Güvenlik Bilgi Formu (SDS) ve Peak™ Universal Bond, Peak™ SE
ve ilgili diğer ürünlerin kullanımına ilişkin ayrıntılı bilgi için www.
ultradent.com adresini ziyaret edin.

45

46

‫‪AR‬‬‫®‬‫‪Peak Universal Bond P e a k‬‬‫‪SE‬‬‫‪Peak™ Universal‬‬‫‪Bond et Peak™ SE‬‬‫لم يظھر أن تضمين الكلوريكسيدين اإلضافي‬‫مرتبط بتخفيض التسوس الثانوي لدى المرضى‪ .‬لم يتم القيام بدراسات سريرية لتقييم آثار‬‫الكلوريكسيدين على البكتيريا أو التسوسات السنية‪.‬‬‫استخدمه لجميع احتياجات التخريش واللصق تقريبا في طب األسنان الترميمي‬‫للمرضى من جميع األعمار‪.‬‬‫يلتصق ‪ Peak Universal Bond‬بالمواد التالية‪:‬‬‫• العاج والمينا‬‫• الخزف‬‫• المعادن‬‫• المواد المركبة‬‫‪47‬‬‫®‬

48

Peak™ Universal Bond(유니버설 본드) 및 Peak™ SE설명:Peak Universal Bond는 병입 또는 1회용 시린지 공급 접착용 레진입니다. 이
제품은 Self-Etch 또는 Total-Etch와 함께 사용이 가능합니다. 용매담체로서에틸 알콜 7.5%로 충전되어 있어 LED를 비롯한 최고 강도의 광선을 이용해중합하게 됩니다. Peak Universal Bond에는 장기간의 접착강도를 보장할 수
있는 0.2% 클로르헥시딘이 함유되어 있습니다.
Peak SE Primer(프라이머)는 자가식각형 상아질 접착 레진으로서, 시린지공급 시스템의 식각제 및 프라이머로 구성되어 있습니다.
Ultra-Etch™는 시린지 공급형 35% 인산 에치 및 린스용 젤입니다.

클로르헥시딘 첨가제의 함유물은 환자들의 2차 우식 감소와 상호관련되어
입증되지는 않았습니다. 구강내의 박테리아 또는 충치(우식증)에 대한클로르헥시딘 효과를 분석하기 위한 임상연구는 실시하지 않았습니다.

사용지시:모든 연령층 환자에 대해서, 치과적 복원에서 에칭 및 접합이 필요한 사실상모든 경우에 사용하십시오.
피크 유니버설 본드는 다음 재료에 접합이 됩니다.
• 상아질과 법랑질• 자기 재질, 지르코니아• 금속• 콤포지트
사용지침:
주: Peak SE를 최초로 사용할 경우에는JetMixTM 시린지에서 분리된 구성물 2가지를활성화시켜야 합니다.
1) Peak SE는 활성화 후 120일 동안 안정상태를
유지합니다.
2) 활성화 전에 플런저 손잡이대의 평평한 면에만기일자를 적어둡니다.
3) 혼합하기 전에는 루어 잠금 캡을 제거하지마십시오.
4) “날짜가 적힌” 플런저를 가운데 배럴 가운데로신속하게 힘주어 눌러 넣습니다.
5) 플러저가 가운데 배럴과 같은 높이인지확인합니다.

직접 접착기법 및 도재/질코니아 수리작업1.조제a) 상아질/법랑질: 충치(우식)부를 격리, 세정 및제거하여 일체의 비광물성 상아질이 제거되도록 합니다 이 경우에는Seek/Sable Seek을 권장함). 치아마모증/특발성 침식증(굴곡파절)클래스 V 조제부의 경우, 다이아먼드 버를 사용해 거칠게 처리합니다.
b) 복합레진(컴포짓): 기존의 복합레진(컴포짓)이 약해진 부위를제거합니다. 다이아먼드 버를 사용해 표면을 거칠게 처리합니다.
c) 금속: 표면에 미세연마작업을 실시합니다.
d) 질코니아(Zirconia): 다이아먼드 버를 사용해 표면을 정리하고 약해진질코니아를 제거합니다.
e) 도재: 다이아먼드 버를 사용해 약해진 도재를 거칠게 처리하고제거합니다. Ultra-Etch를 사용해 파절도재를 5초 동안 다듬어세정합니다. 헹군 후 건조시킵니다.
2.에치
a) 자가부식(에칭)기법 – 상아질/법랑질, 복합레진(컴포짓) 및 금속i. 조제부를 헹구고 촉촉한 상태로 둡니다.
ii. 선택사항 - Black Mini™ Brush Tip을 사용해 Consepsis™를조제물에 문지르는 듯한 동작으로 (가능한 부위에) 도포하고, 가볍게공기건조를 실시하여 조제물을 촉촉한 상태로 둡니다.

KO

iii. Black Mini Brush Tip을 사용해 20초 동안 상아질 표면에서 계속휘저어 섞어가며 치아 조제물에 Peak SE를 도포합니다. 법랑질은문지르지 마십시오.
iv. 조제부 바로 위에 공기/물 시린지를 사용하거나 고용량 흡입기를위치시켜 3초 동안 얇게 펴고/건조시킵니다.
v. 아래의 “접착”단계로 진행합니다.
b) 토탈 에치 기법 - 상아질/법랑질, 복합레진(컴포짓) 및 금속i. 믹싱 패드나 거즈 위에 소량을 압출하여 도포하기 전에 제품의색상 및 일관성 있는 흐름상태를 확인합니다. 압출된 투명한 액체는일체를 폐기합니다.
ii. Blue Micro™ Tip 을 사용해 Ultra-Etch를 20초 동안 치아 조제부전체 면에 도포합니다.
iii. 5초 동안 철저하게 헹굽니다.
iv. 조제부 바로 위에 공기/물 시린지를 사용하거나 고용량 흡입기를위치시켜 가볍게 건조시킵니다. 표면을 약간 촉촉한 상태로 둡니다.
v. 선택사항 - Black Mini Brush Tip을 사용해 Consepsis를 조제물에문지르는 듯한 동작으로 (가능한 부위에) 도포하고, 가볍게공기건조를 실시하여 조제물을 촉촉한 상태로 둡니다.
vi. 아래의 “접착”단계로 진행합니다.
c) Porcelain Etch(도재 에치) - 주의 – 불화수소산(HF)((Ultradent™
Porcelain Etch)을 사용할 경우에는 산 중화(제산)용 배리어(EtchArrest™)와 같은 적절한 격리방법을 사용합니다. 불화수소산이
잇몸이나 상아질에 접촉하지 않도록 합니다.
i. 파절부위에 불화수소산을 90초 동안 도포합니다.
ii. 표면의 산을 흡인한 다음, 철저히 헹구고 말립니다.
iii. Ultra-Etch를 5초 동안 도포하여 도재 염분과 HF 에칭(식각)으로
발생한 부스러기를 제거합니다. 헹군 후 건조시킵니다.
iv. 실란의 퍼들 코팅작업을 60초 동안 실시, 도포합니다.
v. 철저하게 말립니다. 헹굼작업은 하지 마십시오.
vi. 아래의 “접착”단계로 진행합니다.
d) 질코니아 - 에치작업이나 실란은 사용하지 마십시오.
i. 보철물의 파절 표면을 공기연마한 다음, 헹구고 말립니다.
ii. 제조업체의 안내사항에 따라 질코니아 프라이머를 파절부위에
도포합니다.
iii. 아래의 “접착”단계로 진행합니다.
3.접착
a) 병입 공급i. Peak™ Universal Bond 1-3 방울을 일회용 대픈 디시의 “B”면속으로 공급합니다.
ii. Micro Applicator Brush를 사용하여 Peak™ Universal Bond의퍼들 코팅재를 조제물에 도포하고, 10초간 부드럽게 저어줍니다.
iii. ¼ 내지 ½의 공기압을 사용해 10초간 묽게 처리/건조작업을
실시합니다. 조제물은 반짝거리는 외관이 되어야 합니다.
iv. 10초간 광중합을 실시합니다(600mW/cm2 미만의 출력광선으로는
20초간).
v. 제조사의 사용안내에 따라 가류성(유동성) 또는 패킹 가능한컴포짓으로 수복합니다.
b) 시린지 공급
i. Inspiral™ Brush Tip(브러시 팁)으로 Peak™ Universal Bond의퍼들 코팅재를 도포하고, 10초간 부드럽게 저어줍니다.
ii. ¼ 내지 ½의 공기압을 사용해 10초간 묽게 처리/건조작업을
실시합니다. 조제물은 반짝거리는 외관이 되어야 합니다.
iii. 10초간 광중합을 실시합니다(600mW/cm2 미만의 출력광선으로는
20초간).
iv. 제조사의 사용안내에 따라 가류성(유동성) 또는 패킹 가능한컴포짓으로 수복합니다.

간접 접착기법 - 간접 치관, 인레이, 온레이, 질코니아1)조제a) 임시치아의 제거, 조제물의 세정, 린스 및 건조작업을 실시합니다

49

(STARbrush™를 사용한 Consepsis Scrub 작업으로 세정, 소독, 및 잔존시멘트 제거).
b) 보철물이 잘 들어맞는지 확인합니다.
c) 보철물의 내부면을 조제합니다.
i. 금속계:(1) 보철물의 내부면을 미세연마(샌드블라스트)합니다.
(2) 표면을 헹군 후 건조시킵니다.
ii. 세라믹/도재:(1) 보철물 내면에 불화수소산(HF)(Ultradent Porcelain Etch)을 90
초 동안 도포하고, 헹군 후 말립니다.
(2) Ultra-Etch를 5초 동안 도포하여 도재 염분과 HF 에칭(식각)으로
발생한 부스러기를 제거합니다. 헹군 후 건조시킵니다.
(3) 보철물 내부면에 실란(Ultradent™ Silane)을 1분 동안 도포하고,말린 후 보철물을 치워 둡니다. 헹구지 마십시오.
iii. 질코니아(Zirconia): 에치작업이나 실란은 사용하지 마십시오.
(1) 보철물의 내부면에 공기연마작업을 실시하고, 헹군 후 말립니다.
(2) 제조업체의 사용안내에 따라 질코니아 프라이머를 도포합니다.
2)에치 - 치아 표면의 조제a) 자가부식(에칭)기법 – 상아질/법랑질, 복합레진(컴포짓) 및 금속i. 조제부를 헹구고 촉촉한 상태로 둡니다.
ii. 선택사항 - Black Mini Brush Tip을 사용해 Consepsis를 조제물에문지르는 듯한 동작으로 (가능한 부위에) 도포하고, 가볍게공기건조를 실시하여 조제물을 촉촉한 상태로 둡니다.
iii. Black Mini™ Brush Tip을 사용해 20초 동안 상아질 표면에서 계속휘저어 섞어가며 치아 조제물에 Peak™ SE를 도포합니다. 법랑질은문지르지 마십시오.
iv. 조제부 바로 위에 공기/물 시린지를 사용하거나 고용량 흡입기를위치시켜 3초 동안 얇게 펴고/건조시킵니다.
v. 아래의 “접착”단계로 진행합니다.
b) Total Etch (토탈 에치) 기법 - 상아질/법랑질, 복합레진(컴포짓) 및 금속
i. Blue Micro Tip 을 사용해 Ultra-Etch를 20초 동안 치아 조제부전체 면에 도포합니다.
ii. 5초 동안 철저하게 헹굽니다.
iii. 조제부 바로 위에 공기/물 시린지를 사용하거나 고용량 흡입기를위치시켜 가볍게 건조시킵니다. 표면을 약간 촉촉한 상태로 둡니다.
iv. 선택사항 - Black Mini Brush Tip을 사용해 Consepsis를 조제물에문지르는 듯한 동작으로 (가능한 부위에) 도포하고, 가볍게공기건조를 실시하여 조제물을 촉촉한 상태로 둡니다.
v. v) 아래의 “접착”단계로 진행합니다.
c) Porcelain Etch(도재 에치) - 주의 – 불화수소산(HF)((Ultradent™
Porcelain Etch)을 사용할 경우에는 산 중화(제산)용 배리어(EtchArrest)와 같은 적절한 격리방법을 사용합니다. 불화수소산이
잇몸이나 상아질에 접촉하지 않도록 합니다.
i. 파절부위에 불화수소산을 90초 동안 도포합니다.
ii. 표면의 산을 흡인한 다음, 철저히 헹구고 말립니다.
iii. Ultra-Etch를 5초 동안 도포하여 도재 염분과 HF 에칭(식각)으로
발생한 부스러기를 제거합니다. 헹군 후 건조시킵니다.
iv. 실란의 퍼들 코팅작업을 60초 동안 실시, 도포합니다.
v. 철저하게 말립니다. 헹굼작업은 하지 마십시오.
vi. 아래의 “접착”단계로 진행합니다.
d) 질코니아 - 에치작업이나 실란은 사용하지 마십시오.
i. 보철물의 내부면에 공기연마작업을 실시하고, 헹군 후 말립니다.
ii. 제조업체의 안내사항에 따라 질코니아 프라이머를 파절부위에
도포합니다.
iii. 아래의 “접착”단계로 진행합니다.
3.접착
a) 병입식 공급
i. 1회용 대픈디시의 “B”면 안으로 Peak Universal Bond를 1-3방울
공급합니다.
ii. Micro Applicator Brush를 사용해 Peak Universal Bond의퍼들 코팅제를 조제물에 도포하고, 10초 동안 부드럽게 휘저어섞어줍니다.
iii.
최고 공기압을 사용하여 10초간 묽게 처리/건조작업을 실시합니다.
50조제물은 반짝거리는 외관이 되어야 합니다.
iv. 10초 동안 광중합을 실시합니다(광선 출력 <600mW/cm2로는 20초 동안).
b) 시린지 공급
i. Inspiral™ Brush Tip으로 Peak™ Universal Bond의 퍼들 코팅재를도포하고, 10초간 부드럽게 저어줍니다.
ii. 최고 공기압을 사용하여 10초간 묽게 처리/건조작업을 실시합니다.
조제물은 반짝거리는 외관이 되어야 합니다.
iii. 10초간 광중합을 실시합니다(600mW/cm2 미만의 출력광선으로는
20초간).
4)시멘트
a) 반투명 베니어용 광중합 시멘트 또는 이중중합 레진 시멘트를 다른보철물에 도포하고, 제조업체의 사용안내를 따르시기 바랍니다.

주: 즉각적인 상아질 씰링은 위의 단계 2A 및 3의 직접기법이 필요합니다.
Peak Universal Bond 위로 글리세린을 도포하고 10초 동안 광중합을실시합니다. 글리세린을 헹굽니다. 최종 인상채득을 실시합니다.
임시치아를 제자리에 시멘팅하기에 앞서 분리제로서 조제물에글리세린을 다시 도포합니다.

컴포짓 / 금속 / 질코니아 / 도재의 수리
1. 컴포짓: 기존의 컴포짓이 약화된 부분을 제거합니다. 다이아몬드 버로표면을 거칠게 처리합니다.
a) Total-Etch기법
i. Blue Micro Tip으로 치아 조제물 표면 전체에 20초간Ultra-Etch
를 도포합니다.
ii. 5초간 철저히 헹구고 축축한 상태로 둡니다.
2. 금속: 표면 미세연마a) Total-Etch기법
i. Blue Micro Tip으로 치아 조제물 표면 전체에 20초간Ultra-Etch
를 도포합니다.
ii. 5초간 철저히 헹구고 축축한 상태로 둡니다.
3. 질코니아: 표면을 세정하고, 다이아몬드 버로 약화된 질코니아를
제거합니다. 에칭이나 실란의 사용은 금합니다.
a) 보철물 내면을 공기연마합니다.
b) 제조사의 사용설명에 따라 질코니아 프라이머를 파절된 부위에도포합니다.
4. 도재: 다이아몬드 버로 거칠게 처리하고 약화된 도재를 제거합니다. 울트라에치로 파절된 도재부위를 15초간 세정합니다. 헹군 다음 건조작업을
실시합니다.
주의 - 불화수소산(HF) (Ultradent™ Porcelain Etch(도재 에치))을 사용하면서 산중화 배리어(EtchArrest)와 같이 적절한 격리수단을
사용합니다. 불화수소산이 잇몸이나 상아질에 접촉하지 않도록 합니다.
a) 불화수소산을 파절된 부위에 90초간 도포합니다.
b) 표면의 산을 흡입한 다음, 표면을 철저히 헹구고 건조시킵니다.
c) HF 에칭으로 형성된 도재의 염제와 부스러기를 제거하기 위해 울트라에치를 5초간 도포합니다. 헹구고 건조시킵니다.
d) 실란 퍼들 코팅재를 1분간 도포합니다.
e) 철저히 건조시킵니다. 헹구지 마십시오.
5. 본드a) 병입제 공급
i. Peak™ Universal Bond 1-3 방울을 일회용 대픈 디시의 “B”면속으로 공급합니다.
ii. Micro Applicator Brush를 사용하여 Peak™ Universal Bond의퍼들 코팅재를 조제물에 도포하고, 10초간 부드럽게 저어줍니다.
iii. ¼ 내지 ½의 공기압을 사용해 10초간 묽게 처리/건조작업을
실시합니다. 조제물은 반짝거리는 외관이 되어야 합니다.
iv. 10초간 광중합을 실시합니다(600mW/cm2 미만의 출력광선으로는
20초간).
b) 시린지 공급
i. Inspiral™ Brush Tip을 사용하여 Peak™ Universal Bond의 퍼들코팅재를 조제물에 도포하고, 10초간 부드럽게 저어줍니다.
ii. ¼ 내지 ½의 공기압을 사용해 10초간 묽게 처리/건조작업을

실시합니다.
iii. 조제물은 반짝거리는 외관이 되어야 합니다.
iv. 10초간 광중합을 실시합니다(600mW/cm2 미만의 출력광선으로는
20초간).
6. 제조사의 사용안내에 따라 가류성(유동성) 및/또는 패킹 가능한 컴포짓으로
수복합니다.

포스트 및 코어1)조제a) 러버 스톱과 적절한 사이즈의 UniCore™ Drill을 사용해 포스트 구멍을뚫습니다.
b) TriAway 어댑터 및 22ga Endo-Eze™ Tip을 10초 동안 사용해 포스트공간을 철저하게 헹굽니다. TriAway 어댑터 및 22ga Endo-Eze™ Tip 을사용해 조제물 바닥으로부터 위로 완전히 말립니다.
c) 포스트(UniCore Post)가 잘 맞는지 확인하고, 고속 다이아몬드 디스크를사용해 원하는 길이에 맞춰 자릅니다. 주: 카바이드 및 수술용 버로섬유조직을 마손시킬 수 있습니다.
2)에치
a) 자가에치 기법i. 근관 공간을 헹구고 촉촉한 상태로 둡니다.
ii. 청색의 22ga Deliver-Eze™ Brush Tip을 Peak SE 시린지에부착합니다.
iii. 포스트 공간 및 관상 조제물에 휘저어 섞는 동작으로 20초 동안도포합니다.
iv. TriAway 어댑터 및 22ga Endo-Eze Tip을 사용해 공간바닥으로부터 위로 여분을 완전히 불어냅니다. 조제부 바로 위에공기/물 시린지를 사용하거나 고용량 흡입기를 위치시켜 3초 동안얇게 펴고/건조시킵니다.
v. 아래의 “접착”단계로 진행합니다.
b) Total-Etch(토탈에치) 기법i. 청색의 22ga Endo-Eze Tip을 Ultra-Etch 시린지에 부착합니다.
ii. 치근단에서 시작하여 포스트 공간을 관상으로 충전합니다. 관상의조제물에 도포합니다. 20초 동안 에칭(식각)을 실시합니다.
iii. 여분의 식각제를 흡입해냅니다.
iv. TriAway 어댑터 및 22ga Endo-Eze Tip을 사용해 철저히 헹군 후공기건조를 실시하고, 포스트 공간은 약간 촉촉하게 둡니다.
v. 아래의 “접착”단계로 진행합니다.
3)접착
a) 병입식 공급
i. 1회용 대픈디시의 “B”쪽으로 Peak Universal Bond를 1-3방울
공급합니다.
ii. Nano-Brush™ 또는 NaviTip FX를 사용하여 Peak Universal Bond
를 포스트 공간에 도포하고, 근관 및 치아 조제물 전체 길이만큼 10초동안 부드럽게 휘저어줍니다.
iii. TriAway 어댑터 및 22ga Endo-Eze Tip을 사용해 여분을 철저하게제거합니다.
iv. ¼ 내지 ½의 공기압을 사용해 조제물 외부를 10초 동안 얇게 펴기/건조작업을 실시합니다. 조제물은 빛나는 상태로 보여야 합니다.
v. 포스트 공간 아래로 20초 동안 광중합을 실시합니다(광선 출력<600mW/cm2로는 40초 동안 실시함).
vi. 페이퍼 포인트나 이전에 맞춘 포스트를 이용해 포스트 공간이차단되지 않도록 확인합니다.
b) 시린지 공급
i. 30ga NaviTip FX를 Peak™ Universal Bond 시린지에 부착합니다.
ii. 1-2방울은 포스트 공간 속과 조제물 위에 떨어뜨린 다음, 10초간치아 조제물 전체를 포함한 치근관의 전체 길이를 저어줍니다.
iii. TriAway 어댑터와 22ga Endo-Eze 팁을 사용해 과도한 Peak™
Universal Bond를 철저히 제거합니다.
iv. TriAway Adapter와 22ga Endo-Eze Tip으로 물게 처리/건조시키기위해 포스트 공간과 조제물을 최고 공기압을 사용해 10초간공기건조를 시켜 바닥으로부터 위로 잔여 용제 일체를 기화시킵니다.
v. 포스트 공간 아래로 20초간 광중합을 실시합니다(600mW/cm2
미만의 출력광선으로는40초간). 페이퍼 포인트나 이전에 맞춘포스트를 사용해 포스트 공간이 막히지 않도록 확인합니다.

포스트 합착 및 코어 축성1) PermaFlo™ DC 시린지의 캡을 제거합니다.
2) 믹싱 팁을 이중 배럴 시린지 위에 놓고 2개의 포트를 맞춥니다.
시계방향으로 비틀어 제자리에 잠급니다.
3) 이중 배럴 시린지로부터 근관 속으로 직접 공급하기 위해 유연한 Intraoral
Tip™을 믹싱 팁에 부착합니다.
4) 포스트 공간에 넣기 전에 소량을 압착합니다.
5) 팁을 포스트 공간 속으로 전체 깊이만큼 삽입합니다.
6) 균일한 압력을 사용해 치근단으로부터 시작하여 관상으로 움직이며PermaFlo DC를 공급합니다.
7) 포스트(UniCore™ Post)를 천천히 삽입하고, 여분의 시멘트를 제거합니다.
8) 광중합기를 포스트 바로 위에 놓고 20초 동안 광중합을 실시합니다(광선출력 <600mW/cm2로는 40초 동안 실시함).
9) 필요에 따라, 포스트 주변에 PermaFlo™ DC 층을 계속해서 축성합니다.
주: 층과 층 사이로 5초 동안 광중합을 실시하여 젤을 바르고 코어를형성합니다. 40초 동안 코어 위로 최종 중합작업을 실시합니다.
다음에 사용하기까지는 믹싱 팁을 제거하지 않는다. 시린지와 믹싱 팁을소독합니다.

주의 및 경고사항:1. Peak Universal Bond를 사용하기 전에 안내사항 일체를 주의하여 읽고숙지합니다.
2. 전문 취급자용에 한함.
3. 중합을 방지하기 위해 사용 후에는 즉시 캡을 다시 씌웁니다.
4. 구강 내에 사용하기 전에 시린지 소재의 흐름상태를 항상 확인합니다.
저항감이 있을 경우, 팁을 교체한 후 다시 점검합니다.
5. 사용하기까지는 병의 캡을 닫아둡니다.
6. 레진 소재를 중합하는 경우, 임상치과의와 환자는 자외선용 보안경을착용해야 합니다.
7. 매일 사용하지 않을 경우, 제품을 냉장합니다.
8. 냉장된 제품은 사용하기 전에 실온에 놓아둡니다.
9. 접착강도를 최적화하기 위해서는, 오일과 수분이 함유되지 않은 공기를사용합니다.
10. 일체의 레진기반 소재의 광중합이 덜 되지 않도록 오버헤드 중합기의방향을 조정합니다.
11. 레진은 감작의 가능성이 있습니다. 경화되지 않은 치과용 레진이 피부에반복적으로 접촉하지 않도록 합니다. 아크릴산 또는 기타 레진에 대한과민증이 밝혀진 환자에게는 사용하지 마십시오. 알러지 반응, 피부염 또는발진이 진행될 경우, 의사의 진찰을 받습니다.
12. 팁, 빈 시린지 및 병들은 적절히 처리합니다.
13. 어린이의 손길이 닿지 않는 곳에 보관합니다.
14. 용기에 표시된 유효기간 후에는 사용하지 마십시오.
15. 사용 간에는 시린지의 캡을 다시 닫고 소독하며 중간 수준의 소독제로닦아냅니다. 1회용 시린지 커버를 사용할 경우, 팁을 제거하고 캡을 다시씌운 후 시린지 커버는 버립니다.
16. 팁은 1회용품입니다. 교차오염을 방지하려면, 팁은 재사용하지 마십시오.
17. 제품은 열/햇빛이 들지 않는 곳에 보관합니다.
18. 강력한 화학물질은 치료부위로만 격리시킵니다.
주: SDS 및Peak™ Universal Bond, Peak™ SE, 그리고 기타 관련 제품의사용에 관한 추가 정보는 웹사이트 www.ultradent.com을 참고하시기
바랍니다.

51

ZH

Peak™ 通用粘接劑和Peak™ SE说明：Peak Universal Bond 通用粘接劑是瓶裝或單一針管輸送的樹脂粘接劑。
可与自酸蚀或全酸蚀系统配合。
其为浓度7.5%的乙醇溶剂，可在LED等高强度光照下固化。
Peak Universal Bond含0.2%洗必泰成
份，从而确保长期粘接强度。

Peak SE 涂底剂是一种自酸蚀牙本质粘接树脂，包含由酸蚀剂和涂底剂组成组成的针管给药系统。
Ultra-Etch™ 是通过针管给药的35%磷酸酸蚀冲洗凝胶。

没有证据表明添加洗必泰成分与患者继发性蛀牙率降低有关。尚未进行过评估洗必泰成分对口腔细菌或龋齿效果的临床研究。
使用说明：用于所有年龄患者恢复性牙科中的几乎所有蚀刻和粘合需要。
Peak 多功能胶粘合以下材料：• 牙龈和牙釉质• 釉质、氧化锆
• 金属• 复合材料使用说明：
注：首次使用Peak SE要激活分装在JetMixTM 针管中的两种材料。
1) Peak SE激活后稳定期为120天。
2) 激活前在活塞杆平面部分写下有效期。
3) 混合前切勿拧下螺旋锁帽。
4) 用力迅速将“写有日期”活塞的推入针
筒中部。
5) 检查活塞是否与针筒中部平齐。

52直接黏合技术和烤瓷/氧化锆修复
1.准备a) 牙本质/牙釉质：隔离、清洁并去除龋齿，
确保去除所有非矿物牙本质材料（推荐使用Seek/Sable Seek）。级准备 面需用金钢砂钻进行打磨。
b) 合成材料：去除原有强度不够的复合材料。
用金刚砂钻对表面进行打磨。
c) 金属：对表面进行微研磨操作。
d) 氧化锆：清洁表面，用金刚砂钻去除强度不够的氧化锆材料。
e) 烤瓷：用金刚砂钻打磨并去除强度不够的烤瓷材料。
用UltraEtch清洁断裂烤瓷面5秒。
冲洗并烘干。
2.酸蚀
a) 自酸蚀技术——牙本质/牙釉质、复合材料和金属
i. 冲洗准备面并保持湿润。
ii. 选择性步骤－在准备面用擦拭法涂抹Consepsis™（用Black
Mini™ Brush针头），而后轻轻烘干，保持表面微湿。
iii. 在牙齿准备面涂抹Peak SE（用Black Mini Brush针头），停

留20秒并在牙本质表面不断搅动。
切勿擦洗牙釉质。
iv. 用气/水注射器吹薄/烘干3秒，或将大功率抽吸器直接放置
于准备面上方。
v. 继续进行下面的“黏合”步骤。
b) 全酸蚀技术——牙本质/牙釉质、复合材料和金属
i. 使用前,通过将少量产品挤入调和板或纱布上以检查产品成色和流畅性。丢弃挤出的所有透明液体。
ii. 在牙齿准备面涂抹Ultra-Etch（用Blue Micro™ 针头，并停
留20秒。
iii. 彻底冲洗5秒。
iv. 用气/水注射器轻轻烘干，或将大功率抽吸器直接放置于准备面上方。
让准备面略微潮湿。
v. 选择性步骤－在准备面用擦拭法涂抹Consepsis（用Black
Mini Brush针头），而后轻轻烘干，保持表面微湿。
vi. vi) 继续进行下面的“黏合”步骤。
c) 烤瓷酸蚀剂－注意－请选用适当的隔离措施如酸中和屏障(EtchArrest™)配合氢氟酸(Ultradent™ 烤瓷酸蚀剂)使用。
切勿让氢氟酸接触牙龈或牙本质。
i. 在断裂部位涂抹氢氟酸90秒。
ii. 将酸从表面吸除，而后彻底清洗并烘干。
iii. 涂抹Ultra-Etch并停留5秒，去除氢氟酸酸蚀形成的瓷盐和碎片。
冲洗并烘干。
iv. 涂抹一层硅烷并停留60秒。
v. 彻底烘干。
切勿冲洗。
vi. 继续进行下面的“黏合”步骤。
d) 氧化锆——切勿酸蚀或使用硅烷
i. 气磨断裂假体表面，冲洗并烘干。
ii. 按厂商说明将氧化锆涂底剂涂抹在断裂部位。
iii. 继续进行下面的“黏合”步骤。
3.黏合
a. 瓶裝輸送i. 滴 1-3 滴Peak™ 通用粘接劑到牙科調藥皿的B面內。
ii. 用Micro Application Brush在治療區抹上一層Peak™ 通用
粘接劑，輕抹勻達10秒。
iii. 用¼ 到 ½ 的風壓吹薄/吹幹達10秒 。
治療區應呈發亮。
iv. 光固化達10秒（輸出功率<600mW/cm2時光固化20 秒）。
v. 按廠家說明，用流動複合或可充壓複合樹脂修復。
b. 針管輸送
i. 用Inspiral™毛刷輸送頭抹上一層Peak™ 通用粘接劑 - 輕抹勻達10秒。
ii. 用¼ 到 ½ 的氣壓吹薄/吹幹達10秒。
治療區應呈發亮。
iii. 光固化達10秒（輸出功率<600mW/cm2時光固化20 秒）。
iv. 按廠家說明，用流動複合或可充壓複合樹脂修復。
间接粘结技术 - 间接牙冠、嵌体、贴面、氧化锆
1)准备a) 去除临时材料，清洁准备面，冲洗并干燥（选用Consepsis
Scrub和STARbrush™ 洗、消毒并去除黏合剂残留）。
b) 检查假体是否适合。
c) 准备假牙的内表面。

i.

金属质地：
(1) 对假牙内表面进行微研磨（喷砂）。
(2) 冲洗并烘干表面。
ii. 陶瓷质地：(1) 在假体内表面涂抹氢氟酸（HF）（Ultradent Porcelain
Etch），停留90秒，冲洗并烘干。
(2) 涂抹Ultra-Etch并停留5秒，去除氢氟酸酸蚀形成的瓷盐和碎片。
冲洗并烘干。
(3) 在假体内表面涂抹硅烷（Ultradent™ Silane）并停留1秒，
烘干后将假体放在一边。
切勿冲洗。
iii. 氧化锆：切勿酸蚀或使用硅烷(1) 气磨假体内表面，冲洗并烘干。
(2) 按厂家说明涂抹氧化锆涂底剂。
2)酸蚀－准备牙齿表面a) 自酸蚀技术——牙本质/牙釉质、复合材料和金属
i. 冲洗准备面并保持湿润。
ii. 选择性步骤－在准备面用擦拭法涂抹Consepsis（可用情况下）（用Black Mini Brush针头），而后轻轻烘干，保持表
面微湿。
™
iii. 在牙齿准备面涂抹Peak SE（用Black Mini™ Brush针头），停
留20秒并在牙本质表面不断搅动。
切勿刮擦牙釉质。
iv. 用气/水注射器吹薄/烘干3秒，或将大功率抽吸器直接放置
于准备面上方。
v. 继续进行下面的“黏合”步骤。
b) 全酸蚀技术——牙本质/牙釉质、复合材料和金属
i. 在牙齿准备面涂抹Ultra-Etch（用Blue Micro 针头，并停
留20秒。
ii. 彻底冲洗5秒。
iii. 用气/水注射器轻轻烘干，或将大功率抽吸器直接放置于准备面上方。
让准备面略微潮湿。
iv. 选择性步骤－在准备面用擦拭法涂抹Consepsis（可用情况下）（用Black Mini Brush针头），而后轻轻烘干，保持表面微湿。
v. 继续进行下面的“黏合”步骤。
c) 烤瓷酸蚀剂－注意－请选用适当的隔离措施如酸中和屏障(EtchArrest)配合氢氟酸(Ultradent™ 烤瓷酸蚀剂)使用。
切勿让氢氟酸接触牙龈或牙本质。
i. 在断裂部位涂抹氢氟酸90秒。
ii. 将酸从表面吸除，而后彻底清洗并烘干。
iii. 涂抹Ultra-Etch并停留5秒，去除氢氟酸酸蚀形成的瓷盐和碎片。
冲洗并烘干。
iv. 涂抹一层硅烷并停留60秒。
v. 彻底烘干。
切勿冲洗。
vi. 继续进行下面的“黏合”步骤。
d) 氧化锆——切勿酸蚀或使用硅烷
i. 气磨假体内表面，冲洗并烘干。
ii. 按厂商说明将氧化锆涂底剂涂抹在断裂部位。
iii. 继续进行下面的“黏合”步骤。
3)黏合
a) 瓶裝輸送i. 滴1－3滴Peak Universal Bond到一次性调药盘“B”面。

ii. 用Micro Applicator Brush在准备面涂抹一层Peak
Universal Bond，并轻搅10秒钟。
iii. 用全風壓吹薄/吹幹達10秒 。
治療區應呈發亮。
iv. 光固化10秒（输出功率<600mW/cm2的固化光须固化20秒）。
b) 針管輸送
i. 用Inspiral™毛刷輸送頭抹上一層Peak™ 通用粘接劑 - 輕抹勻達10秒。
ii. 用全風壓吹薄/吹幹達10秒 。
治療區應呈發亮。
iii. 光固化達10秒（輸出功率<600mW/cm2時光固化20 秒）。

4)黏接
a) 在半透明贴面上涂抹光固化黏合剂或在其他假体上涂抹双重固化树脂黏合剂，并按照厂家说明使用。

注：即时牙本质密封要用到上文第2A及3步的直接技术。
涂抹Peak Universal Bond后再涂抹甘油，光固化10秒钟。
将甘油洗
净。
制作最终印模。
在黏合临时修复体前再次在准备面涂抹甘油，
作为分离介质。

複合/金屬/氧化鋯/瓷制物的修復
1. 複合物：除去現有複合物的弱化區。
用金剛石鑽針對表面進行粗糙化處理。
a) 全酸蝕技術
i. 用Blue Micro Tip在牙齒所有治療區表面塗抹Ultra-Etch
酸蝕劑達20秒。
ii. 徹底沖洗達5秒，保持濕度。
2. 金屬物：微研磨表面a) 全酸蝕技術
i. 用Blue Micro Tip在牙齒所有治療區表面塗抹Ultra-Etch™
酸蝕劑達20秒。
ii. 徹底沖洗達5秒，保持濕度。
3. 氧化鋯物：清潔表面；用金剛石鑽針對弱化的氧化鋯物表面進行
粗糙化處理。
切勿使用矽烷酸蝕。
a) 氣壓研磨假牙的內表。
b)按廠家說明，將氧化鋯處理劑塗在斷口區。
4. 瓷制物：用金剛石鑽針對弱化的瓷制物表面進行粗糙化和清除處理。
用Ultra-Etch™酸蝕劑對斷裂瓷區清潔達15秒。
沖洗並乾燥。
警告 – 在使用氫氟酸(HF) (Ultradent™ Porcelain Etch)時，務必使用諸如酸性中和隔離劑(EtchArrest)的適當隔離產品。
切勿讓氫氟酸接觸到牙齦或牙本質。
a)在斷口區塗抹氫氟酸達90秒。
b) 吸去表面的酸，然後沖洗，乾燥表面。
c) 塗抹 Ultra-Etch 達5秒，以除去釉鹽及氫氟酸酸蝕形成的殘損物。
沖洗並乾燥。
d) 抹一層矽烷達1分鐘。
e) 徹底乾燥。
切勿沖洗。
5. 粘接劑
a) 瓶裝輸送i. 滴 1-3 滴Peak™ 通用粘接劑到牙科調藥皿的B面內。
ii. 用Micro Applicator Brush在治療區抹上一層Peak™ 通用粘接劑，輕抹勻達10秒。
iii. 用¼ 到 ½ 的風壓吹薄/吹幹達10秒 。
治療區應呈發亮。

53

iv. 光固化達10秒（輸出功率<600mW/cm2時光固化20 秒）。
b) 針管輸送
i. 用Inspiral™毛刷輸送頭抹上一層Peak™ 通用粘接劑 -輕抹勻達10秒。
ii. 用¼ 到 ½ 的氣壓吹薄/吹幹達10秒 。
iii. 治療區應呈發亮。
iv. 光固化達10秒（輸出功率<600mW/cm2時光固化20 秒）。
6. 按廠家說明，用流動複合或可充壓複合樹脂修復。

54

桩和桩核
1) 准备
a) 用橡皮障和大小合适的UniCore™ 钻头钻孔。
b) 用TriAway适配器和22ga Endo-Eze™针头彻底冲洗桩孔10秒
钟。
用TriAway适配器和22ga Endo-Eze™针头从下至上烘干准备面。
c) 检查桩（UniCore Post）合适与否，用圆形高速金刚石锯片切割
至所要的长度。注：硬质合金和手术钻可能磨损纤维。
2)酸蚀
a) 自酸蚀技术
i. 冲洗根管并保持湿润。
ii. 在Peak SE针管上拧紧蓝色22ga Deliver-Eze™ Brush针头。
iii. 涂抹在桩孔和冠准备面并搅动20秒。
iv. 用TriAway适配器和22ga Endo-Eze针头从下至上吹走多余酸蚀剂。
用气/水注射器吹薄/烘干3秒，或将大功率抽吸器直接放置于准备面上方。
v. 继续进行下面的“黏合”步骤。
b) 全酸蚀技术：i. 在Ultra-Etch针管上拧紧蓝色22ga Endo-Eze针头。
ii. 从根尖开始填充桩孔。
涂抹于冠准备面。
酸蚀20秒。
iii. 吸走多余酸蚀剂。
iv. 用TriAway适配器和22ga Endo-Eze针头彻底冲洗并轻轻烘干，保持桩孔微湿。
v. 继续进行下面的“黏合”步骤。
3) 黏合a) 瓶裝輸送i. 滴1－3滴Peak Universal Bond到一次性调药盘“B”面。
ii. 用Nano-Brush™或 NaviTip FX在桩孔中涂抹Peak
Universal Bond，轻搅根管及牙齿准备面10秒钟。
iii. 用TriAway适配器和22ga Endo-Eze针头彻底去除多余黏合剂。
iv. 用¼ 至 ½气压吹薄/烘干外准备面10秒钟。
准备面应该很有光泽。
v. 光固化桩孔20秒（输出功率<600mW/cm2的固化光须固化40秒）。
vi. 用纸尖或事先做好的纤维桩检查桩孔是否畅通。
b) 針管輸送i. 將一個30ga NaviTip FX 接到Peak™ 通用粘接劑針管上。
ii. 滴 1-2 滴到樁腔內和治療區表面，在整個牙根管區抹勻達10秒，包括整個牙齒治療區。
iii. 用TriAway三用槍轉接頭和22ga 的EndoEze 輸送頭徹底除
去多餘的Peak™ 通用粘接劑。
iv. 用全風壓、同時用TriAway三用槍轉接頭和22ga 的EndoEze

輸送頭，吹薄/吹幹吹幹樁腔內和治療區達10秒，以讓任何剩餘的溶劑從下往上徹底蒸發掉。
v. 光固化樁腔達20秒（輸出功率<600mW/cm2時光固化40 秒）。
用根管紙針或前設合適的樁腔檢查樁腔是否被堵。

牙桩胶结和桩核构建
1) 取下PermaFlo™ DC针管盖帽。
2) 在双针筒注射器上拧紧混合头并对准两侧端口。
顺时针旋转直至锁定。
3) 将混合头接上灵活的Intraoral Tip™，以便用双针筒注射器直接根管给药。
4) 用于桩孔前先挤出少量。
5) 将针头在桩孔中插到底。
6) 均匀用力从根尖到冠部涂抹PermaFlo DC。
7) 缓慢插入（UniCore™ Post），挤出多余黏合剂。
8) 将固化灯直接置于纤维桩上固化20秒；输出功率<600mW/cm2
时固化40秒。
9) 必要时继续在纤维桩周围构建PermaFlo™ DC涂层。
注：每涂一层
固化5秒，最终形成桩核。
最终固化桩核40秒。
下次使用前切勿取下混合头。
消毒针管和混合头。

注意事项和警告：
1. 使用Peak Universal Bond前认真阅读并了解所有说明。
2. 仅限专业人士使用。
3. 用后立即盖盖以避免聚合。
4. 在口腔中使用前必须检查针管中材料流动是否顺畅。
如果受阻，更换针头并重新检查。
5. 使用前拧紧瓶盖。
6. 固化树脂材料时，临床医生和患者应佩戴防紫外线眼镜。
7. 若非每天使用，请冷藏保存。
8. 使用前须将冷藏产品恢复至室温。
9. 为最大限度地提高黏接强度，须使用无油、干燥的空气。
10. 为防止树脂材料过早聚合须移走头顶的固化灯。
11. 树脂可能造成过敏。
避免皮肤反复接触未固化牙科树脂。
切勿用于已知对丙烯酸酯或其它树脂过敏的患者。
若出现过敏反应、皮炎或皮疹，请咨询生。
12. 妥善处理针头、空针管和药瓶。
13. 切勿让儿童接触。
14. 切勿在容器所注过期日后使用。
15. 下次使用前重新套上针管帽，用中度消毒剂擦拭针管。
若使用一次性注射器套，请取下针头，套好螺旋锁帽，并丢弃注射器套。
16. 针头为一次性使用。
切勿重复使用针头以防交叉感染。
17. 避免高温/阳光直射。
18. 将强效化学品隔离在治疗部位。
注意：查閱有關的化學品安全技術說明書和使用Peak™ 通用
粘接劑、Peak™ SE及其它相關產品的補充資訊，請訪問www.
ultradent.com

Peak Universal Bond Bottle Delivery

Peak SE

THการรวมสารเติมแต่งคลอโรเฮกซิดนี ไม่ได้สมั พันธ์กบั การลดลงในฟันผุทเี่ กิดซ�ำ้ ภายหลังการอุดฟันในคนไข้ ยังไม่มกี ารศึกษาทางคลีนกิ เพือ่ ประเมินผลกระทบของสาร
คลอโรเฮกซิดนี กับแบคทีเรียในปากและฟันผุ
ใช้ในความต้องการการกัดและการบอนดิง้ เกือบทุกชนิดในทันตกรรมบูรณะส�ำหรับ
ผูป้ ว่ ยทุกวัย
Peak Universal Bond จะยึดกับวัสดุตอ่ ไปนี:้• เดนทีนและอีนาเมล
•• โลหะ
• คอมโพสิท

55

56

57

JA

Peak™ ユニバーサルボンドおよびPeak™ SE

製品説明：
Peak Universal Bond ユニバーサルボンドは、ボトルまたは単回用シリンジに入った結合用樹脂です。
セルフエッチ、またはトータルエッチと共に使用できます。
7.5％がエチルアルコール溶剤単体で、LEDなど輝度の最も高いライトで硬化されます。
Peak Universal Bond には長時間ボンドを強化するために、0.2％のクロルヘ
キシジンが使用されています。
Peak SE プライマーは、
セルフエッチング象牙質接着レジンで、シリンジ抽出シス
テムに収納されるエッチ剤とプライマーから構成されます。
Ultra-Etch™ は、35% がリン酸のエッチングおよびリンスジェルです。

クロルヘキシジンを含むことで、患者さんの歯に見られる二次虫歯を減らすことにつながるという見解はありません。口内のバクテリア、またはカリエスに対するクロルヘキシジンの効果を評価する臨床試験は今までに行われたことはありません。

適用：
すべての年齢層の患者向けに修復歯科のほぼあらゆるエッチングと接着ニー
ズで使用できます。
Peakユニバーサルボンドは次の材料を結合します。
• 象牙質とエナメル• 陶材とジルコニア
• 金属
• 合成物
使用方法：
注記：Peak SE を最初にご使用になる前に、JetMixTMシリンジ内に別々に保存されている2つの薬剤を活性化させる要があります。
1) Peak SE は、活性化されてから120日間安全にご使用いただけます。
2) 活性化する前に、プランジャーシステムの平らな部分に有効期限を記入してください。
3) 混ぜ合わせる前にルア・ロックキャップを外さないでください。
4) 迅速かつ力強く「日付」の入ったプランジャーをバ
レルの中央まで押し入れてください。
5) プランジャーがバレルの中央に到達したかを確認してください。

58

直接的接着技術および陶剤/ジルコニア修復剤
1) 準備a) 象牙質/エナメル：カリエスを隔離、洗浄および除去し、すべての非鉱物象
牙質を除去してください（この場合、安定シークを使用することが勧められます）。
磨耗/破片のクラスV前処理の場合は、
ダイヤモンドバーで粗面化してください。
b) 合成物：現在使用されている合成物で、弱った部分を除去してください。
ダイヤモンドバーで、表面を粗面化してください。
c) 金属：表面をマイクロ摩擦してください。
d) ジルコニア：表面を洗浄し、ダイヤモンドバーで弱った部分を除去してください。
e) ポーセリン：ダイヤモンドバーで弱ったポーセリンを粗面化し、除去します。
破砕されたポーセリン部を、Ultra-Etch で5秒間洗浄しま す。
洗い流し、乾燥します。
2)エッチングa) セルフエッチ技術 – 象牙質/エナメル、合成物、および金属
i. 処理部分を洗い流し、少し湿気のある状態に乾燥させてください。
ii. オプション：Consepsis™（可能な場合）をBlack Mini™ ブラシチップを使ってアプライし、
スクラブしながらエアドライし、表面が少 し湿った状態にしま す。
iii. Black Mini ブラシチップを使用して、Peak SE を攪拌して処置部の象牙質を処理します。
エナメルはスクラブしないでください。
iv. エアー/ウォーターシリンジ、または処置部に高量吸引器を直接当てて、3秒間薄く伸ばすか、または乾燥させてください。
v. 以下の「結合」手順に進みます。
b) 総合エッチ技術 – 象牙質/エナメル、合成物、および金属
i. 本品を使用する前にミキシングパッドに少量押し出して、材料の色調とフローを確認してください。
無色液体が見られる場合はその部分をミキシングパッド上に出し切ってから口腔内にご使用ください。
ii. Ultra-Etch をBlue Micro™ Tipで処置済みのすべての歯の表面に20秒
間アプライしてください。
iii. 5秒間リンスしてください。
iv. エアー/ウォーターシリンジ、または処置部に高量吸引器を直接当てて、3秒間薄く延ばす、または乾燥させてください。
v. オプション：Consepsis（可能な場合）をBlack Mini ブラシチップを使ってアプライし、
スクラブしながらエアドライし、表面が 少し湿った状態にします。
vi. 以下の「結合」手順に進みます。
c) ポーセリンエッチング-注記-フッ化水素（HF）（Ultradent™ ポーセリンエッ
チング）：酸中中剤(EtchArrest™) などにより適切な方法で隔 離してください。
フッ化水素酸を使用する場合は、歯肉、または象牙質に触らないよ
うにしてください。
i. 破砕された場所に、フッ化水素を90分間アプライします。
ii. 表面の酸を吸引して、しっかりとリンスした後、表面を乾燥させてください。
iii. Ultra-Etch を5秒間アプライし、陶剤塩およびHF エッチングにより形成された破片を除去してください。
リンスして乾燥します。
iv. 一定量のシランを60分間アプライしてください。
v. 完全に乾燥させ、絶対に洗い流さないでください。
vi. 以下の「結合」手順に進みます。
d) ジルコニア：エッチングを行ったり、シランを使用しないでください。
i. エアー・アブレードでプロテーゼ表面を形成し、リンス&乾燥させます。
ii. ジルコニアプライマーを、破砕された部分にアプライした後、メーカーの指示に従って処置を行ってください。
iii. 以下の「結合」手順に進みます。
3)接着剤
a. ボトルの場合
i. 使い捨てダッペン皿の「B」側にPeak™ユニバーサルボンドを1～3滴入れます。
ii. Micro Applicator Brushを使用してPeak™ユニバーサルボンドを前処置部に適用し、10秒間ゆっくりかき混ぜます。
iii. ¼～½の空気圧を使用し、10秒間薄めて伸ばすか乾燥させます。
前処
置部は光っているように見えるはずです。
iv. 10秒間、光硬化させます（出力が600mW/cm2未満の光の場合は20秒間）。
v. メーカーの指示に従い、流動性のある合成物かパッキング可能な合成物で修復します。
b. シリンジの場合
i. Peak™ユニバーサルボンドをInspiral™ブラシチップで適用し、10秒間
ゆっくりかき混ぜます。
ii. ¼～½の空気圧を使用して10秒間薄めて伸ばすか乾燥させます。
前処
置部は光っているように見えるはずです。
iii. 10秒間、光硬化させます（出力が600mW/cm2未満の光の場合は20秒間）。
iv. メーカーの指示に従い、流動性のある合成物かパッキング可能な合成物で修復します。
間接的接着技術：間接的クラウン、
インレイ、
オンレイ、ジルコニア
1) 前処置a) 処置部を洗浄し、洗い流してから、乾燥します（Consepsis Scrub とiv. 10秒間光硬化させます (出力600mW/cm2以下の光を使用する場
STARbrush™ で洗浄、殺菌し、処置部に残っているセメントを除 去します）。
合は20秒間)。
b) 歯科補綴物の装着を確認してください。
b) シリンジの場合c) 補綴物の内面の前処理を行ってください。
i.
Peak™ユニバーサルボンドをInspiral™ブラシチップで適用し、10秒間ゆi. 金属ベース：
っくりかき混ぜます。
(1) 補綴物の内面をマイクロ摩擦（サンドブラストで）してください。
ii.
完全な空気圧で10秒間、薄めて伸ばすか乾燥させます。
前処置部は光(2) 表面をよく洗い流し、乾燥します。
っているように見えるはずです。
ii. セラミック/陶材：
™
iii.
10秒間、
光硬化させます（出力が600mW/cm2未満の光の場合は(1) フッ化水素酸（HF）（Ultradent Porcelain Etch）を歯科補綴物の内20秒間）。
面に90秒間アプライした後、リンスして乾燥します。
4)セメント(2) Ultra-Etch を5秒間アプライし、陶剤塩およびHF エッチングにより
a)光硬化セメントを半透明のベニアにアプライするか、または二重重化合樹脂形成された破片を除去してください。
リンスして乾燥します。
を補綴物にアプライし、メーカーの取扱い説明に従います。
(3) シラン（Ultradent™ Silane）を歯科補綴物の内面に1分間アプライした後、乾燥してプロテーゼを硬化させます。
洗い流さないでく ださい。
注記：象牙質を瞬時に固定するには、上記Direct Technique のステップ 2A おiii. ジルコニア：エッチングを行ったり、シランを使用しないでください。
よび 3 を行う必要があります。
グリセリンをPeak Universal Bond にアプライ(1) 歯科補綴物の内表を空気で磨耗してください。
し、10秒間光硬化させます。
グリセリンを洗い流します。
最終的な仕上げを行(2) ジルコニアプライマーを、製造会社の指示に従ってアプライしています。
テンポラリーレストレーションを作成する前に、分離剤としてグリセリください。
ンを処置部に再度アプライします。
2) エッチング-歯の表面の処置a) セルフエッチ技術 – 象牙質/エナメル、合成物、および金属
i. 処理部分を洗い流し、少し湿気のある状態に乾燥させてください。
ii. オプション：Consepsis（可能な場合）をBlack Mini ブラシチップを使ってアプライし、
スクラブしながらエアドライし、表面が少し 湿った状
態にしま す。
iii. Black Mini™ ブラシチップを使用して、Peak™ SE を攪拌して処置部を処理します。
エナメルはスクラブしないでください。
iv. エアー/ウォーターシリンジ、または処置部に高量吸引器を直接当てて、3秒間薄く伸ばすまたは乾燥させてください。
v. 以下の「結合」手順に進みます。
b) 総合エッチ技術 – 象牙質/エナメル、合成物、および金属
i. Ultra-Etch をBlue Micro Tipで処置済みのすべての歯の表面に20秒
間アプライしてください。
ii. 5秒間リンスしてください。
iii. エアー/ウォーターシリンジ、または処置部に高量吸引器を直接当てて、3秒間薄く伸ばす または乾燥させてください。
iv. オプション：Consepsis（可能な場合）をBlack Mini ブラシチップを使ってアプライし、
スクラブしながらエアドライし、表面が少し 湿った状態にします。
v. 以下の「結合」手順に進みます。
c) ポーセチンエッチング-注記-フッ化水素（HF）（Ultradent™ ポーセチンエッ
チング）：酸中中剤(EtchArrest™)などにより適切な方法で 隔離してください。
フッ化水素酸を使用する場合は、歯肉、または象牙質に触らないようにしてください。
i. 破砕された場所に、フッ化水素を90分間アプライします。
ii. 表面の酸を吸引して、しっかりとリンスした後、表面を乾燥させてください。
iii. Ultra-Etch を5秒間アプライし、陶剤塩およびHF エッチングにより形成された破片を除去してください。
リンスして乾燥します。
iv. 一定量のシランを60分間アプライしてください。
v. 完全に乾燥させ、絶対に洗い流さないでください。
vi. 以下の「結合」手順に進みます。
d) ジルコニア：エッチングを行ったり、シランを使用しないでください。
i. 歯科補綴物の内表をエアー・アブレードで磨耗してください。
ii. ジルコニアプライマーを、破砕された部分にアプライした後、メーカーの指示に従って処置を行ってください。
iii. 以下の「結合」手順に進みます。
3)接着剤a) ボトルの場合
i. 1～3滴のPeak Universal Bond を使い捨て用の取り皿の“B”側に取ります。
ii. Micro Applicator Brush を使って、少量のPeak Universal Bond を処
置部ニアアプライし、10秒間やさしく攪拌します。
iii. 完全な空気圧で10秒間、薄めて伸ばすか乾燥させます。
前処置部は光
っているように見えるはずです。

合成物、金属、ジルコニア、ポーセリンの修理
1) 合成物：既存の合成物の劣化した部分を取り除きます。
ダイアモンドバーで表面に凹凸をつけます。
a) トータルエッチ技術
i. Blue Micro Tipを使ってUltra Etchを20秒間、歯の前処置部の表面全体に適用します。
ii. 5秒間よく洗浄し、湿った状態を維持します。
2) 金属：微小摩耗面a) トータルエッチ技術
i. Blue Micro Tipを使ってUltra Etchを20秒間、歯の前処置部の表面全体に適用します。
ii. 5秒間よく洗浄し、湿った状態を維持します。
3) ジルコニア：表面をきれいにし、ダイアモンドバーで劣化したジルコニアを取り除きます。
エッチングを行ったりシランを使用したりしないでください。
a) 人工補綴物の内面を空気で摩耗させます。
b) メーカーの指示に従い、割れた部分にジルコニアのプライマーを適用します。
4) ポーセリン：ダイアモンドバーで劣化したポーセリンの表面に凹凸をつけて取り除きます。
ポーセリンの割れた部分を15秒間、Ultra Etchできれいにし、洗浄して乾燥させます。
注意 -フッ化水素酸（HF）（Ultradent™ポーセリンエッチ）を使い、酸中和バリア（EtchArrest）などの適切な分離手段を使用してください。
フッ化水素酸が歯肉や歯質に触れないようにしてください。
a) フッ化水素酸を割れた部分に90秒間適用します。
b) 表面から酸を吸い取り、表面をよく洗浄して乾燥させます。
c) Ultra Etchを5秒間適用し、HFエッチングで生じたポーセリンソルトや破片を取り除きます。
洗浄して乾燥させます。
d) シランを1分間、適用します。
e) よく乾燥させます。
洗浄しないでください。
5) ボンドa) ボトルの場合
i. 使い捨てダッペン皿の「B」側にPeak™ユニバーサルボンドを1～3滴入れます。
ii. Micro Applicator Brushを使用してPeak™ユニバーサルボンドを前処置部に適用し、10秒間ゆっくりかき混ぜます。
iii. ¼～½の空気圧を使用して10秒間薄めて伸ばすか乾燥させます。
前処
置部は光っているように見えるはずです。
iv. 10秒間、光硬化させます（出力が600mW/cm2未満の光の場合は20秒間）。
b) シリンジの場合
i. Peak™ユニバーサルボンドをInspiral™ブラシチップで適用し、10秒間ゆっくりかき混ぜます。
ii. ¼～½の空気圧を使用して10秒間薄めて伸ばすか乾燥させます。
iii. 前処置部は光っているように見えるはずです。
iv. 10秒間、光硬化させます（出力が600mW/cm2未満の光の場合は
59

20秒間）。
6) メーカーの指示に従い、流動性のある合成物かパッキング可能な合成物で修復します。

ポストセメンテーションおよびコア・ビルドアップ
1) PermaFlo™ DC シリンジのキャップを外します。
2) 混合チップを二重バレル・シリンジに取り付け、2つのポートを合わせます。
しポストおよびコア
っかりとロックされるまで時計回りに回します。
1)前処置
3) フレキシブルなIntraoral Tip™ を混合チップに取付け、二重バレル・シリンジa) ラバーストップおよび適切なサイズのUniCore™ Drillでポスト用の孔を開から直接カナルに抽出します。
けます。
4) ポスト・スペースに抽出する前に、少量を押し出して（流率を）確認します。
b) TriAway アダプタおよび 22ga Endo-Eze™ チップを使用して、ポストスペー
5) チップをポスト・スペースに完全に入れます。
スを10秒間リンスしてください。
TriAway アダプタおよび 22g Endo-Eze チ 6) 均一に圧力をかけながら、PermaFlo DC をベースから舌頂に向けて送り
ップで、処置部下から上方向に乾燥させます。
出してください。
c) ポスト(UniCore Post) の装着具合を確認し、必要であれば拘束ダイヤモン
7) ポスト（UniCore™ ポスト）をゆっくりと挿入し、余分なセメントを除去してドディスクで希望の長さに切断します。
注記：カーバイドおよ び掘削器具なください。
どを使うと、繊維が擦り切れる可能性があります。
8) 硬化ライトを直接ポストに当て、20秒間光硬化させます（出力<600mW/cm2
2)エッチング
以下の光を使用する場合は40秒間）。
a) セルフ・エッチング技術
9) 必要に応じて、引き続きPermaFlo™ DC のレイヤーをポストのまわりに作って
i. カナルスペースを洗い流し、少し湿気のある状態に乾燥させてください。
いきます。
中期：ジェル層の間に光硬化を5秒行い、コアを形成します。
コアのii. ブルーの22gのDeliver-Eze™ ブラシチップをPeak SE シリンジに装
最終硬化には40秒間必要です。
着します。
iii. 20秒間攪拌しながら、ポスト・スペースおよび舌頂部の前処理を施した 次に使用する時まで混合チップを取り外さないでください。
シリンジおよび混合場所にアプライしてください。
チップの殺菌を行ってください。
iv. 余分な分量は、TriAway Adaptorおよび22ga Endo-Eze Tip をスペー
スの下から上方向に動かして除去します。
エアー/ウォーターシリン ジ、 使用上の注意および注意事項：
または処置部に高量吸引器を直接当てて、3秒間薄く伸ばすか、または 1. Peak Universal Bondを使用する前に取り扱い説明をよく読み、理解して乾燥させてください。
ください。
v. 以下の「結合」手順に進みます。
2. 本剤は、歯科医専用です。
b) 総合エッチ技術：
3. 使用後はすばやくキャップを閉めて、硬化しないようにしてください。
i. ブルーの22gのEndo-Eze チップをUltra-Etch シリンジに装着します。 4. 薬剤を口内にアプライする前には、シリンジの流量を確認してください。
抵抗ii. 尖端から舌頂に向けてポストスペースを充填していきます。
舌頂部の前を感じる場合は、チップを取り替えて再度流量を確認してください。
処理剤をアプライします。
20秒間エッチングします。
5. 使用するまでキャップをボトルにつけたままにしてください。
iii. 余分なエッチング液を吸引します。
6. 歯科医および患者は、レジンを硬化する際はUV 保護めがねを装着する必iv. TriAway アダプタおよび22gEndo-Eze チップを使った後、完全に洗い要があります。
流し、軽くエアドライさせ、処置部に少し水が残る状態にします。
7. 毎日使用しない場合は、本剤を冷蔵保存してください。
v. 以下の「結合」手順に進みます。
8. 使用する前に、冷蔵されている本剤を常温に戻してください。
3) 接着剤
9. 接着強度を最大限にするために、
オイルフリーの乾燥した環境で使用してa. ボトルの場合ください。
i. 1～3滴のPeak Universal Bond を使い捨て用の取り皿の「B」側に
10. 頭上ライトの位置を変えて、すべてのレジンベースの素材が早く固まらない取ります。
ようにしてください。
ii. Nano-Brush™ またはNaviTip FXを使って、少量のPeak Universal
11. レジンは増感化合物です。
硬化されていないレジンが、何度も皮膚に接触しBond を処置部に適用し、カナルスペース全体および歯の処置部 を10ないようにしてください。
アクリレート、またはその他のレジンに過症の患者さ
秒間やさしく攪拌します。
んには使用しないでください。
アレルギー反応、皮膚炎、蕁麻疹などが見られ
iii. TriAway アダプタおよび22gの Endo-Eze チップを使い、余分な分量る場合は、医師にご相談ください。
を除去してください。
12. 使用済みチップ、空になったシリンジ、およびボトルは適切に廃棄してく
iv. ¼ ～ ½ の空気圧力で外側の処置部を10秒間乾燥/薄く伸ばします。
処
ださい。
置部に光沢が現れます。
13. 子供の手の届かないところに保管してください。
v. ポスト・スペースを20秒間光硬化させます（出力＜600mw /cm2 の光を 14. 容器に記載の有効期限を過ぎたものは使用しないでください。
使用する場合は40秒間）。
15. 使用後は、キャップを閉め、殺菌し、中程度消毒でシリンジを拭いてください。
vi. ペーパーポイント、
またはあらかじめサイズ調整したポストを使用して、使い捨てのシリンカバーを使用する場合は、チップを取り外し、キャップを再ポストスペースがブロックされていないことを確認します。
度閉めた後にシリンジカバーを廃棄してください。
b) シリンジの場合
16. 交差汚染を防ぐために、チップを再利用しないでください。
i. Peak™ユニバーサルボンドのシリンジに30ga NaviTip FXを取り付
17. 本剤を高熱/直射日光の当たる場所に保管しないでください。
けます。
18. 強い薬品を処置部位に近づけないでください。
ii. ポストのスペースと前処置部に1～2滴塗布し、根管の長さ全体（歯の19. ルアーロックキャップでシリンジにキャップをし、使用後は中程度消毒でシリ前処置部を含む）で10秒間、かき混ぜます。
ンジを殺菌してください。
iii. TriAwayアダプターと22ga Endo-Ezeチップを使い、Peak™ユニバーサ
ルボンドの余剰分をすべて取り除きます。
注：Peak™ユニバーサルボンド、Peak™ SE、他の関連製品のSDSと追加情報
iv. 完全な空気圧でポストのスペースと前処置部を10秒間、空気乾燥さについては、www.ultradent.comをご覧ください。
せ、TriAwayアダプターと22ga Endo-Ezeチップで薄く伸ばすか乾燥さ
せま す。
残りの溶剤は底部から上に向かって蒸発させます。
v. ポストのスペースを20秒間、光硬化させます（出力が600mW/cm2未満の光の場合は40秒間）。
紙の先端または以前に装着されていたポスト を使用して、ポストのスペースがブロックされていないことを確
認します。
60

LOT
EN - For professional use only
DE - Nur zur Verwendung durch Sachkundige
FR - Destiné à un usage professionnel uniquement
NL - Alleen voor professioneel gebruik
IT - Esclusivamente ad uso professionale
ES - Sólo para uso profesional
PT - Apenas para uso profissional
SV - Enbart för yrkesmässig användning
DA - Kun til professionel brug
FI - Vain ammattikäyttöön
NO - Kun for profesjonell brukEL - Για επαγγελματική χρήση μόνοRU - Только для профессионального применения
PL - Wyłącznie do zastosowań profesjonalnych
TR - Sadece profesyonel kullanıma yöneliktir
AR - ‫لالستخدام المهني فقط‬KO - 전문가 전용
ZH - 仅用于专业用途
TH - ส�ำหรับผู้เชีย่ วชาญใช้เท่านัน้
JA - 専門的な使用のみ

EN - Use by date
DE - Verfallsdatum
FR - Date de péremption
NL - Uiterste gebruiksdatum
IT - Utilizzare entro
ES - Usar antes dePT - Usar até a data
SV - Använd före datum
DA - Udløbsdato
FI - Viimeinen käyttöajankohta
NO - Bruk før dato
EL - Ημερομηνία λήξης
RU - Использовать до
PL - Data ważności
TR - Son kullanma tarihi
AR - ‫تاريخ انتهاء الصالحية‬KO - 기재일까지 사용
ZH - 有效期TH - ใช้ภายในวันที่
JA - 使用期限

EN - Lot Number
DE - Chargennummer
FR - Numéro du lot
NL - Batchnummer
IT - Numero del lotto
ES - Número de Lote
PT - Número do loteSV - Satsnummer
DA - Lotnummer
FI - Eränumero
NO - Varenummer
EL - Αριθμός παρτίδας
RU - Номер партии
PL - Numer serii
TR - Lot Numarası
AR - ‫رقم العبوة‬KO - 로트 번호
ZH - 批号
TH - หมายเลขสลาก
JA - ロット番号

EN - Manufacturer
DE - Hersteller
FR - Fabricant
NL - Fabrikant
IT - Fabbricante
ES - Fabricante
PT - Fabricante
SV - Tillverkare
DA - Producent
FI - Valmistaja
NO - Produsent
EL - Κατασκευαστής
RU - Производитель
PL - Producent
TR - Üretici
AR - ‫الشركة المصنعة‬KO - 제조자
ZH - 制造商
TH - ผู้ผลิต
JA - メーカー

EN - See Instructions
DE - Siehe Anleitung
FR - Cf. instructions
NL - Zie gebruiksaanwijzing
IT - Vedere le istruzioni
ES - Vea las Instrucciones
PT - Veja as instruções
SV - Se anvisningar
DA - Se brugsanvisningen
FI - Lue käyttöohjeet
NO - Se instruksjoner
EL - Δείτε τις οδηγίες
RU - См. инструкцию
PL - Patrz: instrukcje
TR - Talimatlara bakın
AR - ‫انظر التعليمات‬KO - 설명서 참고
ZH - 参阅说明TH - ดูขนั้ ตอนการใช้
JA - 指示を参照

EN - Catalog Number
DE - Katalognummer
FR - Numéro de référence
NL - Catalogusnummer
IT - Numero di catalogo
ES - Número de catálogo
PT - Número do catálogo
SV - Katalognummer
DA - Katalognummer
FI - Luettelonumero
NO - Katalognummer
EL - Αριθμός καταλόγου
RU - Номер по каталогу
PL - Numer katalogowy
TR - Katalog Numarası
AR - ‫رقم الكتالوج‬KO - 카탈로그 번호
ZH - 目录号TH - หมายเลขแคตาล็อก
JA - カタログ番号
61

2°C
36°F

62

8°C
46°F

EN - Flammable
DE - Entzündbar
FR - Inflammable
NL - Brandbaar
IT - Infiammabile
ES - Inflamable
PT - Inflamável
SV - Brandfarlig
DA - Brændbar
FI - Syttyvä
NO - Lett antennelig
EL - ΕύφλεκτοRU - Легковоспламеняющееся вещество
PL - Produkt łatwopalny
TR - Yanıcıdır
AR - ‫قابل لالشتعال‬KO - 인화성
ZH - 易燃TH - ติดไฟได้
JA - 可燃性

EN - Health hazard
DE - Gesundheitsgefahr
FR - Dangereux por la santé
NL - Gevaar voor de gezondheid
IT - Pericolo per la salute
ES - Peligro para la salud
PT - Riscos à saúde
SV - Hälsofara
DA - Sundhedsfarlig
FI - Terveysvaara
NO - Helsefare
EL - Κινδυνεύει την υγεία
RU - Опасно для здоровья
PL - Zagrożenie dla zdrowia
TR - Sağlık için tehlikeli
AR - ‫خطر عىل الصحة‬KO - 건강유해물
ZH - 健康危害
TH - อันตรายต่อสุขภาพ
JA - 健康被害

EN - Refrigerate
DE - Kühlen
FR - Réfrigérer
NL - In de koelkast bewaren
IT - Conservare in frigorifero
ES - Refrigere
PT - Refrigerar
SV - Förvaras i kylskåpDA - Opbevares i køleskab
FI - Säilytä jääkaapissa
NO - Kjøl ned
EL - Διατηρήστε το στο ψυγείο
RU - Хранить в холодильнике
PL - Przechowywać w lodówce
TR - Soğutun
AR - ‫قم بوضعه في الثالجة‬KO - 냉장보관
ZH - 冷藏
TH - แช่เย็น
JA - 冷蔵

EN - Dentist Dispensed.
DE - Vom Zahnarzt abzugeben.
FR - Distribué par le chirurgien dentiste.
NL - Door de tandarts verstrekt.
IT - Prescritto dal dentista.
ES - Administrado por el Dentista.
PT - Administrado pelo dentista.
SV - Appliceras av tandläkare.
DA - Administreret af tandlæge.
FI - Hammaslääkärin käyttöön.
NO - Kun for bruk av tannlege.
EL - Διανέμεται από τον οδοντίατρο.
RU - Для применения в стоматологии.
PL - Wydaje się z przepisu dentysty.
TR - Dişçi tarafından dağıtılır.
AR - ‫المستخدمة من قبل طبيب األسنان‬KO - 치과의만 사용할 수 있습니다.
ZH - 由牙科醫師開具處方。
TH - ทันตแพทย์เป็นผู้ใช้เท่านัน้
JA - 歯科医による調合

EN - Destroy after use.
DE - Nach Gebrauch vernichten.
FR - Détruire après utilisation.
NL - Na gebruik vernietigen.
IT - Distruggere dopo l’uso.
ES - Destrúyalo después de usarlo.
PT - Destruir após usar.
SV - Förstøres efter användning.
DA - Destruér efter brug.
FI - Hävitä käytön jälkeen.
NO - Kasseres etter brukEL - Καταστρέψτε το μετά τη χρήση.
RU - После использования уничтожить.
PL - Po użyciu zniszczyć.
TR - Kullandıktan sonra imha edin.
AR - ‫يرمى بعد اإلستخدام‬KO - 사용 후 폐기하십시오.
ZH - 用後銷毀TH - ท�ำลายหลังการใช้งาน
JA - 使用後は廃棄のこと

EN - Not for injection.
DE - Nicht zur Injektion.
FR - Ne pas injecter.
NL - Niet injecteren.
IT - Non per iniezione.
ES - No debe inyectarse.
PT - Não injectar.
SV - Ej för injektion.
DA - Ikke til injektion.
FI - Ei injektiokäyttöön.
NO - Ikke til injeksjon
EL - Μη ενέσιμο.
RU - Не для инъекций.
PL - Nie nadaje się do iniekcji.
TR - Enjekte edilmek için kullanılmaz.
AR - ‫ال يصلح للحقن‬KO - 주입하지 마십시오.
ZH - 非供注射之用
TH - ไม่ใช่สำ� หรับการฉีด
JA - 注射に使用してはならないFlammability

Flammability

Peak™SE

Ultra-Etch™

1

1

0

Peak™ Universal Bond

Health10

HealthReactivity

For product SDS please see our
website: www.ultradent.com

10

Flammability

Reactivity

For product SDS please see our
website: www.ultradent.com

Health2

acid

1

Reactivity

HAZARD RATING
4 = Severe
3 = Serious
2 = Moderate
1 = Slight
0 = Minimal

For product SDS please see our
website: www.ultradent.com

X026 = LOT
X026 = MM
X026 = YYYY

U.S. federal law restricts the sale of this device by or on the order of a dentist.
For immediate reorder and/or complete descriptions of Ultradent’s product line,refer to Ultradent’s catalog or call Toll Free 1-800-552-5512.
Outside U.S. call (801) 572-4200
or visit www.ultradent.com.

1 Evaluation of experimental Peak containing chlorhexidine (CHX) blended at
0.2% within it's formulation. re: Professor Lorenzo Breschi from the Department of
Biomedicine, University of Trieste, Trieste Italy.

© Copyright 2017 Ultradent Products, Inc. All Rights Reserved.
Manufactured by Ultradent Products, Inc.
505 West Ultradent Drive (10200 South),South Jordan, Utah 84095, USA
Made in USA

Ultradent Products GmbHAm Westhover Berg 30
51149 Cologne
Germany45414.6092419